#------------------------------------------------------------------------------
#$Date: 2019-05-21 14:26:13 +0300 (Tue, 21 May 2019) $
#$Revision: 215354 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103510.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103510
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.5 La3 Nb0.5 O14'
_chemical_formula_weight         1070.65
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   7.953
_cell_length_b                   7.953
_cell_length_c                   5.023
_cell_measurement_temperature    293(2)
_cell_volume                     275.1
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         13.1E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.900
_diffrn_measured_fraction_theta_max 0.900
_diffrn_radiation_source         synchrotron
_diffrn_radiation_wavelength     0.56000
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0609
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            473
_diffrn_reflns_theta_full        22.94
_diffrn_reflns_theta_max         22.94
_diffrn_reflns_theta_min         3.20
_exptl_absorpt_coefficient_mu    14.672
_exptl_crystal_density_diffrn    6.462
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             474
_refine_diff_density_max         2.228
_refine_diff_density_min         -1.747
_refine_diff_density_rms         0.457
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.00(11)
_refine_ls_extinction_coef       0.019(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.077
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         473
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.077
_refine_ls_R_factor_all          0.0453
_refine_ls_R_factor_gt           0.0446
_refine_ls_shift/su_max          0.019
_refine_ls_shift/su_mean         0.003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1303
_refine_ls_wR_factor_ref         0.1308
_reflns_number_gt                469
_reflns_number_total             473
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-13.1d3.cif
_cod_data_source_block           13.1d3
_cod_depositor_comments
;
 Correcting the reference to the optimal entry by changing it from
 '2103510' to '2103511'. The reference now correctly refers to the
 entry with the lowest _refine_ls_R_factor_all value.

 Antanas Vaitkus,
 2018-11-16

The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

When more than one structure was present in the sn0021.cif file for a
given pressure, the structure with the minimal _refine_ls_R_factor_all
value was taken as the best one, and all others marked with the
'_cod_suboptimal_structure yes' tag.

Changing (with the help of Perl) all _diffrn_radiation_source values in
the files that were reportedly colected on the HASYLAB D3 beamline
(Hamburg) from 'fine-focus sealed tube' to synchrotron.

The command was:

perl -i -ne \
    "s/'fine-focus sealed tube'/synchrotron/; \
    print unless /_diffrn_radiation_type|_diffrn_radiation_monochromator/" \
    *d3*.cif \
    11.57split.cif \
    21.85split.cif \
    22.85split.cif

Saulius Gra\<zulis

 Removed the _cod_suboptimal_structure data item in preparation for
 its deprecation. The fact that the structure is a suboptimal one
 should be derived from the presence of the _cod_related_optimal_struct
 data item.

 Antanas Vaitkus,
 2019-05-21
;
_cod_original_formula_sum        'Ga5.50 La3 Nb0.50 O14'
_cod_related_optimal_struct      2103511
_cod_database_code               2103510
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La -0.43418(15) 0.0000 0.0000 0.0193(4) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0225(7) Uani 0.50 6 d SP
Ga2 Ga -0.6667 -0.3333 0.4810(6) 0.0178(6) Uani 1 3 d S
Ga3 Ga -0.7666(3) 0.0000 -0.5000 0.0179(5) Uani 1 2 d S
Nb Nb 0.0000 0.0000 0.0000 0.0225(7) Uani 0.50 6 d SP
O1 O -0.3333 0.3333 0.168(4) 0.014(3) Uani 1 3 d S
O2 O -0.447(2) -0.295(3) 0.302(3) 0.055(5) Uani 1 1 d .
O3 O -0.2200(18) -0.069(2) -0.239(3) 0.043(4) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.9400 1.6100 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -0.9600 2.8600 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2400 1.0600 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 66.2(6) . 6
O3 La O2 140.5(6) . 3_455
O3 La O2 107.9(6) 6 3_455
O3 La O2 107.9(6) . 5_455
O3 La O2 140.5(6) 6 5_455
O2 La O2 99.8(8) 3_455 5_455
O3 La O1 122.2(4) . .
O3 La O1 79.5(4) 6 .
O2 La O1 92.9(5) 3_455 .
O2 La O1 71.3(5) 5_455 .
O3 La O1 79.5(4) . 2_455
O3 La O1 122.2(4) 6 2_455
O2 La O1 71.3(5) 3_455 2_455
O2 La O1 92.9(5) 5_455 2_455
O1 La O1 155.84(8) . 2_455
O3 La O2 78.6(5) . .
O3 La O2 62.8(6) 6 .
O2 La O2 65.5(7) 3_455 .
O2 La O2 156.6(3) 5_455 .
O1 La O2 125.0(5) . .
O1 La O2 65.8(5) 2_455 .
O3 La O2 62.8(6) . 6
O3 La O2 78.6(5) 6 6
O2 La O2 156.6(3) 3_455 6
O2 La O2 65.5(7) 5_455 6
O1 La O2 65.8(5) . 6
O1 La O2 125.0(5) 2_455 6
O2 La O2 134.1(7) . 6
O3 La Ga2 110.8(4) . .
O3 La Ga2 84.5(4) 6 .
O2 La Ga2 32.2(4) 3_455 .
O2 La Ga2 130.3(4) 5_455 .
O1 La Ga2 110.5(4) . .
O1 La Ga2 65.5(4) 2_455 .
O2 La Ga2 33.3(3) . .
O2 La Ga2 163.1(3) 6 .
O3 La Ga2 84.5(4) . 2_565
O3 La Ga2 110.8(4) 6 2_565
O2 La Ga2 130.3(4) 3_455 2_565
O2 La Ga2 32.2(4) 5_455 2_565
O1 La Ga2 65.5(4) . 2_565
O1 La Ga2 110.5(4) 2_455 2_565
O2 La Ga2 163.1(3) . 2_565
O2 La Ga2 33.3(3) 6 2_565
Ga2 La Ga2 162.15(4) . 2_565
O3 La Nb 33.1(3) . .
O3 La Nb 33.1(3) 6 .
O2 La Nb 130.1(4) 3_455 .
O2 La Nb 130.1(4) 5_455 .
O1 La Nb 102.08(4) . .
O1 La Nb 102.08(4) 2_455 .
O2 La Nb 67.0(3) . .
O2 La Nb 67.0(3) 6 .
Ga2 La Nb 98.93(2) . .
Ga2 La Nb 98.93(2) 2_565 .
O3 La Ga1 33.1(3) . .
O3 La Ga1 33.1(3) 6 .
O2 La Ga1 130.1(4) 3_455 .
O2 La Ga1 130.1(4) 5_455 .
O1 La Ga1 102.08(4) . .
O1 La Ga1 102.08(4) 2_455 .
O2 La Ga1 67.0(3) . .
O2 La Ga1 67.0(3) 6 .
Ga2 La Ga1 98.93(2) . .
Ga2 La Ga1 98.93(2) 2_565 .
Nb La Ga1 0.0 . .
O3 Ga1 O3 161.0(9) 3 6
O3 Ga1 O3 86.5(5) 3 .
O3 Ga1 O3 82.4(7) 6 .
O3 Ga1 O3 82.4(7) 3 2
O3 Ga1 O3 86.5(5) 6 2
O3 Ga1 O3 108.1(9) . 2
O3 Ga1 O3 108.1(9) 3 5
O3 Ga1 O3 86.5(5) 6 5
O3 Ga1 O3 161.0(9) . 5
O3 Ga1 O3 86.5(5) 2 5
O3 Ga1 O3 86.5(5) 3 4
O3 Ga1 O3 108.1(9) 6 4
O3 Ga1 O3 86.5(5) . 4
O3 Ga1 O3 161.0(9) 2 4
O3 Ga1 O3 82.4(7) 5 4
O3 Ga1 O2 50.3(5) 3 2
O3 Ga1 O2 111.0(4) 6 2
O3 Ga1 O2 52.7(5) . 2
O3 Ga1 O2 67.0(5) 2 2
O3 Ga1 O2 146.3(5) 5 2
O3 Ga1 O2 116.4(5) 4 2
O3 Ga1 O2 67.0(5) 3 3
O3 Ga1 O2 116.4(5) 6 3
O3 Ga1 O2 146.3(5) . 3
O3 Ga1 O2 50.3(5) 2 3
O3 Ga1 O2 52.7(5) 5 3
O3 Ga1 O2 111.0(4) 4 3
O2 Ga1 O2 93.7(6) 2 3
O3 Ga1 O2 52.7(5) 3 5
O3 Ga1 O2 146.3(5) 6 5
O3 Ga1 O2 116.4(5) . 5
O3 Ga1 O2 111.0(4) 2 5
O3 Ga1 O2 67.0(5) 5 5
O3 Ga1 O2 50.3(5) 4 5
O2 Ga1 O2 102.4(3) 2 5
O2 Ga1 O2 63.9(5) 3 5
O3 Ga1 O2 111.0(4) 3 .
O3 Ga1 O2 50.3(5) 6 .
O3 Ga1 O2 67.0(5) . .
O3 Ga1 O2 52.7(5) 2 .
O3 Ga1 O2 116.4(5) 5 .
O3 Ga1 O2 146.3(5) 4 .
O2 Ga1 O2 63.9(5) 2 .
O2 Ga1 O2 102.4(3) 3 .
O2 Ga1 O2 161.1(6) 5 .
O3 Ga1 O2 146.3(5) 3 4
O3 Ga1 O2 52.7(5) 6 4
O3 Ga1 O2 111.0(4) . 4
O3 Ga1 O2 116.4(5) 2 4
O3 Ga1 O2 50.3(5) 5 4
O3 Ga1 O2 67.0(5) 4 4
O2 Ga1 O2 161.1(6) 2 4
O2 Ga1 O2 102.4(3) 3 4
O2 Ga1 O2 93.7(6) 5 4
O2 Ga1 O2 102.4(3) . 4
O3 Ga1 O2 116.4(5) 3 6
O3 Ga1 O2 67.0(5) 6 6
O3 Ga1 O2 50.3(5) . 6
O3 Ga1 O2 146.3(5) 2 6
O3 Ga1 O2 111.0(4) 5 6
O3 Ga1 O2 52.7(5) 4 6
O2 Ga1 O2 102.4(3) 2 6
O2 Ga1 O2 161.1(6) 3 6
O2 Ga1 O2 102.4(3) 5 6
O2 Ga1 O2 93.7(6) . 6
O2 Ga1 O2 63.9(5) 4 6
O1 Ga2 O2 119.1(5) 2_456 4_445
O1 Ga2 O2 119.1(5) 2_456 .
O2 Ga2 O2 98.3(6) 4_445 .
O1 Ga2 O2 119.1(5) 2_456 3_455
O2 Ga2 O2 98.3(6) 4_445 3_455
O2 Ga2 O2 98.3(6) . 3_455
O1 Ga2 O1 179.997(2) 2_456 2_455
O2 Ga2 O1 60.9(5) 4_445 2_455
O2 Ga2 O1 60.9(5) . 2_455
O2 Ga2 O1 60.9(5) 3_455 2_455
O1 Ga2 La 135.74(3) 2_456 4_445
O2 Ga2 La 54.7(6) 4_445 4_445
O2 Ga2 La 43.8(5) . 4_445
O2 Ga2 La 104.8(5) 3_455 4_445
O1 Ga2 La 44.26(3) 2_455 4_445
O1 Ga2 La 135.74(3) 2_456 2_455
O2 Ga2 La 43.8(5) 4_445 2_455
O2 Ga2 La 104.8(5) . 2_455
O2 Ga2 La 54.7(6) 3_455 2_455
O1 Ga2 La 44.26(3) 2_455 2_455
La Ga2 La 74.37(5) 4_445 2_455
O1 Ga2 La 135.74(3) 2_456 .
O2 Ga2 La 104.8(5) 4_445 .
O2 Ga2 La 54.7(6) . .
O2 Ga2 La 43.8(5) 3_455 .
O1 Ga2 La 44.26(3) 2_455 .
La Ga2 La 74.37(5) 4_445 .
La Ga2 La 74.37(5) 2_455 .
O1 Ga2 O3 65.5(2) 2_456 4_446
O2 Ga2 O3 59.4(5) 4_445 4_446
O2 Ga2 O3 104.3(7) . 4_446
O2 Ga2 O3 150.0(6) 3_455 4_446
O1 Ga2 O3 114.5(2) 2_455 4_446
La Ga2 O3 79.6(3) 4_445 4_446
La Ga2 O3 100.0(2) 2_455 4_446
La Ga2 O3 153.9(3) . 4_446
O1 Ga2 O3 65.5(2) 2_456 1_556
O2 Ga2 O3 150.0(6) 4_445 1_556
O2 Ga2 O3 59.4(5) . 1_556
O2 Ga2 O3 104.3(7) 3_455 1_556
O1 Ga2 O3 114.5(2) 2_455 1_556
La Ga2 O3 100.0(2) 4_445 1_556
La Ga2 O3 153.9(3) 2_455 1_556
La Ga2 O3 79.6(3) . 1_556
O3 Ga2 O3 104.0(3) 4_446 1_556
O1 Ga2 O3 65.5(2) 2_456 3_456
O2 Ga2 O3 104.3(7) 4_445 3_456
O2 Ga2 O3 150.0(6) . 3_456
O2 Ga2 O3 59.4(5) 3_455 3_456
O1 Ga2 O3 114.5(2) 2_455 3_456
La Ga2 O3 153.9(3) 4_445 3_456
La Ga2 O3 79.6(3) 2_455 3_456
La Ga2 O3 100.0(2) . 3_456
O3 Ga2 O3 104.0(3) 4_446 3_456
O3 Ga2 O3 104.0(3) 1_556 3_456
O1 Ga2 La 42.09(3) 2_456 4_446
O2 Ga2 La 98.0(5) 4_445 4_446
O2 Ga2 La 90.1(6) . 4_446
O2 Ga2 La 160.2(5) 3_455 4_446
O1 Ga2 La 137.91(3) 2_455 4_446
La Ga2 La 93.652(7) 4_445 4_446
La Ga2 La 139.942(5) 2_455 4_446
La Ga2 La 139.941(5) . 4_446
O3 Ga2 La 39.9(2) 4_446 4_446
O3 Ga2 La 64.8(3) 1_556 4_446
O3 Ga2 La 105.6(2) 3_456 4_446
O2 Ga3 O2 105.7(13) 3_454 5_455
O2 Ga3 O3 99.5(7) 3_454 5_454
O2 Ga3 O3 107.7(6) 5_455 5_454
O2 Ga3 O3 107.7(6) 3_454 3_455
O2 Ga3 O3 99.5(7) 5_455 3_455
O3 Ga3 O3 134.3(9) 5_454 3_455
O2 Ga3 O3 74.6(8) 3_454 2_454
O2 Ga3 O3 177.8(5) 5_455 2_454
O3 Ga3 O3 74.4(6) 5_454 2_454
O3 Ga3 O3 78.3(6) 3_455 2_454
O2 Ga3 O3 177.8(5) 3_454 4_455
O2 Ga3 O3 74.6(8) 5_455 4_455
O3 Ga3 O3 78.3(6) 5_454 4_455
O3 Ga3 O3 74.4(6) 3_455 4_455
O3 Ga3 O3 105.2(6) 2_454 4_455
O2 Ga3 Nb 85.2(6) 3_454 1_454
O2 Ga3 Nb 143.3(4) 5_455 1_454
O3 Ga3 Nb 35.7(4) 5_454 1_454
O3 Ga3 Nb 110.5(5) 3_455 1_454
O3 Ga3 Nb 38.8(3) 2_454 1_454
O3 Ga3 Nb 93.3(3) 4_455 1_454
O2 Ga3 Nb 143.3(4) 3_454 1_455
O2 Ga3 Nb 85.2(6) 5_455 1_455
O3 Ga3 Nb 110.5(5) 5_454 1_455
O3 Ga3 Nb 35.7(4) 3_455 1_455
O3 Ga3 Nb 93.3(3) 2_454 1_455
O3 Ga3 Nb 38.8(3) 4_455 1_455
Nb Ga3 Nb 107.07(6) 1_454 1_455
O2 Ga3 O1 61.6(5) 3_454 2_455
O2 Ga3 O1 75.7(5) 5_455 2_455
O3 Ga3 O1 160.6(5) 5_454 2_455
O3 Ga3 O1 61.5(4) 3_455 2_455
O3 Ga3 O1 102.7(3) 2_454 2_455
O3 Ga3 O1 120.5(4) 4_455 2_455
Nb Ga3 O1 137.2(2) 1_454 2_455
Nb Ga3 O1 88.7(2) 1_455 2_455
O2 Ga3 O1 75.7(6) 3_454 1_554
O2 Ga3 O1 61.6(5) 5_455 1_554
O3 Ga3 O1 61.5(4) 5_454 1_554
O3 Ga3 O1 160.6(5) 3_455 1_554
O3 Ga3 O1 120.5(4) 2_454 1_554
O3 Ga3 O1 102.7(3) 4_455 1_554
Nb Ga3 O1 88.7(2) 1_454 1_554
Nb Ga3 O1 137.2(2) 1_455 1_554
O1 Ga3 O1 106.5(2) 2_455 1_554
O2 Ga3 O3 115.7(7) 3_454 6_454
O2 Ga3 O3 132.9(6) 5_455 6_454
O3 Ga3 O3 45.8(4) 5_454 6_454
O3 Ga3 O3 88.9(6) 3_455 6_454
O3 Ga3 O3 47.9(3) 2_454 6_454
O3 Ga3 O3 63.3(4) 4_455 6_454
Nb Ga3 O3 32.80(19) 1_454 6_454
Nb Ga3 O3 75.2(2) 1_455 6_454
O1 Ga3 O3 144.0(3) 2_455 6_454
O1 Ga3 O3 107.2(3) 1_554 6_454
O2 Ga3 O3 132.9(6) 3_454 1_455
O2 Ga3 O3 115.7(7) 5_455 1_455
O3 Ga3 O3 88.9(6) 5_454 1_455
O3 Ga3 O3 45.8(4) 3_455 1_455
O3 Ga3 O3 63.3(4) 2_454 1_455
O3 Ga3 O3 47.9(3) 4_455 1_455
Nb Ga3 O3 75.2(2) 1_454 1_455
Nb Ga3 O3 32.80(19) 1_455 1_455
O1 Ga3 O3 107.2(3) 2_455 1_455
O1 Ga3 O3 144.0(3) 1_554 1_455
O3 Ga3 O3 45.5(4) 6_454 1_455
O3 Nb O3 161.0(9) 3 6
O3 Nb O3 86.5(5) 3 .
O3 Nb O3 82.4(7) 6 .
O3 Nb O3 82.4(7) 3 2
O3 Nb O3 86.5(5) 6 2
O3 Nb O3 108.1(9) . 2
O3 Nb O3 108.1(9) 3 5
O3 Nb O3 86.5(5) 6 5
O3 Nb O3 161.0(9) . 5
O3 Nb O3 86.5(5) 2 5
O3 Nb O3 86.5(5) 3 4
O3 Nb O3 108.1(9) 6 4
O3 Nb O3 86.5(5) . 4
O3 Nb O3 161.0(9) 2 4
O3 Nb O3 82.4(7) 5 4
O3 Nb Ga3 53.8(5) 3 4_445
O3 Nb Ga3 113.2(3) 6 4_445
O3 Nb Ga3 32.7(4) . 4_445
O3 Nb Ga3 98.2(4) 2 4_445
O3 Nb Ga3 159.9(4) 5 4_445
O3 Nb Ga3 87.4(4) 4 4_445
O3 Nb Ga3 113.2(3) 3 4_446
O3 Nb Ga3 53.8(5) 6 4_446
O3 Nb Ga3 98.2(4) . 4_446
O3 Nb Ga3 32.7(4) 2 4_446
O3 Nb Ga3 87.4(4) 5 4_446
O3 Nb Ga3 159.9(4) 4 4_446
Ga3 Nb Ga3 107.07(6) 4_445 4_446
O3 Nb Ga3 98.2(4) 3 1_656
O3 Nb Ga3 87.4(4) 6 1_656
O3 Nb Ga3 159.9(4) . 1_656
O3 Nb Ga3 53.8(5) 2 1_656
O3 Nb Ga3 32.7(4) 5 1_656
O3 Nb Ga3 113.2(3) 4 1_656
Ga3 Nb Ga3 145.42(3) 4_445 1_656
Ga3 Nb Ga3 61.96(5) 4_446 1_656
O3 Nb Ga3 32.7(4) 3 1_655
O3 Nb Ga3 159.9(4) 6 1_655
O3 Nb Ga3 87.4(4) . 1_655
O3 Nb Ga3 113.2(3) 2 1_655
O3 Nb Ga3 98.2(4) 5 1_655
O3 Nb Ga3 53.8(5) 4 1_655
Ga3 Nb Ga3 61.96(5) 4_445 1_655
Ga3 Nb Ga3 145.42(3) 4_446 1_655
Ga3 Nb Ga3 107.07(6) 1_656 1_655
O3 Nb Ga3 159.9(4) 3 2_565
O3 Nb Ga3 32.7(4) 6 2_565
O3 Nb Ga3 113.2(3) . 2_565
O3 Nb Ga3 87.4(4) 2 2_565
O3 Nb Ga3 53.8(5) 5 2_565
O3 Nb Ga3 98.2(4) 4 2_565
Ga3 Nb Ga3 145.42(3) 4_445 2_565
Ga3 Nb Ga3 61.96(5) 4_446 2_565
Ga3 Nb Ga3 61.96(5) 1_656 2_565
Ga3 Nb Ga3 145.42(3) 1_655 2_565
O3 Nb Ga3 87.4(4) 3 2_564
O3 Nb Ga3 98.2(4) 6 2_564
O3 Nb Ga3 53.8(5) . 2_564
O3 Nb Ga3 159.9(4) 2 2_564
O3 Nb Ga3 113.2(3) 5 2_564
O3 Nb Ga3 32.7(4) 4 2_564
Ga3 Nb Ga3 61.96(5) 4_445 2_564
Ga3 Nb Ga3 145.42(3) 4_446 2_564
Ga3 Nb Ga3 145.42(3) 1_656 2_564
Ga3 Nb Ga3 61.96(5) 1_655 2_564
Ga3 Nb Ga3 107.07(6) 2_565 2_564
Ga2 O1 La 109.8(4) 2_566 .
Ga2 O1 La 109.8(4) 2_566 2_565
La O1 La 109.2(4) . 2_565
Ga2 O1 La 109.8(4) 2_566 4_455
La O1 La 109.2(4) . 4_455
La O1 La 109.2(4) 2_565 4_455
Ga2 O1 O2 145.5(3) 2_566 6
La O1 O2 61.3(5) . 6
La O1 O2 52.8(4) 2_565 6
La O1 O2 104.4(6) 4_455 6
Ga2 O1 O2 145.5(3) 2_566 5_455
La O1 O2 52.8(4) . 5_455
La O1 O2 104.4(6) 2_565 5_455
La O1 O2 61.3(5) 4_455 5_455
O2 O1 O2 58.7(6) 6 5_455
Ga2 O1 O2 145.5(3) 2_566 2_565
La O1 O2 104.4(6) . 2_565
La O1 O2 61.3(5) 2_565 2_565
La O1 O2 52.8(4) 4_455 2_565
O2 O1 O2 58.7(6) 6 2_565
O2 O1 O2 58.7(6) 5_455 2_565
Ga2 O1 O3 83.5(4) 2_566 6
La O1 O3 48.3(2) . 6
La O1 O3 81.8(3) 2_565 6
La O1 O3 157.4(5) 4_455 6
O2 O1 O3 65.9(5) 6 6
O2 O1 O3 97.2(4) 5_455 6
O2 O1 O3 124.3(6) 2_565 6
Ga2 O1 O3 83.5(4) 2_566 2_565
La O1 O3 157.4(5) . 2_565
La O1 O3 48.3(2) 2_565 2_565
La O1 O3 81.8(3) 4_455 2_565
O2 O1 O3 97.2(4) 6 2_565
O2 O1 O3 124.3(6) 5_455 2_565
O2 O1 O3 65.9(5) 2_565 2_565
O3 O1 O3 118.73(15) 6 2_565
Ga2 O1 O3 83.5(4) 2_566 5_455
La O1 O3 81.8(3) . 5_455
La O1 O3 157.4(5) 2_565 5_455
La O1 O3 48.3(2) 4_455 5_455
O2 O1 O3 124.3(6) 6 5_455
O2 O1 O3 65.9(5) 5_455 5_455
O2 O1 O3 97.2(4) 2_565 5_455
O3 O1 O3 118.74(15) 6 5_455
O3 O1 O3 118.74(15) 2_565 5_455
Ga2 O1 O2 31.3(3) 2_566 6_556
La O1 O2 96.0(4) . 6_556
La O1 O2 89.4(4) 2_565 6_556
La O1 O2 140.6(6) 4_455 6_556
O2 O1 O2 114.2(5) 6 6_556
O2 O1 O2 148.4(2) 5_455 6_556
O2 O1 O2 148.4(2) 2_565 6_556
O3 O1 O2 56.1(4) 6 6_556
O3 O1 O2 86.2(6) 2_565 6_556
O3 O1 O2 109.6(5) 5_455 6_556
Ga2 O1 O2 31.3(3) 2_566 5_456
La O1 O2 89.4(4) . 5_456
La O1 O2 140.6(6) 2_565 5_456
La O1 O2 96.0(4) 4_455 5_456
O2 O1 O2 148.4(2) 6 5_456
O2 O1 O2 114.2(5) 5_455 5_456
O2 O1 O2 148.4(2) 2_565 5_456
O3 O1 O2 86.2(6) 6 5_456
O3 O1 O2 109.6(5) 2_565 5_456
O3 O1 O2 56.1(4) 5_455 5_456
O2 O1 O2 53.5(6) 6_556 5_456
Ga2 O1 O2 31.3(3) 2_566 2_566
La O1 O2 140.6(6) . 2_566
La O1 O2 96.0(4) 2_565 2_566
La O1 O2 89.4(4) 4_455 2_566
O2 O1 O2 148.4(2) 6 2_566
O2 O1 O2 148.4(2) 5_455 2_566
O2 O1 O2 114.2(5) 2_565 2_566
O3 O1 O2 109.6(5) 6 2_566
O3 O1 O2 56.1(4) 2_565 2_566
O3 O1 O2 86.2(6) 5_455 2_566
O2 O1 O2 53.5(5) 6_556 2_566
O2 O1 O2 53.5(6) 5_456 2_566
Ga2 O1 Ga2 180.0 2_566 2_565
La O1 Ga2 70.2(4) . 2_565
La O1 Ga2 70.2(4) 2_565 2_565
La O1 Ga2 70.2(4) 4_455 2_565
O2 O1 Ga2 34.5(3) 6 2_565
O2 O1 Ga2 34.5(3) 5_455 2_565
O2 O1 Ga2 34.5(3) 2_565 2_565
O3 O1 Ga2 96.5(4) 6 2_565
O3 O1 Ga2 96.5(4) 2_565 2_565
O3 O1 Ga2 96.5(4) 5_455 2_565
O2 O1 Ga2 148.7(3) 6_556 2_565
O2 O1 Ga2 148.7(3) 5_456 2_565
O2 O1 Ga2 148.7(3) 2_566 2_565
Ga2 O1 Ga3 61.9(3) 2_566 2_565
La O1 Ga3 78.50(10) . 2_565
La O1 Ga3 71.91(11) 2_565 2_565
La O1 Ga3 170.8(6) 4_455 2_565
O2 O1 Ga3 83.7(3) 6 2_565
O2 O1 Ga3 127.7(4) 5_455 2_565
O2 O1 Ga3 131.5(5) 2_565 2_565
O3 O1 Ga3 30.8(2) 6 2_565
O3 O1 Ga3 92.8(3) 2_565 2_565
O3 O1 Ga3 130.5(5) 5_455 2_565
O2 O1 Ga3 30.7(3) 6_556 2_565
O2 O1 Ga3 78.7(5) 5_456 2_565
O2 O1 Ga3 81.4(4) 2_566 2_565
Ga2 O1 Ga3 118.1(3) 2_565 2_565
Ga2 O1 Ga3 61.9(3) 2_566 1_556
La O1 Ga3 71.91(11) . 1_556
La O1 Ga3 170.8(6) 2_565 1_556
La O1 Ga3 78.50(10) 4_455 1_556
O2 O1 Ga3 131.5(5) 6 1_556
O2 O1 Ga3 83.7(3) 5_455 1_556
O2 O1 Ga3 127.7(4) 2_565 1_556
O3 O1 Ga3 92.8(3) 6 1_556
O3 O1 Ga3 130.5(5) 2_565 1_556
O3 O1 Ga3 30.8(2) 5_455 1_556
O2 O1 Ga3 81.4(4) 6_556 1_556
O2 O1 Ga3 30.7(3) 5_456 1_556
O2 O1 Ga3 78.7(5) 2_566 1_556
Ga2 O1 Ga3 118.1(3) 2_565 1_556
Ga3 O1 Ga3 99.7(3) 2_565 1_556
Ga2 O1 Ga3 61.9(3) 2_566 4_456
La O1 Ga3 170.8(6) . 4_456
La O1 Ga3 78.50(10) 2_565 4_456
La O1 Ga3 71.90(11) 4_455 4_456
O2 O1 Ga3 127.7(4) 6 4_456
O2 O1 Ga3 131.5(5) 5_455 4_456
O2 O1 Ga3 83.7(3) 2_565 4_456
O3 O1 Ga3 130.5(5) 6 4_456
O3 O1 Ga3 30.8(2) 2_565 4_456
O3 O1 Ga3 92.8(3) 5_455 4_456
O2 O1 Ga3 78.7(5) 6_556 4_456
O2 O1 Ga3 81.4(4) 5_456 4_456
O2 O1 Ga3 30.7(3) 2_566 4_456
Ga2 O1 Ga3 118.1(3) 2_565 4_456
Ga3 O1 Ga3 99.7(3) 2_565 4_456
Ga3 O1 Ga3 99.7(3) 1_556 4_456
Ga2 O1 O2 79.2(4) 2_566 4
La O1 O2 93.7(3) . 4
La O1 O2 42.5(3) 2_565 4
La O1 O2 149.7(3) 4_455 4
O2 O1 O2 68.9(5) 6 4
O2 O1 O2 126.5(4) 5_455 4
O2 O1 O2 103.3(5) 2_565 4
O3 O1 O2 48.5(4) 6 4
O3 O1 O2 70.3(4) 2_565 4
O3 O1 O2 159.4(6) 5_455 4
O2 O1 O2 50.7(5) 6_556 4
O2 O1 O2 104.0(5) 5_456 4
O2 O1 O2 84.7(4) 2_566 4
Ga2 O1 O2 100.8(4) 2_565 4
Ga3 O1 O2 29.6(2) 2_565 4
Ga3 O1 O2 128.8(5) 1_556 4
Ga3 O1 O2 88.7(4) 4_456 4
Ga2 O1 O2 79.2(4) 2_566 3_455
La O1 O2 42.5(3) . 3_455
La O1 O2 149.7(3) 2_565 3_455
La O1 O2 93.7(3) 4_455 3_455
O2 O1 O2 103.3(5) 6 3_455
O2 O1 O2 68.9(5) 5_455 3_455
O2 O1 O2 126.5(4) 2_565 3_455
O3 O1 O2 70.3(4) 6 3_455
O3 O1 O2 159.4(6) 2_565 3_455
O3 O1 O2 48.5(4) 5_455 3_455
O2 O1 O2 84.7(4) 6_556 3_455
O2 O1 O2 50.7(5) 5_456 3_455
O2 O1 O2 104.0(5) 2_566 3_455
Ga2 O1 O2 100.8(4) 2_565 3_455
Ga3 O1 O2 88.7(4) 2_565 3_455
Ga3 O1 O2 29.6(2) 1_556 3_455
Ga3 O1 O2 128.8(5) 4_456 3_455
O2 O1 O2 116.5(3) 4 3_455
Ga2 O1 O2 79.2(4) 2_566 1_565
La O1 O2 149.7(3) . 1_565
La O1 O2 93.7(3) 2_565 1_565
La O1 O2 42.5(3) 4_455 1_565
O2 O1 O2 126.5(4) 6 1_565
O2 O1 O2 103.3(5) 5_455 1_565
O2 O1 O2 68.9(5) 2_565 1_565
O3 O1 O2 159.4(6) 6 1_565
O3 O1 O2 48.5(4) 2_565 1_565
O3 O1 O2 70.3(4) 5_455 1_565
O2 O1 O2 104.0(5) 6_556 1_565
O2 O1 O2 84.7(4) 5_456 1_565
O2 O1 O2 50.7(5) 2_566 1_565
Ga2 O1 O2 100.8(4) 2_565 1_565
Ga3 O1 O2 128.8(5) 2_565 1_565
Ga3 O1 O2 88.7(4) 1_556 1_565
Ga3 O1 O2 29.6(2) 4_456 1_565
O2 O1 O2 116.5(3) 4 1_565
O2 O1 O2 116.5(3) 3_455 1_565
Ga2 O1 O3 118.7(3) 2_566 .
La O1 O3 28.0(2) . .
La O1 O3 81.3(3) 2_565 .
La O1 O3 123.2(5) 4_455 .
O2 O1 O3 38.4(5) 6 .
O2 O1 O3 62.0(5) 5_455 .
O2 O1 O3 93.8(5) 2_565 .
O3 O1 O3 37.0(4) 6 .
O3 O1 O3 129.6(4) 2_565 .
O3 O1 O3 108.9(4) 5_455 .
O2 O1 O3 93.1(4) 6_556 .
O2 O1 O3 110.0(4) 5_456 .
O2 O1 O3 146.6(5) 2_566 .
Ga2 O1 O3 61.3(3) 2_565 .
Ga3 O1 O3 66.01(17) 2_565 .
Ga3 O1 O3 98.94(19) 1_556 .
Ga3 O1 O3 158.22(17) 4_456 .
O2 O1 O3 70.8(4) 4 .
O2 O1 O3 69.4(3) 3_455 .
O2 O1 O3 162.1(6) 1_565 .
Ga2 O1 O3 118.7(3) 2_566 3_565
La O1 O3 123.2(5) . 3_565
La O1 O3 28.0(2) 2_565 3_565
La O1 O3 81.3(3) 4_455 3_565
O2 O1 O3 62.0(5) 6 3_565
O2 O1 O3 93.8(5) 5_455 3_565
O2 O1 O3 38.4(5) 2_565 3_565
O3 O1 O3 108.9(4) 6 3_565
O3 O1 O3 37.0(4) 2_565 3_565
O3 O1 O3 129.6(4) 5_455 3_565
O2 O1 O3 110.0(4) 6_556 3_565
O2 O1 O3 146.6(5) 5_456 3_565
O2 O1 O3 93.1(4) 2_566 3_565
Ga2 O1 O3 61.3(3) 2_565 3_565
Ga3 O1 O3 98.94(19) 2_565 3_565
Ga3 O1 O3 158.22(17) 1_556 3_565
Ga3 O1 O3 66.01(17) 4_456 3_565
O2 O1 O3 69.4(3) 4 3_565
O2 O1 O3 162.1(6) 3_455 3_565
O2 O1 O3 70.8(4) 1_565 3_565
O3 O1 O3 98.9(4) . 3_565
Ga2 O1 O3 118.7(3) 2_566 4_455
La O1 O3 81.3(3) . 4_455
La O1 O3 123.2(5) 2_565 4_455
La O1 O3 28.0(2) 4_455 4_455
O2 O1 O3 93.8(5) 6 4_455
O2 O1 O3 38.4(5) 5_455 4_455
O2 O1 O3 62.0(5) 2_565 4_455
O3 O1 O3 129.6(4) 6 4_455
O3 O1 O3 108.9(4) 2_565 4_455
O3 O1 O3 37.0(4) 5_455 4_455
O2 O1 O3 146.6(5) 6_556 4_455
O2 O1 O3 93.1(4) 5_456 4_455
O2 O1 O3 110.0(4) 2_566 4_455
Ga2 O1 O3 61.3(3) 2_565 4_455
Ga3 O1 O3 158.23(17) 2_565 4_455
Ga3 O1 O3 66.01(17) 1_556 4_455
Ga3 O1 O3 98.94(19) 4_456 4_455
O2 O1 O3 162.1(6) 4 4_455
O2 O1 O3 70.8(4) 3_455 4_455
O2 O1 O3 69.4(3) 1_565 4_455
O3 O1 O3 98.9(4) . 4_455
O3 O1 O3 98.9(4) 3_565 4_455
Ga2 O1 Ga3 137.05(15) 2_566 2_564
La O1 Ga3 58.4(3) . 2_564
La O1 Ga3 52.4(2) 2_565 2_564
La O1 Ga3 113.1(5) 4_455 2_564
O2 O1 Ga3 8.7(3) 6 2_564
O2 O1 Ga3 64.5(4) 5_455 2_564
O2 O1 Ga3 67.0(4) 2_565 2_564
O3 O1 Ga3 57.4(3) 6 2_564
O3 O1 Ga3 99.3(3) 2_565 2_564
O3 O1 Ga3 128.7(4) 5_455 2_564
O2 O1 Ga3 105.8(3) 6_556 2_564
O2 O1 Ga3 141.6(4) 5_456 2_564
O2 O1 Ga3 145.1(4) 2_566 2_564
Ga2 O1 Ga3 42.95(15) 2_565 2_564
Ga3 O1 Ga3 75.12(11) 2_565 2_564
Ga3 O1 Ga3 130.16(16) 1_556 2_564
Ga3 O1 Ga3 130.16(16) 4_456 2_564
O2 O1 Ga3 62.3(3) 4 2_564
O2 O1 Ga3 100.9(3) 3_455 2_564
O2 O1 Ga3 133.6(5) 1_565 2_564
O3 O1 Ga3 32.9(2) . 2_564
O3 O1 Ga3 66.1(3) 3_565 2_564
O3 O1 Ga3 101.0(4) 4_455 2_564
Ga2 O1 Ga3 137.05(15) 2_566 .
La O1 Ga3 52.4(2) . .
La O1 Ga3 113.1(5) 2_565 .
La O1 Ga3 58.4(3) 4_455 .
O2 O1 Ga3 67.0(4) 6 .
O2 O1 Ga3 8.7(3) 5_455 .
O2 O1 Ga3 64.5(4) 2_565 .
O3 O1 Ga3 99.3(3) 6 .
O3 O1 Ga3 128.7(4) 2_565 .
O3 O1 Ga3 57.4(3) 5_455 .
O2 O1 Ga3 145.1(4) 6_556 .
O2 O1 Ga3 105.8(3) 5_456 .
O2 O1 Ga3 141.6(4) 2_566 .
Ga2 O1 Ga3 42.95(15) 2_565 .
Ga3 O1 Ga3 130.16(16) 2_565 .
Ga3 O1 Ga3 75.12(11) 1_556 .
Ga3 O1 Ga3 130.16(16) 4_456 .
O2 O1 Ga3 133.6(5) 4 .
O2 O1 Ga3 62.3(3) 3_455 .
O2 O1 Ga3 100.9(3) 1_565 .
O3 O1 Ga3 66.1(3) . .
O3 O1 Ga3 101.0(4) 3_565 .
O3 O1 Ga3 32.9(2) 4_455 .
Ga3 O1 Ga3 72.3(2) 2_564 .
Ga2 O1 Ga3 137.05(15) 2_566 4_455
La O1 Ga3 113.1(5) . 4_455
La O1 Ga3 58.4(3) 2_565 4_455
La O1 Ga3 52.4(2) 4_455 4_455
O2 O1 Ga3 64.5(4) 6 4_455
O2 O1 Ga3 67.0(4) 5_455 4_455
O2 O1 Ga3 8.7(3) 2_565 4_455
O3 O1 Ga3 128.7(4) 6 4_455
O3 O1 Ga3 57.4(3) 2_565 4_455
O3 O1 Ga3 99.3(3) 5_455 4_455
O2 O1 Ga3 141.6(4) 6_556 4_455
O2 O1 Ga3 145.1(4) 5_456 4_455
O2 O1 Ga3 105.8(3) 2_566 4_455
Ga2 O1 Ga3 42.95(15) 2_565 4_455
Ga3 O1 Ga3 130.16(16) 2_565 4_455
Ga3 O1 Ga3 130.16(16) 1_556 4_455
Ga3 O1 Ga3 75.12(11) 4_456 4_455
O2 O1 Ga3 100.9(3) 4 4_455
O2 O1 Ga3 133.6(5) 3_455 4_455
O2 O1 Ga3 62.3(3) 1_565 4_455
O3 O1 Ga3 101.0(4) . 4_455
O3 O1 Ga3 32.9(2) 3_565 4_455
O3 O1 Ga3 66.1(3) 4_455 4_455
Ga3 O1 Ga3 72.3(2) 2_564 4_455
Ga3 O1 Ga3 72.3(2) . 4_455
Ga2 O1 O2 81.8(3) 2_566 .
La O1 O2 28.9(2) . .
La O1 O2 114.0(2) 2_565 .
La O1 O2 127.9(2) 4_455 .
O2 O1 O2 80.9(6) 6 .
O2 O1 O2 80.5(4) 5_455 .
O2 O1 O2 132.7(5) 2_565 .
O3 O1 O2 33.5(3) 6 .
O3 O1 O2 149.9(4) 2_565 .
O3 O1 O2 85.4(4) 5_455 .
O2 O1 O2 67.9(4) 6_556 .
O2 O1 O2 67.5(5) 5_456 .
O2 O1 O2 113.1(5) 2_566 .
Ga2 O1 O2 98.3(3) 2_565 .
Ga3 O1 O2 57.1(2) 2_565 .
Ga3 O1 O2 62.3(2) 1_556 .
Ga3 O1 O2 143.6(5) 4_456 .
O2 O1 O2 81.3(5) 4 .
O2 O1 O2 36.9(5) 3_455 .
O2 O1 O2 150.5(6) 1_565 .
O3 O1 O2 42.5(3) . .
O3 O1 O2 138.7(3) 3_565 .
O3 O1 O2 101.1(2) 4_455 .
Ga3 O1 O2 74.8(2) 2_564 .
Ga3 O1 O2 78.4(2) . .
Ga3 O1 O2 141.1(4) 4_455 .
Ga2 O1 O2 81.7(3) 2_566 3_565
La O1 O2 127.9(2) . 3_565
La O1 O2 28.9(2) 2_565 3_565
La O1 O2 114.0(2) 4_455 3_565
O2 O1 O2 80.5(4) 6 3_565
O2 O1 O2 132.7(5) 5_455 3_565
O2 O1 O2 80.9(6) 2_565 3_565
O3 O1 O2 85.4(4) 6 3_565
O3 O1 O2 33.5(3) 2_565 3_565
O3 O1 O2 149.9(4) 5_455 3_565
O2 O1 O2 67.5(5) 6_556 3_565
O2 O1 O2 113.1(5) 5_456 3_565
O2 O1 O2 67.9(4) 2_566 3_565
Ga2 O1 O2 98.3(3) 2_565 3_565
Ga3 O1 O2 62.3(2) 2_565 3_565
Ga3 O1 O2 143.6(5) 1_556 3_565
Ga3 O1 O2 57.1(2) 4_456 3_565
O2 O1 O2 36.9(5) 4 3_565
O2 O1 O2 150.5(6) 3_455 3_565
O2 O1 O2 81.3(5) 1_565 3_565
O3 O1 O2 101.1(2) . 3_565
O3 O1 O2 42.5(3) 3_565 3_565
O3 O1 O2 138.7(3) 4_455 3_565
Ga3 O1 O2 78.4(2) 2_564 3_565
Ga3 O1 O2 141.1(4) . 3_565
Ga3 O1 O2 74.8(2) 4_455 3_565
O2 O1 O2 117.98(14) . 3_565
Ga2 O1 O2 81.7(3) 2_566 4_455
La O1 O2 114.0(2) . 4_455
La O1 O2 127.9(2) 2_565 4_455
La O1 O2 28.9(2) 4_455 4_455
O2 O1 O2 132.7(5) 6 4_455
O2 O1 O2 80.9(6) 5_455 4_455
O2 O1 O2 80.5(4) 2_565 4_455
O3 O1 O2 149.9(4) 6 4_455
O3 O1 O2 85.4(4) 2_565 4_455
O3 O1 O2 33.5(3) 5_455 4_455
O2 O1 O2 113.1(5) 6_556 4_455
O2 O1 O2 67.9(4) 5_456 4_455
O2 O1 O2 67.5(5) 2_566 4_455
Ga2 O1 O2 98.3(3) 2_565 4_455
Ga3 O1 O2 143.6(5) 2_565 4_455
Ga3 O1 O2 57.1(2) 1_556 4_455
Ga3 O1 O2 62.3(2) 4_456 4_455
O2 O1 O2 150.5(6) 4 4_455
O2 O1 O2 81.3(5) 3_455 4_455
O2 O1 O2 36.9(5) 1_565 4_455
O3 O1 O2 138.7(3) . 4_455
O3 O1 O2 101.1(2) 3_565 4_455
O3 O1 O2 42.5(3) 4_455 4_455
Ga3 O1 O2 141.1(4) 2_564 4_455
Ga3 O1 O2 74.8(2) . 4_455
Ga3 O1 O2 78.4(2) 4_455 4_455
O2 O1 O2 117.98(14) . 4_455
O2 O1 O2 117.98(14) 3_565 4_455
Ga2 O1 Nb 100.4(2) 2_566 .
La O1 Nb 46.32(5) . .
La O1 Nb 70.48(10) 2_565 .
La O1 Nb 147.3(6) 4_455 .
O2 O1 Nb 47.9(4) 6 .
O2 O1 Nb 86.6(4) 5_455 .
O2 O1 Nb 106.3(5) 2_565 .
O3 O1 Nb 18.0(3) 6 .
O3 O1 Nb 114.7(3) 2_565 .
O3 O1 Nb 126.5(3) 5_455 .
O2 O1 Nb 71.1(3) 6_556 .
O2 O1 Nb 103.7(4) 5_456 .
O2 O1 Nb 123.4(4) 2_566 .
Ga2 O1 Nb 79.6(2) 2_565 .
Ga3 O1 Nb 41.97(4) 2_565 .
Ga3 O1 Nb 106.04(9) 1_556 .
Ga3 O1 Nb 136.28(18) 4_456 .
O2 O1 Nb 47.7(3) 4 .
O2 O1 Nb 79.5(3) 3_455 .
O2 O1 Nb 163.2(3) 1_565 .
O3 O1 Nb 24.80(16) . .
O3 O1 Nb 95.4(2) 3_565 .
O3 O1 Nb 123.6(4) 4_455 .
Ga3 O1 Nb 39.43(7) 2_564 .
Ga3 O1 Nb 90.9(2) . .
Ga3 O1 Nb 111.1(3) 4_455 .
O2 O1 Nb 43.74(19) . .
O2 O1 Nb 82.03(19) 3_565 .
O2 O1 Nb 159.9(2) 4_455 .
Ga2 O1 Ga1 100.4(2) 2_566 .
La O1 Ga1 46.32(5) . .
La O1 Ga1 70.48(10) 2_565 .
La O1 Ga1 147.3(6) 4_455 .
O2 O1 Ga1 47.9(4) 6 .
O2 O1 Ga1 86.6(4) 5_455 .
O2 O1 Ga1 106.3(5) 2_565 .
O3 O1 Ga1 18.0(3) 6 .
O3 O1 Ga1 114.7(3) 2_565 .
O3 O1 Ga1 126.5(3) 5_455 .
O2 O1 Ga1 71.1(3) 6_556 .
O2 O1 Ga1 103.7(4) 5_456 .
O2 O1 Ga1 123.4(4) 2_566 .
Ga2 O1 Ga1 79.6(2) 2_565 .
Ga3 O1 Ga1 41.97(4) 2_565 .
Ga3 O1 Ga1 106.04(9) 1_556 .
Ga3 O1 Ga1 136.28(18) 4_456 .
O2 O1 Ga1 47.7(3) 4 .
O2 O1 Ga1 79.5(3) 3_455 .
O2 O1 Ga1 163.2(3) 1_565 .
O3 O1 Ga1 24.80(16) . .
O3 O1 Ga1 95.4(2) 3_565 .
O3 O1 Ga1 123.6(4) 4_455 .
Ga3 O1 Ga1 39.43(7) 2_564 .
Ga3 O1 Ga1 90.9(2) . .
Ga3 O1 Ga1 111.1(3) 4_455 .
O2 O1 Ga1 43.74(19) . .
O2 O1 Ga1 82.03(19) 3_565 .
O2 O1 Ga1 159.9(2) 4_455 .
Nb O1 Ga1 0.0 . .
Ga2 O1 Ga1 100.4(2) 2_566 1_455
La O1 Ga1 70.48(10) . 1_455
La O1 Ga1 147.3(6) 2_565 1_455
La O1 Ga1 46.32(5) 4_455 1_455
O2 O1 Ga1 106.3(5) 6 1_455
O2 O1 Ga1 47.9(4) 5_455 1_455
O2 O1 Ga1 86.6(4) 2_565 1_455
O3 O1 Ga1 114.7(3) 6 1_455
O3 O1 Ga1 126.5(3) 2_565 1_455
O3 O1 Ga1 18.0(3) 5_455 1_455
O2 O1 Ga1 123.4(4) 6_556 1_455
O2 O1 Ga1 71.1(3) 5_456 1_455
O2 O1 Ga1 103.7(4) 2_566 1_455
Ga2 O1 Ga1 79.6(2) 2_565 1_455
Ga3 O1 Ga1 136.28(18) 2_565 1_455
Ga3 O1 Ga1 41.97(4) 1_556 1_455
Ga3 O1 Ga1 106.04(9) 4_456 1_455
O2 O1 Ga1 163.2(3) 4 1_455
O2 O1 Ga1 47.7(3) 3_455 1_455
O2 O1 Ga1 79.5(3) 1_565 1_455
O3 O1 Ga1 95.4(2) . 1_455
O3 O1 Ga1 123.6(4) 3_565 1_455
O3 O1 Ga1 24.80(16) 4_455 1_455
Ga3 O1 Ga1 111.1(3) 2_564 1_455
Ga3 O1 Ga1 39.43(7) . 1_455
Ga3 O1 Ga1 90.9(2) 4_455 1_455
O2 O1 Ga1 82.03(19) . 1_455
O2 O1 Ga1 159.9(2) 3_565 1_455
O2 O1 Ga1 43.74(19) 4_455 1_455
Nb O1 Ga1 116.80(13) . 1_455
Ga1 O1 Ga1 116.80(13) . 1_455
Ga2 O1 Nb 100.4(2) 2_566 1_455
La O1 Nb 70.48(10) . 1_455
La O1 Nb 147.3(6) 2_565 1_455
La O1 Nb 46.32(5) 4_455 1_455
O2 O1 Nb 106.3(5) 6 1_455
O2 O1 Nb 47.9(4) 5_455 1_455
O2 O1 Nb 86.6(4) 2_565 1_455
O3 O1 Nb 114.7(3) 6 1_455
O3 O1 Nb 126.5(3) 2_565 1_455
O3 O1 Nb 18.0(3) 5_455 1_455
O2 O1 Nb 123.4(4) 6_556 1_455
O2 O1 Nb 71.1(3) 5_456 1_455
O2 O1 Nb 103.7(4) 2_566 1_455
Ga2 O1 Nb 79.6(2) 2_565 1_455
Ga3 O1 Nb 136.28(18) 2_565 1_455
Ga3 O1 Nb 41.97(4) 1_556 1_455
Ga3 O1 Nb 106.04(9) 4_456 1_455
O2 O1 Nb 163.2(3) 4 1_455
O2 O1 Nb 47.7(3) 3_455 1_455
O2 O1 Nb 79.5(3) 1_565 1_455
O3 O1 Nb 95.4(2) . 1_455
O3 O1 Nb 123.6(4) 3_565 1_455
O3 O1 Nb 24.80(16) 4_455 1_455
Ga3 O1 Nb 111.1(3) 2_564 1_455
Ga3 O1 Nb 39.43(7) . 1_455
Ga3 O1 Nb 90.9(2) 4_455 1_455
O2 O1 Nb 82.03(19) . 1_455
O2 O1 Nb 159.9(2) 3_565 1_455
O2 O1 Nb 43.74(19) 4_455 1_455
Nb O1 Nb 116.80(13) . 1_455
Ga1 O1 Nb 116.80(13) . 1_455
Ga1 O1 Nb 0.0 1_455 1_455
Ga2 O1 Ga1 100.4(2) 2_566 1_565
La O1 Ga1 147.3(6) . 1_565
La O1 Ga1 46.32(5) 2_565 1_565
La O1 Ga1 70.47(10) 4_455 1_565
O2 O1 Ga1 86.6(4) 6 1_565
O2 O1 Ga1 106.3(5) 5_455 1_565
O2 O1 Ga1 47.9(4) 2_565 1_565
O3 O1 Ga1 126.5(3) 6 1_565
O3 O1 Ga1 18.0(3) 2_565 1_565
O3 O1 Ga1 114.7(3) 5_455 1_565
O2 O1 Ga1 103.7(4) 6_556 1_565
O2 O1 Ga1 123.4(4) 5_456 1_565
O2 O1 Ga1 71.1(3) 2_566 1_565
Ga2 O1 Ga1 79.6(2) 2_565 1_565
Ga3 O1 Ga1 106.04(9) 2_565 1_565
Ga3 O1 Ga1 136.28(18) 1_556 1_565
Ga3 O1 Ga1 41.97(4) 4_456 1_565
O2 O1 Ga1 79.5(3) 4 1_565
O2 O1 Ga1 163.2(3) 3_455 1_565
O2 O1 Ga1 47.7(3) 1_565 1_565
O3 O1 Ga1 123.6(4) . 1_565
O3 O1 Ga1 24.80(16) 3_565 1_565
O3 O1 Ga1 95.4(2) 4_455 1_565
Ga3 O1 Ga1 90.9(2) 2_564 1_565
Ga3 O1 Ga1 111.1(3) . 1_565
Ga3 O1 Ga1 39.43(7) 4_455 1_565
O2 O1 Ga1 159.9(2) . 1_565
O2 O1 Ga1 43.74(19) 3_565 1_565
O2 O1 Ga1 82.03(19) 4_455 1_565
Nb O1 Ga1 116.80(13) . 1_565
Ga1 O1 Ga1 116.80(13) . 1_565
Ga1 O1 Ga1 116.79(13) 1_455 1_565
Nb O1 Ga1 116.79(13) 1_455 1_565
Ga2 O1 Nb 100.4(2) 2_566 1_565
La O1 Nb 147.3(6) . 1_565
La O1 Nb 46.32(5) 2_565 1_565
La O1 Nb 70.47(10) 4_455 1_565
O2 O1 Nb 86.6(4) 6 1_565
O2 O1 Nb 106.3(5) 5_455 1_565
O2 O1 Nb 47.9(4) 2_565 1_565
O3 O1 Nb 126.5(3) 6 1_565
O3 O1 Nb 18.0(3) 2_565 1_565
O3 O1 Nb 114.7(3) 5_455 1_565
O2 O1 Nb 103.7(4) 6_556 1_565
O2 O1 Nb 123.4(4) 5_456 1_565
O2 O1 Nb 71.1(3) 2_566 1_565
Ga2 O1 Nb 79.6(2) 2_565 1_565
Ga3 O1 Nb 106.04(9) 2_565 1_565
Ga3 O1 Nb 136.28(18) 1_556 1_565
Ga3 O1 Nb 41.97(4) 4_456 1_565
O2 O1 Nb 79.5(3) 4 1_565
O2 O1 Nb 163.2(3) 3_455 1_565
O2 O1 Nb 47.7(3) 1_565 1_565
O3 O1 Nb 123.6(4) . 1_565
O3 O1 Nb 24.80(16) 3_565 1_565
O3 O1 Nb 95.4(2) 4_455 1_565
Ga3 O1 Nb 90.9(2) 2_564 1_565
Ga3 O1 Nb 111.1(3) . 1_565
Ga3 O1 Nb 39.43(7) 4_455 1_565
O2 O1 Nb 159.9(2) . 1_565
O2 O1 Nb 43.74(19) 3_565 1_565
O2 O1 Nb 82.03(19) 4_455 1_565
Nb O1 Nb 116.80(13) . 1_565
Ga1 O1 Nb 116.80(13) . 1_565
Ga1 O1 Nb 116.79(13) 1_455 1_565
Nb O1 Nb 116.79(13) 1_455 1_565
Ga1 O1 Nb 0.0 1_565 1_565
Ga2 O1 O3 51.4(2) 2_566 1_556
La O1 O3 64.4(3) . 1_556
La O1 O3 102.8(2) 2_565 1_556
La O1 O3 147.4(4) 4_455 1_556
O2 O1 O3 99.7(4) 6 1_556
O2 O1 O3 116.6(4) 5_455 1_556
O2 O1 O3 157.8(4) 2_565 1_556
O3 O1 O3 33.8(4) 6 1_556
O3 O1 O3 116.6(4) 2_565 1_556
O3 O1 O3 99.8(4) 5_455 1_556
O2 O1 O3 31.8(4) 6_556 1_556
O2 O1 O3 53.6(4) 5_456 1_556
O2 O1 O3 81.1(5) 2_566 1_556
Ga2 O1 O3 128.6(2) 2_565 1_556
Ga3 O1 O3 31.02(18) 2_565 1_556
Ga3 O1 O3 69.1(3) 1_556 1_556
Ga3 O1 O3 109.4(4) 4_456 1_556
O2 O1 O3 60.6(3) 4 1_556
O2 O1 O3 59.3(4) 3_455 1_556
O2 O1 O3 130.6(6) 1_565 1_556
O3 O1 O3 67.3(2) . 1_556
O3 O1 O3 129.96(12) 3_565 1_556
O3 O1 O3 129.96(12) 4_455 1_556
Ga3 O1 O3 91.22(14) 2_564 1_556
Ga3 O1 O3 114.08(16) . 1_556
Ga3 O1 O3 160.1(2) 4_455 1_556
O2 O1 O3 36.1(2) . 1_556
O2 O1 O3 91.2(3) 3_565 1_556
O2 O1 O3 121.2(4) 4_455 1_556
Nb O1 O3 51.79(15) . 1_556
Ga1 O1 O3 51.79(15) . 1_556
Ga1 O1 O3 105.9(2) 1_455 1_556
Nb O1 O3 105.9(2) 1_455 1_556
Ga1 O1 O3 133.1(3) 1_565 1_556
Nb O1 O3 133.1(3) 1_565 1_556
Ga2 O1 O3 51.4(2) 2_566 3_566
La O1 O3 147.4(4) . 3_566
La O1 O3 64.4(3) 2_565 3_566
La O1 O3 102.8(2) 4_455 3_566
O2 O1 O3 116.6(4) 6 3_566
O2 O1 O3 157.8(4) 5_455 3_566
O2 O1 O3 99.7(4) 2_565 3_566
O3 O1 O3 99.8(4) 6 3_566
O3 O1 O3 33.8(4) 2_565 3_566
O3 O1 O3 116.6(4) 5_455 3_566
O2 O1 O3 53.6(4) 6_556 3_566
O2 O1 O3 81.1(5) 5_456 3_566
O2 O1 O3 31.8(4) 2_566 3_566
Ga2 O1 O3 128.6(2) 2_565 3_566
Ga3 O1 O3 69.1(3) 2_565 3_566
Ga3 O1 O3 109.4(4) 1_556 3_566
Ga3 O1 O3 31.02(18) 4_456 3_566
O2 O1 O3 59.3(4) 4 3_566
O2 O1 O3 130.6(6) 3_455 3_566
O2 O1 O3 60.6(3) 1_565 3_566
O3 O1 O3 129.96(12) . 3_566
O3 O1 O3 67.3(2) 3_565 3_566
O3 O1 O3 129.96(12) 4_455 3_566
Ga3 O1 O3 114.08(16) 2_564 3_566
Ga3 O1 O3 160.1(2) . 3_566
Ga3 O1 O3 91.22(14) 4_455 3_566
O2 O1 O3 121.2(4) . 3_566
O2 O1 O3 36.1(2) 3_565 3_566
O2 O1 O3 91.2(3) 4_455 3_566
Nb O1 O3 105.9(2) . 3_566
Ga1 O1 O3 105.9(2) . 3_566
Ga1 O1 O3 133.1(3) 1_455 3_566
Nb O1 O3 133.1(3) 1_455 3_566
Ga1 O1 O3 51.79(15) 1_565 3_566
Nb O1 O3 51.79(15) 1_565 3_566
O3 O1 O3 85.2(3) 1_556 3_566
Ga2 O1 O3 51.4(2) 2_566 4_456
La O1 O3 102.8(2) . 4_456
La O1 O3 147.4(4) 2_565 4_456
La O1 O3 64.4(3) 4_455 4_456
O2 O1 O3 157.8(4) 6 4_456
O2 O1 O3 99.7(4) 5_455 4_456
O2 O1 O3 116.6(4) 2_565 4_456
O3 O1 O3 116.6(4) 6 4_456
O3 O1 O3 99.8(4) 2_565 4_456
O3 O1 O3 33.8(4) 5_455 4_456
O2 O1 O3 81.1(5) 6_556 4_456
O2 O1 O3 31.8(4) 5_456 4_456
O2 O1 O3 53.6(4) 2_566 4_456
Ga2 O1 O3 128.6(2) 2_565 4_456
Ga3 O1 O3 109.4(4) 2_565 4_456
Ga3 O1 O3 31.02(18) 1_556 4_456
Ga3 O1 O3 69.1(3) 4_456 4_456
O2 O1 O3 130.6(6) 4 4_456
O2 O1 O3 60.6(3) 3_455 4_456
O2 O1 O3 59.3(4) 1_565 4_456
O3 O1 O3 129.96(12) . 4_456
O3 O1 O3 129.96(12) 3_565 4_456
O3 O1 O3 67.3(2) 4_455 4_456
Ga3 O1 O3 160.1(2) 2_564 4_456
Ga3 O1 O3 91.22(14) . 4_456
Ga3 O1 O3 114.08(16) 4_455 4_456
O2 O1 O3 91.2(3) . 4_456
O2 O1 O3 121.2(4) 3_565 4_456
O2 O1 O3 36.1(2) 4_455 4_456
Nb O1 O3 133.1(3) . 4_456
Ga1 O1 O3 133.1(3) . 4_456
Ga1 O1 O3 51.79(15) 1_455 4_456
Nb O1 O3 51.79(15) 1_455 4_456
Ga1 O1 O3 105.9(2) 1_565 4_456
Nb O1 O3 105.9(2) 1_565 4_456
O3 O1 O3 85.2(3) 1_556 4_456
O3 O1 O3 85.2(3) 3_566 4_456
Ga2 O1 La 29.41(11) 2_566 1_556
La O1 La 80.3(3) . 1_556
La O1 La 121.7(4) 2_565 1_556
La O1 La 121.7(4) 4_455 1_556
O2 O1 La 127.8(4) 6 1_556
O2 O1 La 123.2(3) 5_455 1_556
O2 O1 La 173.5(4) 2_565 1_556
O3 O1 La 62.2(3) 6 1_556
O3 O1 La 111.3(5) 2_565 1_556
O3 O1 La 78.9(3) 5_455 1_556
O2 O1 La 32.8(3) 6_556 1_556
O2 O1 La 25.7(4) 5_456 1_556
O2 O1 La 60.6(4) 2_566 1_556
Ga2 O1 La 150.59(11) 2_565 1_556
Ga3 O1 La 53.4(2) 2_565 1_556
Ga3 O1 La 49.09(19) 1_556 1_556
Ga3 O1 La 91.3(4) 4_456 1_556
O2 O1 La 80.6(3) 4 1_556
O2 O1 La 54.4(4) 3_455 1_556
O2 O1 La 104.7(5) 1_565 1_556
O3 O1 La 92.4(2) . 1_556
O3 O1 La 142.0(4) 3_565 1_556
O3 O1 La 115.1(2) 4_455 1_556
Ga3 O1 La 119.56(6) 2_564 1_556
Ga3 O1 La 116.65(6) . 1_556
Ga3 O1 La 166.2(3) 4_455 1_556
O2 O1 La 52.6(2) . 1_556
O2 O1 La 99.8(3) 3_565 1_556
O2 O1 La 93.5(3) 4_455 1_556
Nb O1 La 80.18(13) . 1_556
Ga1 O1 La 80.18(13) . 1_556
Ga1 O1 La 90.88(16) 1_455 1_556
Nb O1 La 90.88(16) 1_455 1_556
Ga1 O1 La 128.9(3) 1_565 1_556
Nb O1 La 128.9(3) 1_565 1_556
O3 O1 La 28.57(16) 1_556 1_556
O3 O1 La 77.7(3) 3_566 1_556
O3 O1 La 57.5(2) 4_456 1_556
Ga2 O1 La 29.41(11) 2_566 2_566
La O1 La 121.7(4) . 2_566
La O1 La 80.3(3) 2_565 2_566
La O1 La 121.7(4) 4_455 2_566
O2 O1 La 123.2(3) 6 2_566
O2 O1 La 173.5(4) 5_455 2_566
O2 O1 La 127.8(4) 2_565 2_566
O3 O1 La 78.9(3) 6 2_566
O3 O1 La 62.2(3) 2_565 2_566
O3 O1 La 111.3(5) 5_455 2_566
O2 O1 La 25.7(4) 6_556 2_566
O2 O1 La 60.6(4) 5_456 2_566
O2 O1 La 32.8(3) 2_566 2_566
Ga2 O1 La 150.59(11) 2_565 2_566
Ga3 O1 La 49.09(19) 2_565 2_566
Ga3 O1 La 91.3(4) 1_556 2_566
Ga3 O1 La 53.4(2) 4_456 2_566
O2 O1 La 54.4(4) 4 2_566
O2 O1 La 104.7(5) 3_455 2_566
O2 O1 La 80.6(3) 1_565 2_566
O3 O1 La 115.1(2) . 2_566
O3 O1 La 92.4(2) 3_565 2_566
O3 O1 La 142.0(4) 4_455 2_566
Ga3 O1 La 116.65(6) 2_564 2_566
Ga3 O1 La 166.2(3) . 2_566
Ga3 O1 La 119.56(6) 4_455 2_566
O2 O1 La 93.5(3) . 2_566
O2 O1 La 52.6(2) 3_565 2_566
O2 O1 La 99.8(3) 4_455 2_566
Nb O1 La 90.88(16) . 2_566
Ga1 O1 La 90.88(16) . 2_566
Ga1 O1 La 128.9(3) 1_455 2_566
Nb O1 La 128.9(3) 1_455 2_566
Ga1 O1 La 80.18(13) 1_565 2_566
Nb O1 La 80.18(13) 1_565 2_566
O3 O1 La 57.5(2) 1_556 2_566
O3 O1 La 28.57(16) 3_566 2_566
O3 O1 La 77.7(3) 4_456 2_566
La O1 La 50.33(18) 1_556 2_566
Ga2 O1 La 29.40(11) 2_566 4_456
La O1 La 121.7(4) . 4_456
La O1 La 121.7(4) 2_565 4_456
La O1 La 80.3(3) 4_455 4_456
O2 O1 La 173.5(4) 6 4_456
O2 O1 La 127.8(4) 5_455 4_456
O2 O1 La 123.2(3) 2_565 4_456
O3 O1 La 111.3(5) 6 4_456
O3 O1 La 78.9(3) 2_565 4_456
O3 O1 La 62.2(3) 5_455 4_456
O2 O1 La 60.6(4) 6_556 4_456
O2 O1 La 32.8(3) 5_456 4_456
O2 O1 La 25.7(4) 2_566 4_456
Ga2 O1 La 150.59(11) 2_565 4_456
Ga3 O1 La 91.3(4) 2_565 4_456
Ga3 O1 La 53.4(2) 1_556 4_456
Ga3 O1 La 49.09(19) 4_456 4_456
O2 O1 La 104.7(5) 4 4_456
O2 O1 La 80.6(3) 3_455 4_456
O2 O1 La 54.4(4) 1_565 4_456
O3 O1 La 142.0(4) . 4_456
O3 O1 La 115.1(2) 3_565 4_456
O3 O1 La 92.4(2) 4_455 4_456
Ga3 O1 La 166.2(3) 2_564 4_456
Ga3 O1 La 119.56(6) . 4_456
Ga3 O1 La 116.65(6) 4_455 4_456
O2 O1 La 99.8(3) . 4_456
O2 O1 La 93.5(3) 3_565 4_456
O2 O1 La 52.6(2) 4_455 4_456
Nb O1 La 128.9(3) . 4_456
Ga1 O1 La 128.9(3) . 4_456
Ga1 O1 La 80.18(13) 1_455 4_456
Nb O1 La 80.18(13) 1_455 4_456
Ga1 O1 La 90.88(16) 1_565 4_456
Nb O1 La 90.88(16) 1_565 4_456
O3 O1 La 77.7(3) 1_556 4_456
O3 O1 La 57.5(2) 3_566 4_456
O3 O1 La 28.57(16) 4_456 4_456
La O1 La 50.33(18) 1_556 4_456
La O1 La 50.33(18) 2_566 4_456
Ga2 O1 Ga2 71.1(2) 2_566 .
La O1 Ga2 40.64(18) . .
La O1 Ga2 135.64(3) 2_565 .
La O1 Ga2 111.84(5) 4_455 .
O2 O1 Ga2 100.4(4) 6 .
O2 O1 Ga2 81.5(3) 5_455 .
O2 O1 Ga2 140.2(5) 2_565 .
O3 O1 Ga2 53.9(3) 6 .
O3 O1 Ga2 153.9(5) 2_565 .
O3 O1 Ga2 65.2(3) 5_455 .
O2 O1 Ga2 69.1(4) 6_556 .
O2 O1 Ga2 48.9(4) 5_456 .
O2 O1 Ga2 100.6(5) 2_566 .
Ga2 O1 Ga2 108.9(2) 2_565 .
Ga3 O1 Ga2 70.36(13) 2_565 .
Ga3 O1 Ga2 40.04(6) 1_556 .
Ga3 O1 Ga2 130.2(4) 4_456 .
O2 O1 Ga2 98.4(3) 4 .
O2 O1 Ga2 18.4(3) 3_455 .
O2 O1 Ga2 128.3(4) 1_565 .
O3 O1 Ga2 62.6(2) . .
O3 O1 Ga2 160.9(3) 3_565 .
O3 O1 Ga2 88.96(16) 4_455 .
Ga3 O1 Ga2 95.45(9) 2_564 .
Ga3 O1 Ga2 76.31(6) . .
Ga3 O1 Ga2 148.5(3) 4_455 .
O2 O1 Ga2 22.35(19) . .
O2 O1 Ga2 132.3(3) 3_565 .
O2 O1 Ga2 96.4(2) 4_455 .
Nb O1 Ga2 66.01(3) . .
Ga1 O1 Ga2 66.01(3) . .
Ga1 O1 Ga2 66.01(3) 1_455 .
Nb O1 Ga2 66.01(3) 1_455 .
Ga1 O1 Ga2 171.5(4) 1_565 .
Nb O1 Ga2 171.5(4) 1_565 .
O3 O1 Ga2 41.32(18) 1_556 .
O3 O1 Ga2 120.1(4) 3_566 .
O3 O1 Ga2 69.1(2) 4_456 .
La O1 Ga2 42.70(10) 1_556 .
La O1 Ga2 91.9(3) 2_566 .
La O1 Ga2 81.7(2) 4_456 .
Ga2 O1 Ga2 71.1(2) 2_566 1_665
La O1 Ga2 111.84(5) . 1_665
La O1 Ga2 40.64(18) 2_565 1_665
La O1 Ga2 135.64(3) 4_455 1_665
O2 O1 Ga2 81.5(3) 6 1_665
O2 O1 Ga2 140.2(5) 5_455 1_665
O2 O1 Ga2 100.4(4) 2_565 1_665
O3 O1 Ga2 65.2(3) 6 1_665
O3 O1 Ga2 53.9(3) 2_565 1_665
O3 O1 Ga2 153.9(5) 5_455 1_665
O2 O1 Ga2 48.9(4) 6_556 1_665
O2 O1 Ga2 100.6(5) 5_456 1_665
O2 O1 Ga2 69.1(4) 2_566 1_665
Ga2 O1 Ga2 108.9(2) 2_565 1_665
Ga3 O1 Ga2 40.03(6) 2_565 1_665
Ga3 O1 Ga2 130.2(4) 1_556 1_665
Ga3 O1 Ga2 70.36(13) 4_456 1_665
O2 O1 Ga2 18.4(3) 4 1_665
O2 O1 Ga2 128.3(4) 3_455 1_665
O2 O1 Ga2 98.4(3) 1_565 1_665
O3 O1 Ga2 88.96(16) . 1_665
O3 O1 Ga2 62.6(2) 3_565 1_665
O3 O1 Ga2 160.9(3) 4_455 1_665
Ga3 O1 Ga2 76.31(6) 2_564 1_665
Ga3 O1 Ga2 148.5(3) . 1_665
Ga3 O1 Ga2 95.45(9) 4_455 1_665
O2 O1 Ga2 96.4(2) . 1_665
O2 O1 Ga2 22.4(2) 3_565 1_665
O2 O1 Ga2 132.3(3) 4_455 1_665
Nb O1 Ga2 66.01(3) . 1_665
Ga1 O1 Ga2 66.01(3) . 1_665
Ga1 O1 Ga2 171.5(4) 1_455 1_665
Nb O1 Ga2 171.5(4) 1_455 1_665
Ga1 O1 Ga2 66.01(3) 1_565 1_665
Nb O1 Ga2 66.01(3) 1_565 1_665
O3 O1 Ga2 69.1(2) 1_556 1_665
O3 O1 Ga2 41.32(18) 3_566 1_665
O3 O1 Ga2 120.1(4) 4_456 1_665
La O1 Ga2 81.7(2) 1_556 1_665
La O1 Ga2 42.70(10) 2_566 1_665
La O1 Ga2 91.9(3) 4_456 1_665
Ga2 O1 Ga2 110.05(19) . 1_665
Ga2 O1 Ga2 71.1(2) 2_566 1_565
La O1 Ga2 135.64(3) . 1_565
La O1 Ga2 111.84(5) 2_565 1_565
La O1 Ga2 40.64(18) 4_455 1_565
O2 O1 Ga2 140.2(5) 6 1_565
O2 O1 Ga2 100.4(4) 5_455 1_565
O2 O1 Ga2 81.5(3) 2_565 1_565
O3 O1 Ga2 153.9(5) 6 1_565
O3 O1 Ga2 65.2(3) 2_565 1_565
O3 O1 Ga2 53.9(3) 5_455 1_565
O2 O1 Ga2 100.6(5) 6_556 1_565
O2 O1 Ga2 69.1(4) 5_456 1_565
O2 O1 Ga2 48.9(4) 2_566 1_565
Ga2 O1 Ga2 108.9(2) 2_565 1_565
Ga3 O1 Ga2 130.2(4) 2_565 1_565
Ga3 O1 Ga2 70.36(13) 1_556 1_565
Ga3 O1 Ga2 40.03(6) 4_456 1_565
O2 O1 Ga2 128.3(4) 4 1_565
O2 O1 Ga2 98.4(3) 3_455 1_565
O2 O1 Ga2 18.4(3) 1_565 1_565
O3 O1 Ga2 160.9(3) . 1_565
O3 O1 Ga2 88.96(16) 3_565 1_565
O3 O1 Ga2 62.6(2) 4_455 1_565
Ga3 O1 Ga2 148.5(3) 2_564 1_565
Ga3 O1 Ga2 95.45(9) . 1_565
Ga3 O1 Ga2 76.31(6) 4_455 1_565
O2 O1 Ga2 132.3(3) . 1_565
O2 O1 Ga2 96.4(2) 3_565 1_565
O2 O1 Ga2 22.4(2) 4_455 1_565
Nb O1 Ga2 171.5(4) . 1_565
Ga1 O1 Ga2 171.5(4) . 1_565
Ga1 O1 Ga2 66.01(3) 1_455 1_565
Nb O1 Ga2 66.01(3) 1_455 1_565
Ga1 O1 Ga2 66.01(3) 1_565 1_565
Nb O1 Ga2 66.01(3) 1_565 1_565
O3 O1 Ga2 120.1(4) 1_556 1_565
O3 O1 Ga2 69.1(2) 3_566 1_565
O3 O1 Ga2 41.32(18) 4_456 1_565
La O1 Ga2 91.9(3) 1_556 1_565
La O1 Ga2 81.7(2) 2_566 1_565
La O1 Ga2 42.70(10) 4_456 1_565
Ga2 O1 Ga2 110.05(19) . 1_565
Ga2 O1 Ga2 110.05(19) 1_665 1_565
Ga2 O1 O1 110.2(4) 2_566 2_455
La O1 O1 12.08(4) . 2_455
La O1 O1 118.9(5) 2_565 2_455
La O1 O1 98.3(3) 4_455 2_455
O2 O1 O1 68.2(5) 6 2_455
O2 O1 O1 45.9(4) 5_455 2_455
O2 O1 O1 102.2(6) 2_565 2_455
O3 O1 O1 59.4(2) 6 2_455
O3 O1 O1 165.1(7) 2_565 2_455
O3 O1 O1 70.1(3) 5_455 2_455
O2 O1 O1 102.5(4) 6_556 2_455
O2 O1 O1 85.3(4) 5_456 2_455
O2 O1 O1 138.7(6) 2_566 2_455
Ga2 O1 O1 69.8(4) 2_565 2_455
Ga3 O1 O1 88.87(10) 2_565 2_455
Ga3 O1 O1 63.53(11) 1_556 2_455
Ga3 O1 O1 162.4(3) 4_456 2_455
O2 O1 O1 105.7(3) 4 2_455
O2 O1 O1 35.3(3) 3_455 2_455
O2 O1 O1 137.7(3) 1_565 2_455
O3 O1 O1 39.0(2) . 2_455
O3 O1 O1 128.1(6) 3_565 2_455
O3 O1 O1 70.3(3) 4_455 2_455
Ga3 O1 O1 66.8(3) 2_564 2_455
Ga3 O1 O1 43.7(2) . 2_455
Ga3 O1 O1 110.9(5) 4_455 2_455
O2 O1 O1 34.8(2) . 2_455
O2 O1 O1 139.8(2) 3_565 2_455
O2 O1 O1 101.9(2) 4_455 2_455
Nb O1 O1 58.40(7) . 2_455
Ga1 O1 O1 58.40(7) . 2_455
Ga1 O1 O1 58.40(7) 1_455 2_455
Nb O1 O1 58.40(7) 1_455 2_455
Ga1 O1 O1 149.3(6) 1_565 2_455
Nb O1 O1 149.3(6) 1_565 2_455
O3 O1 O1 70.8(3) 1_556 2_455
O3 O1 O1 156.0(5) 3_566 2_455
O3 O1 O1 93.6(2) 4_456 2_455
La O1 O1 81.5(3) 1_556 2_455
La O1 O1 127.9(4) 2_566 2_455
La O1 O1 115.9(3) 4_456 2_455
Ga2 O1 O1 39.1(2) . 2_455
Ga2 O1 O1 123.77(3) 1_665 2_455
Ga2 O1 O1 123.77(3) 1_565 2_455
Ga2 O1 O1 110.2(4) 2_566 2_565
La O1 O1 98.3(3) . 2_565
La O1 O1 12.08(4) 2_565 2_565
La O1 O1 118.9(5) 4_455 2_565
O2 O1 O1 45.9(4) 6 2_565
O2 O1 O1 102.2(6) 5_455 2_565
O2 O1 O1 68.2(5) 2_565 2_565
O3 O1 O1 70.1(3) 6 2_565
O3 O1 O1 59.4(2) 2_565 2_565
O3 O1 O1 165.1(7) 5_455 2_565
O2 O1 O1 85.3(4) 6_556 2_565
O2 O1 O1 138.7(6) 5_456 2_565
O2 O1 O1 102.5(4) 2_566 2_565
Ga2 O1 O1 69.8(4) 2_565 2_565
Ga3 O1 O1 63.53(11) 2_565 2_565
Ga3 O1 O1 162.4(3) 1_556 2_565
Ga3 O1 O1 88.87(10) 4_456 2_565
O2 O1 O1 35.3(3) 4 2_565
O2 O1 O1 137.7(3) 3_455 2_565
O2 O1 O1 105.7(3) 1_565 2_565
O3 O1 O1 70.3(3) . 2_565
O3 O1 O1 39.0(2) 3_565 2_565
O3 O1 O1 128.1(6) 4_455 2_565
Ga3 O1 O1 43.7(2) 2_564 2_565
Ga3 O1 O1 110.9(5) . 2_565
Ga3 O1 O1 66.8(3) 4_455 2_565
O2 O1 O1 101.9(2) . 2_565
O2 O1 O1 34.8(2) 3_565 2_565
O2 O1 O1 139.8(2) 4_455 2_565
Nb O1 O1 58.40(7) . 2_565
Ga1 O1 O1 58.40(7) . 2_565
Ga1 O1 O1 149.3(6) 1_455 2_565
Nb O1 O1 149.3(6) 1_455 2_565
Ga1 O1 O1 58.40(6) 1_565 2_565
Nb O1 O1 58.40(6) 1_565 2_565
O3 O1 O1 93.6(2) 1_556 2_565
O3 O1 O1 70.8(3) 3_566 2_565
O3 O1 O1 156.0(5) 4_456 2_565
La O1 O1 115.9(3) 1_556 2_565
La O1 O1 81.5(3) 2_566 2_565
La O1 O1 127.9(4) 4_456 2_565
Ga2 O1 O1 123.77(3) . 2_565
Ga2 O1 O1 39.1(2) 1_665 2_565
Ga2 O1 O1 123.77(3) 1_565 2_565
O1 O1 O1 108.7(4) 2_455 2_565
Ga2 O1 O1 110.2(4) 2_566 2_465
La O1 O1 118.9(5) . 2_465
La O1 O1 98.3(3) 2_565 2_465
La O1 O1 12.08(4) 4_455 2_465
O2 O1 O1 102.2(6) 6 2_465
O2 O1 O1 68.2(5) 5_455 2_465
O2 O1 O1 45.9(4) 2_565 2_465
O3 O1 O1 165.1(7) 6 2_465
O3 O1 O1 70.1(3) 2_565 2_465
O3 O1 O1 59.4(2) 5_455 2_465
O2 O1 O1 138.7(6) 6_556 2_465
O2 O1 O1 102.5(4) 5_456 2_465
O2 O1 O1 85.3(4) 2_566 2_465
Ga2 O1 O1 69.8(4) 2_565 2_465
Ga3 O1 O1 162.4(3) 2_565 2_465
Ga3 O1 O1 88.87(10) 1_556 2_465
Ga3 O1 O1 63.53(11) 4_456 2_465
O2 O1 O1 137.7(3) 4 2_465
O2 O1 O1 105.7(3) 3_455 2_465
O2 O1 O1 35.3(3) 1_565 2_465
O3 O1 O1 128.1(6) . 2_465
O3 O1 O1 70.3(3) 3_565 2_465
O3 O1 O1 39.0(2) 4_455 2_465
Ga3 O1 O1 110.9(5) 2_564 2_465
Ga3 O1 O1 66.8(3) . 2_465
Ga3 O1 O1 43.7(2) 4_455 2_465
O2 O1 O1 139.8(2) . 2_465
O2 O1 O1 101.9(2) 3_565 2_465
O2 O1 O1 34.8(2) 4_455 2_465
Nb O1 O1 149.3(6) . 2_465
Ga1 O1 O1 149.3(6) . 2_465
Ga1 O1 O1 58.40(7) 1_455 2_465
Nb O1 O1 58.40(7) 1_455 2_465
Ga1 O1 O1 58.40(7) 1_565 2_465
Nb O1 O1 58.40(7) 1_565 2_465
O3 O1 O1 156.0(5) 1_556 2_465
O3 O1 O1 93.6(2) 3_566 2_465
O3 O1 O1 70.8(3) 4_456 2_465
La O1 O1 127.9(4) 1_556 2_465
La O1 O1 115.9(3) 2_566 2_465
La O1 O1 81.5(3) 4_456 2_465
Ga2 O1 O1 123.77(3) . 2_465
Ga2 O1 O1 123.77(3) 1_665 2_465
Ga2 O1 O1 39.1(2) 1_565 2_465
O1 O1 O1 108.7(4) 2_455 2_465
O1 O1 O1 108.7(4) 2_565 2_465
Ga2 O1 O3 115.1(2) 2_566 4
La O1 O3 61.4(2) . 4
La O1 O3 49.11(19) 2_565 4
La O1 O3 134.7(6) 4_455 4
O2 O1 O3 30.5(3) 6 4
O2 O1 O3 84.2(5) 5_455 4
O2 O1 O3 85.1(5) 2_565 4
O3 O1 O3 40.3(4) 6 4
O3 O1 O3 96.6(3) 2_565 4
O3 O1 O3 142.3(4) 5_455 4
O2 O1 O3 83.8(3) 6_556 4
O2 O1 O3 126.2(4) 5_456 4
O2 O1 O3 127.2(4) 2_566 4
Ga2 O1 O3 64.9(2) 2_565 4
Ga3 O1 O3 53.18(15) 2_565 4
Ga3 O1 O3 128.90(14) 1_556 4
Ga3 O1 O3 124.69(14) 4_456 4
O2 O1 O3 42.4(4) 4 4
O2 O1 O3 100.7(3) 3_455 4
O2 O1 O3 142.4(4) 1_565 4
O3 O1 O3 33.6(3) . 4
O3 O1 O3 72.0(3) 3_565 4
O3 O1 O3 122.1(5) 4_455 4
Ga3 O1 O3 22.07(15) 2_564 4
Ga3 O1 O3 91.2(3) . 4
Ga3 O1 O3 88.6(3) 4_455 4
O2 O1 O3 66.7(3) . 4
O2 O1 O3 67.7(3) 3_565 4
O2 O1 O3 163.2(5) 4_455 4
Nb O1 O3 23.74(14) . 4
Ga1 O1 O3 23.74(14) . 4
Ga1 O1 O3 127.1(3) 1_455 4
Nb O1 O3 127.1(3) 1_455 4
Ga1 O1 O3 94.7(2) 1_565 4
Nb O1 O3 94.7(2) 1_565 4
O3 O1 O3 72.75(18) 1_556 4
O3 O1 O3 99.8(2) 3_566 4
O3 O1 O3 156.8(4) 4_456 4
La O1 O3 101.20(18) 1_556 4
La O1 O3 95.87(18) 2_566 4
La O1 O3 144.2(3) 4_456 4
Ga2 O1 O3 89.09(14) . 4
Ga2 O1 O3 58.89(14) 1_665 4
Ga2 O1 O3 160.73(19) 1_565 4
O1 O1 O3 72.6(2) 2_455 4
O1 O1 O3 37.36(18) 2_565 4
O1 O1 O3 130.8(6) 2_465 4
Ga2 O1 O3 115.1(2) 2_566 3_455
La O1 O3 49.11(19) . 3_455
La O1 O3 134.7(6) 2_565 3_455
La O1 O3 61.4(2) 4_455 3_455
O2 O1 O3 85.1(5) 6 3_455
O2 O1 O3 30.5(3) 5_455 3_455
O2 O1 O3 84.2(5) 2_565 3_455
O3 O1 O3 96.6(3) 6 3_455
O3 O1 O3 142.3(4) 2_565 3_455
O3 O1 O3 40.3(4) 5_455 3_455
O2 O1 O3 127.2(4) 6_556 3_455
O2 O1 O3 83.8(3) 5_456 3_455
O2 O1 O3 126.2(4) 2_566 3_455
Ga2 O1 O3 64.9(2) 2_565 3_455
Ga3 O1 O3 124.70(14) 2_565 3_455
Ga3 O1 O3 53.18(15) 1_556 3_455
Ga3 O1 O3 128.90(14) 4_456 3_455
O2 O1 O3 142.4(4) 4 3_455
O2 O1 O3 42.4(4) 3_455 3_455
O2 O1 O3 100.7(3) 1_565 3_455
O3 O1 O3 72.0(3) . 3_455
O3 O1 O3 122.1(5) 3_565 3_455
O3 O1 O3 33.6(3) 4_455 3_455
Ga3 O1 O3 88.6(3) 2_564 3_455
Ga3 O1 O3 22.07(15) . 3_455
Ga3 O1 O3 91.2(3) 4_455 3_455
O2 O1 O3 67.7(3) . 3_455
O2 O1 O3 163.2(5) 3_565 3_455
O2 O1 O3 66.7(3) 4_455 3_455
Nb O1 O3 94.7(2) . 3_455
Ga1 O1 O3 94.7(2) . 3_455
Ga1 O1 O3 23.74(14) 1_455 3_455
Nb O1 O3 23.74(14) 1_455 3_455
Ga1 O1 O3 127.1(3) 1_565 3_455
Nb O1 O3 127.1(3) 1_565 3_455
O3 O1 O3 99.8(2) 1_556 3_455
O3 O1 O3 156.8(4) 3_566 3_455
O3 O1 O3 72.75(18) 4_456 3_455
La O1 O3 95.87(18) 1_556 3_455
La O1 O3 144.2(3) 2_566 3_455
La O1 O3 101.20(18) 4_456 3_455
Ga2 O1 O3 58.89(14) . 3_455
Ga2 O1 O3 160.73(19) 1_665 3_455
Ga2 O1 O3 89.09(14) 1_565 3_455
O1 O1 O3 37.36(18) 2_455 3_455
O1 O1 O3 130.8(6) 2_565 3_455
O1 O1 O3 72.6(2) 2_465 3_455
O3 O1 O3 103.3(3) 4 3_455
Ga2 O1 O3 115.1(2) 2_566 1_565
La O1 O3 134.7(6) . 1_565
La O1 O3 61.4(2) 2_565 1_565
La O1 O3 49.11(19) 4_455 1_565
O2 O1 O3 84.2(5) 6 1_565
O2 O1 O3 85.1(5) 5_455 1_565
O2 O1 O3 30.5(3) 2_565 1_565
O3 O1 O3 142.3(4) 6 1_565
O3 O1 O3 40.3(4) 2_565 1_565
O3 O1 O3 96.6(3) 5_455 1_565
O2 O1 O3 126.2(4) 6_556 1_565
O2 O1 O3 127.2(4) 5_456 1_565
O2 O1 O3 83.8(3) 2_566 1_565
Ga2 O1 O3 64.9(2) 2_565 1_565
Ga3 O1 O3 128.90(14) 2_565 1_565
Ga3 O1 O3 124.69(14) 1_556 1_565
Ga3 O1 O3 53.18(15) 4_456 1_565
O2 O1 O3 100.7(3) 4 1_565
O2 O1 O3 142.4(4) 3_455 1_565
O2 O1 O3 42.4(4) 1_565 1_565
O3 O1 O3 122.1(5) . 1_565
O3 O1 O3 33.6(3) 3_565 1_565
O3 O1 O3 72.0(3) 4_455 1_565
Ga3 O1 O3 91.2(3) 2_564 1_565
Ga3 O1 O3 88.6(3) . 1_565
Ga3 O1 O3 22.07(15) 4_455 1_565
O2 O1 O3 163.2(5) . 1_565
O2 O1 O3 66.7(3) 3_565 1_565
O2 O1 O3 67.7(3) 4_455 1_565
Nb O1 O3 127.1(3) . 1_565
Ga1 O1 O3 127.1(3) . 1_565
Ga1 O1 O3 94.7(2) 1_455 1_565
Nb O1 O3 94.7(2) 1_455 1_565
Ga1 O1 O3 23.74(14) 1_565 1_565
Nb O1 O3 23.74(14) 1_565 1_565
O3 O1 O3 156.8(4) 1_556 1_565
O3 O1 O3 72.75(18) 3_566 1_565
O3 O1 O3 99.8(2) 4_456 1_565
La O1 O3 144.2(3) 1_556 1_565
La O1 O3 101.20(18) 2_566 1_565
La O1 O3 95.86(18) 4_456 1_565
Ga2 O1 O3 160.73(19) . 1_565
Ga2 O1 O3 89.09(14) 1_665 1_565
Ga2 O1 O3 58.89(14) 1_565 1_565
O1 O1 O3 130.8(6) 2_455 1_565
O1 O1 O3 72.6(2) 2_565 1_565
O1 O1 O3 37.36(18) 2_465 1_565
O3 O1 O3 103.3(3) 4 1_565
O3 O1 O3 103.3(3) 3_455 1_565
Ga2 O1 O1 0.0 2_566 1_556
La O1 O1 109.8(4) . 1_556
La O1 O1 109.8(4) 2_565 1_556
La O1 O1 109.8(4) 4_455 1_556
O2 O1 O1 145.5(3) 6 1_556
O2 O1 O1 145.5(3) 5_455 1_556
O2 O1 O1 145.5(3) 2_565 1_556
O3 O1 O1 83.5(4) 6 1_556
O3 O1 O1 83.5(4) 2_565 1_556
O3 O1 O1 83.5(4) 5_455 1_556
O2 O1 O1 31.3(3) 6_556 1_556
O2 O1 O1 31.3(3) 5_456 1_556
O2 O1 O1 31.3(3) 2_566 1_556
Ga2 O1 O1 179.999(1) 2_565 1_556
Ga3 O1 O1 61.9(3) 2_565 1_556
Ga3 O1 O1 61.9(3) 1_556 1_556
Ga3 O1 O1 61.9(3) 4_456 1_556
O2 O1 O1 79.2(4) 4 1_556
O2 O1 O1 79.2(4) 3_455 1_556
O2 O1 O1 79.2(4) 1_565 1_556
O3 O1 O1 118.7(3) . 1_556
O3 O1 O1 118.7(3) 3_565 1_556
O3 O1 O1 118.7(3) 4_455 1_556
Ga3 O1 O1 137.05(15) 2_564 1_556
Ga3 O1 O1 137.05(15) . 1_556
Ga3 O1 O1 137.05(15) 4_455 1_556
O2 O1 O1 81.7(3) . 1_556
O2 O1 O1 81.7(3) 3_565 1_556
O2 O1 O1 81.7(3) 4_455 1_556
Nb O1 O1 100.4(2) . 1_556
Ga1 O1 O1 100.4(2) . 1_556
Ga1 O1 O1 100.4(2) 1_455 1_556
Nb O1 O1 100.4(2) 1_455 1_556
Ga1 O1 O1 100.4(2) 1_565 1_556
Nb O1 O1 100.4(2) 1_565 1_556
O3 O1 O1 51.4(2) 1_556 1_556
O3 O1 O1 51.4(2) 3_566 1_556
O3 O1 O1 51.4(2) 4_456 1_556
La O1 O1 29.41(11) 1_556 1_556
La O1 O1 29.41(11) 2_566 1_556
La O1 O1 29.41(11) 4_456 1_556
Ga2 O1 O1 71.1(2) . 1_556
Ga2 O1 O1 71.1(2) 1_665 1_556
Ga2 O1 O1 71.1(2) 1_565 1_556
O1 O1 O1 110.2(4) 2_455 1_556
O1 O1 O1 110.2(4) 2_565 1_556
O1 O1 O1 110.2(4) 2_465 1_556
O3 O1 O1 115.1(2) 4 1_556
O3 O1 O1 115.1(2) 3_455 1_556
O3 O1 O1 115.1(2) 1_565 1_556
Ga2 O1 O1 180.0 2_566 1_554
La O1 O1 70.2(4) . 1_554
La O1 O1 70.2(4) 2_565 1_554
La O1 O1 70.2(4) 4_455 1_554
O2 O1 O1 34.5(3) 6 1_554
O2 O1 O1 34.5(3) 5_455 1_554
O2 O1 O1 34.5(3) 2_565 1_554
O3 O1 O1 96.5(4) 6 1_554
O3 O1 O1 96.5(4) 2_565 1_554
O3 O1 O1 96.5(4) 5_455 1_554
O2 O1 O1 148.7(3) 6_556 1_554
O2 O1 O1 148.7(3) 5_456 1_554
O2 O1 O1 148.7(3) 2_566 1_554
Ga2 O1 O1 0.0 2_565 1_554
Ga3 O1 O1 118.1(3) 2_565 1_554
Ga3 O1 O1 118.1(3) 1_556 1_554
Ga3 O1 O1 118.1(3) 4_456 1_554
O2 O1 O1 100.8(4) 4 1_554
O2 O1 O1 100.8(4) 3_455 1_554
O2 O1 O1 100.8(4) 1_565 1_554
O3 O1 O1 61.3(3) . 1_554
O3 O1 O1 61.3(3) 3_565 1_554
O3 O1 O1 61.3(3) 4_455 1_554
Ga3 O1 O1 42.95(15) 2_564 1_554
Ga3 O1 O1 42.95(15) . 1_554
Ga3 O1 O1 42.95(15) 4_455 1_554
O2 O1 O1 98.3(3) . 1_554
O2 O1 O1 98.3(3) 3_565 1_554
O2 O1 O1 98.3(3) 4_455 1_554
Nb O1 O1 79.6(2) . 1_554
Ga1 O1 O1 79.6(2) . 1_554
Ga1 O1 O1 79.6(2) 1_455 1_554
Nb O1 O1 79.6(2) 1_455 1_554
Ga1 O1 O1 79.6(2) 1_565 1_554
Nb O1 O1 79.6(2) 1_565 1_554
O3 O1 O1 128.6(2) 1_556 1_554
O3 O1 O1 128.6(2) 3_566 1_554
O3 O1 O1 128.6(2) 4_456 1_554
La O1 O1 150.59(10) 1_556 1_554
La O1 O1 150.59(11) 2_566 1_554
La O1 O1 150.59(10) 4_456 1_554
Ga2 O1 O1 108.9(2) . 1_554
Ga2 O1 O1 108.9(2) 1_665 1_554
Ga2 O1 O1 108.9(2) 1_565 1_554
O1 O1 O1 69.8(4) 2_455 1_554
O1 O1 O1 69.8(4) 2_565 1_554
O1 O1 O1 69.8(4) 2_465 1_554
O3 O1 O1 64.9(2) 4 1_554
O3 O1 O1 64.9(2) 3_455 1_554
O3 O1 O1 64.9(2) 1_565 1_554
O1 O1 O1 180.000(3) 1_556 1_554
Ga2 O1 Ga3 71.41(19) 2_566 4_446
La O1 Ga3 45.59(16) . 4_446
La O1 Ga3 100.56(6) 2_565 4_446
La O1 Ga3 147.11(3) 4_455 4_446
O2 O1 Ga3 82.5(4) 6 4_446
O2 O1 Ga3 98.3(3) 5_455 4_446
O2 O1 Ga3 140.8(4) 2_565 4_446
O3 O1 Ga3 19.7(3) 6 4_446
O3 O1 Ga3 129.9(3) 2_565 4_446
O3 O1 Ga3 101.0(3) 5_455 4_446
O2 O1 Ga3 50.6(3) 6_556 4_446
O2 O1 Ga3 67.6(4) 5_456 4_446
O2 O1 Ga3 101.4(4) 2_566 4_446
Ga2 O1 Ga3 108.59(19) 2_565 4_446
Ga3 O1 Ga3 37.13(7) 2_565 4_446
Ga3 O1 Ga3 73.44(14) 1_556 4_446
Ga3 O1 Ga3 129.2(4) 4_456 4_446
O2 O1 Ga3 63.0(3) 4 4_446
O2 O1 Ga3 53.6(3) 3_455 4_446
O2 O1 Ga3 150.2(6) 1_565 4_446
O3 O1 Ga3 47.4(2) . 4_446
O3 O1 Ga3 128.24(18) 3_565 4_446
O3 O1 Ga3 121.10(18) 4_455 4_446
Ga3 O1 Ga3 74.55(6) 2_564 4_446
Ga3 O1 Ga3 97.42(9) . 4_446
Ga3 O1 Ga3 146.9(3) 4_455 4_446
O2 O1 Ga3 20.08(19) . 4_446
O2 O1 Ga3 98.8(2) 3_565 4_446
O2 O1 Ga3 130.4(3) 4_455 4_446
Nb O1 Ga3 36.25(3) . 4_446
Ga1 O1 Ga3 36.25(3) . 4_446
Ga1 O1 Ga3 100.79(5) 1_455 4_446
Nb O1 Ga3 100.79(5) 1_455 4_446
Ga1 O1 Ga3 142.41(9) 1_565 4_446
Nb O1 Ga3 142.41(9) 1_565 4_446
O3 O1 Ga3 20.30(14) 1_556 4_446
O3 O1 Ga3 102.5(3) 3_566 4_446
O3 O1 Ga3 97.2(3) 4_456 4_446
La O1 Ga3 45.65(9) 1_556 4_446
La O1 Ga3 76.21(19) 2_566 4_446
La O1 Ga3 96.0(3) 4_456 4_446
Ga2 O1 Ga3 35.90(5) . 4_446
Ga2 O1 Ga3 76.83(11) 1_665 4_446
Ga2 O1 Ga3 136.7(3) 1_565 4_446
O1 O1 Ga3 53.79(14) 2_455 4_446
O1 O1 Ga3 89.23(7) 2_565 4_446
O1 O1 Ga3 159.19(4) 2_465 4_446
O3 O1 Ga3 59.62(14) 4 4_446
O3 O1 Ga3 87.74(14) 3_455 4_446
O3 O1 Ga3 161.87(19) 1_565 4_446
O1 O1 Ga3 71.41(19) 1_556 4_446
O1 O1 Ga3 108.59(19) 1_554 4_446
Ga2 O1 Ga3 71.41(19) 2_566 1_666
La O1 Ga3 147.11(3) . 1_666
La O1 Ga3 45.59(16) 2_565 1_666
La O1 Ga3 100.56(6) 4_455 1_666
O2 O1 Ga3 98.3(3) 6 1_666
O2 O1 Ga3 140.8(4) 5_455 1_666
O2 O1 Ga3 82.5(4) 2_565 1_666
O3 O1 Ga3 101.0(3) 6 1_666
O3 O1 Ga3 19.7(3) 2_565 1_666
O3 O1 Ga3 129.9(3) 5_455 1_666
O2 O1 Ga3 67.6(4) 6_556 1_666
O2 O1 Ga3 101.4(4) 5_456 1_666
O2 O1 Ga3 50.6(3) 2_566 1_666
Ga2 O1 Ga3 108.59(19) 2_565 1_666
Ga3 O1 Ga3 73.44(14) 2_565 1_666
Ga3 O1 Ga3 129.2(4) 1_556 1_666
Ga3 O1 Ga3 37.13(7) 4_456 1_666
O2 O1 Ga3 53.6(3) 4 1_666
O2 O1 Ga3 150.2(6) 3_455 1_666
O2 O1 Ga3 63.0(3) 1_565 1_666
O3 O1 Ga3 121.10(18) . 1_666
O3 O1 Ga3 47.4(2) 3_565 1_666
O3 O1 Ga3 128.23(18) 4_455 1_666
Ga3 O1 Ga3 97.42(9) 2_564 1_666
Ga3 O1 Ga3 146.9(3) . 1_666
Ga3 O1 Ga3 74.55(6) 4_455 1_666
O2 O1 Ga3 130.4(3) . 1_666
O2 O1 Ga3 20.08(19) 3_565 1_666
O2 O1 Ga3 98.8(2) 4_455 1_666
Nb O1 Ga3 100.79(5) . 1_666
Ga1 O1 Ga3 100.79(5) . 1_666
Ga1 O1 Ga3 142.41(9) 1_455 1_666
Nb O1 Ga3 142.41(9) 1_455 1_666
Ga1 O1 Ga3 36.25(3) 1_565 1_666
Nb O1 Ga3 36.25(3) 1_565 1_666
O3 O1 Ga3 97.2(3) 1_556 1_666
O3 O1 Ga3 20.30(15) 3_566 1_666
O3 O1 Ga3 102.5(3) 4_456 1_666
La O1 Ga3 96.0(3) 1_556 1_666
La O1 Ga3 45.65(9) 2_566 1_666
La O1 Ga3 76.21(19) 4_456 1_666
Ga2 O1 Ga3 136.7(3) . 1_666
Ga2 O1 Ga3 35.90(5) 1_665 1_666
Ga2 O1 Ga3 76.83(11) 1_565 1_666
O1 O1 Ga3 159.19(4) 2_455 1_666
O1 O1 Ga3 53.79(14) 2_565 1_666
O1 O1 Ga3 89.23(7) 2_465 1_666
O3 O1 Ga3 87.74(14) 4 1_666
O3 O1 Ga3 161.86(19) 3_455 1_666
O3 O1 Ga3 59.62(14) 1_565 1_666
O1 O1 Ga3 71.41(19) 1_556 1_666
O1 O1 Ga3 108.59(19) 1_554 1_666
Ga3 O1 Ga3 110.33(18) 4_446 1_666
Ga2 O1 Ga3 71.40(19) 2_566 2_465
La O1 Ga3 100.56(6) . 2_465
La O1 Ga3 147.11(3) 2_565 2_465
La O1 Ga3 45.59(16) 4_455 2_465
O2 O1 Ga3 140.8(4) 6 2_465
O2 O1 Ga3 82.5(4) 5_455 2_465
O2 O1 Ga3 98.3(3) 2_565 2_465
O3 O1 Ga3 129.9(3) 6 2_465
O3 O1 Ga3 101.0(3) 2_565 2_465
O3 O1 Ga3 19.7(3) 5_455 2_465
O2 O1 Ga3 101.4(4) 6_556 2_465
O2 O1 Ga3 50.6(3) 5_456 2_465
O2 O1 Ga3 67.6(4) 2_566 2_465
Ga2 O1 Ga3 108.59(19) 2_565 2_465
Ga3 O1 Ga3 129.2(4) 2_565 2_465
Ga3 O1 Ga3 37.13(7) 1_556 2_465
Ga3 O1 Ga3 73.44(14) 4_456 2_465
O2 O1 Ga3 150.2(6) 4 2_465
O2 O1 Ga3 63.0(3) 3_455 2_465
O2 O1 Ga3 53.6(3) 1_565 2_465
O3 O1 Ga3 128.24(18) . 2_465
O3 O1 Ga3 121.10(18) 3_565 2_465
O3 O1 Ga3 47.4(2) 4_455 2_465
Ga3 O1 Ga3 146.9(3) 2_564 2_465
Ga3 O1 Ga3 74.55(6) . 2_465
Ga3 O1 Ga3 97.42(9) 4_455 2_465
O2 O1 Ga3 98.8(2) . 2_465
O2 O1 Ga3 130.4(3) 3_565 2_465
O2 O1 Ga3 20.08(19) 4_455 2_465
Nb O1 Ga3 142.41(9) . 2_465
Ga1 O1 Ga3 142.41(9) . 2_465
Ga1 O1 Ga3 36.25(3) 1_455 2_465
Nb O1 Ga3 36.25(3) 1_455 2_465
Ga1 O1 Ga3 100.79(5) 1_565 2_465
Nb O1 Ga3 100.79(5) 1_565 2_465
O3 O1 Ga3 102.5(3) 1_556 2_465
O3 O1 Ga3 97.2(3) 3_566 2_465
O3 O1 Ga3 20.30(15) 4_456 2_465
La O1 Ga3 76.21(19) 1_556 2_465
La O1 Ga3 96.0(3) 2_566 2_465
La O1 Ga3 45.65(9) 4_456 2_465
Ga2 O1 Ga3 76.83(11) . 2_465
Ga2 O1 Ga3 136.7(3) 1_665 2_465
Ga2 O1 Ga3 35.90(5) 1_565 2_465
O1 O1 Ga3 89.23(7) 2_455 2_465
O1 O1 Ga3 159.19(4) 2_565 2_465
O1 O1 Ga3 53.79(14) 2_465 2_465
O3 O1 Ga3 161.87(19) 4 2_465
O3 O1 Ga3 59.62(14) 3_455 2_465
O3 O1 Ga3 87.74(14) 1_565 2_465
O1 O1 Ga3 71.41(19) 1_556 2_465
O1 O1 Ga3 108.59(19) 1_554 2_465
Ga3 O1 Ga3 110.33(18) 4_446 2_465
Ga3 O1 Ga3 110.33(18) 1_666 2_465
Ga2 O1 O3 86.2(2) 2_566 5
La O1 O3 66.52(15) . 5
La O1 O3 60.40(13) 2_565 5
La O1 O3 163.7(6) 4_455 5
O2 O1 O3 59.5(3) 6 5
O2 O1 O3 107.4(4) 5_455 5
O2 O1 O3 112.0(5) 2_565 5
O3 O1 O3 22.3(4) 6 5
O3 O1 O3 97.3(4) 2_565 5
O3 O1 O3 140.9(4) 5_455 5
O2 O1 O3 55.0(3) 6_556 5
O2 O1 O3 99.6(5) 5_456 5
O2 O1 O3 103.7(4) 2_566 5
Ga2 O1 O3 93.8(2) 2_565 5
Ga3 O1 O3 24.27(16) 2_565 5
Ga3 O1 O3 113.2(2) 1_556 5
Ga3 O1 O3 115.0(2) 4_456 5
O2 O1 O3 27.4(3) 4 5
O2 O1 O3 92.5(3) 3_455 5
O2 O1 O3 143.8(3) 1_565 5
O3 O1 O3 46.2(3) . 5
O3 O1 O3 88.2(3) 3_565 5
O3 O1 O3 145.1(3) 4_455 5
Ga3 O1 O3 50.88(14) 2_564 5
Ga3 O1 O3 112.2(2) . 5
Ga3 O1 O3 113.6(2) 4_455 5
O2 O1 O3 55.8(2) . 5
O2 O1 O3 63.8(2) 3_565 5
O2 O1 O3 167.3(4) 4_455 5
Nb O1 O3 21.54(15) . 5
Ga1 O1 O3 21.54(15) . 5
Ga1 O1 O3 136.09(14) 1_455 5
Nb O1 O3 136.09(14) 1_455 5
Ga1 O1 O3 104.24(14) 1_565 5
Nb O1 O3 104.24(14) 1_565 5
O3 O1 O3 46.6(3) 1_556 5
O3 O1 O3 84.4(2) 3_566 5
O3 O1 O3 131.3(3) 4_456 5
La O1 O3 73.88(18) 1_556 5
La O1 O3 70.88(18) 2_566 5
La O1 O3 115.5(3) 4_456 5
Ga2 O1 O3 75.73(14) . 5
Ga2 O1 O3 45.32(14) 1_665 5
Ga2 O1 O3 152.2(3) 1_565 5
O1 O1 O3 78.46(14) 2_455 5
O1 O1 O3 49.24(14) 2_565 5
O1 O1 O3 157.2(4) 2_465 5
O3 O1 O3 29.1(3) 4 5
O3 O1 O3 115.57(16) 3_455 5
O3 O1 O3 121.81(16) 1_565 5
O1 O1 O3 86.2(2) 1_556 5
O1 O1 O3 93.8(2) 1_554 5
Ga3 O1 O3 40.17(13) 4_446 5
Ga3 O1 O3 80.99(15) 1_666 5
Ga3 O1 O3 149.0(3) 2_465 5
Ga2 O1 O3 86.2(2) 2_566 2_455
La O1 O3 60.40(13) . 2_455
La O1 O3 163.7(6) 2_565 2_455
La O1 O3 66.52(15) 4_455 2_455
O2 O1 O3 112.0(5) 6 2_455
O2 O1 O3 59.5(3) 5_455 2_455
O2 O1 O3 107.4(4) 2_565 2_455
O3 O1 O3 97.3(4) 6 2_455
O3 O1 O3 140.9(4) 2_565 2_455
O3 O1 O3 22.3(4) 5_455 2_455
O2 O1 O3 103.7(4) 6_556 2_455
O2 O1 O3 55.0(3) 5_456 2_455
O2 O1 O3 99.6(5) 2_566 2_455
Ga2 O1 O3 93.8(2) 2_565 2_455
Ga3 O1 O3 115.0(2) 2_565 2_455
Ga3 O1 O3 24.27(16) 1_556 2_455
Ga3 O1 O3 113.2(2) 4_456 2_455
O2 O1 O3 143.8(3) 4 2_455
O2 O1 O3 27.4(3) 3_455 2_455
O2 O1 O3 92.5(3) 1_565 2_455
O3 O1 O3 88.2(3) . 2_455
O3 O1 O3 145.1(3) 3_565 2_455
O3 O1 O3 46.2(3) 4_455 2_455
Ga3 O1 O3 113.6(2) 2_564 2_455
Ga3 O1 O3 50.88(14) . 2_455
Ga3 O1 O3 112.2(2) 4_455 2_455
O2 O1 O3 63.8(2) . 2_455
O2 O1 O3 167.3(4) 3_565 2_455
O2 O1 O3 55.8(2) 4_455 2_455
Nb O1 O3 104.24(13) . 2_455
Ga1 O1 O3 104.24(13) . 2_455
Ga1 O1 O3 21.54(15) 1_455 2_455
Nb O1 O3 21.54(15) 1_455 2_455
Ga1 O1 O3 136.09(14) 1_565 2_455
Nb O1 O3 136.09(14) 1_565 2_455
O3 O1 O3 84.4(2) 1_556 2_455
O3 O1 O3 131.3(3) 3_566 2_455
O3 O1 O3 46.6(3) 4_456 2_455
La O1 O3 70.88(18) 1_556 2_455
La O1 O3 115.5(3) 2_566 2_455
La O1 O3 73.88(18) 4_456 2_455
Ga2 O1 O3 45.32(14) . 2_455
Ga2 O1 O3 152.2(3) 1_665 2_455
Ga2 O1 O3 75.73(14) 1_565 2_455
O1 O1 O3 49.24(14) 2_455 2_455
O1 O1 O3 157.2(4) 2_565 2_455
O1 O1 O3 78.46(14) 2_465 2_455
O3 O1 O3 121.81(16) 4 2_455
O3 O1 O3 29.1(3) 3_455 2_455
O3 O1 O3 115.57(16) 1_565 2_455
O1 O1 O3 86.2(2) 1_556 2_455
O1 O1 O3 93.8(2) 1_554 2_455
Ga3 O1 O3 80.99(15) 4_446 2_455
Ga3 O1 O3 149.0(3) 1_666 2_455
Ga3 O1 O3 40.17(13) 2_465 2_455
O3 O1 O3 119.56(5) 5 2_455
Ga2 O1 O3 86.2(2) 2_566 6_565
La O1 O3 163.7(6) . 6_565
La O1 O3 66.52(15) 2_565 6_565
La O1 O3 60.40(13) 4_455 6_565
O2 O1 O3 107.4(4) 6 6_565
O2 O1 O3 112.0(5) 5_455 6_565
O2 O1 O3 59.5(3) 2_565 6_565
O3 O1 O3 140.9(4) 6 6_565
O3 O1 O3 22.3(4) 2_565 6_565
O3 O1 O3 97.3(4) 5_455 6_565
O2 O1 O3 99.6(5) 6_556 6_565
O2 O1 O3 103.7(4) 5_456 6_565
O2 O1 O3 55.0(3) 2_566 6_565
Ga2 O1 O3 93.8(2) 2_565 6_565
Ga3 O1 O3 113.2(2) 2_565 6_565
Ga3 O1 O3 115.0(2) 1_556 6_565
Ga3 O1 O3 24.27(16) 4_456 6_565
O2 O1 O3 92.5(3) 4 6_565
O2 O1 O3 143.8(3) 3_455 6_565
O2 O1 O3 27.4(3) 1_565 6_565
O3 O1 O3 145.1(3) . 6_565
O3 O1 O3 46.2(3) 3_565 6_565
O3 O1 O3 88.2(3) 4_455 6_565
Ga3 O1 O3 112.2(2) 2_564 6_565
Ga3 O1 O3 113.6(2) . 6_565
Ga3 O1 O3 50.88(14) 4_455 6_565
O2 O1 O3 167.3(4) . 6_565
O2 O1 O3 55.8(2) 3_565 6_565
O2 O1 O3 63.8(2) 4_455 6_565
Nb O1 O3 136.09(14) . 6_565
Ga1 O1 O3 136.09(14) . 6_565
Ga1 O1 O3 104.24(14) 1_455 6_565
Nb O1 O3 104.24(14) 1_455 6_565
Ga1 O1 O3 21.54(15) 1_565 6_565
Nb O1 O3 21.54(15) 1_565 6_565
O3 O1 O3 131.3(3) 1_556 6_565
O3 O1 O3 46.6(3) 3_566 6_565
O3 O1 O3 84.4(2) 4_456 6_565
La O1 O3 115.5(3) 1_556 6_565
La O1 O3 73.88(18) 2_566 6_565
La O1 O3 70.88(18) 4_456 6_565
Ga2 O1 O3 152.2(3) . 6_565
Ga2 O1 O3 75.73(14) 1_665 6_565
Ga2 O1 O3 45.32(14) 1_565 6_565
O1 O1 O3 157.2(4) 2_455 6_565
O1 O1 O3 78.46(14) 2_565 6_565
O1 O1 O3 49.24(14) 2_465 6_565
O3 O1 O3 115.56(16) 4 6_565
O3 O1 O3 121.81(16) 3_455 6_565
O3 O1 O3 29.1(3) 1_565 6_565
O1 O1 O3 86.2(2) 1_556 6_565
O1 O1 O3 93.8(2) 1_554 6_565
Ga3 O1 O3 149.0(3) 4_446 6_565
Ga3 O1 O3 40.17(13) 1_666 6_565
Ga3 O1 O3 80.99(15) 2_465 6_565
O3 O1 O3 119.56(5) 5 6_565
O3 O1 O3 119.56(5) 2_455 6_565
Ga2 O1 O3 55.7(2) 2_566 4_556
La O1 O3 83.4(2) . 4_556
La O1 O3 74.0(2) 2_565 4_556
La O1 O3 164.2(6) 4_455 4_556
O2 O1 O3 89.8(3) 6 4_556
O2 O1 O3 133.7(4) 5_455 4_556
O2 O1 O3 134.8(5) 2_565 4_556
O3 O1 O3 36.5(3) 6 4_556
O3 O1 O3 89.9(3) 2_565 4_556
O3 O1 O3 127.9(5) 5_455 4_556
O2 O1 O3 24.4(3) 6_556 4_556
O2 O1 O3 74.2(5) 5_456 4_556
O2 O1 O3 74.9(4) 2_566 4_556
Ga2 O1 O3 124.3(2) 2_565 4_556
Ga3 O1 O3 6.56(18) 2_565 4_556
Ga3 O1 O3 97.2(3) 1_556 4_556
Ga3 O1 O3 94.1(3) 4_456 4_556
O2 O1 O3 31.6(3) 4 4_556
O2 O1 O3 89.4(4) 3_455 4_556
O2 O1 O3 122.9(4) 1_565 4_556
O3 O1 O3 72.33(19) . 4_556
O3 O1 O3 100.0(2) 3_565 4_556
O3 O1 O3 160.2(3) 4_455 4_556
Ga3 O1 O3 81.37(16) 2_564 4_556
Ga3 O1 O3 135.58(17) . 4_556
Ga3 O1 O3 132.29(16) 4_455 4_556
O2 O1 O3 60.2(3) . 4_556
O2 O1 O3 61.1(3) 3_565 4_556
O2 O1 O3 137.5(5) 4_455 4_556
Nb O1 O3 48.48(16) . 4_556
Ga1 O1 O3 48.48(16) . 4_556
Ga1 O1 O3 136.2(2) 1_455 4_556
Nb O1 O3 136.2(2) 1_455 4_556
Ga1 O1 O3 104.31(17) 1_565 4_556
Nb O1 O3 104.31(17) 1_565 4_556
O3 O1 O3 30.4(3) 1_556 4_556
O3 O1 O3 64.1(3) 3_566 4_556
O3 O1 O3 104.2(4) 4_456 4_556
La O1 O3 49.4(2) 1_556 4_556
La O1 O3 42.8(2) 2_566 4_556
La O1 O3 85.0(3) 4_456 4_556
Ga2 O1 O3 71.22(18) . 4_556
Ga2 O1 O3 38.86(14) 1_665 4_556
Ga2 O1 O3 123.6(4) 1_565 4_556
O1 O1 O3 93.2(2) 2_455 4_556
O1 O1 O3 66.6(2) 2_565 4_556
O1 O1 O3 157.6(4) 2_465 4_556
O3 O1 O3 59.35(16) 4 4_556
O3 O1 O3 127.80(8) 3_455 4_556
O3 O1 O3 127.80(8) 1_565 4_556
O1 O1 O3 55.7(2) 1_556 4_556
O1 O1 O3 124.3(2) 1_554 4_556
Ga3 O1 O3 40.17(15) 4_446 4_556
Ga3 O1 O3 70.20(18) 1_666 4_556
Ga3 O1 O3 124.3(4) 2_465 4_556
O3 O1 O3 30.6(3) 5 4_556
O3 O1 O3 114.7(2) 2_455 4_556
O3 O1 O3 109.3(2) 6_565 4_556
Ga2 O1 O3 55.7(2) 2_566 3_456
La O1 O3 74.0(2) . 3_456
La O1 O3 164.2(6) 2_565 3_456
La O1 O3 83.4(2) 4_455 3_456
O2 O1 O3 134.8(5) 6 3_456
O2 O1 O3 89.8(3) 5_455 3_456
O2 O1 O3 133.7(4) 2_565 3_456
O3 O1 O3 89.9(3) 6 3_456
O3 O1 O3 127.9(5) 2_565 3_456
O3 O1 O3 36.5(3) 5_455 3_456
O2 O1 O3 74.9(4) 6_556 3_456
O2 O1 O3 24.4(3) 5_456 3_456
O2 O1 O3 74.2(5) 2_566 3_456
Ga2 O1 O3 124.3(2) 2_565 3_456
Ga3 O1 O3 94.1(3) 2_565 3_456
Ga3 O1 O3 6.56(18) 1_556 3_456
Ga3 O1 O3 97.2(3) 4_456 3_456
O2 O1 O3 122.9(4) 4 3_456
O2 O1 O3 31.6(3) 3_455 3_456
O2 O1 O3 89.4(4) 1_565 3_456
O3 O1 O3 100.0(2) . 3_456
O3 O1 O3 160.2(3) 3_565 3_456
O3 O1 O3 72.33(19) 4_455 3_456
Ga3 O1 O3 132.29(16) 2_564 3_456
Ga3 O1 O3 81.37(16) . 3_456
Ga3 O1 O3 135.58(17) 4_455 3_456
O2 O1 O3 61.1(3) . 3_456
O2 O1 O3 137.5(5) 3_565 3_456
O2 O1 O3 60.2(3) 4_455 3_456
Nb O1 O3 104.31(17) . 3_456
Ga1 O1 O3 104.31(17) . 3_456
Ga1 O1 O3 48.48(16) 1_455 3_456
Nb O1 O3 48.48(16) 1_455 3_456
Ga1 O1 O3 136.2(2) 1_565 3_456
Nb O1 O3 136.2(2) 1_565 3_456
O3 O1 O3 64.1(3) 1_556 3_456
O3 O1 O3 104.2(4) 3_566 3_456
O3 O1 O3 30.4(3) 4_456 3_456
La O1 O3 42.8(2) 1_556 3_456
La O1 O3 85.0(3) 2_566 3_456
La O1 O3 49.4(2) 4_456 3_456
Ga2 O1 O3 38.86(14) . 3_456
Ga2 O1 O3 123.6(4) 1_665 3_456
Ga2 O1 O3 71.22(18) 1_565 3_456
O1 O1 O3 66.6(2) 2_455 3_456
O1 O1 O3 157.6(4) 2_565 3_456
O1 O1 O3 93.2(2) 2_465 3_456
O3 O1 O3 127.80(8) 4 3_456
O3 O1 O3 59.35(16) 3_455 3_456
O3 O1 O3 127.80(8) 1_565 3_456
O1 O1 O3 55.7(2) 1_556 3_456
O1 O1 O3 124.3(2) 1_554 3_456
Ga3 O1 O3 70.20(18) 4_446 3_456
Ga3 O1 O3 124.3(4) 1_666 3_456
Ga3 O1 O3 40.17(15) 2_465 3_456
O3 O1 O3 109.3(2) 5 3_456
O3 O1 O3 30.6(3) 2_455 3_456
O3 O1 O3 114.7(2) 6_565 3_456
O3 O1 O3 91.4(3) 4_556 3_456
Ga2 O1 O3 55.7(2) 2_566 1_566
La O1 O3 164.2(6) . 1_566
La O1 O3 83.4(2) 2_565 1_566
La O1 O3 74.0(2) 4_455 1_566
O2 O1 O3 133.7(4) 6 1_566
O2 O1 O3 134.8(5) 5_455 1_566
O2 O1 O3 89.8(3) 2_565 1_566
O3 O1 O3 127.9(5) 6 1_566
O3 O1 O3 36.5(3) 2_565 1_566
O3 O1 O3 89.9(3) 5_455 1_566
O2 O1 O3 74.2(5) 6_556 1_566
O2 O1 O3 74.9(4) 5_456 1_566
O2 O1 O3 24.4(3) 2_566 1_566
Ga2 O1 O3 124.3(2) 2_565 1_566
Ga3 O1 O3 97.2(3) 2_565 1_566
Ga3 O1 O3 94.1(3) 1_556 1_566
Ga3 O1 O3 6.56(18) 4_456 1_566
O2 O1 O3 89.4(4) 4 1_566
O2 O1 O3 122.9(4) 3_455 1_566
O2 O1 O3 31.6(3) 1_565 1_566
O3 O1 O3 160.2(3) . 1_566
O3 O1 O3 72.33(19) 3_565 1_566
O3 O1 O3 100.0(2) 4_455 1_566
Ga3 O1 O3 135.58(17) 2_564 1_566
Ga3 O1 O3 132.29(16) . 1_566
Ga3 O1 O3 81.37(16) 4_455 1_566
O2 O1 O3 137.5(5) . 1_566
O2 O1 O3 60.2(3) 3_565 1_566
O2 O1 O3 61.1(3) 4_455 1_566
Nb O1 O3 136.2(2) . 1_566
Ga1 O1 O3 136.2(2) . 1_566
Ga1 O1 O3 104.31(17) 1_455 1_566
Nb O1 O3 104.31(17) 1_455 1_566
Ga1 O1 O3 48.48(16) 1_565 1_566
Nb O1 O3 48.48(16) 1_565 1_566
O3 O1 O3 104.2(4) 1_556 1_566
O3 O1 O3 30.4(3) 3_566 1_566
O3 O1 O3 64.1(3) 4_456 1_566
La O1 O3 85.0(3) 1_556 1_566
La O1 O3 49.4(2) 2_566 1_566
La O1 O3 42.8(2) 4_456 1_566
Ga2 O1 O3 123.6(4) . 1_566
Ga2 O1 O3 71.22(18) 1_665 1_566
Ga2 O1 O3 38.86(14) 1_565 1_566
O1 O1 O3 157.6(4) 2_455 1_566
O1 O1 O3 93.2(2) 2_565 1_566
O1 O1 O3 66.6(2) 2_465 1_566
O3 O1 O3 127.80(8) 4 1_566
O3 O1 O3 127.80(8) 3_455 1_566
O3 O1 O3 59.35(16) 1_565 1_566
O1 O1 O3 55.7(2) 1_556 1_566
O1 O1 O3 124.3(2) 1_554 1_566
Ga3 O1 O3 124.3(4) 4_446 1_566
Ga3 O1 O3 40.17(15) 1_666 1_566
Ga3 O1 O3 70.20(18) 2_465 1_566
O3 O1 O3 114.7(2) 5 1_566
O3 O1 O3 109.3(2) 2_455 1_566
O3 O1 O3 30.6(3) 6_565 1_566
O3 O1 O3 91.4(3) 4_556 1_566
O3 O1 O3 91.4(3) 3_456 1_566
Ga2 O1 O3 146.49(16) 2_566 6_554
La O1 O3 47.7(3) . 6_554
La O1 O3 67.5(3) 2_565 6_554
La O1 O3 102.1(5) 4_455 6_554
O2 O1 O3 14.8(4) 6 6_554
O2 O1 O3 48.0(4) 5_455 6_554
O2 O1 O3 64.8(4) 2_565 6_554
O3 O1 O3 63.0(3) 6 6_554
O3 O1 O3 111.6(4) 2_565 6_554
O3 O1 O3 111.6(4) 5_455 6_554
O2 O1 O3 117.1(3) 6_556 6_554
O2 O1 O3 136.8(4) 5_456 6_554
O2 O1 O3 162.2(4) 2_566 6_554
Ga2 O1 O3 33.52(16) 2_565 6_554
Ga3 O1 O3 86.8(2) 2_565 6_554
Ga3 O1 O3 116.7(3) 1_556 6_554
Ga3 O1 O3 141.5(3) 4_456 6_554
O2 O1 O3 78.5(4) 4 6_554
O2 O1 O3 88.9(4) 3_455 6_554
O2 O1 O3 133.6(5) 1_565 6_554
O3 O1 O3 29.1(4) . 6_554
O3 O1 O3 75.5(3) 3_565 6_554
O3 O1 O3 85.6(4) 4_455 6_554
Ga3 O1 O3 17.09(14) 2_564 6_554
Ga3 O1 O3 55.5(2) . 6_554
Ga3 O1 O3 72.0(3) 4_455 6_554
O2 O1 O3 70.4(3) . 6_554
O2 O1 O3 94.8(3) 3_565 6_554
O2 O1 O3 127.6(4) 4_455 6_554
Nb O1 O3 46.29(18) . 6_554
Ga1 O1 O3 46.29(18) . 6_554
Ga1 O1 O3 94.0(3) 1_455 6_554
Nb O1 O3 94.0(3) 1_455 6_554
Ga1 O1 O3 99.7(3) 1_565 6_554
Nb O1 O3 99.7(3) 1_565 6_554
O3 O1 O3 95.6(2) 1_556 6_554
O3 O1 O3 130.8(3) 3_566 6_554
O3 O1 O3 143.9(2) 4_456 6_554
La O1 O3 121.48(15) 1_556 6_554
La O1 O3 132.37(12) 2_566 6_554
La O1 O3 169.39(17) 4_456 6_554
Ga2 O1 O3 87.9(2) . 6_554
Ga2 O1 O3 93.29(17) 1_665 6_554
Ga2 O1 O3 142.1(3) 1_565 6_554
O1 O1 O3 53.7(4) 2_455 6_554
O1 O1 O3 60.1(3) 2_565 6_554
O1 O1 O3 103.1(5) 2_465 6_554
O3 O1 O3 36.5(3) 4 6_554
O3 O1 O3 71.6(3) 3_455 6_554
O3 O1 O3 93.4(3) 1_565 6_554
O1 O1 O3 146.49(16) 1_556 6_554
O1 O1 O3 33.51(16) 1_554 6_554
Ga3 O1 O3 76.28(18) 4_446 6_554
Ga3 O1 O3 113.1(2) 1_666 6_554
Ga3 O1 O3 130.0(3) 2_465 6_554
O3 O1 O3 62.97(17) 5 6_554
O3 O1 O3 97.5(3) 2_455 6_554
O3 O1 O3 119.4(3) 6_565 6_554
O3 O1 O3 93.4(3) 4_556 6_554
O3 O1 O3 120.3(3) 3_456 6_554
O3 O1 O3 147.8(2) 1_566 6_554
Ga2 O1 O3 146.48(16) 2_566 2_564
La O1 O3 102.1(5) . 2_564
La O1 O3 47.7(3) 2_565 2_564
La O1 O3 67.5(3) 4_455 2_564
O2 O1 O3 48.0(4) 6 2_564
O2 O1 O3 64.8(4) 5_455 2_564
O2 O1 O3 14.8(4) 2_565 2_564
O3 O1 O3 111.6(4) 6 2_564
O3 O1 O3 63.0(3) 2_565 2_564
O3 O1 O3 111.6(4) 5_455 2_564
O2 O1 O3 136.8(4) 6_556 2_564
O2 O1 O3 162.2(4) 5_456 2_564
O2 O1 O3 117.1(3) 2_566 2_564
Ga2 O1 O3 33.51(16) 2_565 2_564
Ga3 O1 O3 116.7(3) 2_565 2_564
Ga3 O1 O3 141.5(3) 1_556 2_564
Ga3 O1 O3 86.8(2) 4_456 2_564
O2 O1 O3 88.9(4) 4 2_564
O2 O1 O3 133.6(5) 3_455 2_564
O2 O1 O3 78.5(4) 1_565 2_564
O3 O1 O3 85.6(4) . 2_564
O3 O1 O3 29.1(4) 3_565 2_564
O3 O1 O3 75.5(3) 4_455 2_564
Ga3 O1 O3 55.5(2) 2_564 2_564
Ga3 O1 O3 72.0(3) . 2_564
Ga3 O1 O3 17.09(14) 4_455 2_564
O2 O1 O3 127.6(4) . 2_564
O2 O1 O3 70.4(3) 3_565 2_564
O2 O1 O3 94.8(3) 4_455 2_564
Nb O1 O3 94.0(3) . 2_564
Ga1 O1 O3 94.0(3) . 2_564
Ga1 O1 O3 99.7(3) 1_455 2_564
Nb O1 O3 99.7(3) 1_455 2_564
Ga1 O1 O3 46.29(18) 1_565 2_564
Nb O1 O3 46.29(18) 1_565 2_564
O3 O1 O3 143.9(2) 1_556 2_564
O3 O1 O3 95.6(2) 3_566 2_564
O3 O1 O3 130.8(3) 4_456 2_564
La O1 O3 169.39(17) 1_556 2_564
La O1 O3 121.48(15) 2_566 2_564
La O1 O3 132.37(12) 4_456 2_564
Ga2 O1 O3 142.1(3) . 2_564
Ga2 O1 O3 87.9(2) 1_665 2_564
Ga2 O1 O3 93.29(17) 1_565 2_564
O1 O1 O3 103.1(5) 2_455 2_564
O1 O1 O3 53.6(4) 2_565 2_564
O1 O1 O3 60.1(3) 2_465 2_564
O3 O1 O3 71.6(3) 4 2_564
O3 O1 O3 93.4(3) 3_455 2_564
O3 O1 O3 36.5(3) 1_565 2_564
O1 O1 O3 146.49(16) 1_556 2_564
O1 O1 O3 33.51(16) 1_554 2_564
Ga3 O1 O3 130.0(3) 4_446 2_564
Ga3 O1 O3 76.28(18) 1_666 2_564
Ga3 O1 O3 113.1(2) 2_465 2_564
O3 O1 O3 97.5(3) 5 2_564
O3 O1 O3 119.4(3) 2_455 2_564
O3 O1 O3 62.97(17) 6_565 2_564
O3 O1 O3 120.2(3) 4_556 2_564
O3 O1 O3 147.8(2) 3_456 2_564
O3 O1 O3 93.4(3) 1_566 2_564
O3 O1 O3 57.1(3) 6_554 2_564
Ga2 O1 O3 146.48(16) 2_566 5_454
La O1 O3 67.5(3) . 5_454
La O1 O3 102.1(5) 2_565 5_454
La O1 O3 47.7(3) 4_455 5_454
O2 O1 O3 64.8(4) 6 5_454
O2 O1 O3 14.8(4) 5_455 5_454
O2 O1 O3 48.0(4) 2_565 5_454
O3 O1 O3 111.6(4) 6 5_454
O3 O1 O3 111.6(4) 2_565 5_454
O3 O1 O3 63.0(3) 5_455 5_454
O2 O1 O3 162.2(4) 6_556 5_454
O2 O1 O3 117.1(3) 5_456 5_454
O2 O1 O3 136.8(4) 2_566 5_454
Ga2 O1 O3 33.51(16) 2_565 5_454
Ga3 O1 O3 141.5(3) 2_565 5_454
Ga3 O1 O3 86.8(2) 1_556 5_454
Ga3 O1 O3 116.7(3) 4_456 5_454
O2 O1 O3 133.6(5) 4 5_454
O2 O1 O3 78.5(4) 3_455 5_454
O2 O1 O3 88.9(4) 1_565 5_454
O3 O1 O3 75.5(3) . 5_454
O3 O1 O3 85.6(4) 3_565 5_454
O3 O1 O3 29.1(4) 4_455 5_454
Ga3 O1 O3 72.0(3) 2_564 5_454
Ga3 O1 O3 17.09(14) . 5_454
Ga3 O1 O3 55.5(2) 4_455 5_454
O2 O1 O3 94.8(3) . 5_454
O2 O1 O3 127.6(4) 3_565 5_454
O2 O1 O3 70.4(3) 4_455 5_454
Nb O1 O3 99.7(3) . 5_454
Ga1 O1 O3 99.7(3) . 5_454
Ga1 O1 O3 46.29(18) 1_455 5_454
Nb O1 O3 46.29(18) 1_455 5_454
Ga1 O1 O3 94.0(3) 1_565 5_454
Nb O1 O3 94.0(3) 1_565 5_454
O3 O1 O3 130.8(3) 1_556 5_454
O3 O1 O3 143.9(2) 3_566 5_454
O3 O1 O3 95.6(2) 4_456 5_454
La O1 O3 132.37(12) 1_556 5_454
La O1 O3 169.39(17) 2_566 5_454
La O1 O3 121.48(15) 4_456 5_454
Ga2 O1 O3 93.29(17) . 5_454
Ga2 O1 O3 142.1(3) 1_665 5_454
Ga2 O1 O3 87.9(2) 1_565 5_454
O1 O1 O3 60.1(3) 2_455 5_454
O1 O1 O3 103.1(5) 2_565 5_454
O1 O1 O3 53.7(4) 2_465 5_454
O3 O1 O3 93.4(3) 4 5_454
O3 O1 O3 36.5(3) 3_455 5_454
O3 O1 O3 71.6(3) 1_565 5_454
O1 O1 O3 146.49(16) 1_556 5_454
O1 O1 O3 33.51(16) 1_554 5_454
Ga3 O1 O3 113.1(2) 4_446 5_454
Ga3 O1 O3 130.0(3) 1_666 5_454
Ga3 O1 O3 76.28(18) 2_465 5_454
O3 O1 O3 119.4(3) 5 5_454
O3 O1 O3 62.97(17) 2_455 5_454
O3 O1 O3 97.5(3) 6_565 5_454
O3 O1 O3 147.8(2) 4_556 5_454
O3 O1 O3 93.4(3) 3_456 5_454
O3 O1 O3 120.2(3) 1_566 5_454
O3 O1 O3 57.1(3) 6_554 5_454
O3 O1 O3 57.1(3) 2_564 5_454
Ga2 O1 O2 141.26(18) 2_566 4_554
La O1 O2 74.8(4) . 4_554
La O1 O2 39.3(3) 2_565 4_554
La O1 O2 104.2(5) 4_455 4_554
O2 O1 O2 13.9(3) 6 4_554
O2 O1 O2 68.7(4) 5_455 4_554
O2 O1 O2 53.5(3) 2_565 4_554
O3 O1 O2 71.3(4) 6 4_554
O3 O1 O2 83.5(3) 2_565 4_554
O3 O1 O2 134.3(5) 5_455 4_554
O2 O1 O2 111.4(3) 6_556 4_554
O2 O1 O2 157.4(2) 5_456 4_554
O2 O1 O2 135.3(3) 2_566 4_554
Ga2 O1 O2 38.74(17) 2_565 4_554
Ga3 O1 O2 82.5(2) 2_565 4_554
Ga3 O1 O2 145.4(3) 1_556 4_554
Ga3 O1 O2 114.1(2) 4_456 4_554
O2 O1 O2 62.1(3) 4 4_554
O2 O1 O2 117.0(4) 3_455 4_554
O2 O1 O2 117.0(4) 1_565 4_554
O3 O1 O2 50.1(3) . 4_554
O3 O1 O2 49.0(3) 3_565 4_554
O3 O1 O2 100.0(4) 4_455 4_554
Ga3 O1 O2 17.2(2) 2_564 4_554
Ga3 O1 O2 77.3(3) . 4_554
Ga3 O1 O2 57.4(2) 4_455 4_554
O2 O1 O2 91.9(4) . 4_554
O2 O1 O2 67.6(2) 3_565 4_554
O2 O1 O2 133.1(4) 4_455 4_554
Nb O1 O2 53.7(2) . 4_554
Ga1 O1 O2 53.7(2) . 4_554
Ga1 O1 O2 116.5(3) 1_455 4_554
Nb O1 O2 116.5(3) 1_455 4_554
Ga1 O1 O2 73.8(2) 1_565 4_554
Nb O1 O2 73.8(2) 1_565 4_554
O3 O1 O2 104.4(2) 1_556 4_554
O3 O1 O2 103.6(2) 3_566 4_554
O3 O1 O2 167.3(3) 4_456 4_554
La O1 O2 132.84(17) 1_556 4_554
La O1 O2 114.41(14) 2_566 4_554
La O1 O2 161.0(2) 4_456 4_554
Ga2 O1 O2 112.6(3) . 4_554
Ga2 O1 O2 71.73(16) 1_665 4_554
Ga2 O1 O2 133.3(3) 1_565 4_554
O1 O1 O2 82.0(4) 2_455 4_554
O1 O1 O2 33.8(3) 2_565 4_554
O1 O1 O2 99.2(5) 2_465 4_554
O3 O1 O2 31.6(2) 4 4_554
O3 O1 O2 97.1(3) 3_455 4_554
O3 O1 O2 74.7(3) 1_565 4_554
O1 O1 O2 141.26(17) 1_556 4_554
O1 O1 O2 38.74(17) 1_554 4_554
Ga3 O1 O2 89.8(2) 4_446 4_554
Ga3 O1 O2 84.79(17) 1_666 4_554
Ga3 O1 O2 147.1(3) 2_465 4_554
O3 O1 O2 59.6(2) 5 4_554
O3 O1 O2 125.0(3) 2_455 4_554
O3 O1 O2 95.0(3) 6_565 4_554
O3 O1 O2 88.0(2) 4_556 4_554
O3 O1 O2 148.6(3) 3_456 4_554
O3 O1 O2 120.0(2) 1_566 4_554
O3 O1 O2 28.7(2) 6_554 4_554
O3 O1 O2 40.3(2) 2_564 4_554
O3 O1 O2 71.9(3) 5_454 4_554
Ga2 O1 O2 141.26(18) 2_566 3_454
La O1 O2 39.3(3) . 3_454
La O1 O2 104.2(5) 2_565 3_454
La O1 O2 74.8(4) 4_455 3_454
O2 O1 O2 53.5(3) 6 3_454
O2 O1 O2 13.9(3) 5_455 3_454
O2 O1 O2 68.7(4) 2_565 3_454
O3 O1 O2 83.5(3) 6 3_454
O3 O1 O2 134.3(5) 2_565 3_454
O3 O1 O2 71.3(4) 5_455 3_454
O2 O1 O2 135.3(3) 6_556 3_454
O2 O1 O2 111.4(3) 5_456 3_454
O2 O1 O2 157.4(2) 2_566 3_454
Ga2 O1 O2 38.74(17) 2_565 3_454
Ga3 O1 O2 114.1(2) 2_565 3_454
Ga3 O1 O2 82.5(2) 1_556 3_454
Ga3 O1 O2 145.4(3) 4_456 3_454
O2 O1 O2 117.0(4) 4 3_454
O2 O1 O2 62.1(3) 3_455 3_454
O2 O1 O2 117.0(4) 1_565 3_454
O3 O1 O2 49.0(3) . 3_454
O3 O1 O2 100.0(4) 3_565 3_454
O3 O1 O2 50.1(3) 4_455 3_454
Ga3 O1 O2 57.4(2) 2_564 3_454
Ga3 O1 O2 17.2(2) . 3_454
Ga3 O1 O2 77.3(3) 4_455 3_454
O2 O1 O2 67.6(2) . 3_454
O2 O1 O2 133.1(4) 3_565 3_454
O2 O1 O2 91.9(4) 4_455 3_454
Nb O1 O2 73.8(2) . 3_454
Ga1 O1 O2 73.8(2) . 3_454
Ga1 O1 O2 53.7(2) 1_455 3_454
Nb O1 O2 53.7(2) 1_455 3_454
Ga1 O1 O2 116.5(3) 1_565 3_454
Nb O1 O2 116.5(3) 1_565 3_454
O3 O1 O2 103.6(2) 1_556 3_454
O3 O1 O2 167.3(3) 3_566 3_454
O3 O1 O2 104.4(2) 4_456 3_454
La O1 O2 114.41(14) 1_556 3_454
La O1 O2 161.0(2) 2_566 3_454
La O1 O2 132.83(17) 4_456 3_454
Ga2 O1 O2 71.73(16) . 3_454
Ga2 O1 O2 133.3(3) 1_665 3_454
Ga2 O1 O2 112.6(3) 1_565 3_454
O1 O1 O2 33.8(3) 2_455 3_454
O1 O1 O2 99.2(5) 2_565 3_454
O1 O1 O2 82.0(4) 2_465 3_454
O3 O1 O2 74.7(3) 4 3_454
O3 O1 O2 31.6(2) 3_455 3_454
O3 O1 O2 97.1(3) 1_565 3_454
O1 O1 O2 141.26(18) 1_556 3_454
O1 O1 O2 38.74(17) 1_554 3_454
Ga3 O1 O2 84.79(17) 4_446 3_454
Ga3 O1 O2 147.1(3) 1_666 3_454
Ga3 O1 O2 89.8(2) 2_465 3_454
O3 O1 O2 95.0(3) 5 3_454
O3 O1 O2 59.6(2) 2_455 3_454
O3 O1 O2 125.0(3) 6_565 3_454
O3 O1 O2 120.0(2) 4_556 3_454
O3 O1 O2 88.0(2) 3_456 3_454
O3 O1 O2 148.6(3) 1_566 3_454
O3 O1 O2 40.3(2) 6_554 3_454
O3 O1 O2 71.9(3) 2_564 3_454
O3 O1 O2 28.7(2) 5_454 3_454
O2 O1 O2 65.6(3) 4_554 3_454
Ga2 O1 O2 141.26(17) 2_566 1_564
La O1 O2 104.2(5) . 1_564
La O1 O2 74.8(4) 2_565 1_564
La O1 O2 39.3(3) 4_455 1_564
O2 O1 O2 68.7(4) 6 1_564
O2 O1 O2 53.5(3) 5_455 1_564
O2 O1 O2 13.9(3) 2_565 1_564
O3 O1 O2 134.3(5) 6 1_564
O3 O1 O2 71.3(4) 2_565 1_564
O3 O1 O2 83.5(3) 5_455 1_564
O2 O1 O2 157.4(2) 6_556 1_564
O2 O1 O2 135.3(3) 5_456 1_564
O2 O1 O2 111.4(3) 2_566 1_564
Ga2 O1 O2 38.74(17) 2_565 1_564
Ga3 O1 O2 145.4(3) 2_565 1_564
Ga3 O1 O2 114.1(2) 1_556 1_564
Ga3 O1 O2 82.5(2) 4_456 1_564
O2 O1 O2 117.0(4) 4 1_564
O2 O1 O2 117.0(4) 3_455 1_564
O2 O1 O2 62.1(3) 1_565 1_564
O3 O1 O2 100.0(4) . 1_564
O3 O1 O2 50.1(3) 3_565 1_564
O3 O1 O2 49.0(3) 4_455 1_564
Ga3 O1 O2 77.3(3) 2_564 1_564
Ga3 O1 O2 57.4(2) . 1_564
Ga3 O1 O2 17.2(2) 4_455 1_564
O2 O1 O2 133.1(4) . 1_564
O2 O1 O2 91.9(4) 3_565 1_564
O2 O1 O2 67.6(2) 4_455 1_564
Nb O1 O2 116.5(3) . 1_564
Ga1 O1 O2 116.5(3) . 1_564
Ga1 O1 O2 73.8(2) 1_455 1_564
Nb O1 O2 73.8(2) 1_455 1_564
Ga1 O1 O2 53.7(2) 1_565 1_564
Nb O1 O2 53.7(2) 1_565 1_564
O3 O1 O2 167.3(3) 1_556 1_564
O3 O1 O2 104.4(2) 3_566 1_564
O3 O1 O2 103.6(2) 4_456 1_564
La O1 O2 161.0(2) 1_556 1_564
La O1 O2 132.83(17) 2_566 1_564
La O1 O2 114.41(14) 4_456 1_564
Ga2 O1 O2 133.3(3) . 1_564
Ga2 O1 O2 112.6(3) 1_665 1_564
Ga2 O1 O2 71.73(16) 1_565 1_564
O1 O1 O2 99.2(4) 2_455 1_564
O1 O1 O2 82.0(4) 2_565 1_564
O1 O1 O2 33.8(3) 2_465 1_564
O3 O1 O2 97.1(3) 4 1_564
O3 O1 O2 74.7(3) 3_455 1_564
O3 O1 O2 31.6(2) 1_565 1_564
O1 O1 O2 141.26(17) 1_556 1_564
O1 O1 O2 38.74(17) 1_554 1_564
Ga3 O1 O2 147.1(3) 4_446 1_564
Ga3 O1 O2 89.8(2) 1_666 1_564
Ga3 O1 O2 84.79(17) 2_465 1_564
O3 O1 O2 125.0(3) 5 1_564
O3 O1 O2 95.0(3) 2_455 1_564
O3 O1 O2 59.6(2) 6_565 1_564
O3 O1 O2 148.6(3) 4_556 1_564
O3 O1 O2 120.0(2) 3_456 1_564
O3 O1 O2 87.9(2) 1_566 1_564
O3 O1 O2 71.9(3) 6_554 1_564
O3 O1 O2 28.7(2) 2_564 1_564
O3 O1 O2 40.3(2) 5_454 1_564
O2 O1 O2 65.6(3) 4_554 1_564
O2 O1 O2 65.6(3) 3_454 1_564
Ga2 O1 O1 54.0(3) 2_566 2_456
La O1 O1 57.03(9) . 2_456
La O1 O1 135.8(3) 2_565 2_456
La O1 O1 115.04(16) 4_455 2_456
O2 O1 O1 114.2(5) 6 2_456
O2 O1 O1 97.5(3) 5_455 2_456
O2 O1 O1 155.9(5) 2_565 2_456
O3 O1 O1 57.4(3) 6 2_456
O3 O1 O1 137.2(6) 2_565 2_456
O3 O1 O1 66.8(3) 5_455 2_456
O2 O1 O1 55.3(4) 6_556 2_456
O2 O1 O1 34.2(4) 5_456 2_456
O2 O1 O1 83.8(6) 2_566 2_456
Ga2 O1 O1 126.0(3) 2_565 2_456
Ga3 O1 O1 64.3(2) 2_565 2_456
Ga3 O1 O1 36.77(11) 1_556 2_456
Ga3 O1 O1 113.9(5) 4_456 2_456
O2 O1 O1 93.8(3) 4 2_456
O2 O1 O1 29.5(3) 3_455 2_456
O2 O1 O1 118.1(6) 1_565 2_456
O3 O1 O1 75.8(2) . 2_456
O3 O1 O1 163.2(3) 3_565 2_456
O3 O1 O1 97.68(16) 4_455 2_456
Ga3 O1 O1 107.97(13) 2_564 2_456
Ga3 O1 O1 91.42(13) . 2_456
Ga3 O1 O1 163.0(3) 4_455 2_456
O2 O1 O1 33.31(18) . 2_456
O2 O1 O1 122.1(4) 3_565 2_456
O2 O1 O1 92.9(3) 4_455 2_456
Nb O1 O1 73.047(13) . 2_456
Ga1 O1 O1 73.047(13) . 2_456
Ga1 O1 O1 73.047(13) 1_455 2_456
Nb O1 O1 73.047(13) 1_455 2_456
Ga1 O1 O1 154.5(5) 1_565 2_456
Nb O1 O1 154.5(5) 1_565 2_456
O3 O1 O1 33.28(19) 1_556 2_456
O3 O1 O1 103.6(5) 3_566 2_456
O3 O1 O1 60.1(3) 4_456 2_456
La O1 O1 25.96(19) 1_556 2_456
La O1 O1 76.0(4) 2_566 2_456
La O1 O1 66.8(3) 4_456 2_456
Ga2 O1 O1 17.08(10) . 2_456
Ga2 O1 O1 101.1(3) 1_665 2_456
Ga2 O1 O1 101.1(3) 1_565 2_456
O1 O1 O1 56.19(10) 2_455 2_456
O1 O1 O1 125.6(2) 2_565 2_456
O1 O1 O1 125.6(2) 2_465 2_456
O3 O1 O1 96.77(14) 4 2_456
O3 O1 O1 71.92(15) 3_455 2_456
O3 O1 O1 159.9(3) 1_565 2_456
O1 O1 O1 54.0(3) 1_556 2_456
O1 O1 O1 126.0(3) 1_554 2_456
Ga3 O1 O1 37.64(3) 4_446 2_456
Ga3 O1 O1 121.6(4) 1_666 2_456
Ga3 O1 O1 72.91(16) 2_465 2_456
O3 O1 O1 76.61(16) 5 2_456
O3 O1 O1 51.53(15) 2_455 2_456
O3 O1 O1 137.4(5) 6_565 2_456
O3 O1 O1 63.2(2) 4_556 2_456
O3 O1 O1 32.76(16) 3_456 2_456
O3 O1 O1 107.4(5) 1_566 2_456
O3 O1 O1 103.1(3) 6_554 2_456
O3 O1 O1 159.1(4) 2_564 2_456
O3 O1 O1 107.9(2) 5_454 2_456
O2 O1 O1 124.8(3) 4_554 2_456
O2 O1 O1 88.5(2) 3_454 2_456
O2 O1 O1 146.0(3) 1_564 2_456
Ga2 O1 O1 54.0(3) 2_566 2_566
La O1 O1 115.04(16) . 2_566
La O1 O1 57.03(9) 2_565 2_566
La O1 O1 135.8(3) 4_455 2_566
O2 O1 O1 97.5(3) 6 2_566
O2 O1 O1 155.9(5) 5_455 2_566
O2 O1 O1 114.2(5) 2_565 2_566
O3 O1 O1 66.8(3) 6 2_566
O3 O1 O1 57.4(3) 2_565 2_566
O3 O1 O1 137.2(6) 5_455 2_566
O2 O1 O1 34.2(4) 6_556 2_566
O2 O1 O1 83.8(6) 5_456 2_566
O2 O1 O1 55.3(4) 2_566 2_566
Ga2 O1 O1 126.0(3) 2_565 2_566
Ga3 O1 O1 36.77(11) 2_565 2_566
Ga3 O1 O1 113.9(5) 1_556 2_566
Ga3 O1 O1 64.3(2) 4_456 2_566
O2 O1 O1 29.5(3) 4 2_566
O2 O1 O1 118.1(6) 3_455 2_566
O2 O1 O1 93.8(3) 1_565 2_566
O3 O1 O1 97.68(16) . 2_566
O3 O1 O1 75.8(2) 3_565 2_566
O3 O1 O1 163.2(3) 4_455 2_566
Ga3 O1 O1 91.42(13) 2_564 2_566
Ga3 O1 O1 163.0(3) . 2_566
Ga3 O1 O1 107.97(13) 4_455 2_566
O2 O1 O1 92.9(3) . 2_566
O2 O1 O1 33.31(18) 3_565 2_566
O2 O1 O1 122.1(4) 4_455 2_566
Nb O1 O1 73.047(14) . 2_566
Ga1 O1 O1 73.047(14) . 2_566
Ga1 O1 O1 154.5(5) 1_455 2_566
Nb O1 O1 154.5(5) 1_455 2_566
Ga1 O1 O1 73.046(13) 1_565 2_566
Nb O1 O1 73.046(13) 1_565 2_566
O3 O1 O1 60.1(3) 1_556 2_566
O3 O1 O1 33.28(19) 3_566 2_566
O3 O1 O1 103.6(5) 4_456 2_566
La O1 O1 66.8(3) 1_556 2_566
La O1 O1 25.96(19) 2_566 2_566
La O1 O1 76.0(4) 4_456 2_566
Ga2 O1 O1 101.1(3) . 2_566
Ga2 O1 O1 17.08(10) 1_665 2_566
Ga2 O1 O1 101.1(3) 1_565 2_566
O1 O1 O1 125.6(2) 2_455 2_566
O1 O1 O1 56.19(10) 2_565 2_566
O1 O1 O1 125.6(2) 2_465 2_566
O3 O1 O1 71.92(15) 4 2_566
O3 O1 O1 159.9(3) 3_455 2_566
O3 O1 O1 96.77(14) 1_565 2_566
O1 O1 O1 54.0(3) 1_556 2_566
O1 O1 O1 126.0(3) 1_554 2_566
Ga3 O1 O1 72.91(16) 4_446 2_566
Ga3 O1 O1 37.64(3) 1_666 2_566
Ga3 O1 O1 121.6(4) 2_465 2_566
O3 O1 O1 51.53(15) 5 2_566
O3 O1 O1 137.4(5) 2_455 2_566
O3 O1 O1 76.61(15) 6_565 2_566
O3 O1 O1 32.76(16) 4_556 2_566
O3 O1 O1 107.4(5) 3_456 2_566
O3 O1 O1 63.2(2) 1_566 2_566
O3 O1 O1 107.9(2) 6_554 2_566
O3 O1 O1 103.1(3) 2_564 2_566
O3 O1 O1 159.1(4) 5_454 2_566
O2 O1 O1 88.5(2) 4_554 2_566
O2 O1 O1 146.0(3) 3_454 2_566
O2 O1 O1 124.8(3) 1_564 2_566
O1 O1 O1 89.0(4) 2_456 2_566
Ga2 O1 O1 54.0(3) 2_566 2_466
La O1 O1 135.8(3) . 2_466
La O1 O1 115.03(16) 2_565 2_466
La O1 O1 57.03(9) 4_455 2_466
O2 O1 O1 155.9(5) 6 2_466
O2 O1 O1 114.2(5) 5_455 2_466
O2 O1 O1 97.5(3) 2_565 2_466
O3 O1 O1 137.2(6) 6 2_466
O3 O1 O1 66.8(3) 2_565 2_466
O3 O1 O1 57.4(3) 5_455 2_466
O2 O1 O1 83.8(6) 6_556 2_466
O2 O1 O1 55.3(4) 5_456 2_466
O2 O1 O1 34.2(4) 2_566 2_466
Ga2 O1 O1 126.0(3) 2_565 2_466
Ga3 O1 O1 113.9(5) 2_565 2_466
Ga3 O1 O1 64.3(2) 1_556 2_466
Ga3 O1 O1 36.77(11) 4_456 2_466
O2 O1 O1 118.1(6) 4 2_466
O2 O1 O1 93.8(3) 3_455 2_466
O2 O1 O1 29.5(3) 1_565 2_466
O3 O1 O1 163.2(3) . 2_466
O3 O1 O1 97.67(16) 3_565 2_466
O3 O1 O1 75.8(2) 4_455 2_466
Ga3 O1 O1 163.0(3) 2_564 2_466
Ga3 O1 O1 107.97(13) . 2_466
Ga3 O1 O1 91.42(13) 4_455 2_466
O2 O1 O1 122.1(4) . 2_466
O2 O1 O1 92.9(3) 3_565 2_466
O2 O1 O1 33.31(18) 4_455 2_466
Nb O1 O1 154.5(5) . 2_466
Ga1 O1 O1 154.5(5) . 2_466
Ga1 O1 O1 73.046(14) 1_455 2_466
Nb O1 O1 73.046(14) 1_455 2_466
Ga1 O1 O1 73.046(14) 1_565 2_466
Nb O1 O1 73.046(14) 1_565 2_466
O3 O1 O1 103.6(5) 1_556 2_466
O3 O1 O1 60.1(3) 3_566 2_466
O3 O1 O1 33.3(2) 4_456 2_466
La O1 O1 76.0(4) 1_556 2_466
La O1 O1 66.8(3) 2_566 2_466
La O1 O1 25.96(19) 4_456 2_466
Ga2 O1 O1 101.1(3) . 2_466
Ga2 O1 O1 101.1(3) 1_665 2_466
Ga2 O1 O1 17.08(10) 1_565 2_466
O1 O1 O1 125.6(2) 2_455 2_466
O1 O1 O1 125.6(2) 2_565 2_466
O1 O1 O1 56.19(10) 2_465 2_466
O3 O1 O1 159.9(3) 4 2_466
O3 O1 O1 96.77(14) 3_455 2_466
O3 O1 O1 71.92(15) 1_565 2_466
O1 O1 O1 54.0(3) 1_556 2_466
O1 O1 O1 126.0(3) 1_554 2_466
Ga3 O1 O1 121.6(4) 4_446 2_466
Ga3 O1 O1 72.91(16) 1_666 2_466
Ga3 O1 O1 37.64(3) 2_465 2_466
O3 O1 O1 137.4(5) 5 2_466
O3 O1 O1 76.61(15) 2_455 2_466
O3 O1 O1 51.53(15) 6_565 2_466
O3 O1 O1 107.4(5) 4_556 2_466
O3 O1 O1 63.2(2) 3_456 2_466
O3 O1 O1 32.76(16) 1_566 2_466
O3 O1 O1 159.1(4) 6_554 2_466
O3 O1 O1 107.9(2) 2_564 2_466
O3 O1 O1 103.1(3) 5_454 2_466
O2 O1 O1 146.0(3) 4_554 2_466
O2 O1 O1 124.8(3) 3_454 2_466
O2 O1 O1 88.5(2) 1_564 2_466
O1 O1 O1 89.0(4) 2_456 2_466
O1 O1 O1 89.0(4) 2_566 2_466
Ga2 O1 Ga2 126.94(14) 2_566 1_554
La O1 Ga2 20.5(2) . 1_554
La O1 Ga2 108.0(4) 2_565 1_554
La O1 Ga2 91.1(3) 4_455 1_554
O2 O1 Ga2 55.3(4) 6 1_554
O2 O1 Ga2 32.3(3) 5_455 1_554
O2 O1 Ga2 85.8(4) 2_565 1_554
O3 O1 Ga2 66.5(3) 6 1_554
O3 O1 Ga2 149.1(5) 2_565 1_554
O3 O1 Ga2 75.2(3) 5_455 1_554
O2 O1 Ga2 116.5(3) 6_556 1_554
O2 O1 Ga2 101.1(3) 5_456 1_554
O2 O1 Ga2 154.4(4) 2_566 1_554
Ga2 O1 Ga2 53.06(14) 2_565 1_554
Ga3 O1 Ga2 97.32(9) 2_565 1_554
Ga3 O1 Ga2 76.39(10) 1_556 1_554
Ga3 O1 Ga2 163.0(2) 4_456 1_554
O2 O1 Ga2 106.8(4) 4 1_554
O2 O1 Ga2 50.4(3) 3_455 1_554
O2 O1 Ga2 133.5(3) 1_565 1_554
O3 O1 Ga2 36.00(18) . 1_554
O3 O1 Ga2 112.2(4) 3_565 1_554
O3 O1 Ga2 64.2(3) 4_455 1_554
Ga3 O1 Ga2 55.96(14) 2_564 1_554
Ga3 O1 Ga2 32.86(7) . 1_554
Ga3 O1 Ga2 94.6(3) 4_455 1_554
O2 O1 Ga2 49.02(19) . 1_554
O2 O1 Ga2 134.0(3) 3_565 1_554
O2 O1 Ga2 102.7(2) 4_455 1_554
Nb O1 Ga2 59.88(11) . 1_554
Ga1 O1 Ga2 59.88(11) . 1_554
Ga1 O1 Ga2 59.88(11) 1_455 1_554
Nb O1 Ga2 59.88(11) 1_455 1_554
Ga1 O1 Ga2 132.6(4) 1_565 1_554
Nb O1 Ga2 132.6(4) 1_565 1_554
O3 O1 Ga2 84.89(15) 1_556 1_554
O3 O1 Ga2 165.75(16) 3_566 1_554
O3 O1 Ga2 104.14(15) 4_456 1_554
La O1 Ga2 98.10(4) 1_556 1_554
La O1 Ga2 142.23(15) 2_566 1_554
La O1 Ga2 129.74(10) 4_456 1_554
Ga2 O1 Ga2 55.83(6) . 1_554
Ga2 O1 Ga2 124.93(11) 1_665 1_554
Ga2 O1 Ga2 124.94(11) 1_565 1_554
O1 O1 Ga2 16.7(3) 2_455 1_554
O1 O1 Ga2 99.6(4) 2_565 1_554
O1 O1 Ga2 99.6(4) 2_465 1_554
O3 O1 Ga2 67.4(2) 4 1_554
O3 O1 Ga2 36.21(16) 3_455 1_554
O3 O1 Ga2 115.3(3) 1_565 1_554
O1 O1 Ga2 126.94(14) 1_556 1_554
O1 O1 Ga2 53.06(14) 1_554 1_554
Ga3 O1 Ga2 66.08(5) 4_446 1_554
Ga3 O1 Ga2 153.4(2) 1_666 1_554
Ga3 O1 Ga2 94.96(7) 2_465 1_554
O3 O1 Ga2 81.37(16) 5 1_554
O3 O1 Ga2 57.61(14) 2_455 1_554
O3 O1 Ga2 143.7(3) 6_565 1_554
O3 O1 Ga2 102.75(15) 4_556 1_554
O3 O1 Ga2 80.49(15) 3_456 1_554
O3 O1 Ga2 163.79(14) 1_566 1_554
O3 O1 Ga2 40.49(19) 6_554 1_554
O3 O1 Ga2 86.4(3) 2_564 1_554
O3 O1 Ga2 47.11(18) 5_454 1_554
O2 O1 Ga2 69.1(2) 4_554 1_554
O2 O1 Ga2 18.77(15) 3_454 1_554
O2 O1 Ga2 84.1(3) 1_564 1_554
O1 O1 Ga2 72.91(16) 2_456 1_554
O1 O1 Ga2 132.57(6) 2_566 1_554
O1 O1 Ga2 132.57(6) 2_466 1_554
Ga2 O1 Ga2 126.94(14) 2_566 1_664
La O1 Ga2 91.1(3) . 1_664
La O1 Ga2 20.5(2) 2_565 1_664
La O1 Ga2 108.0(4) 4_455 1_664
O2 O1 Ga2 32.3(3) 6 1_664
O2 O1 Ga2 85.8(4) 5_455 1_664
O2 O1 Ga2 55.3(4) 2_565 1_664
O3 O1 Ga2 75.2(3) 6 1_664
O3 O1 Ga2 66.5(3) 2_565 1_664
O3 O1 Ga2 149.1(5) 5_455 1_664
O2 O1 Ga2 101.1(3) 6_556 1_664
O2 O1 Ga2 154.4(4) 5_456 1_664
O2 O1 Ga2 116.5(3) 2_566 1_664
Ga2 O1 Ga2 53.06(14) 2_565 1_664
Ga3 O1 Ga2 76.39(10) 2_565 1_664
Ga3 O1 Ga2 163.0(2) 1_556 1_664
Ga3 O1 Ga2 97.32(9) 4_456 1_664
O2 O1 Ga2 50.4(3) 4 1_664
O2 O1 Ga2 133.5(3) 3_455 1_664
O2 O1 Ga2 106.8(4) 1_565 1_664
O3 O1 Ga2 64.2(3) . 1_664
O3 O1 Ga2 36.00(18) 3_565 1_664
O3 O1 Ga2 112.2(4) 4_455 1_664
Ga3 O1 Ga2 32.86(7) 2_564 1_664
Ga3 O1 Ga2 94.6(3) . 1_664
Ga3 O1 Ga2 55.96(14) 4_455 1_664
O2 O1 Ga2 102.7(2) . 1_664
O2 O1 Ga2 49.02(19) 3_565 1_664
O2 O1 Ga2 134.0(3) 4_455 1_664
Nb O1 Ga2 59.88(11) . 1_664
Ga1 O1 Ga2 59.88(11) . 1_664
Ga1 O1 Ga2 132.6(4) 1_455 1_664
Nb O1 Ga2 132.6(4) 1_455 1_664
Ga1 O1 Ga2 59.88(11) 1_565 1_664
Nb O1 Ga2 59.88(11) 1_565 1_664
O3 O1 Ga2 104.14(15) 1_556 1_664
O3 O1 Ga2 84.89(15) 3_566 1_664
O3 O1 Ga2 165.75(16) 4_456 1_664
La O1 Ga2 129.74(10) 1_556 1_664
La O1 Ga2 98.10(4) 2_566 1_664
La O1 Ga2 142.23(15) 4_456 1_664
Ga2 O1 Ga2 124.93(11) . 1_664
Ga2 O1 Ga2 55.83(6) 1_665 1_664
Ga2 O1 Ga2 124.94(11) 1_565 1_664
O1 O1 Ga2 99.6(4) 2_455 1_664
O1 O1 Ga2 16.7(3) 2_565 1_664
O1 O1 Ga2 99.6(4) 2_465 1_664
O3 O1 Ga2 36.21(16) 4 1_664
O3 O1 Ga2 115.3(3) 3_455 1_664
O3 O1 Ga2 67.4(2) 1_565 1_664
O1 O1 Ga2 126.94(14) 1_556 1_664
O1 O1 Ga2 53.06(14) 1_554 1_664
Ga3 O1 Ga2 94.95(7) 4_446 1_664
Ga3 O1 Ga2 66.08(5) 1_666 1_664
Ga3 O1 Ga2 153.4(2) 2_465 1_664
O3 O1 Ga2 57.61(14) 5 1_664
O3 O1 Ga2 143.7(3) 2_455 1_664
O3 O1 Ga2 81.37(16) 6_565 1_664
O3 O1 Ga2 80.49(15) 4_556 1_664
O3 O1 Ga2 163.79(14) 3_456 1_664
O3 O1 Ga2 102.75(15) 1_566 1_664
O3 O1 Ga2 47.11(18) 6_554 1_664
O3 O1 Ga2 40.49(19) 2_564 1_664
O3 O1 Ga2 86.4(3) 5_454 1_664
O2 O1 Ga2 18.77(15) 4_554 1_664
O2 O1 Ga2 84.1(3) 3_454 1_664
O2 O1 Ga2 69.1(2) 1_564 1_664
O1 O1 Ga2 132.57(6) 2_456 1_664
O1 O1 Ga2 72.91(15) 2_566 1_664
O1 O1 Ga2 132.57(6) 2_466 1_664
Ga2 O1 Ga2 87.6(2) 1_554 1_664
Ga2 O1 Ga2 126.94(14) 2_566 1_564
La O1 Ga2 108.0(4) . 1_564
La O1 Ga2 91.1(3) 2_565 1_564
La O1 Ga2 20.5(2) 4_455 1_564
O2 O1 Ga2 85.8(4) 6 1_564
O2 O1 Ga2 55.3(4) 5_455 1_564
O2 O1 Ga2 32.3(3) 2_565 1_564
O3 O1 Ga2 149.1(5) 6 1_564
O3 O1 Ga2 75.2(3) 2_565 1_564
O3 O1 Ga2 66.5(3) 5_455 1_564
O2 O1 Ga2 154.4(4) 6_556 1_564
O2 O1 Ga2 116.5(3) 5_456 1_564
O2 O1 Ga2 101.1(3) 2_566 1_564
Ga2 O1 Ga2 53.06(14) 2_565 1_564
Ga3 O1 Ga2 163.0(2) 2_565 1_564
Ga3 O1 Ga2 97.32(9) 1_556 1_564
Ga3 O1 Ga2 76.39(10) 4_456 1_564
O2 O1 Ga2 133.5(3) 4 1_564
O2 O1 Ga2 106.8(4) 3_455 1_564
O2 O1 Ga2 50.4(3) 1_565 1_564
O3 O1 Ga2 112.2(4) . 1_564
O3 O1 Ga2 64.2(3) 3_565 1_564
O3 O1 Ga2 36.00(18) 4_455 1_564
Ga3 O1 Ga2 94.6(3) 2_564 1_564
Ga3 O1 Ga2 55.96(14) . 1_564
Ga3 O1 Ga2 32.86(7) 4_455 1_564
O2 O1 Ga2 134.0(3) . 1_564
O2 O1 Ga2 102.7(2) 3_565 1_564
O2 O1 Ga2 49.02(19) 4_455 1_564
Nb O1 Ga2 132.6(4) . 1_564
Ga1 O1 Ga2 132.6(4) . 1_564
Ga1 O1 Ga2 59.88(11) 1_455 1_564
Nb O1 Ga2 59.88(11) 1_455 1_564
Ga1 O1 Ga2 59.88(11) 1_565 1_564
Nb O1 Ga2 59.88(11) 1_565 1_564
O3 O1 Ga2 165.75(16) 1_556 1_564
O3 O1 Ga2 104.14(15) 3_566 1_564
O3 O1 Ga2 84.89(15) 4_456 1_564
La O1 Ga2 142.23(15) 1_556 1_564
La O1 Ga2 129.74(10) 2_566 1_564
La O1 Ga2 98.10(4) 4_456 1_564
Ga2 O1 Ga2 124.94(11) . 1_564
Ga2 O1 Ga2 124.93(11) 1_665 1_564
Ga2 O1 Ga2 55.83(6) 1_565 1_564
O1 O1 Ga2 99.6(4) 2_455 1_564
O1 O1 Ga2 99.6(4) 2_565 1_564
O1 O1 Ga2 16.7(3) 2_465 1_564
O3 O1 Ga2 115.3(3) 4 1_564
O3 O1 Ga2 67.4(2) 3_455 1_564
O3 O1 Ga2 36.21(16) 1_565 1_564
O1 O1 Ga2 126.94(14) 1_556 1_564
O1 O1 Ga2 53.06(14) 1_554 1_564
Ga3 O1 Ga2 153.4(2) 4_446 1_564
Ga3 O1 Ga2 94.95(7) 1_666 1_564
Ga3 O1 Ga2 66.08(5) 2_465 1_564
O3 O1 Ga2 143.7(3) 5 1_564
O3 O1 Ga2 81.37(16) 2_455 1_564
O3 O1 Ga2 57.61(14) 6_565 1_564
O3 O1 Ga2 163.79(14) 4_556 1_564
O3 O1 Ga2 102.75(15) 3_456 1_564
O3 O1 Ga2 80.49(15) 1_566 1_564
O3 O1 Ga2 86.4(3) 6_554 1_564
O3 O1 Ga2 47.11(18) 2_564 1_564
O3 O1 Ga2 40.49(19) 5_454 1_564
O2 O1 Ga2 84.1(3) 4_554 1_564
O2 O1 Ga2 69.1(2) 3_454 1_564
O2 O1 Ga2 18.77(15) 1_564 1_564
O1 O1 Ga2 132.57(6) 2_456 1_564
O1 O1 Ga2 132.56(6) 2_566 1_564
O1 O1 Ga2 72.91(15) 2_466 1_564
Ga2 O1 Ga2 87.6(2) 1_554 1_564
Ga2 O1 Ga2 87.6(2) 1_664 1_564
Ga2 O1 La 98.37(17) 2_566 4
La O1 La 81.67(11) . 4
La O1 La 36.54(4) 2_565 4
La O1 La 143.2(4) 4_455 4
O2 O1 La 48.9(3) 6 4
O2 O1 La 106.5(5) 5_455 4
O2 O1 La 90.7(4) 2_565 4
O3 O1 La 45.3(3) 6 4
O3 O1 La 78.2(3) 2_565 4
O3 O1 La 163.0(3) 5_455 4
O2 O1 La 68.3(3) 6_556 4
O2 O1 La 119.7(5) 5_456 4
O2 O1 La 104.3(4) 2_566 4
Ga2 O1 La 81.63(17) 2_565 4
Ga3 O1 La 41.10(6) 2_565 4
Ga3 O1 La 137.22(18) 1_556 4
Ga3 O1 La 103.01(7) 4_456 4
O2 O1 La 20.1(3) 4 4
O2 O1 La 115.0(3) 3_455 4
O2 O1 La 126.7(3) 1_565 4
O3 O1 La 55.31(17) . 4
O3 O1 La 64.21(19) 3_565 4
O3 O1 La 142.6(5) 4_455 4
Ga3 O1 La 42.15(3) 2_564 4
Ga3 O1 La 114.0(3) . 4
Ga3 O1 La 90.82(17) 4_455 4
O2 O1 La 78.2(2) . 4
O2 O1 La 46.26(19) 3_565 4
O2 O1 La 163.5(2) 4_455 4
Nb O1 La 36.49(2) . 4
Ga1 O1 La 36.49(2) . 4
Ga1 O1 La 150.3(2) 1_455 4
Nb O1 La 150.3(2) 1_455 4
Ga1 O1 La 81.72(6) 1_565 4
Nb O1 La 81.72(6) 1_565 4
O3 O1 La 69.26(15) 1_556 4
O3 O1 La 76.43(17) 3_566 4
O3 O1 La 149.4(4) 4_456 4
La O1 La 94.41(14) 1_556 4
La O1 La 74.54(8) 2_566 4
La O1 La 124.8(3) 4_456 4
Ga2 O1 La 99.22(3) . 4
Ga2 O1 La 35.49(3) 1_665 4
Ga2 O1 La 142.68(10) 1_565 4
O1 O1 La 93.55(14) 2_455 4
O1 O1 La 25.24(8) 2_565 4
O1 O1 La 133.8(3) 2_465 4
O3 O1 La 23.42(14) 4 4
O3 O1 La 126.6(3) 3_455 4
O3 O1 La 97.84(19) 1_565 4
O1 O1 La 98.37(17) 1_556 4
O1 O1 La 81.63(18) 1_554 4
Ga3 O1 La 64.08(3) 4_446 4
Ga3 O1 La 65.95(3) 1_666 4
Ga3 O1 La 169.7(4) 2_465 4
O3 O1 La 24.00(13) 5 4
O3 O1 La 140.71(14) 2_455 4
O3 O1 La 99.71(13) 6_565 4
O3 O1 La 45.68(15) 4_556 4
O3 O1 La 133.0(2) 3_456 4
O3 O1 La 105.23(16) 1_566 4
O3 O1 La 58.58(15) 6_554 4
O3 O1 La 75.9(2) 2_564 4
O3 O1 La 113.6(3) 5_454 4
O2 O1 La 43.17(16) 4_554 4
O2 O1 La 98.0(2) 3_454 4
O2 O1 La 104.5(3) 1_564 4
O1 O1 La 100.51(9) 2_456 4
O1 O1 La 49.37(9) 2_566 4
O1 O1 La 136.5(3) 2_466 4
Ga2 O1 La 90.46(13) 1_554 4
Ga2 O1 La 35.40(5) 1_664 4
Ga2 O1 La 123.0(2) 1_564 4
Ga2 O1 La 98.37(17) 2_566 2_455
La O1 La 36.54(4) . 2_455
La O1 La 143.2(4) 2_565 2_455
La O1 La 81.67(11) 4_455 2_455
O2 O1 La 90.7(4) 6 2_455
O2 O1 La 48.9(3) 5_455 2_455
O2 O1 La 106.5(5) 2_565 2_455
O3 O1 La 78.2(3) 6 2_455
O3 O1 La 163.0(3) 2_565 2_455
O3 O1 La 45.3(3) 5_455 2_455
O2 O1 La 104.3(4) 6_556 2_455
O2 O1 La 68.3(3) 5_456 2_455
O2 O1 La 119.7(5) 2_566 2_455
Ga2 O1 La 81.63(17) 2_565 2_455
Ga3 O1 La 103.01(7) 2_565 2_455
Ga3 O1 La 41.10(7) 1_556 2_455
Ga3 O1 La 137.22(18) 4_456 2_455
O2 O1 La 126.7(3) 4 2_455
O2 O1 La 20.1(3) 3_455 2_455
O2 O1 La 115.0(3) 1_565 2_455
O3 O1 La 64.21(18) . 2_455
O3 O1 La 142.6(5) 3_565 2_455
O3 O1 La 55.31(17) 4_455 2_455
Ga3 O1 La 90.82(17) 2_564 2_455
Ga3 O1 La 42.15(3) . 2_455
Ga3 O1 La 114.0(3) 4_455 2_455
O2 O1 La 46.26(19) . 2_455
O2 O1 La 163.5(2) 3_565 2_455
O2 O1 La 78.2(2) 4_455 2_455
Nb O1 La 81.72(6) . 2_455
Ga1 O1 La 81.72(6) . 2_455
Ga1 O1 La 36.49(2) 1_455 2_455
Nb O1 La 36.49(2) 1_455 2_455
Ga1 O1 La 150.3(2) 1_565 2_455
Nb O1 La 150.3(2) 1_565 2_455
O3 O1 La 76.43(17) 1_556 2_455
O3 O1 La 149.4(4) 3_566 2_455
O3 O1 La 69.26(15) 4_456 2_455
La O1 La 74.54(9) 1_556 2_455
La O1 La 124.8(3) 2_566 2_455
La O1 La 94.41(13) 4_456 2_455
Ga2 O1 La 35.49(3) . 2_455
Ga2 O1 La 142.68(10) 1_665 2_455
Ga2 O1 La 99.22(3) 1_565 2_455
O1 O1 La 25.24(8) 2_455 2_455
O1 O1 La 133.8(3) 2_565 2_455
O1 O1 La 93.55(14) 2_465 2_455
O3 O1 La 97.84(19) 4 2_455
O3 O1 La 23.42(14) 3_455 2_455
O3 O1 La 126.6(3) 1_565 2_455
O1 O1 La 98.37(18) 1_556 2_455
O1 O1 La 81.63(17) 1_554 2_455
Ga3 O1 La 65.95(3) 4_446 2_455
Ga3 O1 La 169.7(4) 1_666 2_455
Ga3 O1 La 64.08(3) 2_465 2_455
O3 O1 La 99.71(14) 5 2_455
O3 O1 La 24.00(13) 2_455 2_455
O3 O1 La 140.71(14) 6_565 2_455
O3 O1 La 105.23(16) 4_556 2_455
O3 O1 La 45.68(15) 3_456 2_455
O3 O1 La 133.0(2) 1_566 2_455
O3 O1 La 75.9(2) 6_554 2_455
O3 O1 La 113.6(3) 2_564 2_455
O3 O1 La 58.58(15) 5_454 2_455
O2 O1 La 104.5(3) 4_554 2_455
O2 O1 La 43.17(16) 3_454 2_455
O2 O1 La 98.0(2) 1_564 2_455
O1 O1 La 49.37(9) 2_456 2_455
O1 O1 La 136.5(3) 2_566 2_455
O1 O1 La 100.51(9) 2_466 2_455
Ga2 O1 La 35.40(5) 1_554 2_455
Ga2 O1 La 123.0(2) 1_664 2_455
Ga2 O1 La 90.46(13) 1_564 2_455
La O1 La 117.92(9) 4 2_455
Ga2 O1 La 98.37(17) 2_566 1_565
La O1 La 143.2(4) . 1_565
La O1 La 81.67(11) 2_565 1_565
La O1 La 36.54(4) 4_455 1_565
O2 O1 La 106.5(5) 6 1_565
O2 O1 La 90.7(4) 5_455 1_565
O2 O1 La 48.9(3) 2_565 1_565
O3 O1 La 163.0(3) 6 1_565
O3 O1 La 45.3(3) 2_565 1_565
O3 O1 La 78.2(3) 5_455 1_565
O2 O1 La 119.7(5) 6_556 1_565
O2 O1 La 104.3(4) 5_456 1_565
O2 O1 La 68.3(3) 2_566 1_565
Ga2 O1 La 81.63(17) 2_565 1_565
Ga3 O1 La 137.22(18) 2_565 1_565
Ga3 O1 La 103.01(7) 1_556 1_565
Ga3 O1 La 41.10(7) 4_456 1_565
O2 O1 La 115.0(3) 4 1_565
O2 O1 La 126.7(3) 3_455 1_565
O2 O1 La 20.1(3) 1_565 1_565
O3 O1 La 142.6(5) . 1_565
O3 O1 La 55.31(17) 3_565 1_565
O3 O1 La 64.21(18) 4_455 1_565
Ga3 O1 La 114.0(3) 2_564 1_565
Ga3 O1 La 90.82(17) . 1_565
Ga3 O1 La 42.15(3) 4_455 1_565
O2 O1 La 163.5(2) . 1_565
O2 O1 La 78.2(2) 3_565 1_565
O2 O1 La 46.26(19) 4_455 1_565
Nb O1 La 150.3(2) . 1_565
Ga1 O1 La 150.3(2) . 1_565
Ga1 O1 La 81.72(6) 1_455 1_565
Nb O1 La 81.72(6) 1_455 1_565
Ga1 O1 La 36.49(2) 1_565 1_565
Nb O1 La 36.49(2) 1_565 1_565
O3 O1 La 149.4(4) 1_556 1_565
O3 O1 La 69.26(15) 3_566 1_565
O3 O1 La 76.43(17) 4_456 1_565
La O1 La 124.8(3) 1_556 1_565
La O1 La 94.41(13) 2_566 1_565
La O1 La 74.54(9) 4_456 1_565
Ga2 O1 La 142.68(10) . 1_565
Ga2 O1 La 99.22(3) 1_665 1_565
Ga2 O1 La 35.49(3) 1_565 1_565
O1 O1 La 133.8(3) 2_455 1_565
O1 O1 La 93.55(14) 2_565 1_565
O1 O1 La 25.24(8) 2_465 1_565
O3 O1 La 126.6(3) 4 1_565
O3 O1 La 97.84(19) 3_455 1_565
O3 O1 La 23.42(14) 1_565 1_565
O1 O1 La 98.37(17) 1_556 1_565
O1 O1 La 81.63(17) 1_554 1_565
Ga3 O1 La 169.7(4) 4_446 1_565
Ga3 O1 La 64.08(3) 1_666 1_565
Ga3 O1 La 65.95(3) 2_465 1_565
O3 O1 La 140.71(14) 5 1_565
O3 O1 La 99.71(14) 2_455 1_565
O3 O1 La 24.00(13) 6_565 1_565
O3 O1 La 133.0(2) 4_556 1_565
O3 O1 La 105.23(16) 3_456 1_565
O3 O1 La 45.68(15) 1_566 1_565
O3 O1 La 113.6(3) 6_554 1_565
O3 O1 La 58.58(15) 2_564 1_565
O3 O1 La 75.9(2) 5_454 1_565
O2 O1 La 98.0(2) 4_554 1_565
O2 O1 La 104.5(3) 3_454 1_565
O2 O1 La 43.17(16) 1_564 1_565
O1 O1 La 136.5(3) 2_456 1_565
O1 O1 La 100.50(9) 2_566 1_565
O1 O1 La 49.37(9) 2_466 1_565
Ga2 O1 La 123.0(2) 1_554 1_565
Ga2 O1 La 90.46(13) 1_664 1_565
Ga2 O1 La 35.40(5) 1_564 1_565
La O1 La 117.92(9) 4 1_565
La O1 La 117.92(9) 2_455 1_565
Ga2 O1 O3 86.5(2) 2_566 2
La O1 O3 42.01(18) . 2
La O1 O3 85.93(14) 2_565 2
La O1 O3 151.2(3) 4_455 2
O2 O1 O3 64.7(4) 6 2
O2 O1 O3 91.6(4) 5_455 2
O2 O1 O3 123.4(5) 2_565 2
O3 O1 O3 6.3(3) 6 2
O3 O1 O3 124.7(4) 2_565 2
O3 O1 O3 113.8(4) 5_455 2
O2 O1 O3 60.6(3) 6_556 2
O2 O1 O3 85.8(4) 5_456 2
O2 O1 O3 114.0(4) 2_566 2
Ga2 O1 O3 93.5(2) 2_565 2
Ga3 O1 O3 36.83(16) 2_565 2
Ga3 O1 O3 89.38(17) 1_556 2
Ga3 O1 O3 136.5(3) 4_456 2
O2 O1 O3 54.5(3) 4 2
O2 O1 O3 65.3(4) 3_455 2
O2 O1 O3 164.6(5) 1_565 2
O3 O1 O3 32.8(3) . 2
O3 O1 O3 112.34(16) 3_565 2
O3 O1 O3 123.29(17) 4_455 2
Ga3 O1 O3 56.57(12) 2_564 2
Ga3 O1 O3 93.37(18) . 2
Ga3 O1 O3 128.8(3) 4_455 2
O2 O1 O3 28.4(2) . 2
O2 O1 O3 91.3(2) 3_565 2
O2 O1 O3 146.2(2) 4_455 2
Nb O1 O3 18.08(12) . 2
Ga1 O1 O3 18.08(12) . 2
Ga1 O1 O3 108.77(15) 1_455 2
Nb O1 O3 108.77(15) 1_455 2
Ga1 O1 O3 131.47(15) 1_565 2
Nb O1 O3 131.47(15) 1_565 2
O3 O1 O3 35.5(2) 1_556 2
O3 O1 O3 105.92(19) 3_566 2
O3 O1 O3 115.1(2) 4_456 2
La O1 O3 63.14(14) 1_556 2
La O1 O3 84.19(19) 2_566 2
La O1 O3 113.1(3) 4_456 2
Ga2 O1 O3 49.74(14) . 2
Ga2 O1 O3 71.42(15) 1_665 2
Ga2 O1 O3 154.9(3) 1_565 2
O1 O1 O3 53.13(17) 2_455 2
O1 O1 O3 74.02(13) 2_565 2
O1 O1 O3 159.9(5) 2_465 2
O3 O1 O3 41.7(3) 4 2
O3 O1 O3 90.3(3) 3_455 2
O3 O1 O3 145.0(3) 1_565 2
O1 O1 O3 86.5(2) 1_556 2
O1 O1 O3 93.5(2) 1_554 2
Ga3 O1 O3 18.23(12) 4_446 2
Ga3 O1 O3 107.27(17) 1_666 2
Ga3 O1 O3 126.5(2) 2_465 2
O3 O1 O3 27.71(18) 5 2
O3 O1 O3 91.99(18) 2_455 2
O3 O1 O3 147.0(2) 6_565 2
O3 O1 O3 42.3(3) 4_556 2
O3 O1 O3 87.0(2) 3_456 2
O3 O1 O3 133.5(3) 1_566 2
O3 O1 O3 60.17(15) 6_554 2
O3 O1 O3 111.8(3) 2_564 2
O3 O1 O3 106.2(3) 5_454 2
O2 O1 O3 71.6(3) 4_554 2
O2 O1 O3 77.8(2) 3_454 2
O2 O1 O3 132.0(3) 1_564 2
O1 O1 O3 55.13(12) 2_456 2
O1 O1 O3 73.05(16) 2_566 2
O1 O1 O3 139.1(5) 2_466 2
Ga2 O1 O3 60.51(15) 1_554 2
Ga2 O1 O3 77.55(15) 1_664 2
Ga2 O1 O3 144.9(3) 1_564 2
La O1 O3 49.80(14) 4 2
La O1 O3 72.28(15) 2_455 2
La O1 O3 167.6(2) 1_565 2
Ga2 O1 O3 86.5(2) 2_566 5_565
La O1 O3 151.2(3) . 5_565
La O1 O3 42.00(18) 2_565 5_565
La O1 O3 85.93(14) 4_455 5_565
O2 O1 O3 91.6(4) 6 5_565
O2 O1 O3 123.4(5) 5_455 5_565
O2 O1 O3 64.7(4) 2_565 5_565
O3 O1 O3 113.8(4) 6 5_565
O3 O1 O3 6.3(3) 2_565 5_565
O3 O1 O3 124.7(4) 5_455 5_565
O2 O1 O3 85.8(4) 6_556 5_565
O2 O1 O3 114.0(4) 5_456 5_565
O2 O1 O3 60.6(3) 2_566 5_565
Ga2 O1 O3 93.5(2) 2_565 5_565
Ga3 O1 O3 89.38(17) 2_565 5_565
Ga3 O1 O3 136.5(3) 1_556 5_565
Ga3 O1 O3 36.83(16) 4_456 5_565
O2 O1 O3 65.3(4) 4 5_565
O2 O1 O3 164.6(5) 3_455 5_565
O2 O1 O3 54.5(4) 1_565 5_565
O3 O1 O3 123.29(17) . 5_565
O3 O1 O3 32.8(3) 3_565 5_565
O3 O1 O3 112.34(16) 4_455 5_565
Ga3 O1 O3 93.37(18) 2_564 5_565
Ga3 O1 O3 128.8(3) . 5_565
Ga3 O1 O3 56.57(12) 4_455 5_565
O2 O1 O3 146.2(2) . 5_565
O2 O1 O3 28.4(2) 3_565 5_565
O2 O1 O3 91.3(2) 4_455 5_565
Nb O1 O3 108.77(15) . 5_565
Ga1 O1 O3 108.77(15) . 5_565
Ga1 O1 O3 131.47(15) 1_455 5_565
Nb O1 O3 131.47(15) 1_455 5_565
Ga1 O1 O3 18.08(12) 1_565 5_565
Nb O1 O3 18.08(12) 1_565 5_565
O3 O1 O3 115.1(2) 1_556 5_565
O3 O1 O3 35.5(2) 3_566 5_565
O3 O1 O3 105.92(19) 4_456 5_565
La O1 O3 113.1(3) 1_556 5_565
La O1 O3 63.14(14) 2_566 5_565
La O1 O3 84.19(19) 4_456 5_565
Ga2 O1 O3 154.9(3) . 5_565
Ga2 O1 O3 49.74(14) 1_665 5_565
Ga2 O1 O3 71.42(15) 1_565 5_565
O1 O1 O3 159.9(5) 2_455 5_565
O1 O1 O3 53.12(17) 2_565 5_565
O1 O1 O3 74.02(13) 2_465 5_565
O3 O1 O3 90.3(3) 4 5_565
O3 O1 O3 145.0(3) 3_455 5_565
O3 O1 O3 41.7(3) 1_565 5_565
O1 O1 O3 86.5(2) 1_556 5_565
O1 O1 O3 93.5(2) 1_554 5_565
Ga3 O1 O3 126.5(2) 4_446 5_565
Ga3 O1 O3 18.23(12) 1_666 5_565
Ga3 O1 O3 107.27(17) 2_465 5_565
O3 O1 O3 91.99(18) 5 5_565
O3 O1 O3 147.0(2) 2_455 5_565
O3 O1 O3 27.71(18) 6_565 5_565
O3 O1 O3 87.0(2) 4_556 5_565
O3 O1 O3 133.5(3) 3_456 5_565
O3 O1 O3 42.3(3) 1_566 5_565
O3 O1 O3 106.2(3) 6_554 5_565
O3 O1 O3 60.17(15) 2_564 5_565
O3 O1 O3 111.8(3) 5_454 5_565
O2 O1 O3 77.8(2) 4_554 5_565
O2 O1 O3 132.0(3) 3_454 5_565
O2 O1 O3 71.6(3) 1_564 5_565
O1 O1 O3 139.1(5) 2_456 5_565
O1 O1 O3 55.13(12) 2_566 5_565
O1 O1 O3 73.05(16) 2_466 5_565
Ga2 O1 O3 144.9(3) 1_554 5_565
Ga2 O1 O3 60.51(15) 1_664 5_565
Ga2 O1 O3 77.55(15) 1_564 5_565
La O1 O3 72.28(15) 4 5_565
La O1 O3 167.6(2) 2_455 5_565
La O1 O3 49.80(14) 1_565 5_565
O3 O1 O3 119.63(4) 2 5_565
Ga2 O1 O3 86.5(2) 2_566 6_455
La O1 O3 85.93(14) . 6_455
La O1 O3 151.2(3) 2_565 6_455
La O1 O3 42.01(18) 4_455 6_455
O2 O1 O3 123.4(5) 6 6_455
O2 O1 O3 64.7(4) 5_455 6_455
O2 O1 O3 91.6(4) 2_565 6_455
O3 O1 O3 124.7(4) 6 6_455
O3 O1 O3 113.8(4) 2_565 6_455
O3 O1 O3 6.3(3) 5_455 6_455
O2 O1 O3 114.0(4) 6_556 6_455
O2 O1 O3 60.6(3) 5_456 6_455
O2 O1 O3 85.8(4) 2_566 6_455
Ga2 O1 O3 93.5(2) 2_565 6_455
Ga3 O1 O3 136.5(3) 2_565 6_455
Ga3 O1 O3 36.83(16) 1_556 6_455
Ga3 O1 O3 89.38(17) 4_456 6_455
O2 O1 O3 164.6(5) 4 6_455
O2 O1 O3 54.5(3) 3_455 6_455
O2 O1 O3 65.3(4) 1_565 6_455
O3 O1 O3 112.34(16) . 6_455
O3 O1 O3 123.29(17) 3_565 6_455
O3 O1 O3 32.8(3) 4_455 6_455
Ga3 O1 O3 128.8(3) 2_564 6_455
Ga3 O1 O3 56.57(12) . 6_455
Ga3 O1 O3 93.37(18) 4_455 6_455
O2 O1 O3 91.3(2) . 6_455
O2 O1 O3 146.2(2) 3_565 6_455
O2 O1 O3 28.4(2) 4_455 6_455
Nb O1 O3 131.47(15) . 6_455
Ga1 O1 O3 131.47(15) . 6_455
Ga1 O1 O3 18.08(12) 1_455 6_455
Nb O1 O3 18.08(12) 1_455 6_455
Ga1 O1 O3 108.77(15) 1_565 6_455
Nb O1 O3 108.77(15) 1_565 6_455
O3 O1 O3 105.92(19) 1_556 6_455
O3 O1 O3 115.1(2) 3_566 6_455
O3 O1 O3 35.5(2) 4_456 6_455
La O1 O3 84.2(2) 1_556 6_455
La O1 O3 113.1(3) 2_566 6_455
La O1 O3 63.14(14) 4_456 6_455
Ga2 O1 O3 71.42(15) . 6_455
Ga2 O1 O3 154.9(3) 1_665 6_455
Ga2 O1 O3 49.74(14) 1_565 6_455
O1 O1 O3 74.02(13) 2_455 6_455
O1 O1 O3 159.9(5) 2_565 6_455
O1 O1 O3 53.12(17) 2_465 6_455
O3 O1 O3 145.0(3) 4 6_455
O3 O1 O3 41.7(3) 3_455 6_455
O3 O1 O3 90.3(3) 1_565 6_455
O1 O1 O3 86.5(2) 1_556 6_455
O1 O1 O3 93.5(2) 1_554 6_455
Ga3 O1 O3 107.27(17) 4_446 6_455
Ga3 O1 O3 126.5(2) 1_666 6_455
Ga3 O1 O3 18.23(12) 2_465 6_455
O3 O1 O3 147.0(2) 5 6_455
O3 O1 O3 27.71(18) 2_455 6_455
O3 O1 O3 91.99(18) 6_565 6_455
O3 O1 O3 133.5(3) 4_556 6_455
O3 O1 O3 42.3(3) 3_456 6_455
O3 O1 O3 87.0(2) 1_566 6_455
O3 O1 O3 111.8(3) 6_554 6_455
O3 O1 O3 106.2(3) 2_564 6_455
O3 O1 O3 60.17(15) 5_454 6_455
O2 O1 O3 132.0(3) 4_554 6_455
O2 O1 O3 71.6(3) 3_454 6_455
O2 O1 O3 77.8(2) 1_564 6_455
O1 O1 O3 73.05(16) 2_456 6_455
O1 O1 O3 139.1(5) 2_566 6_455
O1 O1 O3 55.13(12) 2_466 6_455
Ga2 O1 O3 77.55(15) 1_554 6_455
Ga2 O1 O3 144.9(3) 1_664 6_455
Ga2 O1 O3 60.51(15) 1_564 6_455
La O1 O3 167.6(2) 4 6_455
La O1 O3 49.80(14) 2_455 6_455
La O1 O3 72.28(15) 1_565 6_455
O3 O1 O3 119.63(4) 2 6_455
O3 O1 O3 119.63(4) 5_565 6_455
Ga2 O1 O2 83.8(2) 2_566 1_665
La O1 O2 103.18(16) . 1_665
La O1 O2 31.6(2) 2_565 1_665
La O1 O2 137.2(3) 4_455 1_665
O2 O1 O2 67.9(4) 6 1_665
O2 O1 O2 126.5(4) 5_455 1_665
O2 O1 O2 92.9(6) 2_565 1_665
O3 O1 O2 60.2(3) 6 1_665
O3 O1 O2 58.9(3) 2_565 1_665
O3 O1 O2 167.3(6) 5_455 1_665
O2 O1 O2 58.6(5) 6_556 1_665
O2 O1 O2 111.8(5) 5_456 1_665
O2 O1 O2 82.6(4) 2_566 1_665
Ga2 O1 O2 96.2(2) 2_565 1_665
Ga3 O1 O2 41.57(18) 2_565 1_665
Ga3 O1 O2 139.3(4) 1_556 1_665
Ga3 O1 O2 80.58(16) 4_456 1_665
O2 O1 O2 12.5(4) 4 1_665
O2 O1 O2 129.0(5) 3_455 1_665
O2 O1 O2 106.6(4) 1_565 1_665
O3 O1 O2 77.9(2) . 1_665
O3 O1 O2 57.4(3) 3_565 1_665
O3 O1 O2 154.6(4) 4_455 1_665
Ga3 O1 O2 62.69(13) 2_564 1_665
Ga3 O1 O2 134.8(3) . 1_665
Ga3 O1 O2 89.6(2) 4_455 1_665
O2 O1 O2 93.4(2) . 1_665
O2 O1 O2 25.5(2) 3_565 1_665
O2 O1 O2 142.8(3) 4_455 1_665
Nb O1 O2 56.91(16) . 1_665
Ga1 O1 O2 56.91(16) . 1_665
Ga1 O1 O2 173.2(3) 1_455 1_665
Nb O1 O2 173.2(3) 1_455 1_665
Ga1 O1 O2 67.16(18) 1_565 1_665
Nb O1 O2 67.16(18) 1_565 1_665
O3 O1 O2 72.5(3) 1_556 1_665
O3 O1 O2 53.59(19) 3_566 1_665
O3 O1 O2 133.7(4) 4_456 1_665
La O1 O2 90.3(3) 1_556 1_665
La O1 O2 56.07(15) 2_566 1_665
La O1 O2 105.6(3) 4_456 1_665
Ga2 O1 O2 110.9(2) . 1_665
Ga2 O1 O2 13.69(13) 1_665 1_665
Ga2 O1 O2 120.60(19) 1_565 1_665
O1 O1 O2 115.25(16) 2_455 1_665
O1 O1 O2 27.0(3) 2_565 1_665
O1 O1 O2 125.3(2) 2_465 1_665
O3 O1 O2 46.19(18) 4 1_665
O3 O1 O2 149.5(3) 3_455 1_665
O3 O1 O2 88.2(2) 1_565 1_665
O1 O1 O2 83.8(2) 1_556 1_665
O1 O1 O2 96.2(2) 1_554 1_665
Ga3 O1 O2 75.4(2) 4_446 1_665
Ga3 O1 O2 43.96(15) 1_666 1_665
Ga3 O1 O2 150.2(3) 2_465 1_665
O3 O1 O2 38.4(2) 5 1_665
O3 O1 O2 156.2(3) 2_455 1_665
O3 O1 O2 81.2(2) 6_565 1_665
O3 O1 O2 42.7(2) 4_556 1_665
O3 O1 O2 133.1(4) 3_456 1_665
O3 O1 O2 82.4(2) 1_566 1_665
O3 O1 O2 79.7(2) 6_554 1_665
O3 O1 O2 79.1(3) 2_564 1_665
O3 O1 O2 129.7(3) 5_454 1_665
O2 O1 O2 58.37(13) 4_554 1_665
O2 O1 O2 119.9(3) 3_454 1_665
O2 O1 O2 106.2(4) 1_564 1_665
O1 O1 O2 105.8(3) 2_456 1_665
O1 O1 O2 30.15(17) 2_566 1_665
O1 O1 O2 113.7(3) 2_466 1_665
Ga2 O1 O2 113.36(17) 1_554 1_665
Ga2 O1 O2 43.46(15) 1_664 1_665
Ga2 O1 O2 121.7(3) 1_564 1_665
La O1 O2 22.91(13) 4 1_665
La O1 O2 138.01(17) 2_455 1_665
La O1 O2 103.01(18) 1_565 1_665
O3 O1 O2 66.0(2) 2 1_665
O3 O1 O2 53.7(2) 5_565 1_665
O3 O1 O2 168.5(3) 6_455 1_665
Ga3 O2 Ga2 117.1(8) 4_446 .
Ga3 O2 La 119.1(7) 4_446 4_445
Ga2 O2 La 104.0(8) . 4_445
Ga3 O2 O3 64.9(6) 4_446 6
Ga2 O2 O3 118.7(8) . 6
La O2 O3 129.2(7) 4_445 6
Ga3 O2 La 116.2(9) 4_446 .
Ga2 O2 La 92.0(6) . .
La O2 La 104.3(5) 4_445 .
O3 O2 La 51.4(4) 6 .
Ga3 O2 O3 40.3(4) 4_446 2
Ga2 O2 O3 157.4(8) . 2
La O2 O3 91.2(5) 4_445 2
O3 O2 O3 58.9(6) 6 2
La O2 O3 100.4(7) . 2
Ga3 O2 O1 157.3(8) 4_446 2_455
Ga2 O2 O1 84.6(6) . 2_455
La O2 O1 55.9(3) 4_445 2_455
O3 O2 O1 100.2(6) 6 2_455
La O2 O1 52.9(3) . 2_455
O3 O2 O1 117.9(6) 2 2_455
Ga3 O2 O2 140.2(10) 4_446 4_445
Ga2 O2 O2 40.8(3) . 4_445
La O2 O2 63.3(7) 4_445 4_445
O3 O2 O2 148.5(9) 6 4_445
La O2 O2 99.6(5) . 4_445
O3 O2 O2 150.8(11) 2 4_445
O1 O2 O2 60.7(3) 2_455 4_445
Ga3 O2 O2 131.8(9) 4_446 3_455
Ga2 O2 O2 40.8(3) . 3_455
La O2 O2 108.9(5) 4_445 3_455
O3 O2 O2 89.1(9) 6 3_455
La O2 O2 51.3(5) . 3_455
O3 O2 O2 147.9(11) 2 3_455
O1 O2 O2 60.7(3) 2_455 3_455
O2 O2 O2 60.000(1) 4_445 3_455
Ga3 O2 O3 36.2(4) 4_446 1_556
Ga2 O2 O3 87.6(5) . 1_556
La O2 O3 153.1(7) 4_445 1_556
O3 O2 O3 59.5(6) 6 1_556
La O2 O3 99.3(6) . 1_556
O3 O2 O3 71.9(6) 2 1_556
O1 O2 O3 150.6(7) 2_455 1_556
O2 O2 O3 125.1(3) 4_445 1_556
O2 O2 O3 95.8(6) 3_455 1_556
Ga3 O2 O2 37.2(7) 4_446 2_556
Ga2 O2 O2 98.8(7) . 2_556
La O2 O2 97.0(6) 4_445 2_556
O3 O2 O2 102.0(4) 6 2_556
La O2 O2 153.0(4) . 2_556
O3 O2 O2 62.3(5) 2 2_556
O1 O2 O2 152.4(6) 2_455 2_556
O2 O2 O2 104.8(5) 4_445 2_556
O2 O2 O2 135.5(5) 3_455 2_556
O3 O2 O2 56.9(5) 1_556 2_556
Ga3 O2 O1 87.7(5) 4_446 2_456
Ga2 O2 O1 29.6(3) . 2_456
La O2 O1 120.0(7) 4_445 2_456
O3 O2 O1 110.6(6) 6 2_456
La O2 O1 109.4(5) . 2_456
O3 O2 O1 127.9(6) 2 2_456
O1 O2 O1 114.2(5) 2_455 2_456
O2 O2 O1 63.3(3) 4_445 2_456
O2 O2 O1 63.3(3) 3_455 2_456
O3 O2 O1 61.9(4) 1_556 2_456
O2 O2 O1 72.6(5) 2_556 2_456
Ga3 O2 O3 97.1(7) 4_446 .
Ga2 O2 O3 135.4(8) . .
La O2 O3 80.3(5) 4_445 .
O3 O2 O3 50.3(5) 6 .
La O2 O3 45.3(4) . .
O3 O2 O3 62.9(5) 2 .
O1 O2 O3 60.8(4) 2_455 .
O2 O2 O3 121.2(3) 4_445 .
O2 O2 O3 95.2(6) 3_455 .
O3 O2 O3 108.5(7) 1_556 .
O2 O2 O3 125.1(6) 2_556 .
O1 O2 O3 153.5(6) 2_456 .
Ga3 O2 Nb 63.5(5) 4_446 .
Ga2 O2 Nb 152.2(9) . .
La O2 Nb 98.2(4) 4_445 .
O3 O2 Nb 34.1(3) 6 .
La O2 Nb 66.1(4) . .
O3 O2 Nb 34.2(3) 2 .
O1 O2 Nb 94.4(5) 2_455 .
O2 O2 Nb 154.1(2) 4_445 .
O2 O2 Nb 115.7(9) 3_455 .
O3 O2 Nb 79.7(5) 1_556 .
O2 O2 Nb 94.8(4) 2_556 .
O1 O2 Nb 140.6(5) 2_456 .
O3 O2 Nb 33.6(3) . .
Ga3 O2 Ga1 63.5(5) 4_446 .
Ga2 O2 Ga1 152.2(9) . .
La O2 Ga1 98.2(4) 4_445 .
O3 O2 Ga1 34.1(3) 6 .
La O2 Ga1 66.1(4) . .
O3 O2 Ga1 34.2(3) 2 .
O1 O2 Ga1 94.4(5) 2_455 .
O2 O2 Ga1 154.1(2) 4_445 .
O2 O2 Ga1 115.7(9) 3_455 .
O3 O2 Ga1 79.7(5) 1_556 .
O2 O2 Ga1 94.8(4) 2_556 .
O1 O2 Ga1 140.6(5) 2_456 .
O3 O2 Ga1 33.6(3) . .
Nb O2 Ga1 0.0 . .
Ga3 O2 O1 74.8(6) 4_446 1_545
Ga2 O2 O1 124.5(9) . 1_545
La O2 O1 44.6(3) 4_445 1_545
O3 O2 O1 115.1(5) 6 1_545
La O2 O1 133.5(6) . 1_545
O3 O2 O1 57.4(4) 2 1_545
O1 O2 O1 98.8(4) 2_455 1_545
O2 O2 O1 93.5(9) 4_445 1_545
O2 O2 O1 151.6(8) 3_455 1_545
O3 O2 O1 108.9(6) 1_556 1_545
O2 O2 O1 56.7(5) 2_556 1_545
O1 O2 O1 116.3(6) 2_456 1_545
O3 O2 O1 90.1(5) . 1_545
Nb O2 O1 83.2(3) . 1_545
Ga1 O2 O1 83.2(3) . 1_545
Ga3 O2 O2 97.3(6) 4_446 2
Ga2 O2 O2 141.6(6) . 2
La O2 O2 40.1(4) 4_445 2
O3 O2 O2 90.1(4) 6 2
La O2 O2 87.0(5) . 2
O3 O2 O2 58.6(5) 2 2
O1 O2 O2 64.5(5) 2_455 2
O2 O2 O2 101.6(3) 4_445 2
O2 O2 O2 124.0(5) 3_455 2
O3 O2 O2 130.5(5) 1_556 2
O2 O2 O2 99.2(8) 2_556 2
O1 O2 O2 158.7(5) 2_456 2
O3 O2 O2 46.6(4) . 2
Nb O2 O2 58.1(2) . 2
Ga1 O2 O2 58.1(2) . 2
O1 O2 O2 46.6(4) 1_545 2
Ga3 O2 Ga2 58.6(5) 4_446 2_556
Ga2 O2 Ga2 108.4(8) . 2_556
La O2 Ga2 67.1(4) 4_445 2_556
O3 O2 Ga2 118.0(5) 6 2_556
La O2 Ga2 159.0(5) . 2_556
O3 O2 Ga2 62.0(4) 2 2_556
O1 O2 Ga2 123.0(5) 2_455 2_556
O2 O2 Ga2 93.4(9) 4_445 2_556
O2 O2 Ga2 148.7(8) 3_455 2_556
O3 O2 Ga2 86.3(5) 1_556 2_556
O2 O2 Ga2 30.0(3) 2_556 2_556
O1 O2 Ga2 91.1(5) 2_456 2_556
O3 O2 Ga2 113.7(4) . 2_556
Nb O2 Ga2 95.4(3) . 2_556
Ga1 O2 Ga2 95.4(3) . 2_556
O1 O2 Ga2 28.2(3) 1_545 2_556
O2 O2 Ga2 74.2(5) 2 2_556
Ga3 O2 O3 111.8(8) 4_446 5_445
Ga2 O2 O3 78.4(7) . 5_445
La O2 O3 35.7(4) 4_445 5_445
O3 O2 O3 162.6(6) 6 5_445
La O2 O3 129.8(5) . 5_445
O3 O2 O3 106.8(6) 2 5_445
O1 O2 O3 77.1(4) 2_455 5_445
O2 O2 O3 44.2(8) 4_445 5_445
O2 O2 O3 103.9(7) 3_455 5_445
O3 O2 O3 128.8(6) 1_556 5_445
O2 O2 O3 76.8(3) 2_556 5_445
O1 O2 O3 85.8(5) 2_456 5_445
O3 O2 O3 115.9(5) . 5_445
Nb O2 O3 128.5(4) . 5_445
Ga1 O2 O3 128.5(4) . 5_445
O1 O2 O3 49.5(3) 1_545 5_445
O2 O2 O3 73.1(3) 2 5_445
Ga2 O2 O3 53.7(3) 2_556 5_445
Ga3 O2 Ga3 50.6(5) 4_446 2_565
Ga2 O2 Ga3 108.5(6) . 2_565
La O2 Ga3 146.5(6) 4_445 2_565
O3 O2 Ga3 21.1(3) 6 2_565
La O2 Ga3 67.1(4) . 2_565
O3 O2 Ga3 60.7(4) 2 2_565
O1 O2 Ga3 119.1(6) 2_455 2_565
O2 O2 Ga3 148.0(7) 4_445 2_565
O2 O2 Ga3 91.0(8) 3_455 2_565
O3 O2 Ga3 38.4(4) 1_556 2_565
O2 O2 Ga3 86.0(3) 2_556 2_565
O1 O2 Ga3 92.8(4) 2_456 2_565
O3 O2 Ga3 71.1(4) . 2_565
Nb O2 Ga3 48.4(2) . 2_565
Ga1 O2 Ga3 48.4(2) . 2_565
O1 O2 Ga3 117.0(4) 1_545 2_565
O2 O2 Ga3 106.4(2) 2 2_565
Ga2 O2 Ga3 108.8(4) 2_556 2_565
O3 O2 Ga3 162.4(5) 5_445 2_565
Ga3 O2 La 66.3(5) 4_446 4_446
Ga2 O2 La 62.1(5) . 4_446
La O2 La 101.0(6) 4_445 4_446
O3 O2 La 122.1(5) 6 4_446
La O2 La 147.6(4) . 4_446
O3 O2 La 99.0(5) 2 4_446
O1 O2 La 134.7(6) 2_455 4_446
O2 O2 La 74.2(4) 4_445 4_446
O2 O2 La 101.3(3) 3_455 4_446
O3 O2 La 62.8(4) 1_556 4_446
O2 O2 La 36.9(3) 2_556 4_446
O1 O2 La 39.0(2) 2_456 4_446
O3 O2 La 161.9(5) . 4_446
Nb O2 La 129.6(4) . 4_446
Ga1 O2 La 129.6(4) . 4_446
O1 O2 La 78.9(5) 1_545 4_446
O2 O2 La 125.3(6) 2 4_446
Ga2 O2 La 52.3(3) 2_556 4_446
O3 O2 La 67.2(4) 5_445 4_446
Ga3 O2 La 101.1(3) 2_565 4_446
Ga3 O2 La 68.3(4) 4_446 1_556
Ga2 O2 La 56.0(4) . 1_556
La O2 La 156.3(7) 4_445 1_556
O3 O2 La 74.4(4) 6 1_556
La O2 La 90.1(4) . 1_556
O3 O2 La 104.8(5) 2 1_556
O1 O2 La 126.2(5) 2_455 1_556
O2 O2 La 96.3(3) 4_445 1_556
O2 O2 La 65.7(4) 3_455 1_556
O3 O2 La 33.0(3) 1_556 1_556
O2 O2 La 76.0(5) 2_556 1_556
O1 O2 La 36.38(17) 2_456 1_556
O3 O2 La 122.4(5) . 1_556
Nb O2 La 104.8(4) . 1_556
Ga1 O2 La 104.8(4) . 1_556
O1 O2 La 132.6(6) 1_545 1_556
O2 O2 La 162.2(3) 2 1_556
Ga2 O2 La 104.8(4) 2_556 1_556
O3 O2 La 121.2(5) 5_445 1_556
Ga3 O2 La 56.6(2) 2_565 1_556
La O2 La 59.8(2) 4_446 1_556
Ga3 O2 Ga3 102.8(6) 4_446 4_445
Ga2 O2 Ga3 139.5(6) . 4_445
La O2 Ga3 57.9(3) 4_445 4_445
O3 O2 Ga3 71.6(4) 6 4_445
La O2 Ga3 62.8(3) . 4_445
O3 O2 Ga3 63.0(4) 2 4_445
O1 O2 Ga3 54.9(3) 2_455 4_445
O2 O2 Ga3 108.9(3) 4_445 4_445
O2 O2 Ga3 106.3(3) 3_455 4_445
O3 O2 Ga3 125.6(6) 1_556 4_445
O2 O2 Ga3 118.1(6) 2_556 4_445
O1 O2 Ga3 168.8(5) 2_456 4_445
O3 O2 Ga3 22.9(2) . 4_445
Nb O2 Ga3 45.85(19) . 4_445
Ga1 O2 Ga3 45.85(19) . 4_445
O1 O2 Ga3 70.7(4) 1_545 4_445
O2 O2 Ga3 24.7(3) 2 4_445
Ga2 O2 Ga3 97.4(3) 2_556 4_445
O3 O2 Ga3 93.5(4) 5_445 4_445
Ga3 O2 Ga3 91.2(4) 2_565 4_445
La O2 Ga3 149.5(4) 4_446 4_445
La O2 Ga3 145.2(5) 1_556 4_445
Ga3 O2 La 167.3(6) 4_446 2_455
Ga2 O2 La 50.2(4) . 2_455
La O2 La 69.4(4) 4_445 2_455
O3 O2 La 118.3(6) 6 2_455
La O2 La 67.4(3) . 2_455
O3 O2 La 152.4(5) 2 2_455
O1 O2 La 34.8(3) 2_455 2_455
O2 O2 La 32.4(3) 4_445 2_455
O2 O2 La 39.8(4) 3_455 2_455
O3 O2 La 132.9(4) 1_556 2_455
O2 O2 La 137.1(3) 2_556 2_455
O1 O2 La 79.7(4) 2_456 2_455
O3 O2 La 93.6(4) . 2_455
Nb O2 La 126.6(5) . 2_455
Ga1 O2 La 126.6(5) . 2_455
O1 O2 La 112.1(4) 1_545 2_455
O2 O2 La 95.0(5) 2 2_455
Ga2 O2 La 122.5(5) 2_556 2_455
O3 O2 La 69.0(4) 5_445 2_455
Ga3 O2 La 128.0(4) 2_565 2_455
La O2 La 103.8(4) 4_446 2_455
La O2 La 100.1(3) 1_556 2_455
Ga3 O2 La 89.6(3) 4_445 2_455
Ga3 O2 O3 1.3(3) 4_446 3_556
Ga2 O2 O3 118.4(6) . 3_556
La O2 O3 118.1(5) 4_445 3_556
O3 O2 O3 64.8(5) 6 3_556
La O2 O3 116.2(6) . 3_556
O3 O2 O3 39.1(4) 2 3_556
O1 O2 O3 156.2(6) 2_455 3_556
O2 O2 O3 140.8(7) 4_445 3_556
O2 O2 O3 132.9(7) 3_455 3_556
O3 O2 O3 37.4(4) 1_556 3_556
O2 O2 O3 37.3(3) 2_556 3_556
O1 O2 O3 88.9(4) 2_456 3_556
O3 O2 O3 96.2(4) . 3_556
Nb O2 O3 62.7(3) . 3_556
Ga1 O2 O3 62.7(3) . 3_556
O1 O2 O3 73.8(4) 1_545 3_556
O2 O2 O3 96.0(5) 2 3_556
Ga2 O2 O3 58.2(3) 2_556 3_556
O3 O2 O3 111.5(5) 5_445 3_556
Ga3 O2 O3 50.9(2) 2_565 3_556
La O2 O3 67.1(3) 4_446 3_556
La O2 O3 69.6(3) 1_556 3_556
Ga3 O2 O3 101.6(4) 4_445 3_556
La O2 O3 168.6(4) 2_455 3_556
Ga3 O2 O3 97.2(7) 4_446 4_446
Ga2 O2 O3 50.7(5) . 4_446
La O2 O3 75.5(5) 4_445 4_446
O3 O2 O3 153.9(5) 6 4_446
La O2 O3 139.6(5) . 4_446
O3 O2 O3 120.1(7) 2 4_446
O1 O2 O3 102.0(5) 2_455 4_446
O2 O2 O3 43.2(4) 4_445 4_446
O2 O2 O3 89.8(5) 3_455 4_446
O3 O2 O3 94.6(6) 1_556 4_446
O2 O2 O3 61.9(3) 2_556 4_446
O1 O2 O3 46.9(3) 2_456 4_446
O3 O2 O3 155.6(5) . 4_446
Nb O2 O3 154.2(5) . 4_446
Ga1 O2 O3 154.2(5) . 4_446
O1 O2 O3 74.8(5) 1_545 4_446
O2 O2 O3 111.8(4) 2 4_446
Ga2 O2 O3 58.9(4) 2_556 4_446
O3 O2 O3 39.9(4) 5_445 4_446
Ga3 O2 O3 132.8(4) 2_565 4_446
La O2 O3 33.1(2) 4_446 4_446
La O2 O3 81.3(3) 1_556 4_446
Ga3 O2 O3 133.4(4) 4_445 4_446
La O2 O3 75.2(3) 2_455 4_446
O3 O2 O3 97.7(5) 3_556 4_446
Ga3 O2 Ga3 121.9(8) 4_446 2_455
Ga2 O2 Ga3 42.5(5) . 2_455
La O2 Ga3 65.5(4) 4_445 2_455
O3 O2 Ga3 160.9(5) 6 2_455
La O2 Ga3 117.6(4) . 2_455
O3 O2 Ga3 138.8(7) 2 2_455
O1 O2 Ga3 77.9(4) 2_455 2_455
O2 O2 Ga3 18.6(4) 4_445 2_455
O2 O2 Ga3 73.3(5) 3_455 2_455
O3 O2 Ga3 114.0(5) 1_556 2_455
O2 O2 Ga3 86.2(3) 2_556 2_455
O1 O2 Ga3 55.1(3) 2_456 2_455
O3 O2 Ga3 136.8(4) . 2_455
Nb O2 Ga3 163.7(4) . 2_455
Ga1 O2 Ga3 163.7(4) . 2_455
O1 O2 Ga3 83.8(4) 1_545 2_455
O2 O2 Ga3 105.64(18) 2 2_455
Ga2 O2 Ga3 77.4(4) 2_556 2_455
O3 O2 Ga3 36.0(3) 5_445 2_455
Ga3 O2 Ga3 147.8(3) 2_565 2_455
La O2 Ga3 56.8(3) 4_446 2_455
La O2 Ga3 91.3(3) 1_556 2_455
Ga3 O2 Ga3 119.8(4) 4_445 2_455
La O2 Ga3 51.0(2) 2_455 2_455
O3 O2 Ga3 122.5(5) 3_556 2_455
O3 O2 Ga3 24.72(18) 4_446 2_455
Ga3 O2 Ga3 116.6(6) 4_446 1_556
Ga2 O2 Ga3 38.6(4) . 1_556
La O2 Ga3 123.5(5) 4_445 1_556
O3 O2 Ga3 83.0(5) 6 1_556
La O2 Ga3 56.5(3) . 1_556
O3 O2 Ga3 140.5(6) 2 1_556
O1 O2 Ga3 75.8(4) 2_455 1_556
O2 O2 Ga3 68.6(5) 4_445 1_556
O2 O2 Ga3 15.4(4) 3_455 1_556
O3 O2 Ga3 80.5(4) 1_556 1_556
O2 O2 Ga3 123.0(6) 2_556 1_556
O1 O2 Ga3 53.5(2) 2_456 1_556
O3 O2 Ga3 101.8(5) . 1_556
Nb O2 Ga3 114.3(5) . 1_556
Ga1 O2 Ga3 114.3(5) . 1_556
O1 O2 Ga3 161.8(6) 1_545 1_556
O2 O2 Ga3 137.8(7) 2 1_556
Ga2 O2 Ga3 144.4(5) 2_556 1_556
O3 O2 Ga3 112.5(5) 5_445 1_556
Ga3 O2 Ga3 80.2(3) 2_565 1_556
La O2 Ga3 92.5(3) 4_446 1_556
La O2 Ga3 50.46(15) 1_556 1_556
Ga3 O2 Ga3 117.1(4) 4_445 1_556
La O2 Ga3 54.04(18) 2_455 1_556
O3 O2 Ga3 117.8(3) 3_556 1_556
O3 O2 Ga3 89.2(3) 4_446 1_556
Ga3 O2 Ga3 78.1(3) 2_455 1_556
Ga3 O2 Ga2 144.6(7) 4_446 1_554
Ga2 O2 Ga2 97.7(5) . 1_554
La O2 Ga2 52.2(3) 4_445 1_554
O3 O2 Ga2 93.8(5) 6 1_554
La O2 Ga2 52.5(2) . 1_554
O3 O2 Ga2 104.9(5) 2 1_554
O1 O2 Ga2 13.0(2) 2_455 1_554
O2 O2 Ga2 71.54(16) 4_445 1_554
O2 O2 Ga2 71.54(16) 3_455 1_554
O3 O2 Ga2 151.3(7) 1_556 1_554
O2 O2 Ga2 148.0(6) 2_556 1_554
O1 O2 Ga2 127.2(5) 2_456 1_554
O3 O2 Ga2 49.7(3) . 1_554
Nb O2 Ga2 82.9(3) . 1_554
Ga1 O2 Ga2 82.9(3) . 1_554
O1 O2 Ga2 91.3(4) 1_545 1_554
O2 O2 Ga2 52.7(4) 2 1_554
Ga2 O2 Ga2 118.1(4) 2_556 1_554
O3 O2 Ga2 79.8(3) 5_445 1_554
Ga3 O2 Ga2 114.3(5) 2_565 1_554
La O2 Ga2 143.6(5) 4_446 1_554
La O2 Ga2 135.6(4) 1_556 1_554
Ga3 O2 Ga2 41.94(14) 4_445 1_554
La O2 Ga2 47.73(16) 2_455 1_554
O3 O2 Ga2 143.5(4) 3_556 1_554
O3 O2 Ga2 110.5(4) 4_446 1_554
Ga3 O2 Ga2 87.6(3) 2_455 1_554
Ga3 O2 Ga2 86.1(3) 1_556 1_554
Ga3 O2 O2 63.0(5) 4_446 6_556
Ga2 O2 O2 85.0(5) . 6_556
La O2 O2 166.7(9) 4_445 6_556
O3 O2 O2 38.1(4) 6 6_556
La O2 O2 65.1(5) . 6_556
O3 O2 O2 83.2(5) 2 6_556
O1 O2 O2 116.4(7) 2_455 6_556
O2 O2 O2 124.7(5) 4_445 6_556
O2 O2 O2 71.5(7) 3_455 6_556
O3 O2 O2 34.5(4) 1_556 6_556
O2 O2 O2 91.2(6) 2_556 6_556
O1 O2 O2 72.5(3) 2_456 6_556
O3 O2 O2 86.4(6) . 6_556
Nb O2 O2 70.5(4) . 6_556
Ga1 O2 O2 70.5(4) . 6_556
O1 O2 O2 136.8(3) 1_545 6_556
O2 O2 O2 128.1(4) 2 6_556
Ga2 O2 O2 119.8(4) 2_556 6_556
O3 O2 O2 157.7(7) 5_445 6_556
Ga3 O2 O2 23.5(2) 2_565 6_556
La O2 O2 91.9(4) 4_446 6_556
La O2 O2 36.5(2) 1_556 6_556
Ga3 O2 O2 108.9(6) 4_445 6_556
La O2 O2 111.1(3) 2_455 6_556
O3 O2 O2 63.8(3) 3_556 6_556
O3 O2 O2 117.7(5) 4_446 6_556
Ga3 O2 O2 125.8(4) 2_455 6_556
Ga3 O2 O2 58.7(2) 1_556 6_556
Ga2 O2 O2 117.6(6) 1_554 6_556
Ga3 O2 La 60.2(4) 4_446 2
Ga2 O2 La 157.6(9) . 2
La O2 La 64.7(3) 4_445 2
O3 O2 La 81.5(4) 6 2
La O2 La 109.2(5) . 2
O3 O2 La 26.8(3) 2 2
O1 O2 La 102.3(4) 2_455 2
O2 O2 La 125.0(8) 4_445 2
O2 O2 La 158.9(4) 3_455 2
O3 O2 La 95.6(4) 1_556 2
O2 O2 La 65.3(5) 2_556 2
O1 O2 La 137.8(5) 2_456 2
O3 O2 La 64.3(3) . 2
Nb O2 La 49.51(18) . 2
Ga1 O2 La 49.51(18) . 2
O1 O2 La 33.88(16) 1_545 2
O2 O2 La 37.9(4) 2 2
Ga2 O2 La 49.91(18) 2_556 2
O3 O2 La 82.4(4) 5_445 2
Ga3 O2 La 87.0(3) 2_565 2
La O2 La 99.7(4) 4_446 2
La O2 La 128.4(4) 1_556 2
Ga3 O2 La 52.81(16) 4_445 2
La O2 La 131.5(3) 2_455 2
O3 O2 La 58.9(3) 3_556 2
O3 O2 La 106.9(5) 4_446 2
Ga3 O2 La 117.6(4) 2_455 2
Ga3 O2 La 163.7(5) 1_556 2
Ga2 O2 La 90.2(2) 1_554 2
O2 O2 La 109.9(3) 6_556 2
Ga3 O2 O3 69.9(5) 4_446 3
Ga2 O2 O3 170.8(8) . 3
La O2 O3 75.7(4) 4_445 3
O3 O2 O3 57.7(5) 6 3
La O2 O3 79.3(4) . 3
O3 O2 O3 30.3(5) 2 3
O1 O2 O3 87.8(4) 2_455 3
O2 O2 O3 137.5(5) 4_445 3
O2 O2 O3 130.3(7) 3_455 3
O3 O2 O3 96.6(5) 1_556 3
O2 O2 O3 90.3(5) 2_556 3
O1 O2 O3 157.4(6) 2_456 3
O3 O2 O3 35.4(3) . 3
Nb O2 O3 23.63(19) . 3
Ga1 O2 O3 23.63(19) . 3
O1 O2 O3 61.8(3) 1_545 3
O2 O2 O3 36.1(3) 2 3
Ga2 O2 O3 80.1(3) 2_556 3
O3 O2 O3 104.9(4) 5_445 3
Ga3 O2 O3 70.9(3) 2_565 3
La O2 O3 127.0(4) 4_446 3
La O2 O3 126.1(5) 1_556 3
Ga3 O2 O3 32.9(2) 4_445 3
La O2 O3 122.6(4) 2_455 3
O3 O2 O3 68.7(3) 3_556 3
O3 O2 O3 136.5(5) 4_446 3
Ga3 O2 O3 140.3(4) 2_455 3
Ga3 O2 O3 134.0(5) 1_556 3
Ga2 O2 O3 74.8(3) 1_554 3
O2 O2 O3 93.8(5) 6_556 3
La O2 O3 30.28(18) 2 3
Ga3 O2 O3 137.3(7) 4_446 4_445
Ga2 O2 O3 86.8(6) . 4_445
La O2 O3 19.6(3) 4_445 4_445
O3 O2 O3 136.0(5) 6 4_445
La O2 O3 96.1(4) . 4_445
O3 O2 O3 110.3(5) 2 4_445
O1 O2 O3 43.5(2) 2_455 4_445
O2 O2 O3 46.3(5) 4_445 4_445
O2 O2 O3 89.8(5) 3_455 4_445
O3 O2 O3 163.8(7) 1_556 4_445
O2 O2 O3 109.1(4) 2_556 4_445
O1 O2 O3 108.0(5) 2_456 4_445
O3 O2 O3 86.0(4) . 4_445
Nb O2 O3 111.5(4) . 4_445
Ga1 O2 O3 111.5(4) . 4_445
O1 O2 O3 62.7(3) 1_545 4_445
O2 O2 O3 55.3(3) 2 4_445
Ga2 O2 O3 81.1(4) 2_556 4_445
O3 O2 O3 35.0(4) 5_445 4_445
Ga3 O2 O3 157.1(5) 2_565 4_445
La O2 O3 101.2(5) 4_446 4_445
La O2 O3 142.5(4) 1_556 4_445
Ga3 O2 O3 66.6(3) 4_445 4_445
La O2 O3 50.1(2) 2_455 4_445
O3 O2 O3 136.4(5) 3_556 4_445
O3 O2 O3 70.1(3) 4_446 4_445
Ga3 O2 O3 53.3(3) 2_455 4_445
Ga3 O2 O3 104.1(3) 1_556 4_445
Ga2 O2 O3 44.82(19) 1_554 4_445
O2 O2 O3 159.1(5) 6_556 4_445
La O2 O3 84.1(3) 2 4_445
O3 O2 O3 91.3(4) 3 4_445
Ga3 O2 O2 73.5(6) 4_446 5_446
Ga2 O2 O2 85.6(9) . 5_446
La O2 O2 66.9(3) 4_445 5_446
O3 O2 O2 137.8(7) 6 5_446
La O2 O2 169.9(7) . 5_446
O3 O2 O2 85.2(5) 2 5_446
O1 O2 O2 117.0(6) 2_455 5_446
O2 O2 O2 72.3(9) 4_445 5_446
O2 O2 O2 125.4(9) 3_455 5_446
O3 O2 O2 90.4(7) 1_556 5_446
O2 O2 O2 37.0(4) 2_556 5_446
O1 O2 O2 72.8(6) 2_456 5_446
O3 O2 O2 133.6(5) . 5_446
Nb O2 O2 118.8(5) . 5_446
Ga1 O2 O2 118.8(5) . 5_446
O1 O2 O2 43.5(3) 1_545 5_446
O2 O2 O2 88.7(4) 2 5_446
Ga2 O2 O2 23.41(15) 2_556 5_446
O3 O2 O2 40.0(3) 5_445 5_446
Ga3 O2 O2 123.0(5) 2_565 5_446
La O2 O2 37.2(4) 4_446 5_446
La O2 O2 96.7(6) 1_556 5_446
Ga3 O2 O2 113.4(3) 4_445 5_446
La O2 O2 103.8(6) 2_455 5_446
O3 O2 O2 73.4(4) 3_556 5_446
O3 O2 O2 35.6(5) 4_446 5_446
Ga3 O2 O2 55.0(4) 2_455 5_446
Ga3 O2 O2 123.3(6) 1_556 5_446
Ga2 O2 O2 118.0(4) 1_554 5_446
O2 O2 O2 124.4(7) 6_556 5_446
La O2 O2 72.2(3) 2 5_446
O3 O2 O2 102.5(4) 3 5_446
O3 O2 O2 74.0(4) 4_445 5_446
Ga3 O2 O2 93.6(7) 4_446 5_456
Ga2 O2 O2 51.7(5) . 5_456
La O2 O2 147.0(7) 4_445 5_456
O3 O2 O2 67.1(5) 6 5_456
La O2 O2 60.8(2) . 5_456
O3 O2 O2 119.4(7) 2 5_456
O1 O2 O2 95.9(5) 2_455 5_456
O2 O2 O2 89.0(5) 4_445 5_456
O2 O2 O2 38.2(5) 3_455 5_456
O3 O2 O2 57.9(4) 1_556 5_456
O2 O2 O2 107.8(7) 2_556 5_456
O1 O2 O2 51.8(3) 2_456 5_456
O3 O2 O2 101.8(5) . 5_456
Nb O2 O2 101.1(5) . 5_456
Ga1 O2 O2 101.1(5) . 5_456
O1 O2 O2 164.4(7) 1_545 5_456
O2 O2 O2 147.5(7) 2 5_456
Ga2 O2 O2 136.3(5) 2_556 5_456
O3 O2 O2 130.1(7) 5_445 5_456
Ga3 O2 O2 59.0(3) 2_565 5_456
La O2 O2 87.0(4) 4_446 5_456
La O2 O2 31.8(3) 1_556 5_456
Ga3 O2 O2 122.9(5) 4_445 5_456
La O2 O2 77.5(4) 2_455 5_456
O3 O2 O2 94.7(5) 3_556 5_456
O3 O2 O2 96.9(5) 4_446 5_456
Ga3 O2 O2 94.1(5) 2_455 5_456
Ga3 O2 O2 23.5(2) 1_556 5_456
Ga2 O2 O2 104.0(4) 1_554 5_456
O2 O2 O2 36.2(4) 6_556 5_456
La O2 O2 146.0(6) 2 5_456
O3 O2 O2 124.4(6) 3 5_456
O3 O2 O2 127.6(5) 4_445 5_456
O2 O2 O2 123.8(7) 5_446 5_456
Ga3 O2 O1 97.8(7) 4_446 .
Ga2 O2 O1 84.6(6) . .
La O2 O1 130.3(6) 4_445 .
O3 O2 O1 39.7(3) 6 .
La O2 O1 26.1(3) . .
O3 O2 O1 98.3(6) 2 .
O1 O2 O1 77.0(5) 2_455 .
O2 O2 O1 108.9(6) 4_445 .
O2 O2 O1 49.6(6) 3_455 .
O3 O2 O1 74.1(5) 1_556 .
O2 O2 O1 130.5(4) 2_556 .
O1 O2 O1 91.4(4) 2_456 .
O3 O2 O1 62.1(4) . .
Nb O2 O1 68.2(4) . .
Ga1 O2 O1 68.2(4) . .
O1 O2 O1 150.5(6) 1_545 .
O2 O2 O1 108.3(6) 2 .
Ga2 O2 O1 156.1(4) 2_556 .
O3 O2 O1 150.2(5) 5_445 .
Ga3 O2 O1 47.3(2) 2_565 .
La O2 O1 125.0(4) 4_446 .
La O2 O1 65.3(3) 1_556 .
Ga3 O2 O1 83.6(4) 4_445 .
La O2 O1 81.2(3) 2_455 .
O3 O2 O1 98.2(4) 3_556 .
O3 O2 O1 134.7(4) 4_446 .
Ga3 O2 O1 122.8(3) 2_455 .
Ga3 O2 O1 46.09(19) 1_556 .
Ga2 O2 O1 78.3(4) 1_554 .
O2 O2 O1 39.6(3) 6_556 .
La O2 O1 117.6(4) 2 .
O3 O2 O1 88.7(4) 3 .
O3 O2 O1 120.4(4) 4_445 .
O2 O2 O1 162.0(6) 5_446 .
O2 O2 O1 39.7(2) 5_456 .
Ga3 O2 O3 44.0(5) 4_446 5
Ga2 O2 O3 140.8(7) . 5
La O2 O3 115.1(5) 4_445 5
O3 O2 O3 29.2(3) 6 5
La O2 O3 76.9(4) . 5
O3 O2 O3 30.2(4) 2 5
O1 O2 O3 115.1(5) 2_455 5
O2 O2 O3 175.8(4) 4_445 5
O2 O2 O3 118.2(9) 3_455 5
O3 O2 O3 58.2(5) 1_556 5
O2 O2 O3 79.2(3) 2_556 5
O1 O2 O3 119.9(5) 2_456 5
O3 O2 O3 54.7(4) . 5
Nb O2 O3 21.97(19) . 5
Ga1 O2 O3 21.97(19) . 5
O1 O2 O3 87.4(4) 1_545 5
O2 O2 O3 76.1(3) 2 5
Ga2 O2 O3 89.4(4) 2_556 5
O3 O2 O3 136.9(5) 5_445 5
Ga3 O2 O3 32.5(2) 2_565 5
La O2 O3 110.0(4) 4_446 5
La O2 O3 86.1(3) 1_556 5
Ga3 O2 O3 67.6(3) 4_445 5
La O2 O3 143.7(5) 2_455 5
O3 O2 O3 43.3(3) 3_556 5
O3 O2 O3 140.9(4) 4_446 5
Ga3 O2 O3 165.4(5) 2_455 5
Ga3 O2 O3 110.6(4) 1_556 5
Ga2 O2 O3 104.3(4) 1_554 5
O2 O2 O3 56.1(3) 6_556 5
La O2 O3 55.1(3) 2 5
O3 O2 O3 40.1(4) 3 5
O3 O2 O3 131.3(3) 4_445 5
O2 O2 O3 111.0(5) 5_446 5
O2 O2 O3 91.2(5) 5_456 5
O1 O2 O3 68.9(3) . 5
Ga3 O2 Ga2 85.9(6) 4_446 2_566
Ga2 O2 Ga2 74.1(5) . 2_566
La O2 Ga2 150.5(6) 4_445 2_566
O3 O2 Ga2 44.6(4) 6 2_566
La O2 Ga2 47.2(3) . 2_566
O3 O2 Ga2 100.6(5) 2 2_566
O1 O2 Ga2 94.9(5) 2_455 2_566
O2 O2 Ga2 108.5(6) 4_445 2_566
O2 O2 Ga2 50.4(6) 3_455 2_566
O3 O2 Ga2 55.8(4) 1_556 2_566
O2 O2 Ga2 112.4(5) 2_556 2_566
O1 O2 Ga2 73.0(3) 2_456 2_566
O3 O2 Ga2 81.3(4) . 2_566
Nb O2 Ga2 78.3(4) . 2_566
Ga1 O2 Ga2 78.3(4) . 2_566
O1 O2 Ga2 157.7(5) 1_545 2_566
O2 O2 Ga2 127.9(5) 2 2_566
Ga2 O2 Ga2 142.0(4) 2_556 2_566
O3 O2 Ga2 152.1(5) 5_445 2_566
Ga3 O2 Ga2 40.72(17) 2_565 2_566
La O2 Ga2 103.6(3) 4_446 2_566
La O2 Ga2 43.83(16) 1_556 2_566
Ga3 O2 Ga2 103.8(4) 4_445 2_566
La O2 Ga2 89.0(3) 2_455 2_566
O3 O2 Ga2 86.7(3) 3_556 2_566
O3 O2 Ga2 119.4(4) 4_446 2_566
Ga3 O2 Ga2 116.4(3) 2_455 2_566
Ga3 O2 Ga2 39.92(14) 1_556 2_566
Ga2 O2 Ga2 98.4(4) 1_554 2_566
O2 O2 Ga2 22.9(2) 6_556 2_566
La O2 Ga2 125.6(4) 2 2_566
O3 O2 Ga2 101.4(4) 3 2_566
O3 O2 Ga2 136.3(4) 4_445 2_566
O2 O2 Ga2 140.4(5) 5_446 2_566
O2 O2 Ga2 22.9(2) 5_456 2_566
O1 O2 Ga2 21.6(2) . 2_566
O3 O2 Ga2 70.8(3) 5 2_566
Ga3 O2 Nb 23.4(3) 4_446 1_556
Ga2 O2 Nb 97.7(5) . 1_556
La O2 Nb 141.1(6) 4_445 1_556
O3 O2 Nb 60.9(4) 6 1_556
La O2 Nb 106.8(5) . 1_556
O3 O2 Nb 60.7(4) 2 1_556
O1 O2 Nb 159.6(6) 2_455 1_556
O2 O2 Nb 131.7(2) 4_445 1_556
O2 O2 Nb 108.7(6) 3_455 1_556
O3 O2 Nb 12.9(3) 1_556 1_556
O2 O2 Nb 47.5(3) 2_556 1_556
O1 O2 Nb 70.0(3) 2_456 1_556
O3 O2 Nb 105.9(4) . 1_556
Nb O2 Nb 74.1(3) . 1_556
Ga1 O2 Nb 74.1(3) . 1_556
O1 O2 Nb 96.5(4) 1_545 1_556
O2 O2 Nb 119.3(4) 2 1_556
Ga2 O2 Nb 75.6(3) 2_556 1_556
O3 O2 Nb 123.2(5) 5_445 1_556
Ga3 O2 Nb 40.99(15) 2_565 1_556
La O2 Nb 61.8(2) 4_446 1_556
La O2 Nb 45.23(14) 1_556 1_556
Ga3 O2 Nb 119.0(4) 4_445 1_556
La O2 Nb 145.3(3) 2_455 1_556
O3 O2 Nb 24.61(17) 3_556 1_556
O3 O2 Nb 94.9(4) 4_446 1_556
Ga3 O2 Nb 117.3(4) 2_455 1_556
Ga3 O2 Nb 93.4(3) 1_556 1_556
Ga2 O2 Nb 154.5(5) 1_554 1_556
O2 O2 Nb 44.2(2) 6_556 1_556
La O2 Nb 83.2(3) 2 1_556
O3 O2 Nb 87.6(4) 3 1_556
O3 O2 Nb 156.5(5) 4_445 1_556
O2 O2 Nb 83.3(5) 5_446 1_556
O2 O2 Nb 70.7(4) 5_456 1_556
O1 O2 Nb 83.0(3) . 1_556
O3 O2 Nb 52.1(2) 5 1_556
Ga2 O2 Nb 66.7(2) 2_566 1_556
Ga3 O2 Ga1 23.4(3) 4_446 1_556
Ga2 O2 Ga1 97.7(5) . 1_556
La O2 Ga1 141.1(6) 4_445 1_556
O3 O2 Ga1 60.9(4) 6 1_556
La O2 Ga1 106.8(5) . 1_556
O3 O2 Ga1 60.7(4) 2 1_556
O1 O2 Ga1 159.6(6) 2_455 1_556
O2 O2 Ga1 131.7(2) 4_445 1_556
O2 O2 Ga1 108.7(6) 3_455 1_556
O3 O2 Ga1 12.9(3) 1_556 1_556
O2 O2 Ga1 47.5(3) 2_556 1_556
O1 O2 Ga1 70.0(3) 2_456 1_556
O3 O2 Ga1 105.9(4) . 1_556
Nb O2 Ga1 74.1(3) . 1_556
Ga1 O2 Ga1 74.1(3) . 1_556
O1 O2 Ga1 96.5(4) 1_545 1_556
O2 O2 Ga1 119.3(4) 2 1_556
Ga2 O2 Ga1 75.6(3) 2_556 1_556
O3 O2 Ga1 123.2(5) 5_445 1_556
Ga3 O2 Ga1 40.99(15) 2_565 1_556
La O2 Ga1 61.8(2) 4_446 1_556
La O2 Ga1 45.23(14) 1_556 1_556
Ga3 O2 Ga1 119.0(4) 4_445 1_556
La O2 Ga1 145.3(3) 2_455 1_556
O3 O2 Ga1 24.61(17) 3_556 1_556
O3 O2 Ga1 94.9(4) 4_446 1_556
Ga3 O2 Ga1 117.3(4) 2_455 1_556
Ga3 O2 Ga1 93.4(3) 1_556 1_556
Ga2 O2 Ga1 154.5(5) 1_554 1_556
O2 O2 Ga1 44.2(2) 6_556 1_556
La O2 Ga1 83.2(3) 2 1_556
O3 O2 Ga1 87.6(4) 3 1_556
O3 O2 Ga1 156.5(5) 4_445 1_556
O2 O2 Ga1 83.3(5) 5_446 1_556
O2 O2 Ga1 70.7(4) 5_456 1_556
O1 O2 Ga1 83.0(3) . 1_556
O3 O2 Ga1 52.1(2) 5 1_556
Ga2 O2 Ga1 66.7(2) 2_566 1_556
Nb O2 Ga1 0.0 1_556 1_556
Ga3 O2 Ga3 23.0(4) 4_446 1_656
Ga2 O2 Ga3 136.0(6) . 1_656
La O2 Ga3 114.3(4) 4_445 1_656
O3 O2 Ga3 48.1(3) 6 1_656
La O2 Ga3 98.4(5) . 1_656
O3 O2 Ga3 23.7(3) 2 1_656
O1 O2 Ga3 134.6(5) 2_455 1_656
O2 O2 Ga3 161.9(7) 4_445 1_656
O2 O2 Ga3 132.5(9) 3_455 1_656
O3 O2 Ga3 48.6(3) 1_556 1_656
O2 O2 Ga3 57.1(3) 2_556 1_656
O1 O2 Ga3 108.1(4) 2_456 1_656
O3 O2 Ga3 74.1(4) . 1_656
Nb O2 Ga3 40.49(17) . 1_656
Ga1 O2 Ga3 40.49(17) . 1_656
O1 O2 Ga3 75.8(3) 1_545 1_656
O2 O2 Ga3 81.8(3) 2 1_656
Ga2 O2 Ga3 70.2(2) 2_556 1_656
O3 O2 Ga3 122.6(4) 5_445 1_656
Ga3 O2 Ga3 41.53(16) 2_565 1_656
La O2 Ga3 89.2(3) 4_446 1_656
La O2 Ga3 81.2(3) 1_556 1_656
Ga3 O2 Ga3 81.7(3) 4_445 1_656
La O2 Ga3 165.7(5) 2_455 1_656
O3 O2 Ga3 22.19(18) 3_556 1_656
O3 O2 Ga3 118.9(4) 4_446 1_656
Ga3 O2 Ga3 143.3(4) 2_455 1_656
Ga3 O2 Ga3 120.5(4) 1_556 1_656
Ga2 O2 Ga3 122.4(4) 1_554 1_656
O2 O2 Ga3 61.86(19) 6_556 1_656
La O2 Ga3 49.65(16) 2 1_656
O3 O2 Ga3 49.4(3) 3 1_656
O3 O2 Ga3 133.7(4) 4_445 1_656
O2 O2 Ga3 90.1(4) 5_446 1_656
O2 O2 Ga3 97.6(5) 5_456 1_656
O1 O2 Ga3 86.5(3) . 1_656
O3 O2 Ga3 22.03(18) 5 1_656
Ga2 O2 Ga3 82.1(3) 2_566 1_656
Nb O2 Ga3 38.36(12) 1_556 1_656
Ga1 O2 Ga3 38.36(12) 1_556 1_656
Ga3 O2 O2 98.1(7) 4_446 6
Ga2 O2 O2 113.8(6) . 6
La O2 O2 104.2(6) 4_445 6
O3 O2 O2 35.0(4) 6 6
La O2 O2 23.0(3) . 6
O3 O2 O2 77.4(5) 2 6
O1 O2 O2 65.2(4) 2_455 6
O2 O2 O2 120.5(4) 4_445 6
O2 O2 O2 73.6(6) 3_455 6
O3 O2 O2 92.6(6) 1_556 6
O2 O2 O2 134.64(11) 2_556 6
O1 O2 O2 125.3(5) 2_456 6
O3 O2 O2 28.2(3) . 6
Nb O2 O2 43.2(3) . 6
Ga1 O2 O2 43.2(3) . 6
O1 O2 O2 117.7(4) 1_545 6
O2 O2 O2 74.7(5) 2 6
Ga2 O2 O2 137.6(3) 2_556 6
O3 O2 O2 138.1(5) 5_445 6
Ga3 O2 O2 54.9(3) 2_565 6
La O2 O2 154.6(5) 4_446 6
La O2 O2 96.4(5) 1_556 6
Ga3 O2 O2 50.3(3) 4_445 6
La O2 O2 88.1(3) 2_455 6
O3 O2 O2 97.7(4) 3_556 6
O3 O2 O2 162.5(3) 4_446 6
Ga3 O2 O2 139.1(3) 2_455 6
Ga3 O2 O2 76.2(3) 1_556 6
Ga2 O2 O2 59.4(3) 1_554 6
O2 O2 O2 62.8(5) 6_556 6
La O2 O2 88.2(3) 2 6
O3 O2 O2 58.0(3) 3 6
O3 O2 O2 103.6(4) 4_445 6
O2 O2 O2 160.4(4) 5_446 6
O2 O2 O2 73.6(4) 5_456 6
O1 O2 O2 33.9(3) . 6
O3 O2 O2 55.6(3) 5 6
Ga2 O2 O2 53.5(3) 2_566 6
Nb O2 O2 95.7(4) 1_556 6
Ga1 O2 O2 95.7(4) 1_556 6
Ga3 O2 O2 77.6(3) 1_656 6
Ga3 O2 O2 107.1(5) 4_446 5_445
Ga2 O2 O2 114.6(8) . 5_445
La O2 O2 12.5(2) 4_445 5_445
O3 O2 O2 123.0(6) 6 5_445
La O2 O2 109.4(5) . 5_445
O3 O2 O2 79.1(5) 2 5_445
O1 O2 O2 65.5(5) 2_455 5_445
O2 O2 O2 74.3(8) 4_445 5_445
O2 O2 O2 121.1(7) 3_455 5_445
O3 O2 O2 142.3(5) 1_556 5_445
O2 O2 O2 88.5(4) 2_556 5_445
O1 O2 O2 125.9(7) 2_456 5_445
O3 O2 O2 77.7(4) . 5_445
Nb O2 O2 89.8(4) . 5_445
Ga1 O2 O2 89.8(4) . 5_445
O1 O2 O2 33.5(3) 1_545 5_445
O2 O2 O2 33.0(4) 2 5_445
Ga2 O2 O2 58.52(12) 2_556 5_445
O3 O2 O2 40.1(3) 5_445 5_445
Ga3 O2 O2 137.0(5) 2_565 5_445
La O2 O2 99.6(4) 4_446 5_445
La O2 O2 159.3(6) 1_556 5_445
Ga3 O2 O2 54.8(3) 4_445 5_445
La O2 O2 81.9(4) 2_455 5_445
O3 O2 O2 106.0(4) 3_556 5_445
O3 O2 O2 79.3(4) 4_446 5_445
Ga3 O2 O2 73.9(4) 2_455 5_445
Ga3 O2 O2 135.9(5) 1_556 5_445
Ga2 O2 O2 59.6(3) 1_554 5_445
O2 O2 O2 160.3(6) 6_556 5_445
La O2 O2 52.5(2) 2 5_445
O3 O2 O2 66.5(4) 3 5_445
O3 O2 O2 32.0(4) 4_445 5_445
O2 O2 O2 63.09(10) 5_446 5_445
O2 O2 O2 159.3(7) 5_456 5_445
O1 O2 O2 134.9(5) . 5_445
O3 O2 O2 104.6(5) 5 5_445
Ga2 O2 O2 156.5(5) 2_566 5_445
Nb O2 O2 129.7(4) 1_556 5_445
Ga1 O2 O2 129.7(4) 1_556 5_445
Ga3 O2 O2 102.0(4) 1_656 5_445
O2 O2 O2 104.3(5) 6 5_445
Ga3 O2 O2 127.1(9) 4_446 5_455
Ga2 O2 O2 86.0(5) . 5_455
La O2 O2 97.0(6) 4_445 5_455
O3 O2 O2 62.3(4) 6 5_455
La O2 O2 10.88(7) . 5_455
O3 O2 O2 108.9(7) 2 5_455
O1 O2 O2 43.2(4) 2_455 5_455
O2 O2 O2 89.1(5) 4_445 5_455
O2 O2 O2 45.5(3) 3_455 5_455
O3 O2 O2 108.1(5) 1_556 5_455
O2 O2 O2 163.6(4) 2_556 5_455
O1 O2 O2 107.3(4) 2_456 5_455
O3 O2 O2 49.7(5) . 5_455
Nb O2 O2 74.8(5) . 5_455
Ga1 O2 O2 74.8(5) . 5_455
O1 O2 O2 132.3(6) 1_545 5_455
O2 O2 O2 86.2(7) 2 5_455
Ga2 O2 O2 160.4(5) 2_556 5_455
O3 O2 O2 119.5(5) 5_445 5_455
Ga3 O2 O2 77.6(3) 2_565 5_455
La O2 O2 146.2(4) 4_446 5_455
La O2 O2 94.2(2) 1_556 5_455
Ga3 O2 O2 63.5(5) 4_445 5_455
La O2 O2 56.8(3) 2_455 5_455
O3 O2 O2 127.1(6) 3_556 5_455
O3 O2 O2 130.4(5) 4_446 5_455
Ga3 O2 O2 107.3(5) 2_455 5_455
Ga3 O2 O2 53.79(16) 1_556 5_455
Ga2 O2 O2 44.8(4) 1_554 5_455
O2 O2 O2 73.6(4) 6_556 5_455
La O2 O2 113.8(6) 2 5_455
O3 O2 O2 85.0(5) 3 5_455
O3 O2 O2 86.7(5) 4_445 5_455
O2 O2 O2 159.3(7) 5_446 5_455
O2 O2 O2 63.09(10) 5_456 5_455
O1 O2 O2 34.0(2) . 5_455
O3 O2 O2 87.2(5) 5 5_455
Ga2 O2 O2 53.65(11) 2_566 5_455
Nb O2 O2 116.5(4) 1_556 5_455
Ga1 O2 O2 116.5(4) 1_556 5_455
Ga3 O2 O2 108.9(5) 1_656 5_455
O2 O2 O2 32.2(4) 6 5_455
O2 O2 O2 103.8(5) 5_445 5_455
Ga3 O2 O2 123.4(5) 4_446 1_554
Ga2 O2 O2 119.1(5) . 1_554
La O2 O2 51.0(5) 4_445 1_554
O3 O2 O2 83.2(4) 6 1_554
La O2 O2 56.6(3) . 1_554
O3 O2 O2 83.4(4) 2 1_554
O1 O2 O2 34.5(3) 2_455 1_554
O2 O2 O2 90.000(2) 4_445 1_554
O2 O2 O2 90.000(1) 3_455 1_554
O3 O2 O2 142.1(5) 1_556 1_554
O2 O2 O2 133.7(5) 2_556 1_554
O1 O2 O2 148.7(3) 2_456 1_554
O3 O2 O2 33.6(3) . 1_554
Nb O2 O2 64.2(2) . 1_554
Ga1 O2 O2 64.2(2) . 1_554
O1 O2 O2 79.2(4) 1_545 1_554
O2 O2 O2 34.5(5) 2 1_554
Ga2 O2 O2 107.4(2) 2_556 1_554
O3 O2 O2 85.3(3) 5_445 1_554
Ga3 O2 O2 104.3(2) 2_565 1_554
La O2 O2 152.0(2) 4_446 1_554
La O2 O2 146.8(3) 1_556 1_554
Ga3 O2 O2 20.6(2) 4_445 1_554
La O2 O2 69.1(2) 2_455 1_554
O3 O2 O2 122.2(3) 3_556 1_554
O3 O2 O2 122.9(3) 4_446 1_554
Ga3 O2 O2 103.62(19) 2_455 1_554
Ga3 O2 O2 103.2(2) 1_556 1_554
Ga2 O2 O2 21.45(19) 1_554 1_554
O2 O2 O2 116.1(5) 6_556 1_554
La O2 O2 70.2(2) 2 1_554
O3 O2 O2 53.5(3) 3 1_554
O3 O2 O2 52.8(3) 4_445 1_554
O2 O2 O2 116.2(3) 5_446 1_554
O2 O2 O2 116.2(3) 5_456 1_554
O1 O2 O2 81.7(3) . 1_554
O3 O2 O2 86.1(2) 5 1_554
Ga2 O2 O2 103.3(2) 2_566 1_554
Nb O2 O2 138.3(2) 1_556 1_554
Ga1 O2 O2 138.3(2) 1_556 1_554
Ga3 O2 O2 101.98(18) 1_656 1_554
O2 O2 O2 53.3(3) 6 1_554
O2 O2 O2 53.2(3) 5_445 1_554
O2 O2 O2 53.2(3) 5_455 1_554
Ga3 O2 O2 56.6(5) 4_446 1_556
Ga2 O2 O2 60.9(5) . 1_556
La O2 O2 129.0(5) 4_445 1_556
O3 O2 O2 96.8(4) 6 1_556
La O2 O2 123.4(3) . 1_556
O3 O2 O2 96.6(4) 2 1_556
O1 O2 O2 145.5(3) 2_455 1_556
O2 O2 O2 90.000(1) 4_445 1_556
O2 O2 O2 90.000(2) 3_455 1_556
O3 O2 O2 37.9(5) 1_556 1_556
O2 O2 O2 46.3(5) 2_556 1_556
O1 O2 O2 31.3(3) 2_456 1_556
O3 O2 O2 146.4(3) . 1_556
Nb O2 O2 115.8(2) . 1_556
Ga1 O2 O2 115.8(2) . 1_556
O1 O2 O2 100.8(4) 1_545 1_556
O2 O2 O2 145.5(5) 2 1_556
Ga2 O2 O2 72.6(2) 2_556 1_556
O3 O2 O2 94.7(3) 5_445 1_556
Ga3 O2 O2 75.7(2) 2_565 1_556
La O2 O2 28.0(2) 4_446 1_556
La O2 O2 33.2(3) 1_556 1_556
Ga3 O2 O2 159.4(2) 4_445 1_556
La O2 O2 110.9(2) 2_455 1_556
O3 O2 O2 57.8(3) 3_556 1_556
O3 O2 O2 57.1(3) 4_446 1_556
Ga3 O2 O2 76.38(19) 2_455 1_556
Ga3 O2 O2 76.8(2) 1_556 1_556
Ga2 O2 O2 158.55(19) 1_554 1_556
O2 O2 O2 63.9(5) 6_556 1_556
La O2 O2 109.8(2) 2 1_556
O3 O2 O2 126.5(3) 3 1_556
O3 O2 O2 127.2(3) 4_445 1_556
O2 O2 O2 63.8(3) 5_446 1_556
O2 O2 O2 63.8(3) 5_456 1_556
O1 O2 O2 98.3(3) . 1_556
O3 O2 O2 93.9(2) 5 1_556
Ga2 O2 O2 76.7(2) 2_566 1_556
Nb O2 O2 41.7(2) 1_556 1_556
Ga1 O2 O2 41.7(2) 1_556 1_556
Ga3 O2 O2 78.02(18) 1_656 1_556
O2 O2 O2 126.7(3) 6 1_556
O2 O2 O2 126.8(3) 5_445 1_556
O2 O2 O2 126.8(3) 5_455 1_556
O2 O2 O2 179.999(9) 1_554 1_556
Ga3 O2 O3 31.8(4) 4_446 4_556
Ga2 O2 O3 109.9(6) . 4_556
La O2 O3 143.9(5) 4_445 4_556
O3 O2 O3 38.1(4) 6 4_556
La O2 O3 86.6(5) . 4_556
O3 O2 O3 52.8(5) 2 4_556
O1 O2 O3 138.1(6) 2_455 4_556
O2 O2 O3 149.7(3) 4_445 4_556
O2 O2 O3 104.7(8) 3_455 4_556
O3 O2 O3 25.3(3) 1_556 4_556
O2 O2 O3 66.5(3) 2_556 4_556
O1 O2 O3 86.7(4) 2_456 4_556
O3 O2 O3 84.0(4) . 4_556
Nb O2 O3 54.5(3) . 4_556
Ga1 O2 O3 54.5(3) . 4_556
O1 O2 O3 103.6(4) 1_545 4_556
O2 O2 O3 108.4(3) 2 4_556
Ga2 O2 O3 90.4(3) 2_556 4_556
O3 O2 O3 143.1(4) 5_445 4_556
Ga3 O2 O3 19.55(17) 2_565 4_556
La O2 O3 84.7(3) 4_446 4_556
La O2 O3 53.9(3) 1_556 4_556
Ga3 O2 O3 100.3(4) 4_445 4_556
La O2 O3 144.2(4) 2_455 4_556
O3 O2 O3 32.3(2) 3_556 4_556
O3 O2 O3 117.8(4) 4_446 4_556
Ga3 O2 O3 139.0(4) 2_455 4_556
Ga3 O2 O3 91.4(4) 1_556 4_556
Ga2 O2 O3 131.6(5) 1_554 4_556
O2 O2 O3 33.2(2) 6_556 4_556
La O2 O3 79.3(3) 2 4_556
O3 O2 O3 72.7(3) 3 4_556
O3 O2 O3 163.1(5) 4_445 4_556
O2 O2 O3 103.4(5) 5_446 4_556
O2 O2 O3 68.1(5) 5_456 4_556
O1 O2 O3 66.1(3) . 4_556
O3 O2 O3 33.2(3) 5 4_556
Ga2 O2 O3 55.3(3) 2_566 4_556
Nb O2 O3 22.93(15) 1_556 4_556
Ga1 O2 O3 22.93(15) 1_556 4_556
Ga3 O2 O3 29.66(19) 1_656 4_556
O2 O2 O3 73.0(4) 6 4_556
O2 O2 O3 131.7(5) 5_445 4_556
O2 O2 O3 97.2(4) 5_455 4_556
O2 O2 O3 117.4(2) 1_554 4_556
O2 O2 O3 62.6(2) 1_556 4_556
Ga3 O2 Ga3 94.5(7) 4_446 1_546
Ga2 O2 Ga3 79.0(6) . 1_546
La O2 Ga3 50.6(4) 4_445 1_546
O3 O2 Ga3 156.9(5) 6 1_546
La O2 Ga3 148.5(5) . 1_546
O3 O2 Ga3 98.9(5) 2 1_546
O1 O2 Ga3 96.0(4) 2_455 1_546
O2 O2 Ga3 54.6(7) 4_445 1_546
O2 O2 Ga3 113.2(7) 3_455 1_546
O3 O2 Ga3 110.2(6) 1_556 1_546
O2 O2 Ga3 58.3(2) 2_556 1_546
O1 O2 Ga3 76.9(4) 2_456 1_546
O3 O2 Ga3 128.4(4) . 1_546
Nb O2 Ga3 128.6(4) . 1_546
Ga1 O2 Ga3 128.6(4) . 1_546
O1 O2 Ga3 45.5(3) 1_545 1_546
O2 O2 Ga3 82.1(3) 2 1_546
Ga2 O2 Ga3 39.0(2) 2_556 1_546
O3 O2 Ga3 18.96(19) 5_445 1_546
Ga3 O2 Ga3 144.3(4) 2_565 1_546
La O2 Ga3 50.4(2) 4_446 1_546
La O2 Ga3 108.6(4) 1_556 1_546
Ga3 O2 Ga3 105.5(3) 4_445 1_546
La O2 Ga3 84.2(3) 2_455 1_546
O3 O2 Ga3 94.3(4) 3_556 1_546
O3 O2 Ga3 30.6(3) 4_446 1_546
Ga3 O2 Ga3 39.95(18) 2_455 1_546
Ga3 O2 Ga3 117.1(4) 1_556 1_546
Ga2 O2 Ga3 98.5(3) 1_554 1_546
O2 O2 Ga3 142.2(6) 6_556 1_546
La O2 Ga3 79.1(3) 2 1_546
O3 O2 Ga3 107.0(4) 3 1_546
O3 O2 Ga3 53.7(3) 4_445 1_546
O2 O2 Ga3 21.4(2) 5_446 1_546
O2 O2 Ga3 127.5(5) 5_456 1_546
O1 O2 Ga3 162.7(4) . 1_546
O3 O2 Ga3 128.0(4) 5 1_546
Ga2 O2 Ga3 149.8(3) 2_566 1_546
Nb O2 Ga3 104.3(3) 1_556 1_546
Ga1 O2 Ga3 104.3(3) 1_556 1_546
Ga3 O2 Ga3 109.1(3) 1_656 1_546
O2 O2 Ga3 154.8(4) 6 1_546
O2 O2 Ga3 50.9(2) 5_445 1_546
O2 O2 Ga3 138.0(5) 5_455 1_546
O2 O2 Ga3 101.59(16) 1_554 1_546
O2 O2 Ga3 78.41(16) 1_556 1_546
O3 O2 Ga3 124.8(4) 4_556 1_546
Ga3 O2 O3 113.6(5) 4_446 3_456
Ga2 O2 O3 19.5(4) . 3_456
La O2 O3 118.9(6) 4_445 3_456
O3 O2 O3 99.4(5) 6 3_456
La O2 O3 76.5(4) . 3_456
O3 O2 O3 149.7(5) 2 3_456
O1 O2 O3 84.7(4) 2_455 3_456
O2 O2 O3 56.7(4) 4_445 3_456
O2 O2 O3 28.1(2) 3_455 3_456
O3 O2 O3 78.8(4) 1_556 3_456
O2 O2 O3 107.5(6) 2_556 3_456
O1 O2 O3 35.2(2) 2_456 3_456
O3 O2 O3 121.8(5) . 3_456
Nb O2 O3 132.7(5) . 3_456
Ga1 O2 O3 132.7(5) . 3_456
O1 O2 O3 143.8(6) 1_545 3_456
O2 O2 O3 148.9(6) 2 3_456
Ga2 O2 O3 124.5(5) 2_556 3_456
O3 O2 O3 97.5(5) 5_445 3_456
Ga3 O2 O3 91.4(3) 2_565 3_456
La O2 O3 73.7(3) 4_446 3_456
La O2 O3 45.8(2) 1_556 3_456
Ga3 O2 O3 134.3(4) 4_445 3_456
La O2 O3 54.4(3) 2_455 3_456
O3 O2 O3 114.9(4) 3_556 3_456
O3 O2 O3 69.3(3) 4_446 3_456
Ga3 O2 O3 61.6(3) 2_455 3_456
Ga3 O2 O3 20.33(15) 1_556 3_456
Ga2 O2 O3 96.9(3) 1_554 3_456
O2 O2 O3 67.9(3) 6_556 3_456
La O2 O3 172.8(4) 2 3_456
O3 O2 O3 154.1(6) 3 3_456
O3 O2 O3 100.0(3) 4_445 3_456
O2 O2 O3 103.0(6) 5_446 3_456
O2 O2 O3 32.8(3) 5_456 3_456
O1 O2 O3 65.5(3) . 3_456
O3 O2 O3 123.8(4) 5 3_456
Ga2 O2 O3 54.8(2) 2_566 3_456
Nb O2 O3 90.9(3) 1_556 3_456
Ga1 O2 O3 90.9(3) 1_556 3_456
Ga3 O2 O3 126.1(4) 1_656 3_456
O2 O2 O3 96.6(4) 6 3_456
O2 O2 O3 130.7(6) 5_445 3_456
O2 O2 O3 72.6(3) 5_455 3_456
O2 O2 O3 117.0(2) 1_554 3_456
O2 O2 O3 63.0(2) 1_556 3_456
O3 O2 O3 96.9(4) 4_556 3_456
Ga3 O2 O3 98.4(4) 1_546 3_456
Ga3 O2 O3 143.7(6) 4_446 2_455
Ga2 O2 O3 35.6(4) . 2_455
La O2 O3 95.2(4) 4_445 2_455
O3 O2 O3 103.6(4) 6 2_455
La O2 O3 60.5(3) . 2_455
O3 O2 O3 160.7(7) 2 2_455
O1 O2 O3 53.5(3) 2_455 2_455
O2 O2 O3 45.1(5) 4_445 2_455
O2 O2 O3 15.4(5) 3_455 2_455
O3 O2 O3 107.6(4) 1_556 2_455
O2 O2 O3 134.3(5) 2_556 2_455
O1 O2 O3 63.3(3) 2_456 2_455
O3 O2 O3 100.3(4) . 2_455
Nb O2 O3 126.6(5) . 2_455
Ga1 O2 O3 126.6(5) . 2_455
O1 O2 O3 136.3(4) 1_545 2_455
O2 O2 O3 117.8(6) 2 2_455
Ga2 O2 O3 137.0(5) 2_556 2_455
O3 O2 O3 88.7(3) 5_445 2_455
Ga3 O2 O3 106.4(4) 2_565 2_455
La O2 O3 97.5(3) 4_446 2_455
La O2 O3 75.4(3) 1_556 2_455
Ga3 O2 O3 105.6(3) 4_445 2_455
La O2 O3 25.86(15) 2_455 2_455
O3 O2 O3 144.9(4) 3_556 2_455
O3 O2 O3 79.2(3) 4_446 2_455
Ga3 O2 O3 59.8(2) 2_455 2_455
Ga3 O2 O3 28.30(19) 1_556 2_455
Ga2 O2 O3 65.9(2) 1_554 2_455
O2 O2 O3 86.5(2) 6_556 2_455
La O2 O3 155.7(3) 2 2_455
O3 O2 O3 135.4(4) 3 2_455
O3 O2 O3 75.8(3) 4_445 2_455
O2 O2 O3 114.0(6) 5_446 2_455
O2 O2 O3 51.8(4) 5_456 2_455
O1 O2 O3 63.9(2) . 2_455
O3 O2 O3 132.8(5) 5 2_455
Ga2 O2 O3 65.8(3) 2_566 2_455
Nb O2 O3 120.3(3) 1_556 2_455
Ga1 O2 O3 120.3(3) 1_556 2_455
Ga3 O2 O3 147.9(4) 1_656 2_455
O2 O2 O3 83.4(2) 6 2_455
O2 O2 O3 107.7(5) 5_445 2_455
O2 O2 O3 52.3(3) 5_455 2_455
O2 O2 O3 86.6(2) 1_554 2_455
O2 O2 O3 93.4(2) 1_556 2_455
O3 O2 O3 119.5(4) 4_556 2_455
Ga3 O2 O3 99.2(3) 1_546 2_455
O3 O2 O3 31.2(3) 3_456 2_455
Ga3 O2 O3 73.2(6) 4_446 4
Ga2 O2 O3 142.7(8) . 4
La O2 O3 99.9(5) 4_445 4
O3 O2 O3 29.5(4) 6 4
La O2 O3 54.1(4) . 4
O3 O2 O3 46.2(4) 2 4
O1 O2 O3 85.6(5) 2_455 4
O2 O2 O3 146.2(4) 4_445 4
O2 O2 O3 104.1(8) 3_455 4
O3 O2 O3 83.6(4) 1_556 4
O2 O2 O3 106.3(4) 2_556 4
O1 O2 O3 140.1(5) 2_456 4
O3 O2 O3 25.6(3) . 4
Nb O2 O3 12.01(18) . 4
Ga1 O2 O3 12.01(18) . 4
O1 O2 O3 92.6(4) 1_545 4
O2 O2 O3 60.7(2) 2 4
Ga2 O2 O3 107.1(3) 2_556 4
O3 O2 O3 133.7(3) 5_445 4
Ga3 O2 O3 48.0(3) 2_565 4
La O2 O3 139.5(4) 4_446 4
La O2 O3 103.8(4) 1_556 4
Ga3 O2 O3 43.3(2) 4_445 4
La O2 O3 115.9(4) 2_455 4
O3 O2 O3 72.5(3) 3_556 4
O3 O2 O3 166.0(5) 4_446 4
Ga3 O2 O3 162.3(4) 2_455 4
Ga3 O2 O3 104.1(4) 1_556 4
Ga2 O2 O3 75.1(3) 1_554 4
O2 O2 O3 67.6(4) 6_556 4
La O2 O3 59.7(2) 2 4
O3 O2 O3 30.9(2) 3 4
O3 O2 O3 109.8(4) 4_445 4
O2 O2 O3 130.5(5) 5_446 4
O2 O2 O3 93.9(5) 5_456 4
O1 O2 O3 58.1(3) . 4
O3 O2 O3 29.6(3) 5 4
Ga2 O2 O3 70.9(3) 2_566 4
Nb O2 O3 80.3(3) 1_556 4
Ga1 O2 O3 80.3(3) 1_556 4
Ga3 O2 O3 50.5(2) 1_656 4
O2 O2 O3 31.2(2) 6 4
O2 O2 O3 93.6(4) 5_445 4
O2 O2 O3 62.8(5) 5_455 4
O2 O2 O3 58.7(2) 1_554 4
O2 O2 O3 121.3(2) 1_556 4
O3 O2 O3 58.7(2) 4_556 4
Ga3 O2 O3 137.9(3) 1_546 4
O3 O2 O3 123.6(5) 3_456 4
O3 O2 O3 114.6(4) 2_455 4
Ga3 O2 Ga2 99.4(5) 4_446 2
Ga2 O2 Ga2 133.2(7) . 2
La O2 Ga2 29.3(2) 4_445 2
O3 O2 Ga2 102.4(5) 6 2
La O2 Ga2 97.2(4) . 2
O3 O2 Ga2 64.2(4) 2 2
O1 O2 Ga2 65.9(3) 2_455 2
O2 O2 Ga2 92.4(6) 4_445 2
O2 O2 Ga2 126.5(3) 3_455 2
O3 O2 Ga2 135.1(4) 1_556 2
O2 O2 Ga2 93.3(5) 2_556 2
O1 O2 Ga2 146.1(6) 2_456 2
O3 O2 Ga2 58.9(3) . 2
Nb O2 Ga2 69.5(2) . 2
Ga1 O2 Ga2 69.5(2) . 2
O1 O2 Ga2 37.5(3) 1_545 2
O2 O2 Ga2 12.6(2) 2 2
Ga2 O2 Ga2 65.7(2) 2_556 2
O3 O2 Ga2 60.6(3) 5_445 2
Ga3 O2 Ga2 117.4(3) 2_565 2
La O2 Ga2 114.7(4) 4_446 2
La O2 Ga2 167.6(4) 1_556 2
Ga3 O2 Ga2 36.47(11) 4_445 2
La O2 Ga2 91.9(3) 2_455 2
O3 O2 Ga2 98.2(3) 3_556 2
O3 O2 Ga2 99.2(4) 4_446 2
Ga3 O2 Ga2 94.2(3) 2_455 2
Ga3 O2 Ga2 141.7(3) 1_556 2
Ga2 O2 Ga2 55.85(15) 1_554 2
O2 O2 Ga2 140.0(5) 6_556 2
La O2 Ga2 39.53(11) 2 2
O3 O2 Ga2 46.5(2) 3 2
O3 O2 Ga2 46.7(2) 4_445 2
O2 O2 Ga2 77.5(2) 5_446 2
O2 O2 Ga2 157.8(5) 5_456 2
O1 O2 Ga2 120.0(4) . 2
O3 O2 Ga2 85.9(3) 5 2
Ga2 O2 Ga2 140.2(4) 2_566 2
Nb O2 Ga2 122.7(3) 1_556 2
Ga1 O2 Ga2 122.7(3) 1_556 2
Ga3 O2 Ga2 87.8(2) 1_656 2
O2 O2 Ga2 86.8(3) 6 2
O2 O2 Ga2 20.6(2) 5_445 2
O2 O2 Ga2 94.8(5) 5_455 2
O2 O2 Ga2 41.6(2) 1_554 2
O2 O2 Ga2 138.4(2) 1_556 2
O3 O2 Ga2 116.4(3) 4_556 2
Ga3 O2 Ga2 69.6(2) 1_546 2
O3 O2 Ga2 145.9(4) 3_456 2
O3 O2 Ga2 116.9(3) 2_455 2
O3 O2 Ga2 73.0(2) 4 2
Ga3 O2 O3 155.4(8) 4_446 3_455
Ga2 O2 O3 63.5(5) . 3_455
La O2 O3 82.4(4) 4_445 3_455
O3 O2 O3 92.6(5) 6 3_455
La O2 O3 41.6(3) . 3_455
O3 O2 O3 136.3(6) 2 3_455
O1 O2 O3 29.1(3) 2_455 3_455
O2 O2 O3 58.1(4) 4_445 3_455
O2 O2 O3 31.8(2) 3_455 3_455
O3 O2 O3 124.3(4) 1_556 3_455
O2 O2 O3 161.3(5) 2_556 3_455
O1 O2 O3 91.4(4) 2_456 3_455
O3 O2 O3 73.4(4) . 3_455
Nb O2 O3 103.8(5) . 3_455
Ga1 O2 O3 103.8(5) . 3_455
O1 O2 O3 126.8(4) 1_545 3_455
O2 O2 O3 92.4(6) 2 3_455
Ga2 O2 O3 146.0(5) 2_556 3_455
O3 O2 O3 92.7(4) 5_445 3_455
Ga3 O2 O3 104.9(4) 2_565 3_455
La O2 O3 124.6(4) 4_446 3_455
La O2 O3 97.1(3) 1_556 3_455
Ga3 O2 O3 77.5(3) 4_445 3_455
La O2 O3 25.88(17) 2_455 3_455
O3 O2 O3 155.8(6) 3_556 3_455
O3 O2 O3 100.1(3) 4_446 3_455
Ga3 O2 O3 76.5(3) 2_455 3_455
Ga3 O2 O3 46.7(2) 1_556 3_455
Ga2 O2 O3 39.75(19) 1_554 3_455
O2 O2 O3 93.3(4) 6_556 3_455
La O2 O3 129.3(3) 2 3_455
O3 O2 O3 107.5(4) 3 3_455
O3 O2 O3 65.9(2) 4_445 3_455
O2 O2 O3 129.6(6) 5_446 3_455
O2 O2 O3 67.1(3) 5_456 3_455
O1 O2 O3 57.6(3) . 3_455
O3 O2 O3 118.2(4) 5 3_455
Ga2 O2 O3 70.4(3) 2_566 3_455
Nb O2 O3 136.5(4) 1_556 3_455
Ga1 O2 O3 136.5(4) 1_556 3_455
Ga3 O2 O3 139.9(5) 1_656 3_455
O2 O2 O3 62.8(3) 6 3_455
O2 O2 O3 93.3(4) 5_445 3_455
O2 O2 O3 31.0(3) 5_455 3_455
O2 O2 O3 59.11(19) 1_554 3_455
O2 O2 O3 120.89(19) 1_556 3_455
O3 O2 O3 123.6(5) 4_556 3_455
Ga3 O2 O3 109.3(4) 1_546 3_455
O3 O2 O3 57.9(2) 3_456 3_455
O3 O2 O3 28.2(3) 2_455 3_455
O3 O2 O3 92.2(4) 4 3_455
Ga2 O2 O3 95.0(3) 2 3_455
Ga3 O2 O2 33.9(4) 4_446 3
Ga2 O2 O2 150.9(5) . 3
La O2 O2 95.1(5) 4_445 3
O3 O2 O2 59.9(3) 6 3
La O2 O2 104.4(4) . 3
O3 O2 O2 6.6(4) 2 3
O1 O2 O2 124.4(3) 2_455 3
O2 O2 O2 151.2(10) 4_445 3
O2 O2 O2 148.8(10) 3_455 3
O3 O2 O2 66.4(3) 1_556 3
O2 O2 O2 56.7(4) 2_556 3
O1 O2 O2 121.3(3) 2_456 3
O3 O2 O2 68.9(3) . 3
Nb O2 O2 38.79(14) . 3
Ga1 O2 O2 38.79(14) . 3
O1 O2 O2 58.3(4) 1_545 3
O2 O2 O2 64.5(5) 2 3
Ga2 O2 O2 59.3(3) 2_556 3
O3 O2 O2 107.2(5) 5_445 3
Ga3 O2 O2 58.86(19) 2_565 3
La O2 O2 93.1(3) 4_446 3
La O2 O2 99.4(2) 1_556 3
Ga3 O2 O2 69.5(2) 4_445 3
La O2 O2 158.83(19) 2_455 3
O3 O2 O2 32.6(3) 3_556 3
O3 O2 O2 116.0(5) 4_446 3
Ga3 O2 O2 136.6(5) 2_455 3
Ga3 O2 O2 139.0(5) 1_556 3
Ga2 O2 O2 111.45(19) 1_554 3
O2 O2 O2 80.6(3) 6_556 3
La O2 O2 30.5(2) 2 3
O3 O2 O2 36.8(3) 3 3
O3 O2 O2 114.5(4) 4_445 3
O2 O2 O2 81.9(5) 5_446 3
O2 O2 O2 116.6(5) 5_456 3
O1 O2 O2 99.6(4) . 3
O3 O2 O2 30.7(2) 5 3
Ga2 O2 O2 99.5(3) 2_566 3
Nb O2 O2 54.80(17) 1_556 3
Ga1 O2 O2 54.80(17) 1_556 3
Ga3 O2 O2 19.20(15) 1_656 3
O2 O2 O2 81.6(3) 6 3
O2 O2 O2 82.8(4) 5_445 3
O2 O2 O2 113.5(5) 5_455 3
O2 O2 O2 90.0 1_554 3
O2 O2 O2 90.000(1) 1_556 3
O3 O2 O2 48.9(2) 4_556 3
Ga3 O2 O2 97.3(4) 1_546 3
O3 O2 O2 145.0(3) 3_456 3
O3 O2 O2 163.5(5) 2_455 3
O3 O2 O2 50.72(17) 4 3
Ga2 O2 O2 69.2(3) 2 3
O3 O2 O2 142.1(4) 3_455 3
Ga3 O2 O2 60.7(5) 4_446 4
Ga2 O2 O2 114.9(8) . 4
La O2 O2 135.5(4) 4_445 4
O3 O2 O2 6.8(4) 6 4
La O2 O2 55.5(5) . 4
O3 O2 O2 59.9(3) 2 4
O1 O2 O2 105.8(5) 2_455 4
O2 O2 O2 148.8(10) 4_445 4
O2 O2 O2 88.8(10) 3_455 4
O3 O2 O2 52.9(5) 1_556 4
O2 O2 O2 97.6(2) 2_556 4
O1 O2 O2 104.5(5) 2_456 4
O3 O2 O2 57.1(3) . 4
Nb O2 O2 38.79(14) . 4
Ga1 O2 O2 38.79(14) . 4
O1 O2 O2 117.1(3) 1_545 4
O2 O2 O2 95.95(12) 2 4
Ga2 O2 O2 116.3(3) 2_556 4
O3 O2 O2 166.4(5) 5_445 4
Ga3 O2 O2 14.4(2) 2_565 4
La O2 O2 115.5(2) 4_446 4
La O2 O2 68.2(4) 1_556 4
Ga3 O2 O2 78.1(2) 4_445 4
La O2 O2 121.0(5) 2_455 4
O3 O2 O2 60.8(2) 3_556 4
O3 O2 O2 147.1(3) 4_446 4
Ga3 O2 O2 157.2(4) 2_455 4
Ga3 O2 O2 81.0(5) 1_556 4
Ga2 O2 O2 100.1(3) 1_554 4
O2 O2 O2 32.2(5) 6_556 4
La O2 O2 84.0(2) 2 4
O3 O2 O2 62.4(2) 3 4
O3 O2 O2 142.8(3) 4_445 4
O2 O2 O2 134.2(5) 5_446 4
O2 O2 O2 63.3(5) 5_456 4
O1 O2 O2 40.4(3) . 4
O3 O2 O2 29.7(2) 5 4
Ga2 O2 O2 41.6(4) 2_566 4
Nb O2 O2 54.80(17) 1_556 4
Ga1 O2 O2 54.80(17) 1_556 4
Ga3 O2 O2 46.12(11) 1_656 4
O2 O2 O2 40.9(3) 6 4
O2 O2 O2 128.5(4) 5_445 4
O2 O2 O2 66.4(4) 5_455 4
O2 O2 O2 90.0 1_554 4
O2 O2 O2 90.0 1_556 4
O3 O2 O2 32.29(19) 4_556 4
Ga3 O2 O2 154.8(4) 1_546 4
O3 O2 O2 96.0(5) 3_456 4
O3 O2 O2 103.8(5) 2_455 4
O3 O2 O2 35.6(2) 4 4
Ga2 O2 O2 107.93(19) 2 4
O3 O2 O2 95.8(5) 3_455 4
O2 O2 O2 60.000(1) 3 4
Ga3 O2 La 105.1(5) 4_446 2_456
Ga2 O2 La 13.0(3) . 2_456
La O2 La 108.4(5) 4_445 2_456
O3 O2 La 119.4(5) 6 2_456
La O2 La 102.4(4) . 2_456
O3 O2 La 145.0(5) 2 2_456
O1 O2 La 97.1(4) 2_455 2_456
O2 O2 La 47.4(2) 4_445 2_456
O2 O2 La 52.0(2) 3_455 2_456
O3 O2 La 78.3(4) 1_556 2_456
O2 O2 La 86.1(5) 2_556 2_456
O1 O2 La 17.4(2) 2_456 2_456
O3 O2 La 147.2(5) . 2_456
Nb O2 La 153.1(4) . 2_456
Ga1 O2 La 153.1(4) . 2_456
O1 O2 La 118.7(5) 1_545 2_456
O2 O2 La 148.37(18) 2 2_456
Ga2 O2 La 98.5(4) 2_556 2_456
O3 O2 La 77.9(4) 5_445 2_456
Ga3 O2 La 105.1(3) 2_565 2_456
La O2 La 49.74(18) 4_446 2_456
La O2 La 49.25(15) 1_556 2_456
Ga3 O2 La 152.0(4) 4_445 2_456
La O2 La 62.4(2) 2_455 2_456
O3 O2 La 106.3(3) 3_556 2_456
O3 O2 La 44.0(2) 4_446 2_456
Ga3 O2 La 43.24(15) 2_455 2_456
Ga3 O2 La 46.52(14) 1_556 2_456
Ga2 O2 La 110.1(3) 1_554 2_456
O2 O2 La 82.6(3) 6_556 2_456
La O2 La 148.4(4) 2 2_456
O3 O2 La 174.8(4) 3 2_456
O3 O2 La 93.4(4) 4_445 2_456
O2 O2 La 76.8(5) 5_446 2_456
O2 O2 La 53.6(3) 5_456 2_456
O1 O2 La 90.8(3) . 2_456
O3 O2 La 135.2(3) 5 2_456
Ga2 O2 La 76.55(19) 2_566 2_456
Nb O2 La 87.2(2) 1_556 2_456
Ga1 O2 La 87.2(2) 1_556 2_456
Ga3 O2 La 125.4(3) 1_656 2_456
O2 O2 La 122.7(3) 6 2_456
O2 O2 La 117.1(5) 5_445 2_456
O2 O2 La 97.5(3) 5_455 2_456
O2 O2 La 131.50(16) 1_554 2_456
O2 O2 La 48.50(16) 1_556 2_456
O3 O2 La 102.3(3) 4_556 2_456
Ga3 O2 La 74.2(3) 1_546 2_456
O3 O2 La 26.20(15) 3_456 2_456
O3 O2 La 48.35(18) 2_455 2_456
O3 O2 La 147.5(4) 4 2_456
Ga2 O2 La 137.4(4) 2 2_456
O3 O2 La 76.5(2) 3_455 2_456
O2 O2 La 138.38(18) 3 2_456
O2 O2 La 114.4(4) 4 2_456
Ga3 O2 Ga1 127.6(8) 4_446 1_445
Ga2 O2 Ga1 75.6(6) . 1_445
La O2 Ga1 29.7(3) 4_445 1_445
O3 O2 Ga1 156.7(5) 6 1_445
La O2 Ga1 113.5(4) . 1_445
O3 O2 Ga1 115.5(5) 2 1_445
O1 O2 Ga1 61.0(3) 2_455 1_445
O2 O2 Ga1 36.0(6) 4_445 1_445
O2 O2 Ga1 92.3(6) 3_455 1_445
O3 O2 Ga1 143.2(6) 1_556 1_445
O2 O2 Ga1 93.2(3) 2_556 1_445
O1 O2 Ga1 90.7(4) 2_456 1_445
O3 O2 Ga1 106.4(4) . 1_445
Nb O2 Ga1 127.9(3) . 1_445
Ga1 O2 Ga1 127.9(3) . 1_445
O1 O2 Ga1 59.5(3) 1_545 1_445
O2 O2 Ga1 69.82(15) 2 1_445
Ga2 O2 Ga1 69.1(3) 2_556 1_445
O3 O2 Ga1 16.3(2) 5_445 1_445
Ga3 O2 Ga1 176.0(3) 2_565 1_445
La O2 Ga1 80.4(3) 4_446 1_445
La O2 Ga1 127.0(4) 1_556 1_445
Ga3 O2 Ga1 85.7(2) 4_445 1_445
La O2 Ga1 54.7(2) 2_455 1_445
O3 O2 Ga1 127.2(5) 3_556 1_445
O3 O2 Ga1 49.5(3) 4_446 1_445
Ga3 O2 Ga1 35.85(14) 2_455 1_445
Ga3 O2 Ga1 103.6(3) 1_556 1_445
Ga2 O2 Ga1 64.7(2) 1_554 1_445
O2 O2 Ga1 160.5(3) 6_556 1_445
La O2 Ga1 89.1(3) 2 1_445
O3 O2 Ga1 105.2(3) 3 1_445
O3 O2 Ga1 20.83(19) 4_445 1_445
O2 O2 Ga1 56.3(3) 5_446 1_445
O2 O2 Ga1 124.9(5) 5_456 1_445
O1 O2 Ga1 134.6(3) . 1_445
O3 O2 Ga1 143.4(3) 5 1_445
Ga2 O2 Ga1 142.7(3) 2_566 1_445
Nb O2 Ga1 139.3(4) 1_556 1_445
Ga1 O2 Ga1 139.3(4) 1_556 1_445
Ga3 O2 Ga1 135.2(3) 1_656 1_445
O2 O2 Ga1 124.1(4) 6 1_445
O2 O2 Ga1 39.0(3) 5_445 1_445
O2 O2 Ga1 103.2(4) 5_455 1_445
O2 O2 Ga1 73.49(18) 1_554 1_445
O2 O2 Ga1 106.51(18) 1_556 1_445
O3 O2 Ga1 159.3(4) 4_556 1_445
Ga3 O2 Ga1 35.10(13) 1_546 1_445
O3 O2 Ga1 92.7(3) 3_456 1_445
O3 O2 Ga1 77.0(2) 2_455 1_445
O3 O2 Ga1 128.8(3) 4 1_445
Ga2 O2 Ga1 58.68(16) 2 1_445
O3 O2 Ga1 77.0(3) 3_455 1_445
O2 O2 Ga1 117.5(4) 3 1_445
O2 O2 Ga1 163.44(17) 4 1_445
La O2 Ga1 78.8(3) 2_456 1_445
Ga3 O2 Nb 127.6(8) 4_446 1_445
Ga2 O2 Nb 75.6(6) . 1_445
La O2 Nb 29.7(3) 4_445 1_445
O3 O2 Nb 156.7(5) 6 1_445
La O2 Nb 113.5(4) . 1_445
O3 O2 Nb 115.5(5) 2 1_445
O1 O2 Nb 61.0(3) 2_455 1_445
O2 O2 Nb 36.0(6) 4_445 1_445
O2 O2 Nb 92.3(6) 3_455 1_445
O3 O2 Nb 143.2(6) 1_556 1_445
O2 O2 Nb 93.2(3) 2_556 1_445
O1 O2 Nb 90.7(4) 2_456 1_445
O3 O2 Nb 106.4(4) . 1_445
Nb O2 Nb 127.9(3) . 1_445
Ga1 O2 Nb 127.9(3) . 1_445
O1 O2 Nb 59.5(3) 1_545 1_445
O2 O2 Nb 69.82(15) 2 1_445
Ga2 O2 Nb 69.1(3) 2_556 1_445
O3 O2 Nb 16.3(2) 5_445 1_445
Ga3 O2 Nb 176.0(3) 2_565 1_445
La O2 Nb 80.4(3) 4_446 1_445
La O2 Nb 127.0(4) 1_556 1_445
Ga3 O2 Nb 85.7(2) 4_445 1_445
La O2 Nb 54.7(2) 2_455 1_445
O3 O2 Nb 127.2(5) 3_556 1_445
O3 O2 Nb 49.5(3) 4_446 1_445
Ga3 O2 Nb 35.85(14) 2_455 1_445
Ga3 O2 Nb 103.6(3) 1_556 1_445
Ga2 O2 Nb 64.7(2) 1_554 1_445
O2 O2 Nb 160.5(3) 6_556 1_445
La O2 Nb 89.1(3) 2 1_445
O3 O2 Nb 105.2(3) 3 1_445
O3 O2 Nb 20.83(19) 4_445 1_445
O2 O2 Nb 56.3(3) 5_446 1_445
O2 O2 Nb 124.9(5) 5_456 1_445
O1 O2 Nb 134.6(3) . 1_445
O3 O2 Nb 143.4(3) 5 1_445
Ga2 O2 Nb 142.7(3) 2_566 1_445
Nb O2 Nb 139.3(4) 1_556 1_445
Ga1 O2 Nb 139.3(4) 1_556 1_445
Ga3 O2 Nb 135.2(3) 1_656 1_445
O2 O2 Nb 124.1(4) 6 1_445
O2 O2 Nb 39.0(3) 5_445 1_445
O2 O2 Nb 103.2(4) 5_455 1_445
O2 O2 Nb 73.49(18) 1_554 1_445
O2 O2 Nb 106.51(18) 1_556 1_445
O3 O2 Nb 159.3(4) 4_556 1_445
Ga3 O2 Nb 35.10(13) 1_546 1_445
O3 O2 Nb 92.7(3) 3_456 1_445
O3 O2 Nb 77.0(2) 2_455 1_445
O3 O2 Nb 128.8(3) 4 1_445
Ga2 O2 Nb 58.68(16) 2 1_445
O3 O2 Nb 77.0(3) 3_455 1_445
O2 O2 Nb 117.5(4) 3 1_445
O2 O2 Nb 163.44(17) 4 1_445
La O2 Nb 78.8(3) 2_456 1_445
Ga1 O2 Nb 0.0 1_445 1_445
Ga3 O2 O2 121.5(8) 4_446 6_446
Ga2 O2 O2 24.4(3) . 6_446
La O2 O2 82.2(6) 4_445 6_446
O3 O2 O2 143.0(6) 6 6_446
La O2 O2 108.0(3) . 6_446
O3 O2 O2 151.6(8) 2 6_446
O1 O2 O2 80.9(3) 2_455 6_446
O2 O2 O2 22.6(3) 4_445 6_446
O2 O2 O2 58.9(3) 3_455 6_446
O3 O2 O2 102.6(5) 1_556 6_446
O2 O2 O2 91.0(5) 2_556 6_446
O1 O2 O2 40.9(3) 2_456 6_446
O3 O2 O2 141.4(5) . 6_446
Nb O2 O2 174.1(6) . 6_446
Ga1 O2 O2 174.1(6) . 6_446
O1 O2 O2 101.0(7) 1_545 6_446
O2 O2 O2 122.1(3) 2 6_446
Ga2 O2 O2 90.2(6) 2_556 6_446
O3 O2 O2 54.1(5) 5_445 6_446
Ga3 O2 O2 131.3(4) 2_565 6_446
La O2 O2 55.9(4) 4_446 6_446
La O2 O2 75.5(3) 1_556 6_446
Ga3 O2 O2 131.4(4) 4_445 6_446
La O2 O2 47.93(11) 2_455 6_446
O3 O2 O2 122.4(5) 3_556 6_446
O3 O2 O2 31.6(3) 4_446 6_446
Ga3 O2 O2 18.1(2) 2_455 6_446
Ga3 O2 O2 61.23(14) 1_556 6_446
Ga2 O2 O2 92.8(3) 1_554 6_446
O2 O2 O2 108.3(4) 6_556 6_446
La O2 O2 134.9(6) 2 6_446
O3 O2 O2 157.8(6) 3 6_446
O3 O2 O2 67.4(4) 4_445 6_446
O2 O2 O2 66.8(7) 5_446 6_446
O2 O2 O2 76.0(3) 5_456 6_446
O1 O2 O2 107.0(3) . 6_446
O3 O2 O2 160.8(5) 5 6_446
Ga2 O2 O2 98.5(3) 2_566 6_446
Nb O2 O2 109.3(4) 1_556 6_446
Ga1 O2 O2 109.3(4) 1_556 6_446
Ga3 O2 O2 144.5(5) 1_656 6_446
O2 O2 O2 131.0(3) 6 6_446
O2 O2 O2 91.4(6) 5_445 6_446
O2 O2 O2 99.3(3) 5_455 6_446
O2 O2 O2 112.2(3) 1_554 6_446
O2 O2 O2 67.8(3) 1_556 6_446
O3 O2 O2 127.6(4) 4_556 6_446
Ga3 O2 O2 55.9(4) 1_546 6_446
O3 O2 O2 43.7(2) 3_456 6_446
O3 O2 O2 47.56(18) 2_455 6_446
O3 O2 O2 162.1(5) 4 6_446
Ga2 O2 O2 111.3(5) 2 6_446
O3 O2 O2 70.3(2) 3_455 6_446
O2 O2 O2 147.2(5) 3 6_446
O2 O2 O2 139.2(6) 4 6_446
La O2 O2 26.32(16) 2_456 6_446
Ga1 O2 O2 52.7(3) 1_445 6_446
Nb O2 O2 52.7(3) 1_445 6_446
Ga3 O2 O2 46.6(3) 4_446 6_546
Ga2 O2 O2 113.0(9) . 6_546
La O2 O2 77.5(5) 4_445 6_546
O3 O2 O2 106.9(4) 6 6_546
La O2 O2 153.9(6) . 6_546
O3 O2 O2 53.6(3) 2 6_546
O1 O2 O2 133.2(6) 2_455 6_546
O2 O2 O2 104.2(10) 4_445 6_546
O2 O2 O2 153.6(6) 3_455 6_546
O3 O2 O2 75.7(5) 1_556 6_546
O2 O2 O2 21.9(3) 2_556 6_546
O1 O2 O2 91.1(6) 2_456 6_546
O3 O2 O2 111.2(4) . 6_546
Nb O2 O2 87.8(2) . 6_546
Ga1 O2 O2 87.8(2) . 6_546
O1 O2 O2 35.0(3) 1_545 6_546
O2 O2 O2 77.8(4) 2 6_546
Ga2 O2 O2 12.07(18) 2_556 6_546
O3 O2 O2 65.7(5) 5_445 6_546
Ga3 O2 O2 96.8(3) 2_565 6_546
La O2 O2 52.4(4) 4_446 6_546
La O2 O2 97.8(4) 1_556 6_546
Ga3 O2 O2 98.8(3) 4_445 6_546
La O2 O2 134.3(6) 2_455 6_546
O3 O2 O2 46.1(2) 3_556 6_546
O3 O2 O2 66.5(5) 4_446 6_546
Ga3 O2 O2 87.2(5) 2_455 6_546
Ga3 O2 O2 143.9(5) 1_556 6_546
Ga2 O2 O2 126.4(4) 1_554 6_546
O2 O2 O2 108.3(4) 6_556 6_546
La O2 O2 47.29(10) 2 6_546
O3 O2 O2 76.0(2) 3 6_546
O3 O2 O2 92.6(5) 4_445 6_546
O2 O2 O2 32.2(3) 5_446 6_546
O2 O2 O2 129.6(6) 5_456 6_546
O1 O2 O2 144.1(5) . 6_546
O3 O2 O2 78.9(3) 5 6_546
Ga2 O2 O2 131.0(4) 2_566 6_546
Nb O2 O2 64.4(3) 1_556 6_546
Ga1 O2 O2 64.4(3) 1_556 6_546
Ga3 O2 O2 58.83(16) 1_656 6_546
O2 O2 O2 131.0(3) 6 6_546
O2 O2 O2 67.73(19) 5_445 6_546
O2 O2 O2 160.9(6) 5_455 6_546
O2 O2 O2 112.2(3) 1_554 6_546
O2 O2 O2 67.8(3) 1_556 6_546
O3 O2 O2 78.4(3) 4_556 6_546
Ga3 O2 O2 50.3(4) 1_546 6_546
O3 O2 O2 126.1(5) 3_456 6_546
O3 O2 O2 145.6(6) 2_455 6_546
O3 O2 O2 99.8(3) 4 6_546
Ga2 O2 O2 71.4(3) 2 6_546
O3 O2 O2 158.0(6) 3_455 6_546
O2 O2 O2 49.9(2) 3 6_546
O2 O2 O2 104.7(2) 4 6_546
La O2 O2 101.6(5) 2_456 6_546
Ga1 O2 O2 81.2(4) 1_445 6_546
Nb O2 O2 81.2(4) 1_445 6_546
O2 O2 O2 98.0(7) 6_446 6_546
Ga3 O2 O3 43.8(4) 4_446 6_556
Ga2 O2 O3 77.7(4) . 6_556
La O2 O3 154.0(7) 4_445 6_556
O3 O2 O3 67.2(4) 6 6_556
La O2 O3 101.6(5) . 6_556
O3 O2 O3 81.4(4) 2 6_556
O1 O2 O3 148.6(5) 2_455 6_556
O2 O2 O3 115.0(2) 4_445 6_556
O2 O2 O3 89.6(5) 3_455 6_556
O3 O2 O3 10.1(3) 1_556 6_556
O2 O2 O3 57.5(4) 2_556 6_556
O1 O2 O3 51.8(3) 2_456 6_556
O3 O2 O3 117.2(5) . 6_556
Nb O2 O3 89.6(4) . 6_556
Ga1 O2 O3 89.6(4) . 6_556
O1 O2 O3 112.7(5) 1_545 6_556
O2 O2 O3 140.0(4) 2 6_556
Ga2 O2 O3 87.5(3) 2_556 6_556
O3 O2 O3 123.4(5) 5_445 6_556
Ga3 O2 O3 46.2(2) 2_565 6_556
La O2 O3 56.2(2) 4_446 6_556
La O2 O3 24.55(16) 1_556 6_556
Ga3 O2 O3 135.4(5) 4_445 6_556
La O2 O3 124.5(3) 2_455 6_556
O3 O2 O3 45.1(3) 3_556 6_556
O3 O2 O3 86.7(3) 4_446 6_556
Ga3 O2 O3 104.5(3) 2_455 6_556
Ga3 O2 O3 74.1(2) 1_556 6_556
Ga2 O2 O3 153.8(5) 1_554 6_556
O2 O2 O3 36.9(3) 6_556 6_556
La O2 O3 103.9(3) 2 6_556
O3 O2 O3 106.7(5) 3 6_556
O3 O2 O3 156.7(5) 4_445 6_556
O2 O2 O3 87.6(5) 5_446 6_556
O2 O2 O3 52.8(4) 5_456 6_556
O1 O2 O3 75.6(3) . 6_556
O3 O2 O3 68.2(2) 5 6_556
Ga2 O2 O3 55.4(2) 2_566 6_556
Nb O2 O3 20.85(14) 1_556 6_556
Ga1 O2 O3 20.85(14) 1_556 6_556
Ga3 O2 O3 58.4(2) 1_656 6_556
O2 O2 O3 98.5(5) 6 6_556
O2 O2 O3 145.8(4) 5_445 6_556
O2 O2 O3 109.0(3) 5_455 6_556
O2 O2 O3 150.4(3) 1_554 6_556
O2 O2 O3 29.6(3) 1_556 6_556
O3 O2 O3 35.1(3) 4_556 6_556
Ga3 O2 O3 105.7(4) 1_546 6_556
O3 O2 O3 70.1(2) 3_456 6_556
O3 O2 O3 99.9(3) 2_455 6_556
O3 O2 O3 92.9(4) 4 6_556
Ga2 O2 O3 143.2(3) 2 6_556
O3 O2 O3 119.9(3) 3_455 6_556
O2 O2 O3 75.6(2) 3 6_556
O2 O2 O3 60.4(3) 4 6_556
La O2 O3 68.2(2) 2_456 6_556
Ga1 O2 O3 136.0(4) 1_445 6_556
Nb O2 O3 136.0(4) 1_445 6_556
O2 O2 O3 92.6(4) 6_446 6_556
O2 O2 O3 78.1(3) 6_546 6_556
Ga3 O2 O3 123.7(7) 4_446 5_455
Ga2 O2 O3 53.3(5) . 5_455
La O2 O3 116.6(5) 4_445 5_455
O3 O2 O3 74.8(5) 6 5_455
La O2 O3 39.4(2) . 5_455
O3 O2 O3 133.4(6) 2 5_455
O1 O2 O3 63.0(4) 2_455 5_455
O2 O2 O3 74.1(6) 4_445 5_455
O2 O2 O3 14.5(5) 3_455 5_455
O3 O2 O3 89.8(5) 1_556 5_455
O2 O2 O3 139.4(6) 2_556 5_455
O1 O2 O3 71.2(3) 2_456 5_455
O3 O2 O3 84.7(4) . 5_455
Nb O2 O3 101.7(4) . 5_455
Ga1 O2 O3 101.7(4) . 5_455
O1 O2 O3 161.2(5) 1_545 5_455
O2 O2 O3 121.0(6) 2 5_455
Ga2 O2 O3 161.5(5) 2_556 5_455
O3 O2 O3 117.6(5) 5_445 5_455
Ga3 O2 O3 78.2(3) 2_565 5_455
La O2 O3 110.2(3) 4_446 5_455
La O2 O3 64.1(2) 1_556 5_455
Ga3 O2 O3 99.5(4) 4_445 5_455
La O2 O3 50.5(2) 2_455 5_455
O3 O2 O3 124.6(4) 3_556 5_455
O3 O2 O3 103.5(4) 4_446 5_455
Ga3 O2 O3 87.8(3) 2_455 5_455
Ga3 O2 O3 17.67(17) 1_556 5_455
Ga2 O2 O3 71.5(3) 1_554 5_455
O2 O2 O3 61.0(3) 6_556 5_455
La O2 O3 148.6(5) 2 5_455
O3 O2 O3 118.4(4) 3 5_455
O3 O2 O3 98.9(4) 4_445 5_455
O2 O2 O3 138.9(6) 5_446 5_455
O2 O2 O3 32.9(3) 5_456 5_455
O1 O2 O3 35.11(16) . 5_455
O3 O2 O3 103.9(4) 5 5_455
Ga2 O2 O3 38.51(18) 2_566 5_455
Nb O2 O3 102.3(3) 1_556 5_455
Ga1 O2 O3 102.3(3) 1_556 5_455
Ga3 O2 O3 119.6(4) 1_656 5_455
O2 O2 O3 60.6(3) 6 5_455
O2 O2 O3 127.8(5) 5_445 5_455
O2 O2 O3 36.1(2) 5_455 5_455
O2 O2 O3 86.6(2) 1_554 5_455
O2 O2 O3 93.4(2) 1_556 5_455
O3 O2 O3 93.8(4) 4_556 5_455
Ga3 O2 O3 127.7(4) 1_546 5_455
O3 O2 O3 37.1(3) 3_456 5_455
O3 O2 O3 29.1(3) 2_455 5_455
O3 O2 O3 90.4(4) 4 5_455
Ga2 O2 O3 127.2(3) 2 5_455
O3 O2 O3 34.5(3) 3_455 5_455
O2 O2 O3 134.6(5) 3 5_455
O2 O2 O3 74.7(5) 4 5_455
La O2 O3 63.0(2) 2_456 5_455
Ga1 O2 O3 104.8(3) 1_445 5_455
Nb O2 O3 104.8(3) 1_445 5_455
O2 O2 O3 73.0(2) 6_446 5_455
O2 O2 O3 161.1(5) 6_546 5_455
O3 O2 O3 85.6(3) 6_556 5_455
Ga3 O2 O3 133.2(8) 4_446 6_445
Ga2 O2 O3 54.4(5) . 6_445
La O2 O3 50.2(4) 4_445 6_445
O3 O2 O3 161.7(6) 6 6_445
La O2 O3 110.3(4) . 6_445
O3 O2 O3 134.9(5) 2 6_445
O1 O2 O3 63.6(4) 2_455 6_445
O2 O2 O3 16.0(6) 4_445 6_445
O2 O2 O3 75.6(6) 3_455 6_445
O3 O2 O3 131.1(5) 1_556 6_445
O2 O2 O3 96.0(2) 2_556 6_445
O1 O2 O3 71.8(4) 2_456 6_445
O3 O2 O3 120.0(4) . 6_445
Nb O2 O3 147.6(4) . 6_445
Ga1 O2 O3 147.6(4) . 6_445
O1 O2 O3 77.6(4) 1_545 6_445
O2 O2 O3 90.1(2) 2 6_445
Ga2 O2 O3 79.6(4) 2_556 6_445
O3 O2 O3 28.3(4) 5_445 6_445
Ga3 O2 O3 162.9(3) 2_565 6_445
La O2 O3 71.8(3) 4_446 6_445
La O2 O3 107.4(3) 1_556 6_445
Ga3 O2 O3 102.6(3) 4_445 6_445
La O2 O3 43.5(2) 2_455 6_445
O3 O2 O3 133.3(5) 3_556 6_445
O3 O2 O3 38.7(3) 4_446 6_445
Ga3 O2 O3 17.24(15) 2_455 6_445
Ga3 O2 O3 84.6(3) 1_556 6_445
Ga2 O2 O3 71.9(3) 1_554 6_445
O2 O2 O3 139.4(3) 6_556 6_445
La O2 O3 109.3(4) 2 6_445
O3 O2 O3 125.9(4) 3 6_445
O3 O2 O3 36.2(3) 4_445 6_445
O2 O2 O3 60.5(4) 5_446 6_445
O2 O2 O3 104.5(5) 5_456 6_445
O1 O2 O3 123.6(3) . 6_445
O3 O2 O3 164.3(4) 5 6_445
Ga2 O2 O3 124.5(3) 2_566 6_445
Nb O2 O3 133.4(4) 1_556 6_445
Ga1 O2 O3 133.4(4) 1_556 6_445
Ga3 O2 O3 149.8(4) 1_656 6_445
O2 O2 O3 128.3(3) 6 6_445
O2 O2 O3 60.1(4) 5_445 6_445
O2 O2 O3 99.4(4) 5_455 6_445
O2 O2 O3 86.6(2) 1_554 6_445
O2 O2 O3 93.4(2) 1_556 6_445
O3 O2 O3 155.9(4) 4_556 6_445
Ga3 O2 O3 40.8(2) 1_546 6_445
O3 O2 O3 71.8(3) 3_456 6_445
O3 O2 O3 60.4(3) 2_455 6_445
O3 O2 O3 145.2(3) 4 6_445
Ga2 O2 O3 79.5(3) 2 6_445
O3 O2 O3 69.1(3) 3_455 6_445
O2 O2 O3 135.5(5) 3 6_445
O2 O2 O3 164.0(5) 4 6_445
La O2 O3 58.3(2) 2_456 6_445
Ga1 O2 O3 21.12(16) 1_445 6_445
Nb O2 O3 21.12(16) 1_445 6_445
O2 O2 O3 32.0(3) 6_446 6_445
O2 O2 O3 91.0(5) 6_546 6_445
O3 O2 O3 121.8(4) 6_556 6_445
O3 O2 O3 89.5(2) 5_455 6_445
Ga3 O2 La 24.4(5) 4_446 2_556
Ga2 O2 La 108.0(6) . 2_556
La O2 La 103.2(5) 4_445 2_556
O3 O2 La 89.2(4) 6 2_556
La O2 La 140.6(5) . 2_556
O3 O2 La 51.4(4) 2 2_556
O1 O2 La 158.3(5) 2_455 2_556
O2 O2 La 117.9(7) 4_445 2_556
O2 O2 La 139.63(19) 3_455 2_556
O3 O2 La 50.0(4) 1_556 2_556
O2 O2 La 13.2(2) 2_556 2_556
O1 O2 La 79.8(3) 2_456 2_556
O3 O2 La 114.1(4) . 2_556
Nb O2 La 82.5(3) . 2_556
Ga1 O2 La 82.5(3) . 2_556
O1 O2 La 59.6(4) 1_545 2_556
O2 O2 La 96.3(5) 2 2_556
Ga2 O2 La 36.93(15) 2_556 2_556
O3 O2 La 88.1(4) 5_445 2_556
Ga3 O2 La 74.4(2) 2_565 2_556
La O2 La 47.88(18) 4_446 2_556
La O2 La 75.0(2) 1_556 2_556
Ga3 O2 La 111.3(3) 4_445 2_556
La O2 La 150.2(5) 2_455 2_556
O3 O2 La 24.4(2) 3_556 2_556
O3 O2 La 74.9(3) 4_446 2_556
Ga3 O2 La 99.3(4) 2_455 2_556
Ga3 O2 La 125.0(3) 1_556 2_556
Ga2 O2 La 148.8(3) 1_554 2_556
O2 O2 La 82.8(3) 6_556 2_556
La O2 La 59.54(18) 2 2_556
O3 O2 La 80.8(3) 3 2_556
O3 O2 La 118.0(4) 4_445 2_556
O2 O2 La 49.1(3) 5_446 2_556
O2 O2 La 105.8(4) 5_456 2_556
O1 O2 La 120.7(3) . 2_556
O3 O2 La 66.1(2) 5 2_556
Ga2 O2 La 105.3(3) 2_566 2_556
Nb O2 La 38.68(12) 1_556 2_556
Ga1 O2 La 38.68(12) 1_556 2_556
Ga3 O2 La 44.03(13) 1_656 2_556
O2 O2 La 121.5(3) 6 2_556
O2 O2 La 93.0(3) 5_445 2_556
O2 O2 La 151.5(5) 5_455 2_556
O2 O2 La 129.78(14) 1_554 2_556
O2 O2 La 50.22(14) 1_556 2_556
O3 O2 La 55.0(2) 4_556 2_556
Ga3 O2 La 70.2(2) 1_546 2_556
O3 O2 La 113.2(3) 3_456 2_556
O3 O2 La 143.0(3) 2_455 2_556
O3 O2 La 93.7(3) 4 2_556
Ga2 O2 La 93.1(2) 2 2_556
O3 O2 La 171.1(3) 3_455 2_556
O2 O2 La 45.25(19) 3 2_556
O2 O2 La 85.13(17) 4 2_556
La O2 La 95.1(3) 2_456 2_556
Ga1 O2 La 104.3(3) 1_445 2_556
Nb O2 La 104.3(3) 1_445 2_556
O2 O2 La 103.3(5) 6_446 2_556
O2 O2 La 25.75(17) 6_546 2_556
O3 O2 La 53.08(18) 6_556 2_556
O3 O2 La 138.6(3) 5_455 2_556
O3 O2 La 108.9(4) 6_445 2_556
Ga3 O2 Ga3 92.0(7) 4_446 2_564
Ga2 O2 Ga3 131.5(7) . 2_564
La O2 Ga3 92.1(4) 4_445 2_564
O3 O2 Ga3 39.0(4) 6 2_564
La O2 Ga3 39.5(3) . 2_564
O3 O2 Ga3 62.9(4) 2 2_564
O1 O2 Ga3 67.2(4) 2_455 2_564
O2 O2 Ga3 127.6(3) 4_445 2_564
O2 O2 Ga3 90.7(6) 3_455 2_564
O3 O2 Ga3 98.1(5) 1_556 2_564
O2 O2 Ga3 124.6(4) 2_556 2_564
O1 O2 Ga3 143.0(5) 2_456 2_564
O3 O2 Ga3 11.9(2) . 2_564
Nb O2 Ga3 29.79(17) . 2_564
Ga1 O2 Ga3 29.79(17) . 2_564
O1 O2 Ga3 99.1(4) 1_545 2_564
O2 O2 Ga3 57.8(3) 2 2_564
Ga2 O2 Ga3 119.9(3) 2_556 2_564
O3 O2 Ga3 127.8(4) 5_445 2_564
Ga3 O2 Ga3 60.0(3) 2_565 2_564
La O2 Ga3 158.1(4) 4_446 2_564
La O2 Ga3 110.6(4) 1_556 2_564
Ga3 O2 Ga3 34.71(16) 4_445 2_564
La O2 Ga3 97.1(3) 2_455 2_564
O3 O2 Ga3 91.3(4) 3_556 2_564
O3 O2 Ga3 167.1(4) 4_446 2_564
Ga3 O2 Ga3 145.1(3) 2_455 2_564
Ga3 O2 Ga3 94.7(3) 1_556 2_564
Ga2 O2 Ga3 57.6(2) 1_554 2_564
O2 O2 Ga3 74.6(5) 6_556 2_564
La O2 Ga3 70.1(2) 2 2_564
O3 O2 Ga3 39.9(2) 3 2_564
O3 O2 Ga3 97.0(3) 4_445 2_564
O2 O2 Ga3 141.9(4) 5_446 2_564
O2 O2 Ga3 91.4(4) 5_456 2_564
O1 O2 Ga3 52.0(3) . 2_564
O3 O2 Ga3 48.2(2) 5 2_564
Ga2 O2 Ga3 70.2(3) 2_566 2_564
Nb O2 Ga3 97.1(3) 1_556 2_564
Ga1 O2 Ga3 97.1(3) 1_556 2_564
Ga3 O2 Ga3 69.3(2) 1_656 2_564
O2 O2 Ga3 18.60(17) 6 2_564
O2 O2 Ga3 89.4(4) 5_445 2_564
O2 O2 Ga3 46.4(4) 5_455 2_564
O2 O2 Ga3 44.23(15) 1_554 2_564
O2 O2 Ga3 135.77(15) 1_556 2_564
O3 O2 Ga3 74.5(3) 4_556 2_564
Ga3 O2 Ga3 139.9(3) 1_546 2_564
O3 O2 Ga3 115.0(4) 3_456 2_564
O3 O2 Ga3 98.6(3) 2_455 2_564
O3 O2 Ga3 18.84(16) 4 2_564
Ga2 O2 Ga3 70.29(19) 2 2_564
O3 O2 Ga3 74.1(3) 3_455 2_564
O2 O2 Ga3 68.15(16) 3 2_564
O2 O2 Ga3 45.82(15) 4 2_564
La O2 Ga3 141.2(3) 2_456 2_564
Ga1 O2 Ga3 117.6(2) 1_445 2_564
Nb O2 Ga3 117.6(2) 1_445 2_564
O2 O2 Ga3 144.4(4) 6_446 2_564
O2 O2 Ga3 115.1(3) 6_546 2_564
O3 O2 Ga3 106.2(4) 6_556 2_564
O3 O2 Ga3 78.5(3) 5_455 2_564
O3 O2 Ga3 129.4(3) 6_445 2_564
La O2 Ga3 112.2(3) 2_556 2_564
Ga3 O2 O3 26.5(4) 4_446 2_556
Ga2 O2 O3 91.2(5) . 2_556
La O2 O3 126.2(6) 4_445 2_556
O3 O2 O3 81.2(4) 6 2_556
La O2 O3 126.7(5) . 2_556
O3 O2 O3 66.3(4) 2 2_556
O1 O2 O3 175.8(5) 2_455 2_556
O2 O2 O3 116.3(4) 4_445 2_556
O2 O2 O3 115.5(4) 3_455 2_556
O3 O2 O3 27.8(4) 1_556 2_556
O2 O2 O3 29.3(4) 2_556 2_556
O1 O2 O3 61.6(3) 2_456 2_556
O3 O2 O3 122.4(5) . 2_556
Nb O2 O3 88.9(3) . 2_556
Ga1 O2 O3 88.9(3) . 2_556
O1 O2 O3 84.2(4) 1_545 2_556
O2 O2 O3 119.6(6) 2 2_556
Ga2 O2 O3 59.1(3) 2_556 2_556
O3 O2 O3 102.9(4) 5_445 2_556
Ga3 O2 O3 61.6(2) 2_565 2_556
La O2 O3 42.8(2) 4_446 2_556
La O2 O3 50.1(2) 1_556 2_556
Ga3 O2 O3 129.2(3) 4_445 2_556
La O2 O3 141.1(4) 2_455 2_556
O3 O2 O3 27.7(3) 3_556 2_556
O3 O2 O3 75.8(3) 4_446 2_556
Ga3 O2 O3 99.5(4) 2_455 2_556
Ga3 O2 O3 100.4(3) 1_556 2_556
Ga2 O2 O3 171.1(4) 1_554 2_556
O2 O2 O3 62.3(3) 6_556 2_556
La O2 O3 81.8(3) 2 2_556
O3 O2 O3 96.3(3) 3 2_556
O3 O2 O3 137.2(5) 4_445 2_556
O2 O2 O3 63.3(4) 5_446 2_556
O2 O2 O3 80.9(4) 5_456 2_556
O1 O2 O3 101.9(3) . 2_556
O3 O2 O3 67.9(2) 5 2_556
Ga2 O2 O3 83.2(2) 2_566 2_556
Nb O2 O3 20.59(14) 1_556 2_556
Ga1 O2 O3 20.59(14) 1_556 2_556
Ga3 O2 O3 48.97(19) 1_656 2_556
O2 O2 O3 116.1(4) 6 2_556
O2 O2 O3 117.2(4) 5_445 2_556
O2 O2 O3 135.8(4) 5_455 2_556
O2 O2 O3 149.7(2) 1_554 2_556
O2 O2 O3 30.3(2) 1_556 2_556
O3 O2 O3 43.0(3) 4_556 2_556
Ga3 O2 O3 83.9(3) 1_546 2_556
O3 O2 O3 91.2(3) 3_456 2_556
O3 O2 O3 122.3(3) 2_455 2_556
O3 O2 O3 97.3(3) 4 2_556
Ga2 O2 O3 117.9(3) 2 2_556
O3 O2 O3 147.2(3) 3_455 2_556
O2 O2 O3 59.7(2) 3 2_556
O2 O2 O3 75.24(18) 4 2_556
La O2 O3 78.8(2) 2_456 2_556
Ga1 O2 O3 118.7(4) 1_445 2_556
Nb O2 O3 118.7(4) 1_445 2_556
O2 O2 O3 95.6(4) 6_446 2_556
O2 O2 O3 49.5(3) 6_546 2_556
O3 O2 O3 28.6(2) 6_556 2_556
O3 O2 O3 113.8(3) 5_455 2_556
O3 O2 O3 114.4(4) 6_445 2_556
La O2 O3 24.95(15) 2_556 2_556
Ga3 O2 O3 115.4(3) 2_564 2_556
Ga3 O2 O1 48.5(5) 4_446 1_546
Ga2 O2 O1 85.6(6) . 1_546
La O2 O1 96.5(5) 4_445 1_546
O3 O2 O1 112.1(5) 6 1_546
La O2 O1 159.0(5) . 1_546
O3 O2 O1 76.1(4) 2 1_546
O1 O2 O1 147.0(6) 2_455 1_546
O2 O2 O1 92.2(6) 4_445 1_546
O2 O2 O1 124.1(3) 3_455 1_546
O3 O2 O1 59.8(4) 1_556 1_546
O2 O2 O1 13.7(3) 2_556 1_546
O1 O2 O1 60.9(3) 2_456 1_546
O3 O2 O1 138.7(4) . 1_546
Nb O2 O1 108.5(3) . 1_546
Ga1 O2 O1 108.5(3) . 1_546
O1 O2 O1 62.1(3) 1_545 1_546
O2 O2 O1 107.7(6) 2 1_546
Ga2 O2 O1 33.90(19) 2_556 1_546
O3 O2 O1 70.1(3) 5_445 1_546
Ga3 O2 O1 93.9(3) 2_565 1_546
La O2 O1 23.49(14) 4_446 1_546
La O2 O1 71.3(3) 1_556 1_546
Ga3 O2 O1 129.2(3) 4_445 1_546
La O2 O1 124.1(4) 2_455 1_546
O3 O2 O1 48.9(3) 3_556 1_546
O3 O2 O1 49.0(3) 4_446 1_546
Ga3 O2 O1 73.7(3) 2_455 1_546
Ga3 O2 O1 113.5(3) 1_556 1_546
Ga2 O2 O1 148.5(4) 1_554 1_546
O2 O2 O1 93.9(4) 6_556 1_546
La O2 O1 77.0(3) 2 1_546
O3 O2 O1 103.6(4) 3 1_546
O3 O2 O1 104.6(4) 4_445 1_546
O2 O2 O1 30.7(3) 5_446 1_546
O2 O2 O1 102.5(4) 5_456 1_546
O1 O2 O1 133.1(4) . 1_546
O3 O2 O1 91.8(3) 5 1_546
Ga2 O2 O1 112.5(3) 2_566 1_546
Nb O2 O1 53.17(18) 1_556 1_546
Ga1 O2 O1 53.17(18) 1_556 1_546
Ga3 O2 O1 69.9(2) 1_656 1_546
O2 O2 O1 146.5(3) 6 1_546
O2 O2 O1 90.5(3) 5_445 1_546
O2 O2 O1 165.5(4) 5_455 1_546
O2 O2 O1 141.26(17) 1_554 1_546
O2 O2 O1 38.74(17) 1_556 1_546
O3 O2 O1 74.7(2) 4_556 1_546
Ga3 O2 O1 51.16(19) 1_546 1_546
O3 O2 O1 96.1(3) 3_456 1_546
O3 O2 O1 121.0(3) 2_455 1_546
O3 O2 O1 119.8(3) 4 1_546
Ga2 O2 O1 99.6(3) 2 1_546
O3 O2 O1 147.5(4) 3_455 1_546
O2 O2 O1 70.4(2) 3 1_546
O2 O2 O1 106.86(18) 4 1_546
La O2 O1 73.1(3) 2_456 1_546
Ga1 O2 O1 86.1(3) 1_445 1_546
Nb O2 O1 86.1(3) 1_445 1_546
O2 O2 O1 77.3(4) 6_446 1_546
O2 O2 O1 30.4(3) 6_546 1_546
O3 O2 O1 57.5(2) 6_556 1_546
O3 O2 O1 131.0(3) 5_455 1_546
O3 O2 O1 85.2(3) 6_445 1_546
La O2 O1 26.11(8) 2_556 1_546
Ga3 O2 O1 138.2(3) 2_564 1_546
O3 O2 O1 32.75(18) 2_556 1_546
Ga3 O2 O2 164.0(10) 4_446 6_445
Ga2 O2 O2 65.8(3) . 6_445
La O2 O2 47.4(4) 4_445 6_445
O3 O2 O2 129.1(7) 6 6_445
La O2 O2 78.6(4) . 6_445
O3 O2 O2 135.0(5) 2 6_445
O1 O2 O2 29.9(2) 2_455 6_445
O2 O2 O2 32.1(3) 4_445 6_445
O2 O2 O2 61.7(3) 3_455 6_445
O3 O2 O2 153.0(4) 1_556 6_445
O2 O2 O2 128.4(4) 2_556 6_445
O1 O2 O2 93.1(4) 2_456 6_445
O3 O2 O2 89.3(5) . 6_445
Nb O2 O2 122.1(5) . 6_445
Ga1 O2 O2 122.1(5) . 6_445
O1 O2 O2 90.6(5) 1_545 6_445
O2 O2 O2 76.5(5) 2 6_445
Ga2 O2 O2 105.3(6) 2_556 6_445
O3 O2 O2 52.4(4) 5_445 6_445
Ga3 O2 O2 145.2(6) 2_565 6_445
La O2 O2 104.9(5) 4_446 6_445
La O2 O2 120.1(2) 1_556 6_445
Ga3 O2 O2 77.8(4) 4_445 6_445
La O2 O2 22.00(9) 2_455 6_445
O3 O2 O2 163.4(6) 3_556 6_445
O3 O2 O2 72.2(4) 4_446 6_445
Ga3 O2 O2 48.2(3) 2_455 6_445
Ga3 O2 O2 76.04(12) 1_556 6_445
Ga2 O2 O2 39.6(2) 1_554 6_445
O2 O2 O2 132.3(4) 6_556 6_445
La O2 O2 110.6(4) 2 6_445
O3 O2 O2 109.2(4) 3 6_445
O3 O2 O2 28.2(3) 4_445 6_445
O2 O2 O2 91.5(6) 5_446 6_445
O2 O2 O2 99.5(3) 5_456 6_445
O1 O2 O2 98.2(4) . 6_445
O3 O2 O2 143.9(5) 5 6_445
Ga2 O2 O2 109.7(3) 2_566 6_445
Nb O2 O2 163.1(4) 1_556 6_445
Ga1 O2 O2 163.1(4) 1_556 6_445
Ga3 O2 O2 158.2(4) 1_656 6_445
O2 O2 O2 94.5(4) 6 6_445
O2 O2 O2 59.9(5) 5_445 6_445
O2 O2 O2 67.8(4) 5_455 6_445
O2 O2 O2 58.1(3) 1_554 6_445
O2 O2 O2 121.9(3) 1_556 6_445
O3 O2 O2 164.3(6) 4_556 6_445
Ga3 O2 O2 70.2(4) 1_546 6_445
O3 O2 O2 74.5(2) 3_456 6_445
O3 O2 O2 47.81(16) 2_455 6_445
O3 O2 O2 114.7(5) 4 6_445
Ga2 O2 O2 71.3(3) 2 6_445
O3 O2 O2 40.7(2) 3_455 6_445
O2 O2 O2 140.4(3) 3 6_445
O2 O2 O2 134.0(6) 4 6_445
La O2 O2 76.0(2) 2_456 6_445
Ga1 O2 O2 36.4(3) 1_445 6_445
Nb O2 O2 36.4(3) 1_445 6_445
O2 O2 O2 54.1(2) 6_446 6_445
O2 O2 O2 117.4(7) 6_546 6_445
O3 O2 O2 143.4(3) 6_556 6_445
O3 O2 O2 71.4(2) 5_455 6_445
O3 O2 O2 33.9(3) 6_445 6_445
La O2 O2 140.4(6) 2_556 6_445
Ga3 O2 O2 96.8(4) 2_564 6_445
O3 O2 O2 147.7(6) 2_556 6_445
O1 O2 O2 118.8(6) 1_546 6_445
Ga3 O2 O2 81.5(3) 4_446 6_545
Ga2 O2 O2 141.7(9) . 6_545
La O2 O2 41.4(4) 4_445 6_545
O3 O2 O2 99.4(5) 6 6_545
La O2 O2 110.1(5) . 6_545
O3 O2 O2 49.9(3) 2 6_545
O1 O2 O2 84.6(4) 2_455 6_545
O2 O2 O2 103.0(9) 4_445 6_545
O2 O2 O2 145.3(3) 3_455 6_545
O3 O2 O2 117.6(4) 1_556 6_545
O2 O2 O2 75.7(5) 2_556 6_545
O1 O2 O2 139.9(7) 2_456 6_545
O3 O2 O2 66.6(4) . 6_545
Nb O2 O2 65.4(2) . 6_545
Ga1 O2 O2 65.4(2) . 6_545
O1 O2 O2 23.6(3) 1_545 6_545
O2 O2 O2 23.9(3) 2 6_545
Ga2 O2 O2 50.5(2) 2_556 6_545
O3 O2 O2 63.3(4) 5_445 6_545
Ga3 O2 O2 108.9(3) 2_565 6_545
La O2 O2 102.3(5) 4_446 6_545
La O2 O2 149.0(4) 1_556 6_545
Ga3 O2 O2 47.2(2) 4_445 6_545
La O2 O2 109.2(4) 2_455 6_545
O3 O2 O2 80.2(2) 3_556 6_545
O3 O2 O2 96.2(6) 4_446 6_545
Ga3 O2 O2 99.3(5) 2_455 6_545
Ga3 O2 O2 160.4(4) 1_556 6_545
Ga2 O2 O2 74.3(3) 1_554 6_545
O2 O2 O2 132.3(4) 6_556 6_545
La O2 O2 23.30(8) 2 6_545
O3 O2 O2 42.0(2) 3 6_545
O3 O2 O2 60.8(4) 4_445 6_545
O2 O2 O2 67.1(2) 5_446 6_545
O2 O2 O2 166.4(7) 5_456 6_545
O1 O2 O2 128.2(6) . 6_545
O3 O2 O2 76.4(3) 5 6_545
Ga2 O2 O2 143.5(6) 2_566 6_545
Nb O2 O2 104.8(2) 1_556 6_545
Ga1 O2 O2 104.8(2) 1_556 6_545
Ga3 O2 O2 72.95(12) 1_656 6_545
O2 O2 O2 94.5(4) 6 6_545
O2 O2 O2 29.3(3) 5_445 6_545
O2 O2 O2 110.0(6) 5_455 6_545
O2 O2 O2 58.1(3) 1_554 6_545
O2 O2 O2 121.9(3) 1_556 6_545
O3 O2 O2 102.6(3) 4_556 6_545
Ga3 O2 O2 65.8(4) 1_546 6_545
O3 O2 O2 159.7(5) 3_456 6_545
O3 O2 O2 134.8(4) 2_455 6_545
O3 O2 O2 72.6(3) 4 6_545
Ga2 O2 O2 18.75(17) 2 6_545
O3 O2 O2 113.7(4) 3_455 6_545
O2 O2 O2 53.75(18) 3 6_545
O2 O2 O2 103.44(19) 4 6_545
La O2 O2 139.9(6) 2_456 6_545
Ga1 O2 O2 67.1(3) 1_445 6_545
Nb O2 O2 67.1(3) 1_445 6_545
O2 O2 O2 117.4(7) 6_446 6_545
O2 O2 O2 54.1(2) 6_546 6_545
O3 O2 O2 124.8(3) 6_556 6_545
O3 O2 O2 144.8(5) 5_455 6_545
O3 O2 O2 88.0(4) 6_445 6_545
La O2 O2 74.5(2) 2_556 6_545
Ga3 O2 O2 76.2(4) 2_564 6_545
O3 O2 O2 99.2(3) 2_556 6_545
O1 O2 O2 83.8(3) 1_546 6_545
O2 O2 O2 87.7(4) 6_445 6_545
Ga3 O2 O2 148.8(6) 4_446 4_444
Ga2 O2 O2 93.2(6) . 4_444
La O2 O2 39.7(3) 4_445 4_444
O3 O2 O2 108.2(5) 6 4_444
La O2 O2 66.5(2) . 4_444
O3 O2 O2 109.0(5) 2 4_444
O1 O2 O2 16.50(16) 2_455 4_444
O2 O2 O2 60.8(2) 4_445 4_444
O2 O2 O2 75.89(10) 3_455 4_444
O3 O2 O2 165.8(7) 1_556 4_444
O2 O2 O2 136.7(6) 2_556 4_444
O1 O2 O2 121.8(5) 2_456 4_444
O3 O2 O2 61.6(2) . 4_444
Nb O2 O2 93.3(2) . 4_444
Ga1 O2 O2 93.3(2) . 4_444
O1 O2 O2 82.3(4) 1_545 4_444
O2 O2 O2 51.6(2) 2 4_444
Ga2 O2 O2 106.8(5) 2_556 4_444
O3 O2 O2 65.1(4) 5_445 4_444
Ga3 O2 O2 129.0(5) 2_565 4_444
La O2 O2 129.6(5) 4_446 4_444
La O2 O2 141.6(5) 1_556 4_444
Ga3 O2 O2 48.73(15) 4_445 4_444
La O2 O2 43.7(3) 2_455 4_444
O3 O2 O2 147.5(4) 3_556 4_444
O3 O2 O2 96.8(4) 4_446 4_444
Ga3 O2 O2 75.1(3) 2_455 4_444
Ga3 O2 O2 91.3(4) 1_556 4_444
Ga2 O2 O2 14.75(11) 1_554 4_444
O2 O2 O2 131.4(7) 6_556 4_444
La O2 O2 89.1(3) 2 4_444
O3 O2 O2 80.8(3) 3 4_444
O3 O2 O2 30.1(3) 4_445 4_444
O2 O2 O2 103.8(5) 5_446 4_444
O2 O2 O2 112.2(5) 5_456 4_444
O1 O2 O2 91.8(4) . 4_444
O3 O2 O2 115.3(3) 5 4_444
Ga2 O2 O2 110.9(4) 2_566 4_444
Nb O2 O2 167.4(4) 1_556 4_444
Ga1 O2 O2 167.4(4) 1_556 4_444
Ga3 O2 O2 130.1(3) 1_656 4_444
O2 O2 O2 74.1(3) 6 4_444
O2 O2 O2 49.0(5) 5_445 4_444
O2 O2 O2 57.9(4) 5_455 4_444
O2 O2 O2 29.2(2) 1_554 4_444
O2 O2 O2 150.8(2) 1_556 4_444
O3 O2 O2 145.4(4) 4_556 4_444
Ga3 O2 O2 83.8(4) 1_546 4_444
O3 O2 O2 97.4(4) 3_456 4_444
O3 O2 O2 66.6(3) 2_455 4_444
O3 O2 O2 87.2(2) 4 4_444
Ga2 O2 O2 50.8(3) 2 4_444
O3 O2 O2 45.1(3) 3_455 4_444
O2 O2 O2 115.3(3) 3 4_444
O2 O2 O2 114.6(3) 4 4_444
La O2 O2 104.4(3) 2_456 4_444
Ga1 O2 O2 50.0(3) 1_445 4_444
Nb O2 O2 50.0(3) 1_445 4_444
O2 O2 O2 83.1(4) 6_446 4_444
O2 O2 O2 116.7(6) 6_546 4_444
O3 O2 O2 165.0(5) 6_556 4_444
O3 O2 O2 79.4(3) 5_455 4_444
O3 O2 O2 58.6(3) 6_445 4_444
La O2 O2 141.9(5) 2_556 4_444
Ga3 O2 O2 70.85(17) 2_564 4_444
O3 O2 O2 165.9(5) 2_556 4_444
O1 O2 O2 134.4(5) 1_546 4_444
O2 O2 O2 29.1(4) 6_445 4_444
O2 O2 O2 69.4(3) 6_545 4_444
Ga3 O2 O2 143.7(9) 4_446 3_454
Ga2 O2 O2 93.2(6) . 3_454
La O2 O2 66.9(2) 4_445 3_454
O3 O2 O2 83.7(6) 6 3_454
La O2 O2 38.2(3) . 3_454
O3 O2 O2 108.2(6) 2 3_454
O1 O2 O2 16.50(16) 2_455 3_454
O2 O2 O2 75.89(10) 4_445 3_454
O2 O2 O2 60.8(2) 3_455 3_454
O3 O2 O2 137.6(7) 1_556 3_454
O2 O2 O2 162.0(7) 2_556 3_454
O1 O2 O2 121.8(5) 2_456 3_454
O3 O2 O2 46.9(4) . 3_454
Nb O2 O2 80.3(4) . 3_454
Ga1 O2 O2 80.3(4) . 3_454
O1 O2 O2 105.3(4) 1_545 3_454
O2 O2 O2 63.5(4) 2 3_454
Ga2 O2 O2 132.6(3) 2_556 3_454
O3 O2 O2 92.6(4) 5_445 3_454
Ga3 O2 O2 102.9(5) 2_565 3_454
La O2 O2 150.0(5) 4_446 3_454
La O2 O2 122.0(4) 1_556 3_454
Ga3 O2 O2 47.1(2) 4_445 3_454
La O2 O2 46.7(2) 2_455 3_454
O3 O2 O2 142.9(6) 3_556 3_454
O3 O2 O2 118.2(4) 4_446 3_454
Ga3 O2 O2 93.7(3) 2_455 3_454
Ga3 O2 O2 74.3(3) 1_556 3_454
Ga2 O2 O2 14.75(11) 1_554 3_454
O2 O2 O2 103.3(6) 6_556 3_454
La O2 O2 99.2(3) 2 3_454
O3 O2 O2 78.2(4) 3 3_454
O3 O2 O2 58.0(2) 4_445 3_454
O2 O2 O2 131.9(5) 5_446 3_454
O2 O2 O2 90.2(5) 5_456 3_454
O1 O2 O2 63.8(4) . 3_454
O3 O2 O2 99.9(5) 5 3_454
Ga2 O2 O2 83.7(4) 2_566 3_454
Nb O2 O2 143.9(6) 1_556 3_454
Ga1 O2 O2 143.9(6) 1_556 3_454
Ga3 O2 O2 120.7(5) 1_656 3_454
O2 O2 O2 48.7(3) 6 3_454
O2 O2 O2 74.2(3) 5_445 3_454
O2 O2 O2 30.1(4) 5_455 3_454
O2 O2 O2 29.2(2) 1_554 3_454
O2 O2 O2 150.8(2) 1_556 3_454
O3 O2 O2 121.7(6) 4_556 3_454
Ga3 O2 O2 111.6(3) 1_546 3_454
O3 O2 O2 88.1(4) 3_456 3_454
O3 O2 O2 58.5(3) 2_455 3_454
O3 O2 O2 70.4(4) 4 3_454
Ga2 O2 O2 68.74(16) 2 3_454
O3 O2 O2 30.4(2) 3_455 3_454
O2 O2 O2 114.6(3) 3 3_454
O2 O2 O2 89.4(5) 4 3_454
La O2 O2 106.1(4) 2_456 3_454
Ga1 O2 O2 76.8(2) 1_445 3_454
Nb O2 O2 76.8(2) 1_445 3_454
O2 O2 O2 94.5(3) 6_446 3_454
O2 O2 O2 140.1(4) 6_546 3_454
O3 O2 O2 139.1(5) 6_556 3_454
O3 O2 O2 58.4(3) 5_455 3_454
O3 O2 O2 80.1(3) 6_445 3_454
La O2 O2 158.4(4) 2_556 3_454
Ga3 O2 O2 51.7(3) 2_564 3_454
O3 O2 O2 164.5(5) 2_556 3_454
O1 O2 O2 162.6(5) 1_546 3_454
O2 O2 O2 46.2(2) 6_445 3_454
O2 O2 O2 86.5(3) 6_545 3_454
O2 O2 O2 28.2(2) 4_444 3_454
Ga3 O2 O2 83.9(5) 4_446 4_446
Ga2 O2 O2 37.5(4) . 4_446
La O2 O2 109.3(7) 4_445 4_446
O3 O2 O2 121.2(5) 6 4_446
La O2 O2 124.1(4) . 4_446
O3 O2 O2 121.7(6) 2 4_446
O1 O2 O2 118.8(5) 2_455 4_446
O2 O2 O2 60.8(2) 4_445 4_446
O2 O2 O2 75.89(10) 3_455 4_446
O3 O2 O2 65.9(4) 1_556 4_446
O2 O2 O2 61.4(4) 2_556 4_446
O1 O2 O2 15.12(14) 2_456 4_446
O3 O2 O2 168.5(6) . 4_446
Nb O2 O2 145.0(4) . 4_446
Ga1 O2 O2 145.0(4) . 4_446
O1 O2 O2 101.2(7) 1_545 4_446
O2 O2 O2 144.8(6) 2 4_446
Ga2 O2 O2 76.6(5) 2_556 4_446
O3 O2 O2 73.9(5) 5_445 4_446
Ga3 O2 O2 101.4(3) 2_565 4_446
La O2 O2 25.4(2) 4_446 4_446
La O2 O2 47.39(11) 1_556 4_446
Ga3 O2 O2 167.2(5) 4_445 4_446
La O2 O2 84.3(3) 2_455 4_446
O3 O2 O2 85.0(3) 3_556 4_446
O3 O2 O2 34.0(3) 4_446 4_446
Ga3 O2 O2 48.1(3) 2_455 4_446
Ga3 O2 O2 67.8(2) 1_556 4_446
Ga2 O2 O2 131.2(4) 1_554 4_446
O2 O2 O2 83.9(3) 6_556 4_446
La O2 O2 125.1(5) 2 4_446
O3 O2 O2 151.5(5) 3 4_446
O3 O2 O2 101.0(5) 4_445 4_446
O2 O2 O2 57.7(6) 5_446 4_446
O2 O2 O2 66.7(3) 5_456 4_446
O1 O2 O2 106.4(3) . 4_446
O3 O2 O2 123.0(3) 5 4_446
Ga2 O2 O2 87.4(2) 2_566 4_446
Nb O2 O2 70.90(19) 1_556 4_446
Ga1 O2 O2 70.90(19) 1_556 4_446
Ga3 O2 O2 106.4(3) 1_656 4_446
O2 O2 O2 140.3(5) 6 4_446
O2 O2 O2 113.0(6) 5_445 4_446
O2 O2 O2 121.0(4) 5_455 4_446
O2 O2 O2 150.8(2) 1_554 4_446
O2 O2 O2 29.2(2) 1_556 4_446
O3 O2 O2 91.1(3) 4_556 4_446
Ga3 O2 O2 62.7(4) 1_546 4_446
O3 O2 O2 48.4(2) 3_456 4_446
O3 O2 O2 73.0(3) 2_455 4_446
O3 O2 O2 149.2(4) 4 4_446
Ga2 O2 O2 132.3(6) 2 4_446
O3 O2 O2 101.0(3) 3_455 4_446
O2 O2 O2 115.3(3) 3 4_446
O2 O2 O2 114.6(3) 4 4_446
La O2 O2 24.70(16) 2_456 4_446
Ga1 O2 O2 81.6(4) 1_445 4_446
Nb O2 O2 81.6(4) 1_445 4_446
O2 O2 O2 38.7(3) 6_446 4_446
O2 O2 O2 77.8(5) 6_546 4_446
O3 O2 O2 56.4(2) 6_556 4_446
O3 O2 O2 85.3(3) 5_455 4_446
O3 O2 O2 65.3(3) 6_445 4_446
La O2 O2 70.7(3) 2_556 4_446
Ga3 O2 O2 157.4(5) 2_564 4_446
O3 O2 O2 57.5(2) 2_556 4_446
O1 O2 O2 48.6(3) 1_546 4_446
O2 O2 O2 92.7(4) 6_445 4_446
O2 O2 O2 124.8(7) 6_545 4_446
O2 O2 O2 121.6(5) 4_444 4_446
O2 O2 O2 130.0(4) 3_454 4_446
Ga3 O2 O2 81.0(4) 4_446 3_456
Ga2 O2 O2 37.5(4) . 3_456
La O2 O2 135.0(7) 4_445 3_456
O3 O2 O2 95.5(6) 6 3_456
La O2 O2 100.1(4) . 3_456
O3 O2 O2 120.8(5) 2 3_456
O1 O2 O2 118.8(5) 2_455 3_456
O2 O2 O2 75.89(10) 4_445 3_456
O2 O2 O2 60.8(2) 3_455 3_456
O3 O2 O2 50.3(3) 1_556 3_456
O2 O2 O2 75.2(4) 2_556 3_456
O1 O2 O2 15.12(13) 2_456 3_456
O3 O2 O2 140.5(6) . 3_456
Nb O2 O2 126.3(5) . 3_456
Ga1 O2 O2 126.3(5) . 3_456
O1 O2 O2 126.4(5) 1_545 3_456
O2 O2 O2 172.7(7) 2 3_456
Ga2 O2 O2 99.0(3) 2_556 3_456
O3 O2 O2 100.9(5) 5_445 3_456
Ga3 O2 O2 78.1(3) 2_565 3_456
La O2 O2 47.53(11) 4_446 3_456
La O2 O2 21.49(17) 1_556 3_456
Ga3 O2 O2 162.6(5) 4_445 3_456
La O2 O2 86.4(4) 2_455 3_456
O3 O2 O2 82.3(3) 3_556 3_456
O3 O2 O2 61.6(3) 4_446 3_456
Ga3 O2 O2 69.8(3) 2_455 3_456
Ga3 O2 O2 47.9(3) 1_556 3_456
Ga2 O2 O2 131.2(4) 1_554 3_456
O2 O2 O2 57.4(3) 6_556 3_456
La O2 O2 138.6(3) 2 3_456
O3 O2 O2 146.6(5) 3 3_456
O3 O2 O2 121.8(5) 4_445 3_456
O2 O2 O2 84.0(5) 5_446 3_456
O2 O2 O2 39.7(4) 5_456 3_456
O1 O2 O2 79.0(4) . 3_456
O3 O2 O2 106.8(4) 5 3_456
Ga2 O2 O2 59.2(3) 2_566 3_456
Nb O2 O2 60.3(2) 1_556 3_456
Ga1 O2 O2 60.3(2) 1_556 3_456
Ga3 O2 O2 98.5(3) 1_656 3_456
O2 O2 O2 112.6(5) 6 3_456
O2 O2 O2 140.8(6) 5_445 3_456
O2 O2 O2 100.5(4) 5_455 3_456
O2 O2 O2 150.8(2) 1_554 3_456
O2 O2 O2 29.2(2) 1_556 3_456
O3 O2 O2 73.9(3) 4_556 3_456
Ga3 O2 O2 91.0(3) 1_546 3_456
O3 O2 O2 34.3(3) 3_456 3_456
O3 O2 O2 65.3(3) 2_455 3_456
O3 O2 O2 124.9(5) 4 3_456
Ga2 O2 O2 160.5(5) 2 3_456
O3 O2 O2 91.9(4) 3_455 3_456
O2 O2 O2 114.6(3) 3 3_456
O2 O2 O2 89.4(5) 4 3_456
La O2 O2 28.5(2) 2_456 3_456
Ga1 O2 O2 105.6(4) 1_445 3_456
Nb O2 O2 105.6(4) 1_445 3_456
O2 O2 O2 54.4(3) 6_446 3_456
O2 O2 O2 96.1(4) 6_546 3_456
O3 O2 O2 40.3(3) 6_556 3_456
O3 O2 O2 65.1(3) 5_455 3_456
O3 O2 O2 86.0(4) 6_445 3_456
La O2 O2 79.2(2) 2_556 3_456
Ga3 O2 O2 129.2(4) 2_564 3_456
O3 O2 O2 57.0(3) 2_556 3_456
O1 O2 O2 65.93(19) 1_546 3_456
O2 O2 O2 103.3(4) 6_445 3_456
O2 O2 O2 149.5(5) 6_545 3_456
O2 O2 O2 130.0(4) 4_444 3_456
O2 O2 O2 121.6(5) 3_454 3_456
O2 O2 O2 28.2(2) 4_446 3_456
Ga3 O2 O3 105.8(7) 4_446 6_554
Ga2 O2 O3 128.7(6) . 6_554
La O2 O3 75.8(4) 4_445 6_554
O3 O2 O3 56.7(4) 6 6_554
La O2 O3 42.0(3) . 6_554
O3 O2 O3 70.8(5) 2 6_554
O1 O2 O3 52.1(3) 2_455 6_554
O2 O2 O3 112.56(19) 4_445 6_554
O2 O2 O3 89.6(4) 3_455 6_554
O3 O2 O3 115.8(6) 1_556 6_554
O2 O2 O3 132.5(5) 2_556 6_554
O1 O2 O3 151.3(5) 2_456 6_554
O3 O2 O3 8.7(2) . 6_554
Nb O2 O3 42.3(2) . 6_554
Ga1 O2 O3 42.3(2) . 6_554
O1 O2 O3 91.9(4) 1_545 6_554
O2 O2 O3 46.2(4) 2 6_554
Ga2 O2 O3 117.6(3) 2_556 6_554
O3 O2 O3 111.1(4) 5_445 6_554
Ga3 O2 O3 77.7(4) 2_565 6_554
La O2 O3 169.1(3) 4_446 6_554
La O2 O3 125.7(5) 1_556 6_554
Ga3 O2 O3 21.54(16) 4_445 6_554
La O2 O3 85.0(3) 2_455 6_554
O3 O2 O3 104.9(4) 3_556 6_554
O3 O2 O3 149.4(4) 4_446 6_554
Ga3 O2 O3 128.6(3) 2_455 6_554
Ga3 O2 O3 97.9(4) 1_556 6_554
Ga2 O2 O3 41.15(18) 1_554 6_554
O2 O2 O3 90.9(6) 6_556 6_554
La O2 O3 69.4(2) 2 6_554
O3 O2 O3 42.2(3) 3 6_554
O3 O2 O3 79.3(3) 4_445 6_554
O2 O2 O3 134.9(4) 5_446 6_554
O2 O2 O3 101.3(4) 5_456 6_554
O1 O2 O3 62.2(4) . 6_554
O3 O2 O3 63.3(3) 5 6_554
Ga2 O2 O3 82.7(3) 2_566 6_554
Nb O2 O3 114.1(4) 1_556 6_554
Ga1 O2 O3 114.1(4) 1_556 6_554
Ga3 O2 O3 82.8(3) 1_656 6_554
O2 O2 O3 29.3(2) 6 6_554
O2 O2 O3 75.0(3) 5_445 6_554
O2 O2 O3 44.5(4) 5_455 6_554
O2 O2 O3 26.6(2) 1_554 6_554
O2 O2 O3 153.4(2) 1_556 6_554
O3 O2 O3 91.9(4) 4_556 6_554
Ga3 O2 O3 125.7(3) 1_546 6_554
O3 O2 O3 117.1(4) 3_456 6_554
O3 O2 O3 93.2(3) 2_455 6_554
O3 O2 O3 34.0(3) 4 6_554
Ga2 O2 O3 57.82(19) 2 6_554
O3 O2 O3 65.7(3) 3_455 6_554
O2 O2 O3 76.95(18) 3 6_554
O2 O2 O3 63.4(2) 4 6_554
La O2 O3 141.2(3) 2_456 6_554
Ga1 O2 O3 100.0(3) 1_445 6_554
Nb O2 O3 100.0(3) 1_445 6_554
O2 O2 O3 132.7(4) 6_446 6_554
O2 O2 O3 116.7(3) 6_546 6_554
O3 O2 O3 123.9(5) 6_556 6_554
O3 O2 O3 80.3(3) 5_455 6_554
O3 O2 O3 112.2(3) 6_445 6_554
La O2 O3 122.2(3) 2_556 6_554
Ga3 O2 O3 17.70(14) 2_564 6_554
O3 O2 O3 131.1(3) 2_556 6_554
O1 O2 O3 145.7(3) 1_546 6_554
O2 O2 O3 80.8(4) 6_445 6_554
O2 O2 O3 68.3(3) 6_545 6_554
O2 O2 O3 53.56(18) 4_444 6_554
O2 O2 O3 38.3(3) 3_454 6_554
O2 O2 O3 165.5(4) 4_446 6_554
O2 O2 O3 141.0(4) 3_456 6_554
Ga3 O2 La 86.6(5) 4_446 1_545
Ga2 O2 La 115.8(7) . 1_545
La O2 La 33.7(3) 4_445 1_545
O3 O2 La 125.3(4) 6 1_545
La O2 La 131.5(4) . 1_545
O3 O2 La 69.0(4) 2 1_545
O1 O2 La 89.3(4) 2_455 1_545
O2 O2 La 81.8(8) 4_445 1_545
O2 O2 La 139.2(7) 3_455 1_545
O3 O2 La 119.4(5) 1_556 1_545
O2 O2 La 64.5(4) 2_556 1_545
O1 O2 La 113.9(5) 2_456 1_545
O3 O2 La 92.5(3) . 1_545
Nb O2 La 91.9(3) . 1_545
Ga1 O2 La 91.9(3) . 1_545
O1 O2 La 12.44(14) 1_545 1_545
O2 O2 La 46.2(3) 2 1_545
Ga2 O2 La 34.47(15) 2_556 1_545
O3 O2 La 38.3(3) 5_445 1_545
Ga3 O2 La 129.2(3) 2_565 1_545
La O2 La 79.8(3) 4_446 1_545
La O2 La 138.2(4) 1_556 1_545
Ga3 O2 La 70.90(19) 4_445 1_545
La O2 La 99.8(3) 2_455 1_545
O3 O2 La 85.7(3) 3_556 1_545
O3 O2 La 68.8(3) 4_446 1_545
Ga3 O2 La 73.8(3) 2_455 1_545
Ga3 O2 La 150.4(4) 1_556 1_545
Ga2 O2 La 83.6(2) 1_554 1_545
O2 O2 La 149.1(2) 6_556 1_545
La O2 La 44.04(14) 2 1_545
O3 O2 La 69.1(3) 3 1_545
O3 O2 La 50.8(3) 4_445 1_545
O2 O2 La 42.69(19) 5_446 1_545
O2 O2 La 165.6(6) 5_456 1_545
O1 O2 La 154.5(4) . 1_545
O3 O2 La 98.8(3) 5 1_545
Ga2 O2 La 169.6(4) 2_566 1_545
Nb O2 La 107.5(3) 1_556 1_545
Ga1 O2 La 107.5(3) 1_556 1_545
Ga3 O2 La 88.2(2) 1_656 1_545
O2 O2 La 120.7(3) 6 1_545
O2 O2 La 24.06(13) 5_445 1_545
O2 O2 La 127.4(4) 5_455 1_545
O2 O2 La 75.01(16) 1_554 1_545
O2 O2 La 105.00(16) 1_556 1_545
O3 O2 La 116.0(3) 4_556 1_545
Ga3 O2 La 38.29(13) 1_546 1_545
O3 O2 La 135.3(4) 3_456 1_545
O3 O2 La 123.9(3) 2_455 1_545
O3 O2 La 99.9(3) 4 1_545
Ga2 O2 La 34.83(10) 2 1_545
O3 O2 La 116.0(3) 3_455 1_545
O2 O2 La 70.4(3) 3 1_545
O2 O2 La 128.1(3) 4 1_545
La O2 La 112.4(4) 2_456 1_545
Ga1 O2 La 47.16(15) 1_445 1_545
Nb O2 La 47.16(15) 1_445 1_545
O2 O2 La 91.6(5) 6_446 1_545
O2 O2 La 43.9(3) 6_546 1_545
O3 O2 La 121.8(3) 6_556 1_545
O3 O2 La 149.7(3) 5_455 1_545
O3 O2 La 65.9(3) 6_445 1_545
La O2 La 69.5(2) 2_556 1_545
Ga3 O2 La 102.9(2) 2_564 1_545
O3 O2 La 93.2(3) 2_556 1_545
O1 O2 La 67.1(2) 1_546 1_545
O2 O2 La 78.4(4) 6_445 1_545
O2 O2 La 27.5(3) 6_545 1_545
O2 O2 La 72.8(3) 4_444 1_545
O2 O2 La 98.2(2) 3_454 1_545
O2 O2 La 99.0(5) 4_446 1_545
O2 O2 La 126.5(4) 3_456 1_545
O3 O2 La 92.4(2) 6_554 1_545
Ga3 O2 O3 96.3(5) 4_446 2_554
Ga2 O2 O3 146.3(6) . 2_554
La O2 O3 58.9(4) 4_445 2_554
O3 O2 O3 70.3(4) 6 2_554
La O2 O3 67.8(3) . 2_554
O3 O2 O3 56.2(3) 2 2_554
O1 O2 O3 61.7(3) 2_455 2_554
O2 O2 O3 113.7(3) 4_445 2_554
O2 O2 O3 113.0(3) 3_455 2_554
O3 O2 O3 121.1(6) 1_556 2_554
O2 O2 O3 111.3(6) 2_556 2_554
O1 O2 O3 175.9(5) 2_456 2_554
O3 O2 O3 24.9(3) . 2_554
Nb O2 O3 41.8(2) . 2_554
Ga1 O2 O3 41.8(2) . 2_554
O1 O2 O3 66.0(4) 1_545 2_554
O2 O2 O3 21.8(2) 2 2_554
Ga2 O2 O3 91.9(3) 2_556 2_554
O3 O2 O3 93.7(4) 5_445 2_554
Ga3 O2 O3 88.9(3) 2_565 2_554
La O2 O3 144.2(4) 4_446 2_554
La O2 O3 144.8(4) 1_556 2_554
Ga3 O2 O3 7.04(16) 4_445 2_554
La O2 O3 96.3(3) 2_455 2_554
O3 O2 O3 95.0(3) 3_556 2_554
O3 O2 O3 133.2(4) 4_446 2_554
Ga3 O2 O3 123.0(3) 2_455 2_554
Ga3 O2 O3 123.2(4) 1_556 2_554
Ga2 O2 O3 48.7(2) 1_554 2_554
O2 O2 O3 108.3(5) 6_556 2_554
La O2 O3 46.02(19) 2 2_554
O3 O2 O3 26.4(3) 3 2_554
O3 O2 O3 69.8(2) 4_445 2_554
O2 O2 O3 109.3(3) 5_446 2_554
O2 O2 O3 126.6(5) 5_456 2_554
O1 O2 O3 86.9(4) . 2_554
O3 O2 O3 62.9(2) 5 2_554
Ga2 O2 O3 106.1(4) 2_566 2_554
Nb O2 O3 113.5(3) 1_556 2_554
Ga1 O2 O3 113.5(3) 1_556 2_554
Ga3 O2 O3 75.6(2) 1_656 2_554
O2 O2 O3 53.1(3) 6 2_554
O2 O2 O3 54.0(3) 5_445 2_554
O2 O2 O3 69.4(4) 5_455 2_554
O2 O2 O3 27.3(2) 1_554 2_554
O2 O2 O3 152.7(2) 1_556 2_554
O3 O2 O3 96.1(4) 4_556 2_554
Ga3 O2 O3 103.9(3) 1_546 2_554
O3 O2 O3 141.0(4) 3_456 2_554
O3 O2 O3 112.6(4) 2_455 2_554
O3 O2 O3 41.1(3) 4 2_554
Ga2 O2 O3 34.31(15) 2 2_554
O3 O2 O3 84.5(3) 3_455 2_554
O2 O2 O3 62.7(2) 3 2_554
O2 O2 O3 76.63(16) 4 2_554
La O2 O3 158.7(3) 2_456 2_554
Ga1 O2 O3 87.8(2) 1_445 2_554
Nb O2 O3 87.8(2) 1_445 2_554
O2 O2 O3 136.2(4) 6_446 2_554
O2 O2 O3 92.5(3) 6_546 2_554
O3 O2 O3 131.2(3) 6_556 2_554
O3 O2 O3 105.5(4) 5_455 2_554
O3 O2 O3 106.0(3) 6_445 2_554
La O2 O3 104.3(3) 2_556 2_554
Ga3 O2 O3 36.00(15) 2_564 2_554
O3 O2 O3 122.4(4) 2_556 2_554
O1 O2 O3 122.8(3) 1_546 2_554
O2 O2 O3 83.4(4) 6_445 2_554
O2 O2 O3 42.4(3) 6_545 2_554
O2 O2 O3 54.6(2) 4_444 2_554
O2 O2 O3 54.1(3) 3_454 2_554
O2 O2 O3 166.5(5) 4_446 2_554
O2 O2 O3 165.1(5) 3_456 2_554
O3 O2 O3 25.9(2) 6_554 2_554
La O2 O3 67.58(18) 1_545 2_554
Ga3 O2 La 83.8(7) 4_446 2_565
Ga2 O2 La 106.0(6) . 2_565
La O2 La 126.4(5) 4_445 2_565
O3 O2 La 19.7(3) 6 2_565
La O2 La 32.5(3) . 2_565
O3 O2 La 76.7(5) 2 2_565
O1 O2 La 84.1(4) 2_455 2_565
O2 O2 La 129.1(7) 4_445 2_565
O2 O2 La 71.2(7) 3_455 2_565
O3 O2 La 71.0(5) 1_556 2_565
O2 O2 La 120.53(17) 2_556 2_565
O1 O2 La 107.7(4) 2_456 2_565
O3 O2 La 47.5(3) . 2_565
Nb O2 La 46.5(2) . 2_565
Ga1 O2 La 46.5(2) . 2_565
O1 O2 La 129.5(4) 1_545 2_565
O2 O2 La 93.5(3) 2 2_565
Ga2 O2 La 137.5(4) 2_556 2_565
O3 O2 La 160.2(4) 5_445 2_565
Ga3 O2 La 35.05(17) 2_565 2_565
La O2 La 132.2(3) 4_446 2_565
La O2 La 75.1(3) 1_556 2_565
Ga3 O2 La 70.5(3) 4_445 2_565
La O2 La 98.6(3) 2_455 2_565
O3 O2 La 83.8(3) 3_556 2_565
O3 O2 La 154.2(4) 4_446 2_565
Ga3 O2 La 144.5(3) 2_455 2_565
Ga3 O2 La 67.8(3) 1_556 2_565
Ga2 O2 La 80.5(3) 1_554 2_565
O2 O2 La 40.5(4) 6_556 2_565
La O2 La 96.0(3) 2 2_565
O3 O2 La 68.0(3) 3 2_565
O3 O2 La 125.3(4) 4_445 2_565
O2 O2 La 157.2(5) 5_446 2_565
O2 O2 La 57.4(3) 5_456 2_565
O1 O2 La 21.93(13) . 2_565
O3 O2 La 48.2(2) 5 2_565
Ga2 O2 La 34.89(15) 2_566 2_565
Nb O2 La 75.8(3) 1_556 2_565
Ga1 O2 La 75.8(3) 1_556 2_565
Ga3 O2 La 67.8(2) 1_656 2_565
O2 O2 La 22.4(2) 6 2_565
O2 O2 La 125.2(4) 5_445 2_565
O2 O2 La 43.3(2) 5_455 2_565
O2 O2 La 75.67(13) 1_554 2_565
O2 O2 La 104.32(13) 1_556 2_565
O3 O2 La 54.4(3) 4_556 2_565
Ga3 O2 La 175.0(3) 1_546 2_565
O3 O2 La 86.6(3) 3_456 2_565
O3 O2 La 84.9(3) 2_455 2_565
O3 O2 La 37.1(2) 4 2_565
Ga2 O2 La 106.1(3) 2 2_565
O3 O2 La 73.0(3) 3_455 2_565
O2 O2 La 78.6(3) 3 2_565
O2 O2 La 23.0(2) 4 2_565
La O2 La 110.7(3) 2_456 2_565
Ga1 O2 La 144.9(3) 1_445 2_565
Nb O2 La 144.9(3) 1_445 2_565
O2 O2 La 128.9(4) 6_446 2_565
O2 O2 La 126.6(4) 6_546 2_565
O3 O2 La 76.2(3) 6_556 2_565
O3 O2 La 56.7(2) 5_455 2_565
O3 O2 La 142.1(3) 6_445 2_565
La O2 La 108.2(3) 2_556 2_565
Ga3 O2 La 35.86(13) 2_564 2_565
O3 O2 La 96.4(3) 2_556 2_565
O1 O2 La 128.9(3) 1_546 2_565
O2 O2 La 111.1(5) 6_445 2_565
O2 O2 La 109.3(4) 6_545 2_565
O2 O2 La 95.2(3) 4_444 2_565
O2 O2 La 68.1(4) 3_454 2_565
O2 O2 La 121.5(3) 4_446 2_565
O2 O2 La 93.4(3) 3_456 2_565
O3 O2 La 50.8(2) 6_554 2_565
La O2 La 136.8(3) 1_545 2_565
O3 O2 La 71.8(2) 2_554 2_565
Ga3 O2 O2 92.9(5) 4_446 3_445
Ga2 O2 O2 93.1(8) . 3_445
La O2 O2 39.9(5) 4_445 3_445
O3 O2 O2 146.7(5) 6 3_445
La O2 O2 143.8(4) . 3_445
O3 O2 O2 88.0(4) 2 3_445
O1 O2 O2 92.0(5) 2_455 3_445
O2 O2 O2 63.6(9) 4_445 3_445
O2 O2 O2 123.6(9) 3_455 3_445
O3 O2 O2 116.7(4) 1_556 3_445
O2 O2 O2 60.5(4) 2_556 3_445
O1 O2 O2 91.9(5) 2_456 3_445
O3 O2 O2 113.8(3) . 3_445
Nb O2 O2 114.7(3) . 3_445
Ga1 O2 O2 114.7(3) . 3_445
O1 O2 O2 31.73(13) 1_545 3_445
O2 O2 O2 67.3(3) 2 3_445
Ga2 O2 O2 34.25(10) 2_556 3_445
O3 O2 O2 20.1(3) 5_445 3_445
Ga3 O2 O2 142.9(4) 2_565 3_445
La O2 O2 62.3(2) 4_446 3_445
La O2 O2 122.0(3) 1_556 3_445
Ga3 O2 O2 91.2(2) 4_445 3_445
La O2 O2 89.0(5) 2_455 3_445
O3 O2 O2 92.4(3) 3_556 3_445
O3 O2 O2 45.8(4) 4_446 3_445
Ga3 O2 O2 52.1(4) 2_455 3_445
Ga3 O2 O2 130.2(5) 1_556 3_445
Ga2 O2 O2 91.3(3) 1_554 3_445
O2 O2 O2 151.1(4) 6_556 3_445
La O2 O2 65.60(15) 2 3_445
O3 O2 O2 92.3(3) 3 3_445
O3 O2 O2 48.6(4) 4_445 3_445
O2 O2 O2 27.0(3) 5_446 3_445
O2 O2 O2 142.7(6) 5_456 3_445
O1 O2 O2 169.0(4) . 3_445
O3 O2 O2 118.1(4) 5 3_445
Ga2 O2 O2 164.8(3) 2_566 3_445
Nb O2 O2 108.0(2) 1_556 3_445
Ga1 O2 O2 108.0(2) 1_556 3_445
Ga3 O2 O2 102.5(2) 1_656 3_445
O2 O2 O2 141.4(3) 6 3_445
O2 O2 O2 37.3(3) 5_445 3_445
O2 O2 O2 135.2(4) 5_455 3_445
O2 O2 O2 90.000(1) 1_554 3_445
O2 O2 O2 90.0 1_556 3_445
O3 O2 O2 124.6(3) 4_556 3_445
Ga3 O2 O2 15.18(18) 1_546 3_445
O3 O2 O2 112.6(5) 3_456 3_445
O3 O2 O2 108.5(5) 2_455 3_445
O3 O2 O2 123.2(3) 4 3_445
Ga2 O2 O2 54.89(16) 2 3_445
O3 O2 O2 111.8(5) 3_455 3_445
O2 O2 O2 87.6(4) 3 3_445
O2 O2 O2 147.6(4) 4 3_445
La O2 O2 89.2(4) 2_456 3_445
Ga1 O2 O2 34.9(3) 1_445 3_445
Nb O2 O2 34.9(3) 1_445 3_445
O2 O2 O2 69.3(6) 6_446 3_445
O2 O2 O2 46.3(2) 6_546 3_445
O3 O2 O2 114.5(2) 6_556 3_445
O3 O2 O2 137.6(5) 5_455 3_445
O3 O2 O2 48.1(4) 6_445 3_445
La O2 O2 70.29(13) 2_556 3_445
Ga3 O2 O2 125.03(16) 2_564 3_445
O3 O2 O2 89.0(2) 2_556 3_445
O1 O2 O2 57.19(14) 1_546 3_445
O2 O2 O2 71.1(6) 6_445 3_445
O2 O2 O2 50.7(3) 6_545 3_445
O2 O2 O2 77.5(5) 4_444 3_445
O2 O2 O2 105.6(4) 3_454 3_445
O2 O2 O2 77.5(5) 4_446 3_445
O2 O2 O2 105.6(4) 3_456 3_445
O3 O2 O2 112.09(19) 6_554 3_445
La O2 O2 23.24(11) 1_545 3_445
O3 O2 O2 89.06(19) 2_554 3_445
La O2 O2 160.0(3) 2_565 3_445
Ga3 O2 O2 45.9(4) 4_446 4_545
Ga2 O2 O2 141.5(7) . 4_545
La O2 O2 73.8(3) 4_445 4_545
O3 O2 O2 87.3(5) 6 4_545
La O2 O2 126.2(5) . 4_545
O3 O2 O2 28.6(4) 2 4_545
O1 O2 O2 120.4(3) 2_455 4_545
O2 O2 O2 123.6(9) 4_445 4_545
O2 O2 O2 176.4(9) 3_455 4_545
O3 O2 O2 82.0(4) 1_556 4_545
O2 O2 O2 45.2(5) 2_556 4_545
O1 O2 O2 117.7(3) 2_456 4_545
O3 O2 O2 82.8(4) . 4_545
Nb O2 O2 61.2(3) . 4_545
Ga1 O2 O2 61.2(3) . 4_545
O1 O2 O2 31.73(13) 1_545 4_545
O2 O2 O2 56.4(5) 2 4_545
Ga2 O2 O2 34.25(10) 2_556 4_545
O3 O2 O2 79.6(3) 5_445 4_545
Ga3 O2 O2 85.5(4) 2_565 4_545
La O2 O2 80.29(19) 4_446 4_545
La O2 O2 112.8(3) 1_556 4_545
Ga3 O2 O2 73.0(2) 4_445 4_545
La O2 O2 143.2(4) 2_455 4_545
O3 O2 O2 44.7(3) 3_556 4_545
O3 O2 O2 93.2(4) 4_446 4_545
Ga3 O2 O2 110.2(4) 2_455 4_545
Ga3 O2 O2 162.5(4) 1_556 4_545
Ga2 O2 O2 109.12(17) 1_554 4_545
O2 O2 O2 105.3(2) 6_556 4_545
La O2 O2 20.1(2) 2 4_545
O3 O2 O2 47.5(3) 3 4_545
O3 O2 O2 93.0(3) 4_445 4_545
O2 O2 O2 57.66(18) 5_446 4_545
O2 O2 O2 139.2(6) 5_456 4_545
O1 O2 O2 126.9(5) . 4_545
O3 O2 O2 58.2(4) 5 4_545
Ga2 O2 O2 126.2(5) 2_566 4_545
Nb O2 O2 69.1(3) 1_556 4_545
Ga1 O2 O2 69.1(3) 1_556 4_545
Ga3 O2 O2 44.1(3) 1_656 4_545
O2 O2 O2 103.6(2) 6 4_545
O2 O2 O2 61.49(17) 5_445 4_545
O2 O2 O2 132.5(5) 5_455 4_545
O2 O2 O2 90.0 1_554 4_545
O2 O2 O2 90.0 1_556 4_545
O3 O2 O2 72.2(3) 4_556 4_545
Ga3 O2 O2 70.3(2) 1_546 4_545
O3 O2 O2 152.7(3) 3_456 4_545
O3 O2 O2 168.0(5) 2_455 4_545
O3 O2 O2 72.8(3) 4 4_545
Ga2 O2 O2 54.89(16) 2 4_545
O3 O2 O2 148.83(18) 3_455 4_545
O2 O2 O2 27.6(4) 3 4_545
O2 O2 O2 87.6(4) 4 4_545
La O2 O2 129.9(3) 2_456 4_545
Ga1 O2 O2 91.1(3) 1_445 4_545
Nb O2 O2 91.1(3) 1_445 4_545
O2 O2 O2 124.4(6) 6_446 4_545
O2 O2 O2 28.5(3) 6_546 4_545
O3 O2 O2 88.7(3) 6_556 4_545
O3 O2 O2 162.0(5) 5_455 4_545
O3 O2 O2 107.9(4) 6_445 4_545
La O2 O2 39.94(15) 2_556 4_545
Ga3 O2 O2 86.8(3) 2_564 4_545
O3 O2 O2 63.5(2) 2_556 4_545
O1 O2 O2 57.19(14) 1_546 4_545
O2 O2 O2 121.2(4) 6_445 4_545
O2 O2 O2 36.2(2) 6_545 4_545
O2 O2 O2 105.6(4) 4_444 4_545
O2 O2 O2 119.1(2) 3_454 4_545
O2 O2 O2 105.6(4) 4_446 4_545
O2 O2 O2 119.1(2) 3_456 4_545
O3 O2 O2 88.8(2) 6_554 4_545
La O2 O2 44.16(15) 1_545 4_545
O3 O2 O2 66.1(2) 2_554 4_545
La O2 O2 105.3(4) 2_565 4_545
O2 O2 O2 60.0 3_445 4_545
Ga3 O2 O3 77.3(6) 4_446 5_446
Ga2 O2 O3 58.0(6) . 5_446
La O2 O3 90.3(5) 4_445 5_446
O3 O2 O3 134.7(5) 6 5_446
La O2 O3 149.4(4) . 5_446
O3 O2 O3 106.1(5) 2 5_446
O1 O2 O3 122.7(5) 2_455 5_446
O2 O2 O3 62.9(4) 4_445 5_446
O2 O2 O3 98.8(4) 3_455 5_446
O3 O2 O3 75.2(4) 1_556 5_446
O2 O2 O3 44.3(3) 2_556 5_446
O1 O2 O3 41.2(3) 2_456 5_446
O3 O2 O3 165.1(5) . 5_446
Nb O2 O3 139.1(4) . 5_446
Ga1 O2 O3 139.1(4) . 5_446
O1 O2 O3 75.1(5) 1_545 5_446
O2 O2 O3 119.7(5) 2 5_446
Ga2 O2 O3 51.5(3) 2_556 5_446
O3 O2 O3 55.5(3) 5_445 5_446
Ga3 O2 O3 113.6(3) 2_565 5_446
La O2 O3 12.61(15) 4_446 5_446
La O2 O3 68.8(3) 1_556 5_446
Ga3 O2 O3 144.3(4) 4_445 5_446
La O2 O3 93.9(4) 2_455 5_446
O3 O2 O3 78.0(3) 3_556 5_446
O3 O2 O3 20.7(2) 4_446 5_446
Ga3 O2 O3 44.9(2) 2_455 5_446
Ga3 O2 O3 93.0(3) 1_556 5_446
Ga2 O2 O3 131.1(4) 1_554 5_446
O2 O2 O3 102.9(5) 6_556 5_446
La O2 O3 101.3(4) 2 5_446
O3 O2 O3 130.9(4) 3 5_446
O3 O2 O3 88.9(4) 4_445 5_446
O2 O2 O3 31.6(4) 5_446 5_446
O2 O2 O3 92.5(4) 5_456 5_446
O1 O2 O3 132.0(4) . 5_446
O3 O2 O3 121.3(4) 5 5_446
Ga2 O2 O3 111.7(3) 2_566 5_446
Nb O2 O3 74.4(3) 1_556 5_446
Ga1 O2 O3 74.4(3) 1_556 5_446
Ga3 O2 O3 99.8(3) 1_656 5_446
O2 O2 O3 165.1(4) 6 5_446
O2 O2 O3 90.6(4) 5_445 5_446
O2 O2 O3 144.0(5) 5_455 5_446
O2 O2 O3 140.77(19) 1_554 5_446
O2 O2 O3 39.23(19) 1_556 5_446
O3 O2 O3 97.3(3) 4_556 5_446
Ga3 O2 O3 40.0(2) 1_546 5_446
O3 O2 O3 73.0(3) 3_456 5_446
O3 O2 O3 92.0(3) 2_455 5_446
O3 O2 O3 150.2(3) 4 5_446
Ga2 O2 O3 107.9(3) 2 5_446
O3 O2 O3 117.0(4) 3_455 5_446
O2 O2 O3 100.8(3) 3 5_446
O2 O2 O3 128.08(19) 4 5_446
La O2 O3 47.1(2) 2_456 5_446
Ga1 O2 O3 68.0(3) 1_445 5_446
Nb O2 O3 68.0(3) 1_445 5_446
O2 O2 O3 46.7(4) 6_446 5_446
O2 O2 O3 55.0(4) 6_546 5_446
O3 O2 O3 68.3(3) 6_556 5_446
O3 O2 O3 110.0(4) 5_455 5_446
O3 O2 O3 59.4(3) 6_445 5_446
La O2 O3 56.6(2) 2_556 5_446
Ga3 O2 O3 168.8(3) 2_564 5_446
O3 O2 O3 55.1(3) 2_556 5_446
O1 O2 O3 30.60(16) 1_546 5_446
O2 O2 O3 92.8(5) 6_445 5_446
O2 O2 O3 98.7(5) 6_545 5_446
O2 O2 O3 117.0(4) 4_444 5_446
O2 O2 O3 138.7(5) 3_454 5_446
O2 O2 O3 26.1(3) 4_446 5_446
O2 O2 O3 53.0(2) 3_456 5_446
O3 O2 O3 165.5(3) 6_554 5_446
La O2 O3 73.5(3) 1_545 5_446
O3 O2 O3 140.9(3) 2_554 5_446
La O2 O3 143.3(3) 2_565 5_446
O2 O2 O3 53.4(2) 3_445 5_446
O2 O2 O3 83.4(2) 4_545 5_446
Ga3 O3 Nb 111.6(6) 4_445 .
Ga3 O3 Ga1 111.6(6) 4_445 .
Nb O3 Ga1 0.0 . .
Ga3 O3 La 138.1(6) 4_445 .
Nb O3 La 105.7(5) . .
Ga1 O3 La 105.7(5) . .
Ga3 O3 Ga3 94.2(5) 4_445 2_564
Nb O3 Ga3 87.4(5) . 2_564
Ga1 O3 Ga3 87.4(5) . 2_564
La O3 Ga3 106.2(6) . 2_564
Ga3 O3 O2 126.7(7) 4_445 6
Nb O3 O2 95.6(6) . 6
Ga1 O3 O2 95.6(6) . 6
La O3 O2 65.7(5) . 6
Ga3 O3 O2 40.5(4) 2_564 6
Ga3 O3 O3 154.4(9) 4_445 6
Nb O3 O3 48.8(3) . 6
Ga1 O3 O3 48.8(3) . 6
La O3 O3 56.9(3) . 6
Ga3 O3 O3 100.2(8) 2_564 6
O2 O3 O3 76.3(7) 6 6
Ga3 O3 O3 62.2(4) 4_445 6_554
Nb O3 O3 119.4(6) . 6_554
Ga1 O3 O3 119.4(6) . 6_554
La O3 O3 114.1(5) . 6_554
Ga3 O3 O3 39.5(4) 2_564 6_554
O2 O3 O3 64.5(6) 6 6_554
O3 O3 O3 138.3(12) 6 6_554
Ga3 O3 O3 64.9(6) 4_445 3
Nb O3 O3 46.8(3) . 3
Ga1 O3 O3 46.8(3) . 3
La O3 O3 149.5(3) . 3
Ga3 O3 O3 87.8(4) 2_564 3
O2 O3 O3 121.6(7) 6 3
O3 O3 O3 94.43(9) 6 3
O3 O3 O3 94.09(9) 6_554 3
Ga3 O3 O3 105.1(4) 4_445 4
Nb O3 O3 46.8(3) . 4
Ga1 O3 O3 46.8(3) . 4
La O3 O3 114.3(8) . 4
Ga3 O3 O3 40.7(4) 2_564 4
O2 O3 O3 62.1(7) 6 4
O3 O3 O3 74.0(6) 6 4
O3 O3 O3 75.3(5) 6_554 4
O3 O3 O3 60.0 3 4
Ga3 O3 O2 40.1(4) 4_445 2
Nb O3 O2 93.1(7) . 2
Ga1 O3 O2 93.1(7) . 2
La O3 O2 121.4(6) . 2
Ga3 O3 O2 130.2(6) 2_564 2
O2 O3 O2 166.6(8) 6 2
O3 O3 O2 117.0(9) 6 2
O3 O3 O2 102.3(7) 6_554 2
O3 O3 O2 59.0(8) 3 2
O3 O3 O2 118.6(7) 4 2
Ga3 O3 O2 36.1(4) 4_445 1_554
Nb O3 O2 147.6(6) . 1_554
Ga1 O3 O2 147.6(6) . 1_554
La O3 O2 104.4(5) . 1_554
Ga3 O3 O2 95.5(6) 2_564 1_554
O2 O3 O2 107.4(7) 6 1_554
O3 O3 O2 158.4(6) 6 1_554
O3 O3 O2 55.9(6) 6_554 1_554
O3 O3 O2 101.0(6) 3 1_554
O3 O3 O2 127.0(4) 4 1_554
O2 O3 O2 60.8(7) 2 1_554
Ga3 O3 O1 87.7(5) 4_445 2_455
Nb O3 O1 132.7(7) . 2_455
Ga1 O3 O1 132.7(7) . 2_455
La O3 O1 52.2(3) . 2_455
Ga3 O3 O1 135.7(5) 2_564 2_455
O2 O3 O1 106.8(5) 6 2_455
O3 O3 O1 96.4(5) 6 2_455
O3 O3 O1 107.8(5) 6_554 2_455
O3 O3 O1 131.6(8) 3 2_455
O3 O3 O1 166.4(7) 4 2_455
O2 O3 O1 74.1(5) 2 2_455
O2 O3 O1 62.0(5) 1_554 2_455
Ga3 O3 O2 112.9(7) 4_445 .
Nb O3 O2 79.4(5) . .
Ga1 O3 O2 79.4(5) . .
La O3 O2 56.0(4) . .
Ga3 O3 O2 152.7(5) 2_564 .
O2 O3 O2 116.8(6) 6 .
O3 O3 O2 53.3(6) 6 .
O3 O3 O2 161.2(5) 6_554 .
O3 O3 O2 99.9(5) 3 .
O3 O3 O2 122.7(3) 4 .
O2 O3 O2 74.8(6) 2 .
O2 O3 O2 108.5(7) 1_554 .
O1 O3 O2 53.4(4) 2_455 .
Ga3 O3 O3 99.9(6) 4_445 2
Nb O3 O3 36.0(5) . 2
Ga1 O3 O3 36.0(5) . 2
La O3 O3 99.1(5) . 2
Ga3 O3 O3 122.8(3) 2_564 2
O2 O3 O3 125.9(5) 6 2
O3 O3 O3 54.5(6) 6 2
O3 O3 O3 145.3(4) 6_554 2
O3 O3 O3 51.5(5) 3 2
O3 O3 O3 82.1(4) 4 2
O2 O3 O3 66.1(5) 2 2
O2 O3 O3 126.7(6) 1_554 2
O1 O3 O3 100.3(4) 2_455 2
O2 O3 O3 51.0(4) . 2
Ga3 O3 Ga2 65.7(4) 4_445 1_554
Nb O3 Ga2 159.7(7) . 1_554
Ga1 O3 Ga2 159.7(7) . 1_554
La O3 Ga2 72.6(3) . 1_554
Ga3 O3 Ga2 112.7(4) 2_564 1_554
O2 O3 Ga2 101.7(5) 6 1_554
O3 O3 Ga2 125.7(4) 6 1_554
O3 O3 Ga2 78.1(4) 6_554 1_554
O3 O3 Ga2 127.5(7) 3 1_554
O3 O3 Ga2 152.9(5) 4 1_554
O2 O3 Ga2 72.0(5) 2 1_554
O2 O3 Ga2 33.0(3) 1_554 1_554
O1 O3 Ga2 31.0(4) 2_455 1_554
O2 O3 Ga2 83.4(4) . 1_554
O3 O3 Ga2 123.8(3) 2 1_554
Ga3 O3 O3 22.9(4) 4_445 2_554
Nb O3 O3 98.7(5) . 2_554
Ga1 O3 O3 98.7(5) . 2_554
La O3 O3 155.6(6) . 2_554
Ga3 O3 O3 74.4(3) 2_564 2_554
O2 O3 O3 112.2(6) 6 2_554
O3 O3 O3 147.5(4) 6 2_554
O3 O3 O3 50.8(5) 6_554 2_554
O3 O3 O3 53.9(5) 3 2_554
O3 O3 O3 82.6(4) 4 2_554
O2 O3 O3 56.3(4) 2 2_554
O2 O3 O3 51.8(4) 1_554 2_554
O1 O3 O3 109.8(4) 2_455 2_554
O2 O3 O3 130.9(6) . 2_554
O3 O3 O3 100.8(7) 2 2_554
Ga2 O3 O3 84.5(3) 1_554 2_554
Ga3 O3 Ga3 62.8(3) 4_445 1_655
Nb O3 Ga3 59.8(3) . 1_655
Ga1 O3 Ga3 59.8(3) . 1_655
La O3 Ga3 158.5(5) . 1_655
Ga3 O3 Ga3 60.1(3) 2_564 1_655
O2 O3 Ga3 98.3(5) 6 1_655
O3 O3 Ga3 106.8(3) 6 1_655
O3 O3 Ga3 67.2(2) 6_554 1_655
O3 O3 Ga3 29.1(2) 3 1_655
O3 O3 Ga3 44.3(3) 4 1_655
O2 O3 Ga3 77.4(5) 2 1_655
O2 O3 Ga3 93.9(4) 1_554 1_655
O1 O3 Ga3 149.3(5) 2_455 1_655
O2 O3 Ga3 128.5(5) . 1_655
O3 O3 Ga3 78.2(4) 2 1_655
Ga2 O3 Ga3 126.8(3) 1_554 1_655
O3 O3 Ga3 42.3(3) 2_554 1_655
Ga3 O3 La 73.9(5) 4_445 4_445
Nb O3 La 100.6(6) . 4_445
Ga1 O3 La 100.6(6) . 4_445
La O3 La 81.2(4) . 4_445
Ga3 O3 La 167.4(4) 2_564 4_445
O2 O3 La 146.1(5) 6 4_445
O3 O3 La 92.4(7) 6 4_445
O3 O3 La 128.3(6) 6_554 4_445
O3 O3 La 90.7(7) 3 4_445
O3 O3 La 145.6(6) 4 4_445
O2 O3 La 40.5(4) 2 4_445
O2 O3 La 72.6(5) 1_554 4_445
O1 O3 La 41.9(2) 2_455 4_445
O2 O3 La 39.8(3) . 4_445
O3 O3 La 64.67(19) 2 4_445
Ga2 O3 La 59.1(2) 1_554 4_445
O3 O3 La 94.6(3) 2_554 4_445
Ga3 O3 La 115.6(4) 1_655 4_445
Ga3 O3 Ga2 114.0(5) 4_445 2_565
Nb O3 Ga2 119.8(6) . 2_565
Ga1 O3 Ga2 119.8(6) . 2_565
La O3 Ga2 58.7(3) . 2_565
Ga3 O3 Ga2 52.6(3) 2_564 2_565
O2 O3 Ga2 24.5(3) 6 2_565
O3 O3 Ga2 91.5(6) 6 2_565
O3 O3 Ga2 57.8(4) 6_554 2_565
O3 O3 Ga2 140.4(6) 3 2_565
O3 O3 Ga2 84.4(7) 4 2_565
O2 O3 Ga2 146.6(5) 2 2_565
O2 O3 Ga2 86.2(5) 1_554 2_565
O1 O3 Ga2 86.3(3) 2_455 2_565
O2 O3 Ga2 114.8(4) . 2_565
O3 O3 Ga2 145.7(5) 2 2_565
Ga2 O3 Ga2 77.3(3) 1_554 2_565
O3 O3 Ga2 108.5(5) 2_554 2_565
Ga3 O3 Ga2 112.4(4) 1_655 2_565
La O3 Ga2 128.2(3) 4_445 2_565
Ga3 O3 O2 117.4(6) 4_445 5_455
Nb O3 O2 130.0(6) . 5_455
Ga1 O3 O2 130.0(6) . 5_455
La O3 O2 36.4(3) . 5_455
Ga3 O3 O2 80.2(4) 2_564 5_455
O2 O3 O2 46.7(5) 6 5_455
O3 O3 O2 86.0(4) 6 5_455
O3 O3 O2 77.8(4) 6_554 5_455
O3 O3 O2 167.8(7) 3 5_455
O3 O3 O2 108.7(8) 4 5_455
O2 O3 O2 131.2(7) 2 5_455
O2 O3 O2 82.1(4) 1_554 5_455
O1 O3 O2 60.3(3) 2_455 5_455
O2 O3 O2 90.2(4) . 5_455
O3 O3 O2 135.2(6) 2 5_455
Ga2 O3 O2 60.2(3) 1_554 5_455
O3 O3 O2 123.3(6) 2_554 5_455
Ga3 O3 O2 139.6(5) 1_655 5_455
La O3 O2 101.5(4) 4_445 5_455
Ga2 O3 O2 27.5(2) 2_565 5_455
Ga3 O3 O3 119.2(5) 4_445 5
Nb O3 O3 9.5(4) . 5
Ga1 O3 O3 9.5(4) . 5
La O3 O3 100.1(4) . 5
Ga3 O3 O3 81.5(4) 2_564 5
O2 O3 O3 86.3(4) 6 5
O3 O3 O3 43.8(3) 6 5
O3 O3 O3 116.7(6) 6_554 5
O3 O3 O3 54.4(5) 3 5
O3 O3 O3 41.7(3) 4 5
O2 O3 O3 102.6(5) 2 5
O2 O3 O3 155.2(5) 1_554 5
O1 O3 O3 134.8(6) 2_455 5
O2 O3 O3 81.9(5) . 5
O3 O3 O3 43.5(3) 2 5
Ga2 O3 O3 165.2(6) 1_554 5
O3 O3 O3 104.1(4) 2_554 5
Ga3 O3 O3 63.1(3) 1_655 5
La O3 O3 107.7(4) 4_445 5
Ga2 O3 O3 110.37(19) 2_565 5
O2 O3 O3 121.2(3) 5_455 5
Ga3 O3 O3 64.2(5) 4_445 5_554
Nb O3 O3 79.4(5) . 5_554
Ga1 O3 O3 79.4(5) . 5_554
La O3 O3 143.5(4) . 5_554
Ga3 O3 O3 37.4(3) 2_564 5_554
O2 O3 O3 77.9(4) 6 5_554
O3 O3 O3 117.9(6) 6 5_554
O3 O3 O3 41.9(3) 6_554 5_554
O3 O3 O3 55.9(4) 3 5_554
O3 O3 O3 44.0(3) 4 5_554
O2 O3 O3 93.8(4) 2 5_554
O2 O3 O3 83.5(5) 1_554 5_554
O1 O3 O3 145.2(6) 2_455 5_554
O2 O3 O3 155.3(5) . 5_554
O3 O3 O3 104.3(4) 2 5_554
Ga2 O3 O3 114.4(5) 1_554 5_554
O3 O3 O3 41.6(3) 2_554 5_554
Ga3 O3 O3 26.9(2) 1_655 5_554
La O3 O3 134.2(2) 4_445 5_554
Ga2 O3 O3 87.0(2) 2_565 5_554
O2 O3 O3 113.3(4) 5_455 5_554
O3 O3 O3 79.3(5) 5 5_554
Ga3 O3 Ga3 117.6(6) 4_445 4_446
Nb O3 Ga3 52.1(3) . 4_446
Ga1 O3 Ga3 52.1(3) . 4_446
La O3 Ga3 72.2(3) . 4_446
Ga3 O3 Ga3 134.5(4) 2_564 4_446
O2 O3 Ga3 115.3(5) 6 4_446
O3 O3 Ga3 39.4(5) 6 4_446
O3 O3 Ga3 171.4(3) 6_554 4_446
O3 O3 Ga3 78.7(3) 3 4_446
O3 O3 Ga3 96.94(16) 4 4_446
O2 O3 Ga3 78.0(5) 2 4_446
O2 O3 Ga3 129.6(6) 1_554 4_446
O1 O3 Ga3 80.6(4) 2_455 4_446
O2 O3 Ga3 27.3(3) . 4_446
O3 O3 Ga3 27.2(3) 2 4_446
Ga2 O3 Ga3 109.9(4) 1_554 4_446
O3 O3 Ga3 125.4(6) 2_554 4_446
Ga3 O3 Ga3 104.7(3) 1_655 4_446
La O3 Ga3 57.1(2) 4_445 4_446
Ga2 O3 Ga3 125.9(3) 2_565 4_446
O2 O3 Ga3 108.6(4) 5_455 4_446
O3 O3 Ga3 55.3(3) 5 4_446
O3 O3 Ga3 129.7(4) 5_554 4_446
Ga3 O3 Nb 45.1(3) 4_445 1_554
Nb O3 Nb 105.7(4) . 1_554
Ga1 O3 Nb 105.7(4) . 1_554
La O3 Nb 138.2(5) . 1_554
Ga3 O3 Nb 49.1(2) 2_564 1_554
O2 O3 Nb 84.4(5) 6 1_554
O3 O3 Nb 144.9(7) 6 1_554
O3 O3 Nb 24.4(2) 6_554 1_554
O3 O3 Nb 71.03(14) 3 1_554
O3 O3 Nb 71.03(14) 4 1_554
O2 O3 Nb 83.5(4) 2 1_554
O2 O3 Nb 56.0(4) 1_554 1_554
O1 O3 Nb 117.4(5) 2_455 1_554
O2 O3 Nb 158.0(5) . 1_554
O3 O3 Nb 122.4(5) 2 1_554
Ga2 O3 Nb 86.6(3) 1_554 1_554
O3 O3 Nb 28.0(3) 2_554 1_554
Ga3 O3 Nb 47.02(15) 1_655 1_554
La O3 Nb 118.8(3) 4_445 1_554
Ga2 O3 Nb 81.9(3) 2_565 1_554
O2 O3 Nb 101.8(4) 5_455 1_554
O3 O3 Nb 106.7(5) 5 1_554
O3 O3 Nb 27.8(2) 5_554 1_554
Ga3 O3 Nb 149.5(3) 4_446 1_554
Ga3 O3 Ga1 45.1(3) 4_445 1_554
Nb O3 Ga1 105.7(4) . 1_554
Ga1 O3 Ga1 105.7(4) . 1_554
La O3 Ga1 138.2(5) . 1_554
Ga3 O3 Ga1 49.1(2) 2_564 1_554
O2 O3 Ga1 84.4(5) 6 1_554
O3 O3 Ga1 144.9(7) 6 1_554
O3 O3 Ga1 24.4(2) 6_554 1_554
O3 O3 Ga1 71.03(14) 3 1_554
O3 O3 Ga1 71.03(14) 4 1_554
O2 O3 Ga1 83.5(4) 2 1_554
O2 O3 Ga1 56.0(4) 1_554 1_554
O1 O3 Ga1 117.4(5) 2_455 1_554
O2 O3 Ga1 158.0(5) . 1_554
O3 O3 Ga1 122.4(5) 2 1_554
Ga2 O3 Ga1 86.6(3) 1_554 1_554
O3 O3 Ga1 28.0(3) 2_554 1_554
Ga3 O3 Ga1 47.02(15) 1_655 1_554
La O3 Ga1 118.8(3) 4_445 1_554
Ga2 O3 Ga1 81.9(3) 2_565 1_554
O2 O3 Ga1 101.8(4) 5_455 1_554
O3 O3 Ga1 106.7(5) 5 1_554
O3 O3 Ga1 27.8(2) 5_554 1_554
Ga3 O3 Ga1 149.5(3) 4_446 1_554
Nb O3 Ga1 0.0 1_554 1_554
Ga3 O3 O1 158.2(6) 4_445 .
Nb O3 O1 89.4(4) . .
Ga1 O3 O1 89.4(4) . .
La O3 O1 29.8(2) . .
Ga3 O3 O1 80.7(4) 2_564 .
O2 O3 O1 41.4(4) 6 .
O3 O3 O1 46.6(4) 6 .
O3 O3 O1 103.2(6) 6_554 .
O3 O3 O1 135.3(5) 3 .
O3 O3 O1 84.8(6) 4 .
O2 O3 O1 149.1(6) 2 .
O2 O3 O1 122.9(5) 1_554 .
O1 O3 O1 81.6(3) 2_455 .
O2 O3 O1 75.4(4) . .
O3 O3 O1 100.6(5) 2 .
Ga2 O3 O1 96.6(3) 1_554 .
O3 O3 O1 153.4(6) 2_554 .
Ga3 O3 O1 129.1(4) 1_655 .
La O3 O1 108.8(3) 4_445 .
Ga2 O3 O1 46.7(3) 2_565 .
O2 O3 O1 40.9(3) 5_455 .
O3 O3 O1 81.1(3) 5 .
O3 O3 O1 116.9(3) 5_554 .
Ga3 O3 O1 79.4(3) 4_446 .
Nb O3 O1 125.4(5) 1_554 .
Ga1 O3 O1 125.4(5) 1_554 .
Ga3 O3 O2 93.6(6) 4_445 4_554
Nb O3 O2 88.3(5) . 4_554
Ga1 O3 O2 88.3(5) . 4_554
La O3 O2 106.2(6) . 4_554
Ga3 O3 O2 0.9(2) 2_564 4_554
O2 O3 O2 40.6(6) 6 4_554
O3 O3 O2 101.1(8) 6 4_554
O3 O3 O2 38.6(5) 6_554 4_554
O3 O3 O2 88.1(4) 3 4_554
O3 O3 O2 41.6(4) 4 4_554
O2 O3 O2 129.9(6) 2 4_554
O2 O3 O2 94.5(6) 1_554 4_554
O1 O3 O2 135.0(5) 2_455 4_554
O2 O3 O2 153.4(4) . 4_554
O3 O3 O2 123.6(3) 2 4_554
Ga2 O3 O2 111.8(4) 1_554 4_554
O3 O3 O2 74.0(4) 2_554 4_554
Ga3 O3 O2 60.4(3) 1_655 4_554
La O3 O2 166.6(4) 4_445 4_554
Ga2 O3 O2 52.3(3) 2_565 4_554
O2 O3 O2 79.8(5) 5_455 4_554
O3 O3 O2 82.4(4) 5 4_554
O3 O3 O2 37.3(3) 5_554 4_554
Ga3 O3 O2 135.4(4) 4_446 4_554
Nb O3 O2 48.4(3) 1_554 4_554
Ga1 O3 O2 48.4(3) 1_554 4_554
O1 O3 O2 81.0(5) . 4_554
Ga3 O3 La 64.4(4) 4_445 1_554
Nb O3 La 149.0(6) . 1_554
Ga1 O3 La 149.0(6) . 1_554
La O3 La 92.5(4) . 1_554
Ga3 O3 La 63.1(3) 2_564 1_554
O2 O3 La 68.9(4) 6 1_554
O3 O3 La 141.2(6) 6 1_554
O3 O3 La 29.9(2) 6_554 1_554
O3 O3 La 118.01(15) 3 1_554
O3 O3 La 102.9(4) 4 1_554
O2 O3 La 98.7(5) 2 1_554
O2 O3 La 38.8(4) 1_554 1_554
O1 O3 La 78.3(4) 2_455 1_554
O2 O3 La 131.4(4) . 1_554
O3 O3 La 164.2(5) 2 1_554
Ga2 O3 La 49.97(17) 1_554 1_554
O3 O3 La 65.6(4) 2_554 1_554
Ga3 O3 La 94.9(3) 1_655 1_554
La O3 La 106.9(3) 4_445 1_554
Ga2 O3 La 50.03(17) 2_565 1_554
O2 O3 La 57.7(3) 5_455 1_554
O3 O3 La 144.5(5) 5 1_554
O3 O3 La 71.3(3) 5_554 1_554
Ga3 O3 La 158.7(3) 4_446 1_554
Nb O3 La 48.10(15) 1_554 1_554
Ga1 O3 La 48.10(15) 1_554 1_554
O1 O3 La 94.8(4) . 1_554
O2 O3 La 62.2(3) 4_554 1_554
Ga3 O3 Ga3 152.8(6) 4_445 2_565
Nb O3 Ga3 42.0(3) . 2_565
Ga1 O3 Ga3 42.0(3) . 2_565
La O3 Ga3 64.5(3) . 2_565
Ga3 O3 Ga3 91.2(3) 2_564 2_565
O2 O3 Ga3 72.0(4) 6 2_565
O3 O3 Ga3 10.5(4) 6 2_565
O3 O3 Ga3 130.3(7) 6_554 2_565
O3 O3 Ga3 88.7(2) 3 2_565
O3 O3 Ga3 63.5(3) 4 2_565
O2 O3 Ga3 120.9(5) 2 2_565
O2 O3 Ga3 168.4(5) 1_554 2_565
O1 O3 Ga3 106.7(4) 2_455 2_565
O2 O3 Ga3 63.1(3) . 2_565
O3 O3 Ga3 55.5(3) 2 2_565
Ga2 O3 Ga3 135.4(3) 1_554 2_565
O3 O3 Ga3 139.5(4) 2_554 2_565
Ga3 O3 Ga3 97.6(3) 1_655 2_565
La O3 Ga3 101.3(3) 4_445 2_565
Ga2 O3 Ga3 90.3(3) 2_565 2_565
O2 O3 Ga3 89.8(3) 5_455 2_565
O3 O3 Ga3 35.6(3) 5 2_565
O3 O3 Ga3 107.4(4) 5_554 2_565
Ga3 O3 Ga3 45.85(14) 4_446 2_565
Nb O3 Ga3 134.4(3) 1_554 2_565
Ga1 O3 Ga3 134.4(3) 1_554 2_565
O1 O3 Ga3 48.9(2) . 2_565
O2 O3 Ga3 92.1(3) 4_554 2_565
La O3 Ga3 140.2(4) 1_554 2_565
Ga3 O3 O2 76.9(4) 4_445 3_454
Nb O3 O2 171.3(6) . 3_454
Ga1 O3 O2 171.3(6) . 3_454
La O3 O2 66.9(3) . 3_454
Ga3 O3 O2 90.4(4) 2_564 3_454
O2 O3 O2 77.4(3) 6 3_454
O3 O3 O2 123.6(3) 6 3_454
O3 O3 O2 62.3(3) 6_554 3_454
O3 O3 O2 141.6(4) 3 3_454
O3 O3 O2 130.8(6) 4 3_454
O2 O3 O2 94.8(4) 2 3_454
O2 O3 O2 41.0(5) 1_554 3_454
O1 O3 O2 47.0(4) 2_455 3_454
O2 O3 O2 99.1(4) . 3_454
O3 O3 O2 146.8(3) 2 3_454
Ga2 O3 O2 25.0(2) 1_554 3_454
O3 O3 O2 88.7(5) 2_554 3_454
Ga3 O3 O2 125.8(4) 1_655 3_454
La O3 O2 83.1(3) 4_445 3_454
Ga2 O3 O2 52.9(3) 2_565 3_454
O2 O3 O2 41.3(5) 5_455 3_454
O3 O3 O2 162.2(3) 5 3_454
O3 O3 O2 103.7(4) 5_554 3_454
Ga3 O3 O2 126.3(4) 4_446 3_454
Nb O3 O2 78.9(3) 1_554 3_454
Ga1 O3 O2 78.9(3) 1_554 3_454
O1 O3 O2 81.9(4) . 3_454
O2 O3 O2 89.5(5) 4_554 3_454
La O3 O2 32.5(2) 1_554 3_454
Ga3 O3 O2 129.8(4) 2_565 3_454
Ga3 O3 La 67.0(4) 4_445 2
Nb O3 La 53.4(3) . 2
Ga1 O3 La 53.4(3) . 2
La O3 La 127.5(5) . 2
Ga3 O3 La 118.2(4) 2_564 2
O2 O3 La 147.2(5) 6 2
O3 O3 La 87.5(5) 6 2
O3 O3 La 117.9(3) 6_554 2
O3 O3 La 30.5(4) 3 2
O3 O3 La 86.2(4) 4 2
O2 O3 La 39.7(5) 2 2
O2 O3 La 98.1(5) 1_554 2
O1 O3 La 103.2(4) 2_455 2
O2 O3 La 72.0(4) . 2
O3 O3 La 33.4(3) 2 2
Ga2 O3 La 110.8(4) 1_554 2
O3 O3 La 68.5(4) 2_554 2
Ga3 O3 La 59.02(18) 1_655 2
La O3 La 61.3(2) 4_445 2
Ga2 O3 La 170.5(4) 2_565 2
O2 O3 La 161.3(5) 5_455 2
O3 O3 La 62.91(17) 5 2
O3 O3 La 85.1(2) 5_554 2
Ga3 O3 La 57.1(2) 4_446 2
Nb O3 La 93.5(2) 1_554 2
Ga1 O3 La 93.5(2) 1_554 2
O1 O3 La 133.9(4) . 2
O2 O3 La 118.6(4) 4_554 2
La O3 La 131.2(3) 1_554 2
Ga3 O3 La 87.0(2) 2_565 2
O2 O3 La 134.5(4) 3_454 2
Ga3 O3 O2 148.8(6) 4_445 4
Nb O3 O2 45.4(3) . 4
Ga1 O3 O2 45.4(3) . 4
La O3 O2 72.9(4) . 4
Ga3 O3 O2 67.9(4) 2_564 4
O2 O3 O2 53.7(5) 6 4
O3 O3 O2 32.8(5) 6 4
O3 O3 O2 107.0(7) 6_554 4
O3 O3 O2 88.2(4) 3 4
O3 O3 O2 44.7(4) 4 4
O2 O3 O2 137.3(7) 2 4
O2 O3 O2 160.8(6) 1_554 4
O1 O3 O2 123.1(5) 2_455 4
O2 O3 O2 86.1(4) . 4
O3 O3 O2 72.1(3) 2 4
Ga2 O3 O2 144.0(5) 1_554 4
O3 O3 O2 127.0(3) 2_554 4
Ga3 O3 O2 86.0(3) 1_655 4
La O3 O2 124.6(4) 4_445 4
Ga2 O3 O2 76.1(4) 2_565 4
O2 O3 O2 85.6(4) 5_455 4
O3 O3 O2 36.0(3) 5 4
O3 O3 O2 88.0(4) 5_554 4
Ga3 O3 O2 68.5(2) 4_446 4
Nb O3 O2 113.0(4) 1_554 4
Ga1 O3 O2 113.0(4) 1_554 4
O1 O3 O2 47.4(3) . 4
O2 O3 O2 68.7(3) 4_554 4
La O3 O2 122.0(4) 1_554 4
Ga3 O3 O2 23.35(19) 2_565 4
O2 O3 O2 126.2(5) 3_454 4
La O3 O2 98.3(3) 2 4
Ga3 O3 O2 126.5(6) 4_445 3_455
Nb O3 O2 104.6(5) . 3_455
Ga1 O3 O2 104.6(5) . 3_455
La O3 O2 19.9(3) . 3_455
Ga3 O3 O2 126.1(5) 2_564 3_455
O2 O3 O2 85.7(4) 6 3_455
O3 O3 O2 59.0(4) 6 3_455
O3 O3 O2 127.7(3) 6_554 3_455
O3 O3 O2 138.0(4) 3 3_455
O3 O3 O2 128.3(6) 4 3_455
O2 O3 O2 102.0(5) 2 3_455
O2 O3 O2 99.6(4) 1_554 3_455
O1 O3 O2 39.3(3) 2_455 3_455
O2 O3 O2 38.5(4) . 3_455
O3 O3 O2 87.0(5) 2 3_455
Ga2 O3 O2 66.7(3) 1_554 3_455
O3 O3 O2 149.0(3) 2_554 3_455
Ga3 O3 O2 164.1(4) 1_655 3_455
La O3 O2 61.5(2) 4_445 3_455
Ga2 O3 O2 77.0(3) 2_565 3_455
O2 O3 O2 51.6(4) 5_455 3_455
O3 O3 O2 102.0(5) 5 3_455
O3 O3 O2 163.4(3) 5_554 3_455
Ga3 O3 O2 60.0(3) 4_446 3_455
Nb O3 O2 148.9(4) 1_554 3_455
Ga1 O3 O2 148.9(4) 1_554 3_455
O1 O3 O2 47.9(3) . 3_455
O2 O3 O2 126.1(5) 4_554 3_455
La O3 O2 100.9(3) 1_554 3_455
Ga3 O3 O2 68.8(3) 2_565 3_455
O2 O3 O2 70.1(3) 3_454 3_455
La O3 O2 110.4(4) 2 3_455
O2 O3 O2 83.9(5) 4 3_455
Ga3 O3 La 146.1(6) 4_445 2_565
Nb O3 La 74.7(4) . 2_565
Ga1 O3 La 74.7(4) . 2_565
La O3 La 62.3(3) . 2_565
Ga3 O3 La 52.2(3) 2_564 2_565
O2 O3 La 23.9(3) 6 2_565
O3 O3 La 53.6(6) 6 2_565
O3 O3 La 85.4(6) 6_554 2_565
O3 O3 La 111.3(5) 3 2_565
O3 O3 La 53.6(6) 4 2_565
O2 O3 La 167.7(6) 2 2_565
O2 O3 La 131.2(6) 1_554 2_565
O1 O3 La 113.0(3) 2_455 2_565
O2 O3 La 101.0(4) . 2_565
O3 O3 La 102.1(3) 2 2_565
Ga2 O3 La 119.5(3) 1_554 2_565
O3 O3 La 126.1(3) 2_554 2_565
Ga3 O3 La 97.2(3) 1_655 2_565
La O3 La 139.3(3) 4_445 2_565
Ga2 O3 La 45.76(16) 2_565 2_565
O2 O3 La 59.5(3) 5_455 2_565
O3 O3 La 65.18(15) 5 2_565
O3 O3 La 85.5(2) 5_554 2_565
Ga3 O3 La 92.9(2) 4_446 2_565
Nb O3 La 101.0(3) 1_554 2_565
Ga1 O3 La 101.0(3) 1_554 2_565
O1 O3 La 32.51(13) . 2_565
O2 O3 La 52.7(3) 4_554 2_565
La O3 La 92.8(3) 1_554 2_565
Ga3 O3 La 48.27(14) 2_565 2_565
O2 O3 La 97.3(4) 3_454 2_565
La O3 La 128.1(3) 2 2_565
O2 O3 La 30.4(2) 4 2_565
O2 O3 La 80.2(3) 3_455 2_565
Ga3 O3 Ga2 31.1(4) 4_445 2
Nb O3 Ga2 98.1(5) . 2
Ga1 O3 Ga2 98.1(5) . 2
La O3 Ga2 126.3(5) . 2
Ga3 O3 Ga2 122.6(4) 2_564 2
O2 O3 Ga2 157.7(5) 6 2
O3 O3 Ga2 125.8(8) 6 2
O3 O3 Ga2 93.3(5) 6_554 2
O3 O3 Ga2 59.5(5) 3 2
O3 O3 Ga2 117.1(5) 4 2
O2 O3 Ga2 9.0(3) 2 2
O2 O3 Ga2 53.6(4) 1_554 2
O1 O3 Ga2 76.2(3) 2_455 2
O2 O3 Ga2 83.1(4) . 2
O3 O3 Ga2 73.9(3) 2 2
Ga2 O3 Ga2 69.1(2) 1_554 2
O3 O3 Ga2 48.2(2) 2_554 2
Ga3 O3 Ga2 73.9(2) 1_655 2
La O3 Ga2 47.00(17) 4_445 2
Ga2 O3 Ga2 139.8(3) 2_565 2
O2 O3 Ga2 129.3(4) 5_455 2
O3 O3 Ga2 107.55(15) 5 2
O3 O3 Ga2 87.4(2) 5_554 2
Ga3 O3 Ga2 87.0(3) 4_446 2
Nb O3 Ga2 74.9(2) 1_554 2
Ga1 O3 Ga2 74.9(2) 1_554 2
O1 O3 Ga2 155.6(4) . 2
O2 O3 Ga2 122.2(4) 4_554 2
La O3 Ga2 90.6(2) 1_554 2
Ga3 O3 Ga2 129.2(3) 2_565 2
O2 O3 Ga2 90.2(3) 3_454 2
La O3 Ga2 45.05(14) 2 2
O2 O3 Ga2 143.3(4) 4 2
O2 O3 Ga2 107.7(4) 3_455 2
La O3 Ga2 170.7(3) 2_565 2
Ga3 O3 O2 82.5(4) 4_445 5
Nb O3 O2 41.6(3) . 5
Ga1 O3 O2 41.6(3) . 5
La O3 O2 139.4(5) . 5
Ga3 O3 O2 59.5(3) 2_564 5
O2 O3 O2 90.4(3) 6 5
O3 O3 O2 86.7(3) 6 5
O3 O3 O2 80.0(3) 6_554 5
O3 O3 O2 31.2(4) 3 5
O3 O3 O2 29.2(5) 4 5
O2 O3 O2 89.4(4) 2 5
O2 O3 O2 114.2(4) 1_554 5
O1 O3 O2 162.8(5) 2_455 5
O2 O3 O2 118.3(4) . 5
O3 O3 O2 67.8(3) 2 5
Ga2 O3 O2 147.2(4) 1_554 5
O3 O3 O2 62.7(3) 2_554 5
Ga3 O3 O2 20.4(2) 1_655 5
La O3 O2 121.2(4) 4_445 5
Ga2 O3 O2 110.6(4) 2_565 5
O2 O3 O2 136.9(5) 5_455 5
O3 O3 O2 43.4(4) 5 5
O3 O3 O2 38.4(3) 5_554 5
Ga3 O3 O2 91.5(3) 4_446 5
Nb O3 O2 64.1(2) 1_554 5
Ga1 O3 O2 64.1(2) 1_554 5
O1 O3 O2 112.1(4) . 5
O2 O3 O2 60.1(4) 4_554 5
La O3 O2 109.6(3) 1_554 5
Ga3 O3 O2 77.3(3) 2_565 5
O2 O3 O2 142.1(3) 3_454 5
La O3 O2 60.0(2) 2 5
O2 O3 O2 66.5(5) 4 5
O2 O3 O2 145.5(3) 3_455 5
La O3 O2 82.4(3) 2_565 5
Ga2 O3 O2 88.2(3) 2 5
Ga3 O3 O1 93.9(5) 4_445 1_554
Nb O3 O1 129.4(6) . 1_554
Ga1 O3 O1 129.4(6) . 1_554
La O3 O1 76.1(4) . 1_554
Ga3 O3 O1 46.3(2) 2_564 1_554
O2 O3 O1 37.6(4) 6 1_554
O3 O3 O1 111.4(6) 6 1_554
O3 O3 O1 38.3(3) 6_554 1_554
O3 O3 O1 129.3(4) 3 1_554
O3 O3 O1 85.4(5) 4 1_554
O2 O3 O1 130.1(5) 2 1_554
O2 O3 O1 69.8(5) 1_554 1_554
O1 O3 O1 89.3(3) 2_455 1_554
O2 O3 O1 130.7(4) . 1_554
O3 O3 O1 163.4(3) 2 1_554
Ga2 O3 O1 70.5(2) 1_554 1_554
O3 O3 O1 88.4(5) 2_554 1_554
Ga3 O3 O1 100.3(3) 1_655 1_554
La O3 O1 128.9(3) 4_445 1_554
Ga2 O3 O1 20.52(18) 2_565 1_554
O2 O3 O1 40.6(3) 5_455 1_554
O3 O3 O1 121.0(3) 5 1_554
O3 O3 O1 73.4(3) 5_554 1_554
Ga3 O3 O1 146.2(3) 4_446 1_554
Nb O3 O1 62.7(3) 1_554 1_554
Ga1 O3 O1 62.7(3) 1_554 1_554
O1 O3 O1 67.3(2) . 1_554
O2 O3 O1 45.6(3) 4_554 1_554
La O3 O1 31.39(19) 1_554 1_554
Ga3 O3 O1 108.9(3) 2_565 1_554
O2 O3 O1 45.9(2) 3_454 1_554
La O3 O1 156.2(3) 2 1_554
O2 O3 O1 91.3(4) 4 1_554
O2 O3 O1 92.2(3) 3_455 1_554
La O3 O1 61.5(2) 2_565 1_554
Ga2 O3 O1 121.9(3) 2 1_554
O2 O3 O1 105.3(3) 5 1_554
Ga3 O3 Ga3 98.8(4) 4_445 .
Nb O3 Ga3 149.6(5) . .
Ga1 O3 Ga3 149.6(5) . .
La O3 Ga3 46.8(2) . .
Ga3 O3 Ga3 89.1(4) 2_564 .
O2 O3 Ga3 63.5(4) 6 .
O3 O3 Ga3 102.5(2) 6 .
O3 O3 Ga3 73.18(16) 6_554 .
O3 O3 Ga3 163.1(3) 3 .
O3 O3 Ga3 124.6(7) 4 .
O2 O3 Ga3 111.9(5) 2 .
O2 O3 Ga3 62.8(3) 1_554 .
O1 O3 Ga3 47.1(2) 2_455 .
O2 O3 Ga3 90.5(3) . .
O3 O3 Ga3 141.3(4) 2 .
Ga2 O3 Ga3 40.13(14) 1_554 .
O3 O3 Ga3 109.3(5) 2_554 .
Ga3 O3 Ga3 140.4(4) 1_655 .
La O3 Ga3 88.8(2) 4_445 .
Ga2 O3 Ga3 40.20(12) 2_565 .
O2 O3 Ga3 20.4(3) 5_455 .
O3 O3 Ga3 141.3(2) 5 .
O3 O3 Ga3 114.3(4) 5_554 .
Ga3 O3 Ga3 114.8(3) 4_446 .
Nb O3 Ga3 94.5(3) 1_554 .
Ga1 O3 Ga3 94.5(3) 1_554 .
O1 O3 Ga3 60.2(2) . .
O2 O3 Ga3 88.5(4) 4_554 .
La O3 Ga3 46.52(13) 1_554 .
Ga3 O3 Ga3 108.0(2) 2_565 .
O2 O3 Ga3 21.8(2) 3_454 .
La O3 Ga3 149.1(4) 2 .
O2 O3 Ga3 105.9(4) 4 .
O2 O3 Ga3 54.8(3) 3_455 .
La O3 Ga3 79.4(2) 2_565 .
Ga2 O3 Ga3 109.1(2) 2 .
O2 O3 Ga3 148.5(4) 5 .
O1 O3 Ga3 43.26(13) 1_554 .
Ga3 O3 Ga2 118.0(6) 4_445 .
Nb O3 Ga2 91.4(4) . .
Ga1 O3 Ga2 91.4(4) . .
La O3 Ga2 41.5(3) . .
Ga3 O3 Ga2 145.6(4) 2_564 .
O2 O3 Ga2 105.6(4) 6 .
O3 O3 Ga2 55.6(5) 6 .
O3 O3 Ga2 147.63(18) 6_554 .
O3 O3 Ga2 115.8(4) 3 .
O3 O3 Ga2 129.5(2) 4 .
O2 O3 Ga2 84.2(4) 2 .
O2 O3 Ga2 103.5(5) 1_554 .
O1 O3 Ga2 42.9(4) 2_455 .
O2 O3 Ga2 15.9(3) . .
O3 O3 Ga2 66.4(3) 2 .
Ga2 O3 Ga2 73.9(2) 1_554 .
O3 O3 Ga2 139.5(3) 2_554 .
Ga3 O3 Ga2 144.3(4) 1_655 .
La O3 Ga2 44.89(15) 4_445 .
Ga2 O3 Ga2 99.8(2) 2_565 .
O2 O3 Ga2 74.4(3) 5_455 .
O3 O3 Ga2 92.1(4) 5 .
O3 O3 Ga2 170.5(4) 5_554 .
Ga3 O3 Ga2 40.83(13) 4_446 .
Nb O3 Ga2 159.4(3) 1_554 .
Ga1 O3 Ga2 159.4(3) 1_554 .
O1 O3 Ga2 64.9(2) . .
O2 O3 Ga2 145.9(4) 4_554 .
La O3 Ga2 118.2(3) 1_554 .
Ga3 O3 Ga2 66.15(17) 2_565 .
O2 O3 Ga2 85.7(3) 3_454 .
La O3 Ga2 87.5(3) 2 .
O2 O3 Ga2 87.1(3) 4 .
O2 O3 Ga2 22.89(19) 3_455 .
La O3 Ga2 94.4(2) 2_565 .
Ga2 O3 Ga2 91.6(3) 2 .
O2 O3 Ga2 132.2(3) 5 .
O1 O3 Ga2 114.8(3) 1_554 .
Ga3 O3 Ga2 74.99(17) . .
Ga3 O3 La 115.1(5) 4_445 4
Nb O3 La 35.0(3) . 4
Ga1 O3 La 35.0(3) . 4
La O3 La 106.4(4) . 4
Ga3 O3 La 53.0(2) 2_564 4
O2 O3 La 65.5(4) 6 4
O3 O3 La 60.5(4) 6 4
O3 O3 La 89.3(5) 6_554 4
O3 O3 La 60.4(4) 3 4
O3 O3 La 14.26(15) 4 4
O2 O3 La 118.8(6) 2 4
O2 O3 La 140.9(5) 1_554 4
O1 O3 La 156.4(4) 2_455 4
O2 O3 La 108.5(4) . 4
O3 O3 La 71.00(18) 2 4
Ga2 O3 La 165.2(4) 1_554 4
O3 O3 La 93.5(2) 2_554 4
Ga3 O3 La 52.35(16) 1_655 4
La O3 La 135.7(3) 4_445 4
Ga2 O3 La 89.6(3) 2_565 4
O2 O3 La 109.9(4) 5_455 4
O3 O3 La 28.5(2) 5 4
O3 O3 La 57.4(3) 5_554 4
Ga3 O3 La 83.2(2) 4_446 4
Nb O3 La 84.9(2) 1_554 4
Ga1 O3 La 84.9(2) 1_554 4
O1 O3 La 78.7(2) . 4
O2 O3 La 53.9(2) 4_554 4
La O3 La 116.0(3) 1_554 4
Ga3 O3 La 50.02(13) 2_565 4
O2 O3 La 140.7(4) 3_454 4
La O3 La 81.7(2) 2 4
O2 O3 La 33.8(2) 4 4
O2 O3 La 117.3(4) 3_455 4
La O3 La 50.92(14) 2_565 4
Ga2 O3 La 119.9(3) 2 4
O2 O3 La 33.4(2) 5 4
O1 O3 La 94.8(3) 1_554 4
Ga3 O3 La 128.7(3) . 4
Ga2 O3 La 115.5(2) . 4
Ga3 O3 O1 71.6(5) 4_445 1_545
Nb O3 O1 73.7(5) . 1_545
Ga1 O3 O1 73.7(5) . 1_545
La O3 O1 102.3(5) . 1_545
Ga3 O3 O1 149.2(4) 2_564 1_545
O2 O3 O1 161.7(5) 6 1_545
O3 O3 O1 85.5(7) 6 1_545
O3 O3 O1 133.6(6) 6_554 1_545
O3 O3 O1 61.5(5) 3 1_545
O3 O3 O1 115.4(5) 4 1_545
O2 O3 O1 31.6(4) 2 1_545
O2 O3 O1 88.6(5) 1_554 1_545
O1 O3 O1 72.5(3) 2_455 1_545
O2 O3 O1 47.5(4) . 1_545
O3 O3 O1 39.4(2) 2 1_545
Ga2 O3 O1 86.8(3) 1_554 1_545
O3 O3 O1 84.5(4) 2_554 1_545
Ga3 O3 O1 89.1(3) 1_655 1_545
La O3 O1 30.69(12) 4_445 1_545
Ga2 O3 O1 158.1(3) 2_565 1_545
O2 O3 O1 130.6(4) 5_455 1_545
O3 O3 O1 82.2(3) 5 1_545
O3 O3 O1 113.6(2) 5_554 1_545
Ga3 O3 O1 46.4(3) 4_446 1_545
Nb O3 O1 112.5(3) 1_554 1_545
Ga1 O3 O1 112.5(3) 1_554 1_545
O1 O3 O1 122.1(5) . 1_545
O2 O3 O1 149.5(4) 4_554 1_545
La O3 O1 127.4(3) 1_554 1_545
Ga3 O3 O1 90.5(3) 2_565 1_545
O2 O3 O1 111.7(4) 3_454 1_545
La O3 O1 31.20(11) 2 1_545
O2 O3 O1 110.6(4) 4 1_545
O2 O3 O1 82.9(3) 3_455 1_545
La O3 O1 138.8(3) 2_565 1_545
Ga2 O3 O1 40.6(2) 2 1_545
O2 O3 O1 91.0(3) 5 1_545
O1 O3 O1 156.8(4) 1_554 1_545
Ga3 O3 O1 119.5(3) . 1_545
Ga2 O3 O1 60.9(2) . 1_545
La O3 O1 107.6(3) 4 1_545
Ga3 O3 O3 43.7(5) 4_445 1_554
Nb O3 O3 127.7(4) . 1_554
Ga1 O3 O3 127.7(4) . 1_554
La O3 O3 120.5(3) . 1_554
Ga3 O3 O3 58.6(3) 2_564 1_554
O2 O3 O3 83.2(4) 6 1_554
O3 O3 O3 158.3(7) 6 1_554
O3 O3 O3 20.0(6) 6_554 1_554
O3 O3 O3 90.001(1) 3 1_554
O3 O3 O3 90.000(2) 4 1_554
O2 O3 O3 83.4(4) 2 1_554
O2 O3 O3 37.9(5) 1_554 1_554
O1 O3 O3 96.5(4) 2_455 1_554
O2 O3 O3 146.4(3) . 1_554
O3 O3 O3 139.1(4) 2 1_554
Ga2 O3 O3 65.5(2) 1_554 1_554
O3 O3 O3 38.3(5) 2_554 1_554
Ga3 O3 O3 68.7(2) 1_655 1_554
La O3 O3 108.87(18) 4_445 1_554
Ga2 O3 O3 71.94(18) 2_565 1_554
O2 O3 O3 85.3(3) 5_455 1_554
O3 O3 O3 128.3(4) 5 1_554
O3 O3 O3 49.1(3) 5_554 1_554
Ga3 O3 O3 161.3(2) 4_446 1_554
Nb O3 O3 22.05(16) 1_554 1_554
Ga1 O3 O3 22.05(16) 1_554 1_554
O1 O3 O3 118.7(3) . 1_554
O2 O3 O3 57.8(3) 4_554 1_554
La O3 O3 28.02(15) 1_554 1_554
Ga3 O3 O3 149.8(2) 2_565 1_554
O2 O3 O3 57.1(3) 3_454 1_554
La O3 O3 106.41(16) 2 1_554
O2 O3 O3 126.5(3) 4 1_554
O2 O3 O3 127.2(3) 3_455 1_554
La O3 O3 105.09(17) 2_565 1_554
Ga2 O3 O3 74.42(18) 2 1_554
O2 O3 O3 86.1(2) 5 1_554
O1 O3 O3 51.4(2) 1_554 1_554
Ga3 O3 O3 74.22(15) . 1_554
Ga2 O3 O3 139.44(14) . 1_554
La O3 O3 104.25(16) 4 1_554
O1 O3 O3 115.1(2) 1_545 1_554
Ga3 O3 O3 136.3(5) 4_445 1_556
Nb O3 O3 52.3(4) . 1_556
Ga1 O3 O3 52.3(4) . 1_556
La O3 O3 59.5(3) . 1_556
Ga3 O3 O3 121.4(3) 2_564 1_556
O2 O3 O3 96.8(4) 6 1_556
O3 O3 O3 21.7(7) 6 1_556
O3 O3 O3 160.0(6) 6_554 1_556
O3 O3 O3 90.000(1) 3 1_556
O3 O3 O3 90.000(1) 4 1_556
O2 O3 O3 96.6(4) 2 1_556
O2 O3 O3 142.1(5) 1_554 1_556
O1 O3 O3 83.5(4) 2_455 1_556
O2 O3 O3 33.6(3) . 1_556
O3 O3 O3 40.9(4) 2 1_556
Ga2 O3 O3 114.5(2) 1_554 1_556
O3 O3 O3 141.7(5) 2_554 1_556
Ga3 O3 O3 111.3(2) 1_655 1_556
La O3 O3 71.14(18) 4_445 1_556
Ga2 O3 O3 108.06(18) 2_565 1_556
O2 O3 O3 94.7(3) 5_455 1_556
O3 O3 O3 51.7(4) 5 1_556
O3 O3 O3 130.9(3) 5_554 1_556
Ga3 O3 O3 18.7(2) 4_446 1_556
Nb O3 O3 157.95(16) 1_554 1_556
Ga1 O3 O3 157.95(16) 1_554 1_556
O1 O3 O3 61.3(3) . 1_556
O2 O3 O3 122.2(3) 4_554 1_556
La O3 O3 151.98(15) 1_554 1_556
Ga3 O3 O3 30.2(2) 2_565 1_556
O2 O3 O3 122.9(3) 3_454 1_556
La O3 O3 73.59(16) 2 1_556
O2 O3 O3 53.5(3) 4 1_556
O2 O3 O3 52.8(3) 3_455 1_556
La O3 O3 74.91(17) 2_565 1_556
Ga2 O3 O3 105.58(18) 2 1_556
O2 O3 O3 93.9(2) 5 1_556
O1 O3 O3 128.6(2) 1_554 1_556
Ga3 O3 O3 105.78(15) . 1_556
Ga2 O3 O3 40.56(14) . 1_556
La O3 O3 75.75(16) 4 1_556
O1 O3 O3 64.9(2) 1_545 1_556
O3 O3 O3 179.999(1) 1_554 1_556
Ga3 O3 O2 48.1(4) 4_445 3_554
Nb O3 O2 69.3(4) . 3_554
Ga1 O3 O2 69.3(4) . 3_554
La O3 O2 173.7(5) . 3_554
Ga3 O3 O2 70.3(3) 2_564 3_554
O2 O3 O2 110.3(6) 6 3_554
O3 O3 O2 118.0(3) 6 3_554
O3 O3 O2 66.8(3) 6_554 3_554
O3 O3 O2 27.8(2) 3 3_554
O3 O3 O2 59.6(4) 4 3_554
O2 O3 O2 63.6(6) 2 3_554
O2 O3 O2 81.3(4) 1_554 3_554
O1 O3 O2 134.0(5) 2_455 3_554
O2 O3 O2 125.0(4) . 3_554
O3 O3 O2 79.1(4) 2 3_554
Ga2 O3 O2 113.4(4) 1_554 3_554
O3 O3 O2 29.7(4) 2_554 3_554
Ga3 O3 O2 15.3(2) 1_655 3_554
La O3 O2 103.3(4) 4_445 3_554
Ga2 O3 O2 119.9(3) 2_565 3_554
O2 O3 O2 144.4(4) 5_455 3_554
O3 O3 O2 74.4(4) 5 3_554
O3 O3 O2 33.4(2) 5_554 3_554
Ga3 O3 O2 106.3(3) 4_446 3_554
Nb O3 O2 43.3(2) 1_554 3_554
Ga1 O3 O2 43.3(2) 1_554 3_554
O1 O3 O2 144.3(4) . 3_554
O2 O3 O2 70.3(3) 4_554 3_554
La O3 O2 90.5(3) 1_554 3_554
Ga3 O3 O2 109.9(3) 2_565 3_554
O2 O3 O2 117.8(4) 3_454 3_554
La O3 O2 53.0(2) 2 3_554
O2 O3 O2 100.8(2) 4 3_554
O2 O3 O2 163.1(5) 3_455 3_554
La O3 O2 112.0(3) 2_565 3_554
Ga2 O3 O2 59.2(3) 2 3_554
O2 O3 O2 34.3(4) 5 3_554
O1 O3 O2 103.9(3) 1_554 3_554
Ga3 O3 O2 136.8(3) . 3_554
Ga2 O3 O2 140.3(4) . 3_554
La O3 O2 67.3(3) 4 3_554
O1 O3 O2 80.2(3) 1_545 3_554
O3 O3 O2 62.6(2) 1_554 3_554
O3 O3 O2 117.4(2) 1_556 3_554
Ga3 O3 Ga3 113.3(5) 4_445 1_656
Nb O3 Ga3 12.4(3) . 1_656
Ga1 O3 Ga3 12.4(3) . 1_656
La O3 Ga3 99.3(3) . 1_656
Ga3 O3 Ga3 99.4(3) 2_564 1_656
O2 O3 Ga3 102.8(4) 6 1_656
O3 O3 Ga3 43.7(2) 6 1_656
O3 O3 Ga3 131.6(4) 6_554 1_656
O3 O3 Ga3 50.92(15) 3 1_656
O3 O3 Ga3 58.92(18) 4 1_656
O2 O3 Ga3 87.6(5) 2 1_656
O2 O3 Ga3 147.2(5) 1_554 1_656
O1 O3 Ga3 120.4(5) 2_455 1_656
O2 O3 Ga3 67.2(3) . 1_656
O3 O3 Ga3 25.08(18) 2 1_656
Ga2 O3 Ga3 148.0(4) 1_554 1_656
O3 O3 Ga3 104.7(5) 2_554 1_656
Ga3 O3 Ga3 69.12(19) 1_655 1_656
La O3 Ga3 89.3(3) 4_445 1_656
Ga2 O3 Ga3 125.9(3) 2_565 1_656
O2 O3 Ga3 129.2(4) 5_455 1_656
O3 O3 Ga3 18.46(17) 5 1_656
O3 O3 Ga3 90.8(4) 5_554 1_656
Ga3 O3 Ga3 39.93(12) 4_446 1_656
Nb O3 Ga3 116.0(3) 1_554 1_656
Ga1 O3 Ga3 116.0(3) 1_554 1_656
O1 O3 Ga3 88.5(3) . 1_656
O2 O3 Ga3 100.3(3) 4_554 1_656
La O3 Ga3 161.3(3) 1_554 1_656
Ga3 O3 Ga3 39.52(11) 2_565 1_656
O2 O3 Ga3 165.1(4) 3_454 1_656
La O3 Ga3 49.12(14) 2 1_656
O2 O3 Ga3 49.7(2) 4 1_656
O2 O3 Ga3 95.0(3) 3_455 1_656
La O3 Ga3 80.13(19) 2_565 1_656
Ga2 O3 Ga3 94.0(3) 2 1_656
O2 O3 Ga3 52.5(2) 5 1_656
O1 O3 Ga3 139.0(3) 1_554 1_656
Ga3 O3 Ga3 146.0(3) . 1_656
Ga2 O3 Ga3 79.8(2) . 1_656
La O3 Ga3 46.58(11) 4 1_656
O1 O3 Ga3 64.2(2) 1_545 1_656
O3 O3 Ga3 137.80(14) 1_554 1_656
O3 O3 Ga3 42.20(14) 1_556 1_656
O2 O3 Ga3 76.5(3) 3_554 1_656
Ga3 O3 O2 56.3(4) 4_445 4_444
Nb O3 O2 153.1(7) . 4_444
Ga1 O3 O2 153.1(7) . 4_444
La O3 O2 81.8(4) . 4_444
Ga3 O3 O2 115.8(4) 2_564 4_444
O2 O3 O2 110.8(5) 6 4_444
O3 O3 O2 131.6(5) 6 4_444
O3 O3 O2 78.3(4) 6_554 4_444
O3 O3 O2 117.0(7) 3 4_444
O3 O3 O2 153.0(3) 4 4_444
O2 O3 O2 62.0(3) 2 4_444
O2 O3 O2 26.8(3) 1_554 4_444
O1 O3 O2 35.2(4) 2_455 4_444
O2 O3 O2 84.1(3) . 4_444
O3 O3 O2 118.1(3) 2 4_444
Ga2 O3 O2 10.5(2) 1_554 4_444
O3 O3 O2 76.4(3) 2_554 4_444
Ga3 O3 O2 118.6(4) 1_655 4_444
La O3 O2 54.3(3) 4_445 4_444
Ga2 O3 O2 86.4(3) 2_565 4_444
O2 O3 O2 70.6(4) 5_455 4_444
O3 O3 O2 161.6(4) 5 4_444
O3 O3 O2 110.2(5) 5_554 4_444
Ga3 O3 O2 109.0(4) 4_446 4_444
Nb O3 O2 82.6(3) 1_554 4_444
Ga1 O3 O2 82.6(3) 1_554 4_444
O1 O3 O2 106.8(4) . 4_444
O2 O3 O2 114.9(4) 4_554 4_444
La O3 O2 52.8(2) 1_554 4_444
Ga3 O3 O2 142.0(4) 2_565 4_444
O2 O3 O2 33.4(3) 3_454 4_444
La O3 O2 101.3(4) 2 4_444
O2 O3 O2 154.1(6) 4 4_444
O2 O3 O2 73.55(18) 3_455 4_444
La O3 O2 129.7(4) 2_565 4_444
Ga2 O3 O2 58.7(3) 2 4_444
O2 O3 O2 138.7(3) 5 4_444
O1 O3 O2 77.3(3) 1_554 4_444
Ga3 O3 O2 50.4(2) . 4_444
Ga2 O3 O2 77.1(3) . 4_444
La O3 O2 167.2(4) 4 4_444
O1 O3 O2 79.5(3) 1_545 4_444
O3 O3 O2 63.0(2) 1_554 4_444
O3 O3 O2 117.0(2) 1_556 4_444
O2 O3 O2 104.4(5) 3_554 4_444
Ga3 O3 O2 143.2(4) 1_656 4_444
Ga3 O3 O2 129.5(6) 4_445 2_565
Nb O3 O2 106.1(5) . 2_565
Ga1 O3 O2 106.1(5) . 2_565
La O3 O2 51.6(4) . 2_565
Ga3 O3 O2 54.9(3) 2_564 2_565
O2 O3 O2 16.1(4) 6 2_565
O3 O3 O2 75.8(6) 6 2_565
O3 O3 O2 70.5(5) 6_554 2_565
O3 O3 O2 137.6(6) 3 2_565
O3 O3 O2 77.7(6) 4 2_565
O2 O3 O2 160.7(7) 2 2_565
O2 O3 O2 101.8(4) 1_554 2_565
O1 O3 O2 90.8(4) 2_455 2_565
O2 O3 O2 106.0(3) . 2_565
O3 O3 O2 129.8(5) 2 2_565
Ga2 O3 O2 88.9(4) 1_554 2_565
O3 O3 O2 121.1(5) 2_554 2_565
Ga3 O3 O2 114.0(4) 1_655 2_565
La O3 O2 130.3(3) 4_445 2_565
Ga2 O3 O2 15.9(2) 2_565 2_565
O2 O3 O2 31.0(3) 5_455 2_565
O3 O3 O2 96.5(2) 5 2_565
O3 O3 O2 92.0(2) 5_554 2_565
Ga3 O3 O2 111.8(3) 4_446 2_565
Nb O3 O2 93.3(3) 1_554 2_565
Ga1 O3 O2 93.3(3) 1_554 2_565
O1 O3 O2 32.7(3) . 2_565
O2 O3 O2 54.8(3) 4_554 2_565
La O3 O2 65.9(3) 1_554 2_565
Ga3 O3 O2 74.4(3) 2_565 2_565
O2 O3 O2 66.0(4) 3_454 2_565
La O3 O2 159.4(3) 2 2_565
O2 O3 O2 61.2(3) 4 2_565
O2 O3 O2 71.4(3) 3_455 2_565
La O3 O2 31.4(2) 2_565 2_565
Ga2 O3 O2 155.3(3) 2 2_565
O2 O3 O2 106.4(5) 5 2_565
O1 O3 O2 35.6(2) 1_554 2_565
Ga3 O3 O2 49.2(3) . 2_565
Ga2 O3 O2 92.8(3) . 2_565
La O3 O2 79.6(3) 4 2_565
O1 O3 O2 153.5(3) 1_545 2_565
O3 O3 O2 86.6(2) 1_554 2_565
O3 O3 O2 93.4(2) 1_556 2_565
O2 O3 O2 125.2(3) 3_554 2_565
Ga3 O3 O2 110.7(3) 1_656 2_565
O2 O3 O2 98.8(5) 4_444 2_565
Ga3 O3 La 26.1(3) 4_445 4_444
Nb O3 La 136.4(5) . 4_444
Ga1 O3 La 136.4(5) . 4_444
La O3 La 112.4(4) . 4_444
Ga3 O3 La 101.1(3) 2_564 4_444
O2 O3 La 118.6(5) 6 4_444
O3 O3 La 158.2(8) 6 4_444
O3 O3 La 62.1(5) 6_554 4_444
O3 O3 La 90.5(5) 3 4_444
O3 O3 La 126.1(2) 4 4_444
O2 O3 La 49.2(4) 2 4_444
O2 O3 La 12.1(3) 1_554 4_444
O1 O3 La 65.1(4) 2_455 4_444
O2 O3 La 104.9(4) . 4_444
O3 O3 La 115.2(4) 2 4_444
Ga2 O3 La 39.81(13) 1_554 4_444
O3 O3 La 45.4(2) 2_554 4_444
Ga3 O3 La 87.5(2) 1_655 4_444
La O3 La 66.4(2) 4_445 4_444
Ga2 O3 La 98.1(2) 2_565 4_444
O2 O3 La 93.6(3) 5_455 4_444
O3 O3 La 144.8(3) 5 4_444
O3 O3 La 82.2(3) 5_554 4_444
Ga3 O3 La 121.9(3) 4_446 4_444
Nb O3 La 56.39(14) 1_554 4_444
Ga1 O3 La 56.39(14) 1_554 4_444
O1 O3 La 134.0(3) . 4_444
O2 O3 La 100.3(3) 4_554 4_444
La O3 La 49.73(12) 1_554 4_444
Ga3 O3 La 167.6(4) 2_565 4_444
O2 O3 La 52.3(2) 3_454 4_444
La O3 La 86.0(2) 2 4_444
O2 O3 La 169.0(4) 4 4_444
O2 O3 La 104.2(3) 3_455 4_444
La O3 La 142.5(3) 2_565 4_444
Ga2 O3 La 41.67(11) 2 4_444
O2 O3 La 107.8(3) 5 4_444
O1 O3 La 81.1(2) 1_554 4_444
Ga3 O3 La 73.83(16) . 4_444
Ga2 O3 La 103.3(3) . 4_444
La O3 La 138.5(3) 4 4_444
O1 O3 La 78.2(3) 1_545 4_444
O3 O3 La 42.51(17) 1_554 4_444
O3 O3 La 137.49(17) 1_556 4_444
O2 O3 La 73.6(3) 3_554 4_444
Ga3 O3 La 135.1(3) 1_656 4_444
O2 O3 La 31.1(2) 4_444 4_444
O2 O3 La 113.8(3) 2_565 4_444
Ga3 O3 O2 93.1(5) 4_445 3
Nb O3 O2 21.7(3) . 3
Ga1 O3 O2 21.7(3) . 3
La O3 O2 117.9(4) . 3
Ga3 O3 O2 100.2(4) 2_564 3
O2 O3 O2 116.6(5) 6 3
O3 O3 O2 63.7(3) 6 3
O3 O3 O2 121.7(2) 6_554 3
O3 O3 O2 31.6(2) 3 3
O3 O3 O2 60.8(3) 4 3
O2 O3 O2 71.4(6) 2 3
O2 O3 O2 127.9(4) 1_554 3
O1 O3 O2 124.0(5) 2_455 3
O2 O3 O2 75.6(4) . 3
O3 O3 O2 24.7(3) 2 3
Ga2 O3 O2 141.4(5) 1_554 3
O3 O3 O2 85.4(5) 2_554 3
Ga3 O3 O2 54.7(2) 1_655 3
La O3 O2 84.8(3) 4_445 3
Ga2 O3 O2 141.0(4) 2_565 3
O2 O3 O2 149.4(3) 5_455 3
O3 O3 O2 31.2(2) 5 3
O3 O3 O2 80.0(4) 5_554 3
Ga3 O3 O2 50.1(2) 4_446 3
Nb O3 O2 101.0(3) 1_554 3
Ga1 O3 O2 101.0(3) 1_554 3
O1 O3 O2 108.6(3) . 3
O2 O3 O2 100.9(2) 4_554 3
La O3 O2 149.1(3) 1_554 3
Ga3 O3 O2 59.7(2) 2_565 3
O2 O3 O2 166.0(5) 3_454 3
La O3 O2 31.7(2) 2 3
O2 O3 O2 66.9(3) 4 3
O2 O3 O2 109.8(4) 3_455 3
La O3 O2 96.3(3) 2_565 3
Ga2 O3 O2 76.5(3) 2 3
O2 O3 O2 43.2(3) 5 3
O1 O3 O2 146.2(4) 1_554 3
Ga3 O3 O2 164.4(3) . 3
Ga2 O3 O2 90.5(3) . 3
La O3 O2 52.6(2) 4 3
O1 O3 O2 55.1(3) 1_545 3
O3 O3 O2 121.3(2) 1_554 3
O3 O3 O2 58.7(2) 1_556 3
O2 O3 O2 58.7(2) 3_554 3
Ga3 O3 O2 20.25(17) 1_656 3
O2 O3 O2 132.6(5) 4_444 3
O2 O3 O2 127.7(3) 2_565 3
La O3 O2 116.0(3) 4_444 3
Ga3 O3 O1 124.1(5) 4_445 2_565
Nb O3 O1 61.1(4) . 2_565
Ga1 O3 O1 61.1(4) . 2_565
La O3 O1 90.3(4) . 2_565
Ga3 O3 O1 35.2(3) 2_564 2_565
O2 O3 O1 37.5(3) 6 2_565
O3 O3 O1 65.4(7) 6 2_565
O3 O3 O1 74.7(6) 6_554 2_565
O3 O3 O1 85.8(5) 3 2_565
O3 O3 O1 26.1(5) 4 2_565
O2 O3 O1 144.7(5) 2 2_565
O2 O3 O1 130.4(6) 1_554 2_565
O1 O3 O1 140.9(4) 2_455 2_565
O2 O3 O1 118.7(4) . 2_565
O3 O3 O1 96.0(2) 2 2_565
Ga2 O3 O1 138.2(4) 1_554 2_565
O3 O3 O1 101.5(2) 2_554 2_565
Ga3 O3 O1 68.9(2) 1_655 2_565
La O3 O1 157.1(4) 4_445 2_565
Ga2 O3 O1 61.4(2) 2_565 2_565
O2 O3 O1 83.3(3) 5_455 2_565
O3 O3 O1 52.7(2) 5 2_565
O3 O3 O1 60.0(3) 5_554 2_565
Ga3 O3 O1 100.0(3) 4_446 2_565
Nb O3 O1 81.5(3) 1_554 2_565
Ga1 O3 O1 81.5(3) 1_554 2_565
O1 O3 O1 60.5(2) . 2_565
O2 O3 O1 36.1(3) 4_554 2_565
La O3 O1 94.6(3) 1_554 2_565
Ga3 O3 O1 56.0(3) 2_565 2_565
O2 O3 O1 113.2(4) 3_454 2_565
La O3 O1 109.8(2) 2 2_565
O2 O3 O1 32.7(3) 4 2_565
O2 O3 O1 107.4(4) 3_455 2_565
La O3 O1 28.21(12) 2_565 2_565
Ga2 O3 O1 142.8(3) 2 2_565
O2 O3 O1 55.3(3) 5 2_565
O1 O3 O1 68.4(3) 1_554 2_565
Ga3 O3 O1 101.0(3) . 2_565
Ga2 O3 O1 117.5(3) . 2_565
La O3 O1 28.12(12) 4 2_565
O1 O3 O1 134.7(3) 1_545 2_565
O3 O3 O1 93.8(2) 1_554 2_565
O3 O3 O1 86.2(2) 1_556 2_565
O2 O3 O1 83.9(3) 3_554 2_565
Ga3 O3 O1 71.0(2) 1_656 2_565
O2 O3 O1 145.7(4) 4_444 2_565
O2 O3 O1 52.3(2) 2_565 2_565
La O3 O1 136.2(3) 4_444 2_565
O2 O3 O1 80.4(3) 3 2_565
Ga3 O3 Ga2 168.7(5) 4_445 2_566
Nb O3 Ga2 77.9(3) . 2_566
Ga1 O3 Ga2 77.9(3) . 2_566
La O3 Ga2 30.7(2) . 2_566
Ga3 O3 Ga2 92.5(3) 2_564 2_566
O2 O3 Ga2 56.0(4) 6 2_566
O3 O3 Ga2 31.2(3) 6 2_566
O3 O3 Ga2 119.5(6) 6_554 2_566
O3 O3 Ga2 124.6(3) 3 2_566
O3 O3 Ga2 85.9(5) 4 2_566
O2 O3 Ga2 136.3(5) 2 2_566
O2 O3 Ga2 134.0(4) 1_554 2_566
O1 O3 Ga2 81.1(3) 2_455 2_566
O2 O3 Ga2 61.5(3) . 2_566
O3 O3 Ga2 84.1(4) 2 2_566
Ga2 O3 Ga2 103.2(3) 1_554 2_566
O3 O3 Ga2 166.7(3) 2_554 2_566
Ga3 O3 Ga2 128.6(3) 1_655 2_566
La O3 Ga2 98.7(3) 4_445 2_566
Ga2 O3 Ga2 63.59(18) 2_565 2_566
O2 O3 Ga2 54.8(3) 5_455 2_566
O3 O3 Ga2 70.9(3) 5 2_566
O3 O3 Ga2 125.3(3) 5_554 2_566
Ga3 O3 Ga2 62.58(16) 4_446 2_566
Nb O3 Ga2 140.3(4) 1_554 2_566
Ga1 O3 Ga2 140.3(4) 1_554 2_566
O1 O3 Ga2 16.8(2) . 2_566
O2 O3 Ga2 93.0(4) 4_554 2_566
La O3 Ga2 111.0(3) 1_554 2_566
Ga3 O3 Ga2 35.90(10) 2_565 2_566
O2 O3 Ga2 93.9(3) 3_454 2_566
La O3 Ga2 117.4(3) 2 2_566
O2 O3 Ga2 42.5(3) 4 2_566
O2 O3 Ga2 42.7(3) 3_455 2_566
La O3 Ga2 40.59(10) 2_565 2_566
Ga2 O3 Ga2 144.7(3) 2 2_566
O2 O3 Ga2 108.8(3) 5 2_566
O1 O3 Ga2 84.1(3) 1_554 2_566
Ga3 O3 Ga2 72.15(16) . 2_566
Ga2 O3 Ga2 53.83(12) . 2_566
La O3 Ga2 76.26(17) 4 2_566
O1 O3 Ga2 106.5(3) 1_545 2_566
O3 O3 Ga2 135.53(16) 1_554 2_566
O3 O3 Ga2 44.47(16) 1_556 2_566
O2 O3 Ga2 143.1(3) 3_554 2_566
Ga3 O3 Ga2 74.57(16) 1_656 2_566
O2 O3 Ga2 112.4(3) 4_444 2_566
O2 O3 Ga2 49.30(19) 2_565 2_566
La O3 Ga2 143.0(2) 4_444 2_566
O2 O3 Ga2 94.8(3) 3 2_566
O1 O3 Ga2 65.5(2) 2_565 2_566
Ga3 O3 O2 98.8(6) 4_445 4_445
Nb O3 O2 106.1(5) . 4_445
Ga1 O3 O2 106.1(5) . 4_445
La O3 O2 51.7(3) . 4_445
Ga3 O3 O2 156.1(5) 2_564 4_445
O2 O3 O2 117.0(5) 6 4_445
O3 O3 O2 75.9(6) 6 4_445
O3 O3 O2 134.3(4) 6_554 4_445
O3 O3 O2 115.9(7) 3 4_445
O3 O3 O2 149.1(2) 4 4_445
O2 O3 O2 69.9(4) 2 4_445
O2 O3 O2 83.7(4) 1_554 4_445
O1 O3 O2 26.6(4) 2_455 4_445
O2 O3 O2 27.0(3) . 4_445
O3 O3 O2 74.7(3) 2 4_445
Ga2 O3 O2 56.4(2) 1_554 4_445
O3 O3 O2 121.3(3) 2_554 4_445
Ga3 O3 O2 143.8(5) 1_655 4_445
La O3 O2 29.5(2) 4_445 4_445
Ga2 O3 O2 103.5(3) 2_565 4_445
O2 O3 O2 76.0(3) 5_455 4_445
O3 O3 O2 108.9(5) 5 4_445
O3 O3 O2 162.8(4) 5_554 4_445
Ga3 O3 O2 54.0(2) 4_446 4_445
Nb O3 O2 139.2(3) 1_554 4_445
Ga1 O3 O2 139.2(3) 1_554 4_445
O1 O3 O2 79.8(3) . 4_445
O2 O3 O2 155.8(6) 4_554 4_445
La O3 O2 104.9(3) 1_554 4_445
Ga3 O3 O2 86.4(3) 2_565 4_445
O2 O3 O2 73.29(19) 3_454 4_445
La O3 O2 85.4(3) 2 4_445
O2 O3 O2 107.5(4) 4 4_445
O2 O3 O2 32.1(3) 3_455 4_445
La O3 O2 111.6(3) 2_565 4_445
Ga2 O3 O2 75.8(3) 2 4_445
O2 O3 O2 142.0(3) 5 4_445
O1 O3 O2 112.4(3) 1_554 4_445
Ga3 O3 O2 69.2(2) . 4_445
Ga2 O3 O2 20.42(18) . 4_445
La O3 O2 134.9(3) 4 4_445
O1 O3 O2 54.7(3) 1_545 4_445
O3 O3 O2 120.89(19) 1_554 4_445
O3 O3 O2 59.11(19) 1_556 4_445
O2 O3 O2 132.7(5) 3_554 4_445
Ga3 O3 O2 93.8(3) 1_656 4_445
O2 O3 O2 57.9(2) 4_444 4_445
O2 O3 O2 101.8(4) 2_565 4_445
La O3 O2 82.9(3) 4_444 4_445
O2 O3 O2 99.1(4) 3 4_445
O1 O3 O2 137.1(4) 2_565 4_445
Ga2 O3 O2 71.9(3) 2_566 4_445
Ga3 O3 O1 12.9(4) 4_445 1_544
Nb O3 O1 108.9(5) . 1_544
Ga1 O3 O1 108.9(5) . 1_544
La O3 O1 132.6(4) . 1_544
Ga3 O3 O1 106.8(4) 2_564 1_544
O2 O3 O1 138.9(5) 6 1_544
O3 O3 O1 144.2(8) 6 1_544
O3 O3 O1 74.7(5) 6_554 1_544
O3 O3 O1 64.2(5) 3 1_544
O3 O3 O1 113.0(4) 4 1_544
O2 O3 O1 27.7(4) 2 1_544
O2 O3 O1 39.5(4) 1_554 1_544
O1 O3 O1 80.4(4) 2_455 1_544
O2 O3 O1 100.1(4) . 1_544
O3 O3 O1 90.8(4) 2 1_544
Ga2 O3 O1 63.6(2) 1_554 1_544
O3 O3 O1 33.62(18) 2_554 1_544
Ga3 O3 O1 68.96(19) 1_655 1_544
La O3 O1 61.5(2) 4_445 1_544
Ga2 O3 O1 123.5(3) 2_565 1_544
O2 O3 O1 121.0(4) 5_455 1_544
O3 O3 O1 117.7(2) 5 1_544
O3 O3 O1 75.1(3) 5_554 1_544
Ga3 O3 O1 105.7(4) 4_446 1_544
Nb O3 O1 57.9(2) 1_554 1_544
Ga1 O3 O1 57.9(2) 1_554 1_544
O1 O3 O1 160.2(3) . 1_544
O2 O3 O1 106.2(4) 4_554 1_544
La O3 O1 73.5(2) 1_554 1_544
Ga3 O3 O1 146.1(4) 2_565 1_544
O2 O3 O1 79.7(3) 3_454 1_544
La O3 O1 59.2(2) 2 1_544
O2 O3 O1 152.4(4) 4 1_544
O2 O3 O1 117.5(4) 3_455 1_544
La O3 O1 158.9(4) 2_565 1_544
Ga2 O3 O1 18.71(18) 2 1_544
O2 O3 O1 87.2(3) 5 1_544
O1 O3 O1 104.2(4) 1_554 1_544
Ga3 O3 O1 101.0(2) . 1_544
Ga2 O3 O1 106.1(3) . 1_544
La O3 O1 120.6(2) 4 1_544
O1 O3 O1 59.35(16) 1_545 1_544
O3 O3 O1 55.7(2) 1_554 1_544
O3 O3 O1 124.3(2) 1_556 1_544
O2 O3 O1 53.7(3) 3_554 1_544
Ga3 O3 O1 107.8(3) 1_656 1_544
O2 O3 O1 53.4(3) 4_444 1_544
O2 O3 O1 139.4(4) 2_565 1_544
La O3 O1 27.61(12) 4_444 1_544
O2 O3 O1 88.4(3) 3 1_544
O1 O3 O1 134.8(2) 2_565 1_544
Ga2 O3 O1 159.6(3) 2_566 1_544
O2 O3 O1 87.7(4) 4_445 1_544
Ga3 O3 O3 63.5(5) 4_445 4_445
Nb O3 O3 121.9(6) . 4_445
Ga1 O3 O3 121.9(6) . 4_445
La O3 O3 81.0(2) . 4_445
Ga3 O3 O3 147.4(3) 2_564 4_445
O2 O3 O3 135.8(5) 6 4_445
O3 O3 O3 109.8(6) 6 4_445
O3 O3 O3 108.2(5) 6_554 4_445
O3 O3 O3 101.9(8) 3 4_445
O3 O3 O3 161.9(8) 4 4_445
O2 O3 O3 43.5(5) 2 4_445
O2 O3 O3 52.3(5) 1_554 4_445
O1 O3 O3 30.63(7) 2_455 4_445
O2 O3 O3 56.7(3) . 4_445
O3 O3 O3 86.1(2) 2 4_445
Ga2 O3 O3 37.99(13) 1_554 4_445
O3 O3 O3 86.3(2) 2_554 4_445
Ga3 O3 O3 119.7(5) 1_655 4_445
La O3 O3 21.84(19) 4_445 4_445
Ga2 O3 O3 112.7(3) 2_565 4_445
O2 O3 O3 89.3(3) 5_455 4_445
O3 O3 O3 129.4(3) 5 4_445
O3 O3 O3 127.7(3) 5_554 4_445
Ga3 O3 O3 78.1(2) 4_446 4_445
Nb O3 O3 104.5(3) 1_554 4_445
Ga1 O3 O3 104.5(3) 1_554 4_445
O1 O3 O3 110.9(2) . 4_445
O2 O3 O3 146.5(2) 4_554 4_445
La O3 O3 85.12(14) 1_554 4_445
Ga3 O3 O3 119.72(18) 2_565 4_445
O2 O3 O3 62.7(2) 3_454 4_445
La O3 O3 76.4(4) 2 4_445
O2 O3 O3 142.4(3) 4 4_445
O2 O3 O3 64.2(2) 3_455 4_445
La O3 O3 143.1(3) 2_565 4_445
Ga2 O3 O3 45.9(3) 2 4_445
O2 O3 O3 132.8(5) 5 4_445
O1 O3 O3 108.5(2) 1_554 4_445
Ga3 O3 O3 72.60(15) . 4_445
Ga2 O3 O3 55.73(11) . 4_445
La O3 O3 156.6(4) 4 4_445
O1 O3 O3 49.1(3) 1_545 4_445
O3 O3 O3 90.000(1) 1_554 4_445
O3 O3 O3 90.000(1) 1_556 4_445
O2 O3 O3 104.8(4) 3_554 4_445
Ga3 O3 O3 110.9(3) 1_656 4_445
O2 O3 O3 32.4(2) 4_444 4_445
O2 O3 O3 120.3(4) 2_565 4_445
La O3 O3 48.48(19) 4_444 4_445
O2 O3 O3 104.2(4) 3 4_445
O1 O3 O3 171.3(4) 2_565 4_445
Ga2 O3 O3 106.52(16) 2_566 4_445
O2 O3 O3 35.6(2) 4_445 4_445
O1 O3 O3 53.3(3) 1_544 4_445
Ga3 O3 O3 103.5(4) 4_445 3_455
Nb O3 O3 140.7(4) . 3_455
Ga1 O3 O3 140.7(4) . 3_455
La O3 O3 35.7(3) . 3_455
Ga3 O3 O3 107.5(5) 2_564 3_455
O2 O3 O3 76.3(5) 6 3_455
O3 O3 O3 92.22(5) 6 3_455
O3 O3 O3 92.05(5) 6_554 3_455
O3 O3 O3 161.9(8) 3 3_455
O3 O3 O3 138.1(8) 4 3_455
O2 O3 O3 103.1(5) 2 3_455
O2 O3 O3 68.7(3) 1_554 3_455
O1 O3 O3 30.63(7) 2_455 3_455
O2 O3 O3 71.0(3) . 3_455
O3 O3 O3 122.0(2) 2 3_455
Ga2 O3 O3 37.99(13) 1_554 3_455
O3 O3 O3 120.1(3) 2_554 3_455
Ga3 O3 O3 158.6(2) 1_655 3_455
La O3 O3 72.26(17) 4_445 3_455
Ga2 O3 O3 56.0(3) 2_565 3_455
O2 O3 O3 29.7(3) 5_455 3_455
O3 O3 O3 135.8(3) 5 3_455
O3 O3 O3 133.7(3) 5_554 3_455
Ga3 O3 O3 96.23(16) 4_446 3_455
Nb O3 O3 111.55(18) 1_554 3_455
Ga1 O3 O3 111.55(18) 1_554 3_455
O1 O3 O3 58.9(3) . 3_455
O2 O3 O3 107.0(5) 4_554 3_455
La O3 O3 63.73(17) 1_554 3_455
Ga3 O3 O3 100.2(2) 2_565 3_455
O2 O3 O3 33.0(3) 3_454 3_455
La O3 O3 133.5(4) 2 3_455
O2 O3 O3 106.2(4) 4 3_455
O2 O3 O3 37.3(3) 3_455 3_455
La O3 O3 86.1(3) 2_565 3_455
Ga2 O3 O3 103.2(3) 2 3_455
O2 O3 O3 166.5(5) 5 3_455
O1 O3 O3 62.6(2) 1_554 3_455
Ga3 O3 O3 19.68(16) . 3_455
Ga2 O3 O3 55.73(11) . 3_455
La O3 O3 136.7(4) 4 3_455
O1 O3 O3 102.4(3) 1_545 3_455
O3 O3 O3 90.0 1_554 3_455
O3 O3 O3 89.999(1) 1_556 3_455
O2 O3 O3 149.8(3) 3_554 3_455
Ga3 O3 O3 132.17(14) 1_656 3_455
O2 O3 O3 48.0(3) 4_444 3_455
O2 O3 O3 60.4(4) 2_565 3_455
La O3 O3 77.43(15) 4_444 3_455
O2 O3 O3 146.3(3) 3 3_455
O1 O3 O3 112.2(4) 2_565 3_455
Ga2 O3 O3 65.6(2) 2_566 3_455
O2 O3 O3 49.87(19) 4_445 3_455
O1 O3 O3 101.3(2) 1_544 3_455
O3 O3 O3 60.0 4_445 3_455
Ga3 O3 Ga2 108.0(5) 4_445 1_664
Nb O3 Ga2 74.2(4) . 1_664
Ga1 O3 Ga2 74.2(4) . 1_664
La O3 Ga2 99.7(4) . 1_664
Ga3 O3 Ga2 16.48(16) 2_564 1_664
O2 O3 Ga2 36.3(4) 6 1_664
O3 O3 Ga2 84.0(7) 6 1_664
O3 O3 Ga2 56.0(5) 6_554 1_664
O3 O3 Ga2 86.0(5) 3 1_664
O3 O3 Ga2 29.6(4) 4 1_664
O2 O3 Ga2 138.9(5) 2 1_664
O2 O3 Ga2 111.9(5) 1_554 1_664
O1 O3 Ga2 142.0(4) 2_455 1_664
O2 O3 Ga2 137.2(4) . 1_664
O3 O3 Ga2 110.22(13) 2 1_664
Ga2 O3 Ga2 126.0(4) 1_554 1_664
O3 O3 Ga2 86.6(2) 2_554 1_664
Ga3 O3 Ga2 62.3(2) 1_655 1_664
La O3 Ga2 174.9(3) 4_445 1_664
Ga2 O3 Ga2 55.74(19) 2_565 1_664
O2 O3 Ga2 81.9(3) 5_455 1_664
O3 O3 Ga2 67.2(3) 5 1_664
O3 O3 Ga2 45.90(15) 5_554 1_664
Ga3 O3 Ga2 118.3(3) 4_446 1_664
Nb O3 Ga2 63.7(2) 1_554 1_664
Ga1 O3 Ga2 63.7(2) 1_554 1_664
O1 O3 Ga2 71.2(2) . 1_664
O2 O3 Ga2 17.4(2) 4_554 1_664
La O3 Ga2 78.1(2) 1_554 1_664
Ga3 O3 Ga2 74.8(2) 2_565 1_664
O2 O3 Ga2 101.9(3) 3_454 1_664
La O3 Ga2 114.8(2) 2 1_664
O2 O3 Ga2 51.5(3) 4 1_664
O2 O3 Ga2 119.0(3) 3_455 1_664
La O3 Ga2 39.70(12) 2_565 1_664
Ga2 O3 Ga2 133.2(3) 2 1_664
O2 O3 Ga2 55.1(2) 5 1_664
O1 O3 Ga2 56.08(17) 1_554 1_664
Ga3 O3 Ga2 95.5(3) . 1_664
Ga2 O3 Ga2 133.8(3) . 1_664
La O3 Ga2 39.22(11) 4 1_664
O1 O3 Ga2 144.9(3) 1_545 1_664
O3 O3 Ga2 75.06(13) 1_554 1_664
O3 O3 Ga2 104.94(13) 1_556 1_664
O2 O3 Ga2 75.4(2) 3_554 1_664
Ga3 O3 Ga2 85.59(19) 1_656 1_664
O2 O3 Ga2 130.8(3) 4_444 1_664
O2 O3 Ga2 52.3(2) 2_565 1_664
La O3 Ga2 117.5(3) 4_444 1_664
O2 O3 Ga2 90.3(3) 3 1_664
O1 O3 Ga2 18.8(2) 2_565 1_664
Ga2 O3 Ga2 80.10(19) 2_566 1_664
O2 O3 Ga2 151.0(4) 4_445 1_664
O1 O3 Ga2 120.1(3) 1_544 1_664
O3 O3 Ga2 163.2(2) 4_445 1_664
O3 O3 Ga2 111.4(4) 3_455 1_664
Ga3 O3 O2 165.4(7) 4_445 6_556
Nb O3 O2 58.7(3) . 6_556
Ga1 O3 O2 58.7(3) . 6_556
La O3 O2 47.5(3) . 6_556
Ga3 O3 O2 96.1(4) 2_564 6_556
O2 O3 O2 67.2(4) 6 6_556
O3 O3 O2 11.5(3) 6 6_556
O3 O3 O2 131.2(8) 6_554 6_556
O3 O3 O2 105.1(2) 3 6_556
O3 O3 O2 76.5(4) 4 6_556
O2 O3 O2 126.1(6) 2 6_556
O2 O3 O2 151.8(5) 1_554 6_556
O1 O3 O2 92.2(4) 2_455 6_556
O2 O3 O2 56.7(5) . 6_556
O3 O3 O2 65.7(4) 2 6_556
Ga2 O3 O2 119.1(3) 1_554 6_556
O3 O3 O2 156.4(4) 2_554 6_556
Ga3 O3 O2 114.1(3) 1_655 6_556
La O3 O2 96.4(3) 4_445 6_556
Ga2 O3 O2 80.5(3) 2_565 6_556
O2 O3 O2 74.7(3) 5_455 6_556
O3 O3 O2 52.6(3) 5 6_556
O3 O3 O2 120.3(4) 5_554 6_556
Ga3 O3 O2 48.2(2) 4_446 6_556
Nb O3 O2 144.3(4) 1_554 6_556
Ga1 O3 O2 144.3(4) 1_554 6_556
O1 O3 O2 35.1(3) . 6_556
O2 O3 O2 96.8(5) 4_554 6_556
La O3 O2 129.8(4) 1_554 6_556
Ga3 O3 O2 16.98(17) 2_565 6_556
O2 O3 O2 113.3(3) 3_454 6_556
La O3 O2 98.9(3) 2 6_556
O2 O3 O2 32.2(4) 4 6_556
O2 O3 O2 53.2(2) 3_455 6_556
La O3 O2 45.9(3) 2_565 6_556
Ga2 O3 O2 135.1(4) 2 6_556
O2 O3 O2 93.8(3) 5 6_556
O1 O3 O2 100.7(3) 1_554 6_556
Ga3 O3 O2 91.8(2) . 6_556
Ga2 O3 O2 55.1(2) . 6_556
La O3 O2 64.2(2) 4 6_556
O1 O3 O2 94.5(4) 1_545 6_556
O3 O3 O2 150.4(3) 1_554 6_556
O3 O3 O2 29.6(3) 1_556 6_556
O2 O3 O2 126.8(4) 3_554 6_556
Ga3 O3 O2 54.7(2) 1_656 6_556
O2 O3 O2 126.7(3) 4_444 6_556
O2 O3 O2 65.1(2) 2_565 6_556
La O3 O2 157.2(3) 4_444 6_556
O2 O3 O2 74.9(3) 3 6_556
O1 O3 O2 62.9(4) 2_565 6_556
Ga2 O3 O2 19.85(17) 2_566 6_556
O2 O3 O2 75.5(2) 4_445 6_556
O1 O3 O2 153.8(5) 1_544 6_556
O3 O3 O2 110.9(2) 4_445 6_556
O3 O3 O2 83.2(2) 3_455 6_556
Ga2 O3 O2 80.7(3) 1_664 6_556
Ga3 O3 O2 46.7(4) 4_445 5_445
Nb O3 O2 102.5(5) . 5_445
Ga1 O3 O2 102.5(5) . 5_445
La O3 O2 107.5(5) . 5_445
Ga3 O3 O2 140.7(4) 2_564 5_445
O2 O3 O2 161.9(5) 6 5_445
O3 O3 O2 115.0(8) 6 5_445
O3 O3 O2 106.5(6) 6_554 5_445
O3 O3 O2 73.2(6) 3 5_445
O3 O3 O2 133.1(6) 4 5_445
O2 O3 O2 14.7(6) 2 5_445
O2 O3 O2 56.7(5) 1_554 5_445
O1 O3 O2 59.5(4) 2_455 5_445
O2 O3 O2 66.2(4) . 5_445
O3 O3 O2 70.8(3) 2 5_445
Ga2 O3 O2 60.3(3) 1_554 5_445
O3 O3 O2 66.5(3) 2_554 5_445
Ga3 O3 O2 91.9(3) 1_655 5_445
La O3 O2 28.2(2) 4_445 5_445
Ga2 O3 O2 137.5(4) 2_565 5_445
O2 O3 O2 117.6(5) 5_455 5_445
O3 O3 O2 111.7(2) 5 5_445
O3 O3 O2 106.4(3) 5_554 5_445
Ga3 O3 O2 75.9(3) 4_446 5_445
Nb O3 O2 91.8(3) 1_554 5_445
Ga1 O3 O2 91.8(3) 1_554 5_445
O1 O3 O2 136.5(4) . 5_445
O2 O3 O2 140.1(3) 4_554 5_445
La O3 O2 95.5(3) 1_554 5_445
Ga3 O3 O2 121.6(3) 2_565 5_445
O2 O3 O2 84.5(3) 3_454 5_445
La O3 O2 50.6(2) 2 5_445
O2 O3 O2 142.5(3) 4 5_445
O2 O3 O2 88.6(4) 3_455 5_445
La O3 O2 167.2(3) 2_565 5_445
Ga2 O3 O2 19.1(2) 2 5_445
O2 O3 O2 103.9(4) 5 5_445
O1 O3 O2 125.7(3) 1_554 5_445
Ga3 O3 O2 99.3(3) . 5_445
Ga2 O3 O2 73.0(3) . 5_445
La O3 O2 132.0(3) 4 5_445
O1 O3 O2 31.9(2) 1_545 5_445
O3 O3 O2 86.6(2) 1_554 5_445
O3 O3 O2 93.4(2) 1_556 5_445
O2 O3 O2 77.8(3) 3_554 5_445
Ga3 O3 O2 94.8(3) 1_656 5_445
O2 O3 O2 51.1(4) 4_444 5_445
O2 O3 O2 148.4(3) 2_565 5_445
La O3 O2 46.7(2) 4_444 5_445
O2 O3 O2 81.5(3) 3 5_445
O1 O3 O2 159.1(3) 2_565 5_445
Ga2 O3 O2 126.7(3) 2_566 5_445
O2 O3 O2 56.7(5) 4_445 5_445
O1 O3 O2 33.9(2) 1_544 5_445
O3 O3 O2 28.9(3) 4_445 5_445
O3 O3 O2 88.8(3) 3_455 5_445
Ga2 O3 O2 152.3(3) 1_664 5_445
O2 O3 O2 121.8(4) 6_556 5_445
Ga3 O3 La 97.6(4) 4_445 2_455
Nb O3 La 128.9(5) . 2_455
Ga1 O3 La 128.9(5) . 2_455
La O3 La 42.2(2) . 2_455
Ga3 O3 La 132.6(4) 2_564 2_455
O2 O3 La 99.3(4) 6 2_455
O3 O3 La 88.1(4) 6 2_455
O3 O3 La 111.1(2) 6_554 2_455
O3 O3 La 138.5(7) 3 2_455
O3 O3 La 156.4(6) 4 2_455
O2 O3 La 83.0(5) 2 2_455
O2 O3 La 70.3(4) 1_554 2_455
O1 O3 La 10.1(2) 2_455 2_455
O2 O3 La 50.3(3) . 2_455
O3 O3 La 100.1(3) 2 2_455
Ga2 O3 La 37.89(14) 1_554 2_455
O3 O3 La 119.5(2) 2_554 2_455
Ga3 O3 La 159.2(4) 1_655 2_455
La O3 La 47.77(14) 4_445 2_455
Ga2 O3 La 80.79(19) 2_565 2_455
O2 O3 La 53.7(3) 5_455 2_455
O3 O3 La 129.1(5) 5 2_455
O3 O3 La 151.6(5) 5_554 2_455
Ga3 O3 La 77.4(2) 4_446 2_455
Nb O3 La 124.2(3) 1_554 2_455
Ga1 O3 La 124.2(3) 1_554 2_455
O1 O3 La 71.68(17) . 2_455
O2 O3 La 132.0(4) 4_554 2_455
La O3 La 81.27(18) 1_554 2_455
Ga3 O3 La 98.2(2) 2_565 2_455
O2 O3 La 48.9(2) 3_454 2_455
La O3 La 108.6(3) 2 2_455
O2 O3 La 113.4(4) 4 2_455
O2 O3 La 29.8(3) 3_455 2_455
La O3 La 103.4(2) 2_565 2_455
Ga2 O3 La 85.7(2) 2 2_455
O2 O3 La 167.6(4) 5 2_455
O1 O3 La 87.05(19) 1_554 2_455
Ga3 O3 La 43.81(10) . 2_455
Ga2 O3 La 37.48(10) . 2_455
La O3 La 147.0(2) 4 2_455
O1 O3 La 77.4(2) 1_545 2_455
O3 O3 La 102.56(13) 1_554 2_455
O3 O3 La 77.44(13) 1_556 2_455
O2 O3 La 144.0(4) 3_554 2_455
Ga3 O3 La 117.1(3) 1_656 2_455
O2 O3 La 43.8(2) 4_444 2_455
O2 O3 La 83.2(3) 2_565 2_455
La O3 La 74.38(16) 4_444 2_455
O2 O3 La 124.7(3) 3 2_455
O1 O3 La 131.5(3) 2_565 2_455
Ga2 O3 La 71.16(14) 2_566 2_455
O2 O3 La 25.65(18) 4_445 2_455
O1 O3 La 90.5(2) 1_544 2_455
O3 O3 La 39.85(12) 4_445 2_455
O3 O3 La 25.06(10) 3_455 2_455
Ga2 O3 La 135.4(3) 1_664 2_455
O2 O3 La 83.0(2) 6_556 2_455
O2 O3 La 68.3(3) 5_445 2_455
Ga3 O3 O2 43.7(4) 4_445 6_545
Nb O3 O2 78.7(4) . 6_545
Ga1 O3 O2 78.7(4) . 6_545
La O3 O2 132.5(5) . 6_545
Ga3 O3 O2 121.3(4) 2_564 6_545
O2 O3 O2 161.7(6) 6 6_545
O3 O3 O2 110.9(6) 6 6_545
O3 O3 O2 102.9(5) 6_554 6_545
O3 O3 O2 43.0(5) 3 6_545
O3 O3 O2 102.9(5) 4 6_545
O2 O3 O2 16.2(6) 2 6_545
O2 O3 O2 72.3(4) 1_554 6_545
O1 O3 O2 89.5(4) 2_455 6_545
O2 O3 O2 79.5(4) . 6_545
O3 O3 O2 56.8(4) 2 6_545
Ga2 O3 O2 87.7(3) 1_554 6_545
O3 O3 O2 52.6(4) 2_554 6_545
Ga3 O3 O2 63.7(3) 1_655 6_545
La O3 O2 52.1(3) 4_445 6_545
Ga2 O3 O2 157.5(3) 2_565 6_545
O2 O3 O2 147.4(4) 5_455 6_545
O3 O3 O2 88.14(19) 5 6_545
O3 O3 O2 84.0(2) 5_554 6_545
Ga3 O3 O2 74.9(3) 4_446 6_545
Nb O3 O2 80.5(3) 1_554 6_545
Ga1 O3 O2 80.5(3) 1_554 6_545
O1 O3 O2 153.8(5) . 6_545
O2 O3 O2 121.3(3) 4_554 6_545
La O3 O2 107.4(3) 1_554 6_545
Ga3 O3 O2 112.0(3) 2_565 6_545
O2 O3 O2 109.6(4) 3_454 6_545
La O3 O2 25.83(16) 2 6_545
O2 O3 O2 123.9(3) 4 6_545
O2 O3 O2 112.6(4) 3_455 6_545
La O3 O2 152.7(3) 2_565 6_545
Ga2 O3 O2 19.42(16) 2 6_545
O2 O3 O2 73.7(4) 5 6_545
O1 O3 O2 137.5(3) 1_554 6_545
Ga3 O3 O2 127.9(3) . 6_545
Ga2 O3 O2 92.0(3) . 6_545
La O3 O2 102.7(2) 4 6_545
O1 O3 O2 32.1(2) 1_545 6_545
O3 O3 O2 86.6(2) 1_554 6_545
O3 O3 O2 93.4(2) 1_556 6_545
O2 O3 O2 51.37(18) 3_554 6_545
Ga3 O3 O2 74.9(2) 1_656 6_545
O2 O3 O2 77.6(4) 4_444 6_545
O2 O3 O2 173.2(4) 2_565 6_545
La O3 O2 60.2(2) 4_444 6_545
O2 O3 O2 57.1(2) 3 6_545
O1 O3 O2 128.8(3) 2_565 6_545
Ga2 O3 O2 137.4(3) 2_566 6_545
O2 O3 O2 81.3(4) 4_445 6_545
O1 O3 O2 34.0(2) 1_544 6_545
O3 O3 O2 59.1(4) 4_445 6_545
O3 O3 O2 119.0(4) 3_455 6_545
Ga2 O3 O2 126.0(3) 1_664 6_545
O2 O3 O2 121.8(4) 6_556 6_545
O2 O3 O2 30.2(2) 5_445 6_545
La O3 O2 97.8(3) 2_455 6_545
Ga3 O3 O2 106.1(6) 4_445 2_556
Nb O3 O2 57.6(4) . 2_556
Ga1 O3 O2 57.6(4) . 2_556
La O3 O2 78.3(4) . 2_556
Ga3 O3 O2 143.8(4) 2_564 2_556
O2 O3 O2 127.1(5) 6 2_556
O3 O3 O2 51.3(6) 6 2_556
O3 O3 O2 167.0(5) 6_554 2_556
O3 O3 O2 74.8(4) 3 2_556
O3 O3 O2 104.1(3) 4 2_556
O2 O3 O2 66.3(4) 2 2_556
O2 O3 O2 118.6(7) 1_554 2_556
O1 O3 O2 75.9(5) 2_455 2_556
O2 O3 O2 25.7(4) . 2_556
O3 O3 O2 25.5(3) 2 2_556
Ga2 O3 O2 103.0(4) 1_554 2_556
O3 O3 O2 116.2(5) 2_554 2_556
Ga3 O3 O2 103.0(3) 1_655 2_556
La O3 O2 46.8(3) 4_445 2_556
Ga2 O3 O2 135.2(3) 2_565 2_556
O2 O3 O2 114.2(4) 5_455 2_556
O3 O3 O2 62.6(3) 5 2_556
O3 O3 O2 129.6(4) 5_554 2_556
Ga3 O3 O2 11.9(2) 4_446 2_556
Nb O3 O2 142.8(4) 1_554 2_556
Ga1 O3 O2 142.8(4) 1_554 2_556
O1 O3 O2 89.6(4) . 2_556
O2 O3 O2 144.8(3) 4_554 2_556
La O3 O2 152.9(4) 1_554 2_556
Ga3 O3 O2 57.6(2) 2_565 2_556
O2 O3 O2 122.9(3) 3_454 2_556
La O3 O2 49.4(2) 2 2_556
O2 O3 O2 79.9(3) 4 2_556
O2 O3 O2 63.1(3) 3_455 2_556
La O3 O2 104.8(3) 2_565 2_556
Ga2 O3 O2 75.3(3) 2 2_556
O2 O3 O2 93.3(3) 5 2_556
O1 O3 O2 154.4(3) 1_554 2_556
Ga3 O3 O2 116.1(3) . 2_556
Ga2 O3 O2 41.3(2) . 2_556
La O3 O2 91.0(3) 4 2_556
O1 O3 O2 34.6(3) 1_545 2_556
O3 O3 O2 149.7(2) 1_554 2_556
O3 O3 O2 30.3(2) 1_556 2_556
O2 O3 O2 101.4(4) 3_554 2_556
Ga3 O3 O2 45.2(2) 1_656 2_556
O2 O3 O2 100.4(3) 4_444 2_556
O2 O3 O2 122.3(3) 2_565 2_556
La O3 O2 110.3(3) 4_444 2_556
O2 O3 O2 50.2(4) 3 2_556
O1 O3 O2 110.7(3) 2_565 2_556
Ga2 O3 O2 73.1(2) 2_566 2_556
O2 O3 O2 49.6(2) 4_445 2_556
O1 O3 O2 94.0(3) 1_544 2_556
O3 O3 O2 68.4(3) 4_445 2_556
O3 O3 O2 96.6(2) 3_455 2_556
Ga2 O3 O2 128.3(3) 1_664 2_556
O2 O3 O2 59.9(4) 6_556 2_556
O2 O3 O2 64.1(2) 5_445 2_556
La O3 O2 74.8(3) 2_455 2_556
O2 O3 O2 64.3(3) 6_545 2_556
Ga3 O3 O1 47.9(3) 4_445 2_454
Nb O3 O1 157.7(5) . 2_454
Ga1 O3 O1 157.7(5) . 2_454
La O3 O1 96.6(3) . 2_454
Ga3 O3 O1 86.0(3) 2_564 2_454
O2 O3 O1 93.1(4) 6 2_454
O3 O3 O1 153.47(15) 6 2_454
O3 O3 O1 47.7(4) 6_554 2_454
O3 O3 O1 111.7(3) 3 2_454
O3 O3 O1 122.7(2) 4 2_454
O2 O3 O1 75.3(4) 2 2_454
O2 O3 O1 14.5(4) 1_554 2_454
O1 O3 O1 63.0(3) 2_455 2_454
O2 O3 O1 114.6(4) . 2_454
O3 O3 O1 141.0(3) 2 2_454
Ga2 O3 O1 32.00(17) 1_554 2_454
O3 O3 O1 59.0(4) 2_554 2_454
Ga3 O3 O1 98.7(3) 1_655 2_454
La O3 O1 82.9(2) 4_445 2_454
Ga2 O3 O1 71.70(19) 2_565 2_454
O2 O3 O1 69.6(3) 5_455 2_454
O3 O3 O1 161.4(5) 5 2_454
O3 O3 O1 82.5(4) 5_554 2_454
Ga3 O3 O1 139.3(3) 4_446 2_454
Nb O3 O1 54.85(17) 1_554 2_454
Ga1 O3 O1 54.85(17) 1_554 2_454
O1 O3 O1 110.4(3) . 2_454
O2 O3 O1 85.1(3) 4_554 2_454
La O3 O1 25.28(9) 1_554 2_454
Ga3 O3 O1 159.3(3) 2_565 2_454
O2 O3 O1 30.0(2) 3_454 2_454
La O3 O1 112.3(3) 2 2_454
O2 O3 O1 146.8(4) 4 2_454
O2 O3 O1 96.4(3) 3_455 2_454
La O3 O1 116.8(3) 2_565 2_454
Ga2 O3 O1 68.09(16) 2 2_454
O2 O3 O1 118.1(3) 5 2_454
O1 O3 O1 55.56(17) 1_554 2_454
Ga3 O3 O1 51.52(13) . 2_454
Ga2 O3 O1 105.9(2) . 2_454
La O3 O1 136.9(3) 4 2_454
O1 O3 O1 102.3(3) 1_545 2_454
O3 O3 O1 33.51(16) 1_554 2_454
O3 O3 O1 146.49(16) 1_556 2_454
O2 O3 O1 88.5(3) 3_554 2_454
Ga3 O3 O1 161.0(3) 1_656 2_454
O2 O3 O1 30.6(2) 4_444 2_454
O2 O3 O1 87.3(3) 2_565 2_454
La O3 O1 26.46(6) 4_444 2_454
O2 O3 O1 141.0(3) 3 2_454
O1 O3 O1 119.4(3) 2_565 2_454
Ga2 O3 O1 123.7(2) 2_566 2_454
O2 O3 O1 87.9(2) 4_445 2_454
O1 O3 O1 53.30(15) 1_544 2_454
O3 O3 O1 61.43(13) 4_445 2_454
O3 O3 O1 61.43(13) 3_455 2_454
Ga2 O3 O1 101.9(2) 1_664 2_454
O2 O3 O1 143.2(3) 6_556 2_454
O2 O3 O1 70.4(2) 5_445 2_454
La O3 O1 69.38(17) 2_455 2_454
O2 O3 O1 86.7(2) 6_545 2_454
O2 O3 O1 129.7(3) 2_556 2_454
Ga3 O3 La 18.7(3) 4_445 2_554
Nb O3 La 95.6(4) . 2_554
Ga1 O3 La 95.6(4) . 2_554
La O3 La 156.7(4) . 2_554
Ga3 O3 La 83.8(3) 2_564 2_554
O2 O3 La 122.2(5) 6 2_554
O3 O3 La 143.4(3) 6 2_554
O3 O3 La 60.7(4) 6_554 2_554
O3 O3 La 49.1(3) 3 2_554
O3 O3 La 87.2(3) 4 2_554
O2 O3 La 46.6(4) 2 2_554
O2 O3 La 53.0(3) 1_554 2_554
O1 O3 La 106.0(4) 2_455 2_554
O2 O3 La 121.0(4) . 2_554
O3 O3 La 92.6(5) 2 2_554
Ga2 O3 La 84.1(2) 1_554 2_554
O3 O3 La 10.1(3) 2_554 2_554
Ga3 O3 La 44.11(13) 1_655 2_554
La O3 La 85.8(2) 4_445 2_554
Ga2 O3 La 118.0(3) 2_565 2_554
O2 O3 La 130.2(4) 5_455 2_554
O3 O3 La 102.2(3) 5 2_554
O3 O3 La 49.2(2) 5_554 2_554
Ga3 O3 La 116.0(3) 4_446 2_554
Nb O3 La 38.05(10) 1_554 2_554
Ga1 O3 La 38.05(10) 1_554 2_554
O1 O3 La 163.5(4) . 2_554
O2 O3 La 83.4(3) 4_554 2_554
La O3 La 72.94(17) 1_554 2_554
Ga3 O3 La 137.6(3) 2_565 2_554
O2 O3 La 92.5(3) 3_454 2_554
La O3 La 59.64(15) 2 2_554
O2 O3 La 130.1(4) 4 2_554
O2 O3 La 143.9(4) 3_455 2_554
La O3 La 134.6(3) 2_565 2_554
Ga2 O3 La 38.91(10) 2 2_554
O2 O3 La 63.8(2) 5 2_554
O1 O3 La 97.7(3) 1_554 2_554
Ga3 O3 La 114.0(2) . 2_554
Ga2 O3 La 130.5(3) . 2_554
La O3 La 96.45(19) 4 2_554
O1 O3 La 74.4(2) 1_545 2_554
O3 O3 La 46.77(15) 1_554 2_554
O3 O3 La 133.23(15) 1_556 2_554
O2 O3 La 29.5(2) 3_554 2_554
Ga3 O3 La 99.7(2) 1_656 2_554
O2 O3 La 75.0(3) 4_444 2_554
O2 O3 La 131.1(3) 2_565 2_554
La O3 La 44.30(10) 4_444 2_554
O2 O3 La 79.7(2) 3 2_554
O1 O3 La 108.5(3) 2_565 2_554
Ga2 O3 La 172.6(3) 2_566 2_554
O2 O3 La 113.7(4) 4_445 2_554
O1 O3 La 26.42(10) 1_544 2_554
O3 O3 La 79.7(3) 4_445 2_554
O3 O3 La 121.53(19) 3_455 2_554
Ga2 O3 La 94.9(2) 1_664 2_554
O2 O3 La 154.2(3) 6_556 2_554
O2 O3 La 57.6(2) 5_445 2_554
La O3 La 116.0(2) 2_455 2_554
O2 O3 La 42.5(2) 6_545 2_554
O2 O3 La 106.4(3) 2_556 2_554
O1 O3 La 62.54(14) 2_454 2_554
Ga3 O3 O3 33.1(3) 4_445 3_554
Nb O3 O3 102.5(5) . 3_554
Ga1 O3 O3 102.5(5) . 3_554
La O3 O3 148.6(4) . 3_554
Ga3 O3 O3 61.5(2) 2_564 3_554
O2 O3 O3 98.2(5) 6 3_554
O3 O3 O3 148.8(5) 6 3_554
O3 O3 O3 37.3(3) 6_554 3_554
O3 O3 O3 61.89(18) 3 3_554
O3 O3 O3 76.37(8) 4 3_554
O2 O3 O3 69.9(4) 2 3_554
O2 O3 O3 52.7(4) 1_554 3_554
O1 O3 O3 114.4(5) 2_455 3_554
O2 O3 O3 144.7(5) . 3_554
O3 O3 O3 111.9(5) 2 3_554
Ga2 O3 O3 85.5(3) 1_554 3_554
O3 O3 O3 14.1(2) 2_554 3_554
Ga3 O3 O3 42.9(2) 1_655 3_554
La O3 O3 106.9(4) 4_445 3_554
Ga2 O3 O3 95.1(2) 2_565 3_554
O2 O3 O3 112.8(3) 5_455 3_554
O3 O3 O3 105.8(5) 5 3_554
O3 O3 O3 32.6(3) 5_554 3_554
Ga3 O3 O3 138.0(4) 4_446 3_554
Nb O3 O3 13.90(8) 1_554 3_554
Ga1 O3 O3 13.90(8) 1_554 3_554
O1 O3 O3 139.3(4) . 3_554
O2 O3 O3 61.0(3) 4_554 3_554
La O3 O3 56.13(12) 1_554 3_554
Ga3 O3 O3 138.7(4) 2_565 3_554
O2 O3 O3 83.7(3) 3_454 3_554
La O3 O3 81.0(3) 2 3_554
O2 O3 O3 120.7(4) 4 3_554
O2 O3 O3 152.0(4) 3_455 3_554
La O3 O3 113.6(3) 2_565 3_554
Ga2 O3 O3 61.6(2) 2 3_554
O2 O3 O3 62.5(3) 5 3_554
O1 O3 O3 75.4(2) 1_554 3_554
Ga3 O3 O3 102.2(2) . 3_554
Ga2 O3 O3 151.0(4) . 3_554
La O3 O3 89.1(3) 4 3_554
O1 O3 O3 98.6(3) 1_545 3_554
O3 O3 O3 28.11(18) 1_554 3_554
O3 O3 O3 151.89(18) 1_556 3_554
O2 O3 O3 34.6(3) 3_554 3_554
Ga3 O3 O3 110.9(3) 1_656 3_554
O2 O3 O3 79.3(3) 4_444 3_554
O2 O3 O3 107.2(3) 2_565 3_554
La O3 O3 49.8(2) 4_444 3_554
O2 O3 O3 93.3(3) 3 3_554
O1 O3 O3 91.4(3) 2_565 3_554
Ga2 O3 O3 153.7(4) 2_566 3_554
O2 O3 O3 131.2(4) 4_445 3_554
O1 O3 O3 45.4(2) 1_544 3_554
O3 O3 O3 95.6(4) 4_445 3_554
O3 O3 O3 116.6(2) 3_455 3_554
Ga2 O3 O3 74.9(2) 1_664 3_554
O2 O3 O3 152.9(4) 6_556 3_554
O2 O3 O3 79.2(3) 5_445 3_554
La O3 O3 123.0(3) 2_455 3_554
O2 O3 O3 66.6(3) 6_545 3_554
O2 O3 O3 129.7(4) 2_556 3_554
O1 O3 O3 55.8(2) 2_454 3_554
La O3 O3 24.15(16) 2_554 3_554
Ga3 O3 O3 116.0(6) 4_445 3_556
Nb O3 O3 30.4(3) . 3_556
Ga1 O3 O3 30.4(3) . 3_556
La O3 O3 87.6(3) . 3_556
Ga3 O3 O3 116.1(4) 2_564 3_556
O2 O3 O3 110.5(4) 6 3_556
O3 O3 O3 38.5(4) 6 3_556
O3 O3 O3 149.6(5) 6_554 3_556
O3 O3 O3 61.89(18) 3 3_556
O3 O3 O3 76.37(8) 4 3_556
O2 O3 O3 81.9(6) 2 3_556
O2 O3 O3 141.8(6) 1_554 3_556
O1 O3 O3 102.3(5) 2_455 3_556
O2 O3 O3 49.2(4) . 3_556
O3 O3 O3 16.2(3) 2 3_556
Ga2 O3 O3 130.7(5) 1_554 3_556
O3 O3 O3 114.5(6) 2_554 3_556
Ga3 O3 O3 84.8(3) 1_655 3_556
La O3 O3 73.8(3) 4_445 3_556
Ga2 O3 O3 129.5(3) 2_565 3_556
O2 O3 O3 122.2(3) 5_455 3_556
O3 O3 O3 34.8(3) 5 3_556
O3 O3 O3 108.3(5) 5_554 3_556
Ga3 O3 O3 21.86(15) 4_446 3_556
Nb O3 O3 131.6(3) 1_554 3_556
Ga1 O3 O3 131.6(3) 1_554 3_556
O1 O3 O3 84.9(3) . 3_556
O2 O3 O3 117.1(4) 4_554 3_556
La O3 O3 179.3(5) 1_554 3_556
Ga3 O3 O3 39.33(9) 2_565 3_556
O2 O3 O3 148.0(4) 3_454 3_556
La O3 O3 49.1(2) 2 3_556
O2 O3 O3 57.4(2) 4 3_556
O2 O3 O3 79.4(3) 3_455 3_556
La O3 O3 86.7(2) 2_565 3_556
Ga2 O3 O3 89.9(3) 2 3_556
O2 O3 O3 69.9(3) 5 3_556
O1 O3 O3 148.0(4) 1_554 3_556
Ga3 O3 O3 133.7(3) . 3_556
Ga2 O3 O3 62.3(2) . 3_556
La O3 O3 63.26(19) 4 3_556
O1 O3 O3 53.3(3) 1_545 3_556
O3 O3 O3 151.89(18) 1_554 3_556
O3 O3 O3 28.11(18) 1_556 3_556
O2 O3 O3 89.4(3) 3_554 3_556
Ga3 O3 O3 18.12(14) 1_656 3_556
O2 O3 O3 127.9(5) 4_444 3_556
O2 O3 O3 113.6(3) 2_565 3_556
La O3 O3 130.9(4) 4_444 3_556
O2 O3 O3 30.7(2) 3 3_556
O1 O3 O3 84.7(3) 2_565 3_556
Ga2 O3 O3 68.78(13) 2_566 3_556
O2 O3 O3 75.7(3) 4_445 3_556
O1 O3 O3 107.0(4) 1_544 3_556
O3 O3 O3 95.6(4) 4_445 3_556
O3 O3 O3 116.6(2) 3_455 3_556
Ga2 O3 O3 101.2(3) 1_664 3_556
O2 O3 O3 49.9(2) 6_556 3_556
O2 O3 O3 85.2(4) 5_445 3_556
La O3 O3 99.3(3) 2_455 3_556
O2 O3 O3 73.0(3) 6_545 3_556
O2 O3 O3 27.8(3) 2_556 3_556
O1 O3 O3 155.4(4) 2_454 3_556
La O3 O3 107.2(3) 2_554 3_556
O3 O3 O3 123.8(4) 3_554 3_556
Ga3 O3 O3 59.0(3) 4_445 4_554
Nb O3 O3 102.5(5) . 4_554
Ga1 O3 O3 102.5(5) . 4_554
La O3 O3 129.9(6) . 4_554
Ga3 O3 O3 35.3(3) 2_564 4_554
O2 O3 O3 71.1(5) 6 4_554
O3 O3 O3 133.6(8) 6 4_554
O3 O3 O3 18.5(3) 6_554 4_554
O3 O3 O3 76.37(8) 3 4_554
O3 O3 O3 61.89(18) 4 4_554
O2 O3 O3 97.2(4) 2 4_554
O2 O3 O3 65.6(4) 1_554 4_554
O1 O3 O3 123.9(4) 2_455 4_554
O2 O3 O3 171.9(5) . 4_554
O3 O3 O3 127.0(5) 2 4_554
Ga2 O3 O3 93.1(3) 1_554 4_554
O3 O3 O3 41.1(3) 2_554 4_554
Ga3 O3 O3 48.85(19) 1_655 4_554
La O3 O3 132.4(3) 4_445 4_554
Ga2 O3 O3 71.4(3) 2_565 4_554
O2 O3 O3 94.5(4) 5_455 4_554
O3 O3 O3 101.3(5) 5 4_554
O3 O3 O3 23.6(3) 5_554 4_554
Ga3 O3 O3 153.2(3) 4_446 4_554
Nb O3 O3 13.90(8) 1_554 4_554
Ga1 O3 O3 13.90(8) 1_554 4_554
O1 O3 O3 112.4(5) . 4_554
O2 O3 O3 34.6(3) 4_554 4_554
La O3 O3 47.70(19) 1_554 4_554
Ga3 O3 O3 123.5(4) 2_565 4_554
O2 O3 O3 80.2(3) 3_454 4_554
La O3 O3 102.6(3) 2 4_554
O2 O3 O3 100.9(4) 4 4_554
O2 O3 O3 145.7(4) 3_455 4_554
La O3 O3 87.1(4) 2_565 4_554
Ga2 O3 O3 88.7(2) 2 4_554
O2 O3 O3 61.9(3) 5 4_554
O1 O3 O3 54.0(3) 1_554 4_554
Ga3 O3 O3 91.6(3) . 4_554
Ga2 O3 O3 165.9(3) . 4_554
La O3 O3 76.1(3) 4 4_554
O1 O3 O3 125.1(3) 1_545 4_554
O3 O3 O3 28.11(18) 1_554 4_554
O3 O3 O3 151.89(18) 1_556 4_554
O2 O3 O3 49.9(2) 3_554 4_554
Ga3 O3 O3 114.2(3) 1_656 4_554
O2 O3 O3 91.1(3) 4_444 4_554
O2 O3 O3 81.2(4) 2_565 4_554
La O3 O3 68.13(13) 4_444 4_554
O2 O3 O3 103.2(3) 3 4_554
O1 O3 O3 68.6(3) 2_565 4_554
Ga2 O3 O3 126.6(4) 2_566 4_554
O2 O3 O3 149.0(3) 4_445 4_554
O1 O3 O3 71.8(2) 1_544 4_554
O3 O3 O3 116.6(2) 4_445 4_554
O3 O3 O3 110.5(3) 3_455 4_554
Ga2 O3 O3 50.4(2) 1_664 4_554
O2 O3 O3 131.1(4) 6_556 4_554
O2 O3 O3 105.7(3) 5_445 4_554
La O3 O3 128.6(3) 2_455 4_554
O2 O3 O3 93.0(3) 6_545 4_554
O2 O3 O3 151.2(4) 2_556 4_554
O1 O3 O3 61.26(17) 2_454 4_554
La O3 O3 51.13(14) 2_554 4_554
O3 O3 O3 27.25(16) 3_554 4_554
O3 O3 O3 131.8(3) 3_556 4_554
Ga3 O3 O3 139.5(6) 4_445 4_556
Nb O3 O3 30.4(3) . 4_556
Ga1 O3 O3 30.4(3) . 4_556
La O3 O3 75.3(3) . 4_556
Ga3 O3 O3 95.8(4) 2_564 4_556
O2 O3 O3 83.3(5) 6 4_556
O3 O3 O3 18.4(2) 6 4_556
O3 O3 O3 135.2(7) 6_554 4_556
O3 O3 O3 76.37(8) 3 4_556
O3 O3 O3 61.89(18) 4 4_556
O2 O3 O3 109.1(5) 2 4_556
O2 O3 O3 168.3(6) 1_554 4_556
O1 O3 O3 111.0(4) 2_455 4_556
O2 O3 O3 61.3(3) . 4_556
O3 O3 O3 43.0(3) 2 4_556
Ga2 O3 O3 141.7(3) 1_554 4_556
O3 O3 O3 129.1(6) 2_554 4_556
Ga3 O3 O3 89.1(3) 1_655 4_556
La O3 O3 96.0(2) 4_445 4_556
Ga2 O3 O3 103.2(4) 2_565 4_556
O2 O3 O3 102.9(4) 5_455 4_556
O3 O3 O3 26.0(4) 5 4_556
O3 O3 O3 103.8(5) 5_554 4_556
Ga3 O3 O3 38.87(8) 4_446 4_556
Nb O3 O3 131.6(3) 1_554 4_556
Ga1 O3 O3 131.6(3) 1_554 4_556
O1 O3 O3 62.2(3) . 4_556
O2 O3 O3 96.8(4) 4_554 4_556
La O3 O3 152.2(4) 1_554 4_556
Ga3 O3 O3 13.38(15) 2_565 4_556
O2 O3 O3 141.9(4) 3_454 4_556
La O3 O3 73.7(2) 2 4_556
O2 O3 O3 30.7(2) 4 4_556
O2 O3 O3 76.1(3) 3_455 4_556
La O3 O3 59.4(2) 2_565 4_556
Ga2 O3 O3 116.8(3) 2 4_556
O2 O3 O3 69.4(3) 5 4_556
O1 O3 O3 120.8(4) 1_554 4_556
Ga3 O3 O3 120.5(3) . 4_556
Ga2 O3 O3 68.26(14) . 4_556
La O3 O3 47.6(2) 4 4_556
O1 O3 O3 80.1(3) 1_545 4_556
O3 O3 O3 151.89(18) 1_554 4_556
O3 O3 O3 28.11(18) 1_556 4_556
O2 O3 O3 99.6(4) 3_554 4_556
Ga3 O3 O3 26.29(16) 1_656 4_556
O2 O3 O3 145.1(4) 4_444 4_556
O2 O3 O3 87.3(3) 2_565 4_556
La O3 O3 158.1(4) 4_444 4_556
O2 O3 O3 46.5(3) 3 4_556
O1 O3 O3 61.2(3) 2_565 4_556
Ga2 O3 O3 48.4(2) 2_566 4_556
O2 O3 O3 87.2(2) 4_445 4_556
O1 O3 O3 132.9(4) 1_544 4_556
O3 O3 O3 116.6(2) 4_445 4_556
O3 O3 O3 110.5(3) 3_455 4_556
Ga2 O3 O3 79.5(3) 1_664 4_556
O2 O3 O3 28.7(2) 6_556 4_556
O2 O3 O3 111.9(3) 5_445 4_556
La O3 O3 103.9(2) 2_455 4_556
O2 O3 O3 99.0(3) 6_545 4_556
O2 O3 O3 49.7(2) 2_556 4_556
O1 O3 O3 171.9(3) 2_454 4_556
La O3 O3 125.5(3) 2_554 4_556
O3 O3 O3 131.8(3) 3_554 4_556
O3 O3 O3 27.25(16) 3_556 4_556
O3 O3 O3 123.8(4) 4_554 4_556
Ga3 O3 La 91.8(5) 4_445 2_564
Nb O3 La 108.5(5) . 2_564
Ga1 O3 La 108.5(5) . 2_564
La O3 La 94.0(4) . 2_564
Ga3 O3 La 21.98(18) 2_564 2_564
O2 O3 La 35.1(4) 6 2_564
O3 O3 La 109.3(7) 6 2_564
O3 O3 La 29.8(5) 6_554 2_564
O3 O3 La 106.6(4) 3 2_564
O3 O3 La 62.3(4) 4 2_564
O2 O3 La 132.0(4) 2 2_564
O2 O3 La 80.8(5) 1_554 2_564
O1 O3 La 113.8(4) 2_455 2_564
O2 O3 La 149.7(4) . 2_564
O3 O3 La 144.34(13) 2 2_564
Ga2 O3 La 91.8(3) 1_554 2_564
O3 O3 La 77.9(4) 2_554 2_564
Ga3 O3 La 77.6(3) 1_655 2_564
La O3 La 150.7(3) 4_445 2_564
Ga2 O3 La 35.58(14) 2_565 2_564
O2 O3 La 62.0(3) 5_455 2_564
O3 O3 La 101.7(3) 5 2_564
O3 O3 La 51.49(16) 5_554 2_564
Ga3 O3 La 148.4(3) 4_446 2_564
Nb O3 La 49.92(17) 1_554 2_564
Ga1 O3 La 49.92(17) 1_554 2_564
O1 O3 La 75.5(3) . 2_564
O2 O3 La 21.2(2) 4_554 2_564
La O3 La 44.06(14) 1_554 2_564
Ga3 O3 La 102.6(3) 2_565 2_564
O2 O3 La 68.6(3) 3_454 2_564
La O3 La 136.6(3) 2 2_564
O2 O3 La 80.4(3) 4 2_564
O2 O3 La 112.6(3) 3_455 2_564
La O3 La 55.82(17) 2_565 2_564
Ga2 O3 La 123.0(2) 2 2_564
O2 O3 La 80.7(3) 5 2_564
O1 O3 La 24.60(10) 1_554 2_564
Ga3 O3 La 67.79(18) . 2_564
Ga2 O3 La 135.3(3) . 2_564
La O3 La 73.5(2) 4 2_564
O1 O3 La 162.4(3) 1_545 2_564
O3 O3 La 49.27(12) 1_554 2_564
O3 O3 La 130.73(12) 1_556 2_564
O2 O3 La 84.3(2) 3_554 2_564
Ga3 O3 La 120.0(3) 1_656 2_564
O2 O3 La 96.5(3) 4_444 2_564
O2 O3 La 43.83(18) 2_565 2_564
La O3 La 89.48(19) 4_444 2_564
O2 O3 La 122.1(3) 3 2_564
O1 O3 La 50.6(2) 2_565 2_564
Ga2 O3 La 90.9(2) 2_566 2_564
O2 O3 La 136.8(3) 4_445 2_564
O1 O3 La 104.5(3) 1_544 2_564
O3 O3 La 128.89(17) 4_445 2_564
O3 O3 La 86.9(3) 3_455 2_564
Ga2 O3 La 34.43(10) 1_664 2_564
O2 O3 La 101.5(3) 6_556 2_564
O2 O3 La 135.6(3) 5_445 2_564
La O3 La 111.6(2) 2_455 2_564
O2 O3 La 130.3(3) 6_545 2_564
O2 O3 La 160.2(3) 2_556 2_564
O1 O3 La 68.84(16) 2_454 2_564
La O3 La 87.98(18) 2_554 2_564
O3 O3 La 63.83(16) 3_554 2_564
O3 O3 La 135.2(3) 3_556 2_564
O3 O3 La 37.4(2) 4_554 2_564
O3 O3 La 110.9(3) 4_556 2_564
Ga3 O3 O2 70.1(5) 4_445 6_554
Nb O3 O2 124.0(5) . 6_554
Ga1 O3 O2 124.0(5) . 6_554
La O3 O2 104.0(4) . 6_554
Ga3 O3 O2 38.7(2) 2_564 6_554
O2 O3 O2 56.7(4) 6 6_554
O3 O3 O2 132.5(8) 6 6_554
O3 O3 O2 10.1(3) 6_554 6_554
O3 O3 O2 103.6(2) 3 6_554
O3 O3 O2 77.8(4) 4 6_554
O2 O3 O2 110.0(5) 2 6_554
O2 O3 O2 58.1(6) 1_554 6_554
O1 O3 O2 103.0(4) 2_455 6_554
O2 O3 O2 154.7(5) . 6_554
O3 O3 O2 154.1(4) 2 6_554
Ga2 O3 O2 75.1(3) 1_554 6_554
O3 O3 O2 60.6(4) 2_554 6_554
Ga3 O3 O2 76.0(3) 1_655 6_554
La O3 O2 130.2(3) 4_445 6_554
Ga2 O3 O2 47.9(2) 2_565 6_554
O2 O3 O2 67.8(4) 5_455 6_554
O3 O3 O2 119.5(4) 5 6_554
O3 O3 O2 49.8(3) 5_554 6_554
Ga3 O3 O2 171.8(4) 4_446 6_554
Nb O3 O2 34.55(19) 1_554 6_554
Ga1 O3 O2 34.55(19) 1_554 6_554
O1 O3 O2 93.8(4) . 6_554
O2 O3 O2 37.8(3) 4_554 6_554
La O3 O2 25.15(18) 1_554 6_554
Ga3 O3 O2 126.0(4) 2_565 6_554
O2 O3 O2 56.3(2) 3_454 6_554
La O3 O2 128.0(3) 2 6_554
O2 O3 O2 103.6(4) 4 6_554
O2 O3 O2 118.3(3) 3_455 6_554
La O3 O2 78.9(3) 2_565 6_554
Ga2 O3 O2 101.0(3) 2 6_554
O2 O3 O2 86.9(3) 5 6_554
O1 O3 O2 28.2(3) 1_554 6_554
Ga3 O3 O2 64.5(2) . 6_554
Ga2 O3 O2 139.5(3) . 6_554
La O3 O2 91.2(3) 4 6_554
O1 O3 O2 141.6(4) 1_545 6_554
O3 O3 O2 26.6(2) 1_554 6_554
O3 O3 O2 153.4(2) 1_556 6_554
O2 O3 O2 76.7(3) 3_554 6_554
Ga3 O3 O2 136.3(3) 1_656 6_554
O2 O3 O2 77.2(3) 4_444 6_554
O2 O3 O2 61.1(3) 2_565 6_554
La O3 O2 66.1(2) 4_444 6_554
O2 O3 O2 129.7(3) 3 6_554
O1 O3 O2 72.5(3) 2_565 6_554
Ga2 O3 O2 110.4(3) 2_566 6_554
O2 O3 O2 129.5(2) 4_445 6_554
O1 O3 O2 82.3(3) 1_544 6_554
O3 O3 O2 108.82(19) 4_445 6_554
O3 O3 O2 83.9(2) 3_455 6_554
Ga2 O3 O2 54.5(2) 1_664 6_554
O2 O3 O2 123.9(5) 6_556 6_554
O2 O3 O2 112.2(3) 5_445 6_554
La O3 O2 104.8(2) 2_455 6_554
O2 O3 O2 112.2(3) 6_545 6_554
O2 O3 O2 176.2(3) 2_556 6_554
O1 O3 O2 47.4(2) 2_454 6_554
La O3 O2 70.3(2) 2_554 6_554
O3 O3 O2 47.3(2) 3_554 6_554
O3 O3 O2 154.2(4) 3_556 6_554
O3 O3 O2 27.3(2) 4_554 6_554
O3 O3 O2 133.6(4) 4_556 6_554
La O3 O2 23.43(18) 2_564 6_554
Ga3 O3 O1 64.1(4) 4_445 2
Nb O3 O1 47.7(3) . 2
Ga1 O3 O1 47.7(3) . 2
La O3 O1 145.7(5) . 2
Ga3 O3 O1 95.1(3) 2_564 2
O2 O3 O1 128.4(4) 6 2
O3 O3 O1 93.4(3) 6 2
O3 O3 O1 99.5(2) 6_554 2
O3 O3 O1 7.3(4) 3 2
O3 O3 O1 66.4(4) 4 2
O2 O3 O1 53.3(5) 2 2
O2 O3 O1 100.0(4) 1_554 2
O1 O3 O1 124.7(4) 2_455 2
O2 O3 O1 93.5(4) . 2
O3 O3 O1 46.6(4) 2 2
Ga2 O3 O1 123.6(3) 1_554 2
O3 O3 O1 56.1(5) 2_554 2
Ga3 O3 O1 36.0(2) 1_655 2
La O3 O1 83.5(3) 4_445 2
Ga2 O3 O1 147.7(3) 2_565 2
O2 O3 O1 175.0(4) 5_455 2
O3 O3 O1 56.1(2) 5 2
O3 O3 O1 62.6(2) 5_554 2
Ga3 O3 O1 73.7(3) 4_446 2
Nb O3 O1 75.8(3) 1_554 2
Ga1 O3 O1 75.8(3) 1_554 2
O1 O3 O1 137.1(3) . 2
O2 O3 O1 95.4(4) 4_554 2
La O3 O1 121.4(3) 1_554 2
Ga3 O3 O1 88.9(2) 2_565 2
O2 O3 O1 140.9(4) 3_454 2
La O3 O1 23.25(12) 2 2
O2 O3 O1 91.3(3) 4 2
O2 O3 O1 131.9(4) 3_455 2
La O3 O1 116.4(2) 2_565 2
Ga2 O3 O1 54.72(16) 2 2
O2 O3 O1 38.1(2) 5 2
O1 O3 O1 135.8(3) 1_554 2
Ga3 O3 O1 162.6(3) . 2
Ga2 O3 O1 109.3(3) . 2
La O3 O1 65.64(14) 4 2
O1 O3 O1 54.23(18) 1_545 2
O3 O3 O1 93.5(2) 1_554 2
O3 O3 O1 86.5(2) 1_556 2
O2 O3 O1 32.7(2) 3_554 2
Ga3 O3 O1 49.84(19) 1_656 2
O2 O3 O1 113.1(4) 4_444 2
O2 O3 O1 144.2(3) 2_565 2
La O3 O1 88.8(2) 4_444 2
O2 O3 O1 29.7(2) 3 2
O1 O3 O1 91.99(18) 2_565 2
Ga2 O3 O1 124.4(3) 2_566 2
O2 O3 O1 108.7(3) 4_445 2
O1 O3 O1 61.6(2) 1_544 2
O3 O3 O1 95.5(4) 4_445 2
O3 O3 O1 155.3(4) 3_455 2
Ga2 O3 O1 93.06(18) 1_664 2
O2 O3 O1 104.6(3) 6_556 2
O2 O3 O1 67.1(2) 5_445 2
La O3 O1 131.3(3) 2_455 2
O2 O3 O1 37.11(18) 6_545 2
O2 O3 O1 68.9(3) 2_556 2
O1 O3 O1 111.8(3) 2_454 2
La O3 O1 50.0(2) 2_554 2
O3 O3 O1 65.6(3) 3_554 2
O3 O3 O1 58.6(3) 3_556 2
O3 O3 O1 82.3(3) 4_554 2
O3 O3 O1 76.0(3) 4_556 2
La O3 O1 113.6(2) 2_564 2
O2 O3 O1 109.3(3) 6_554 2
Ga3 O3 La 137.9(5) 4_445 4_455
Nb O3 La 109.4(4) . 4_455
Ga1 O3 La 109.4(4) . 4_455
La O3 La 28.2(3) . 4_455
Ga3 O3 La 78.3(3) 2_564 4_455
O2 O3 La 38.5(4) 6 4_455
O3 O3 La 66.5(3) 6 4_455
O3 O3 La 89.4(4) 6_554 4_455
O3 O3 La 153.5(6) 3 4_455
O3 O3 La 95.8(6) 4 4_455
O2 O3 La 145.4(5) 2 4_455
O2 O3 La 102.7(4) 1_554 4_455
O1 O3 La 71.2(2) 2_455 4_455
O2 O3 La 83.7(3) . 4_455
O3 O3 La 119.1(5) 2 4_455
Ga2 O3 La 79.0(2) 1_554 4_455
O3 O3 La 139.5(6) 2_554 4_455
Ga3 O3 La 136.6(4) 1_655 4_455
La O3 La 107.6(2) 4_445 4_455
Ga2 O3 La 31.79(11) 2_565 4_455
O2 O3 La 20.6(2) 5_455 4_455
O3 O3 La 100.8(2) 5 4_455
O3 O3 La 115.50(15) 5_554 4_455
Ga3 O3 La 95.0(2) 4_446 4_455
Nb O3 La 113.6(3) 1_554 4_455
Ga1 O3 La 113.6(3) 1_554 4_455
O1 O3 La 20.4(2) . 4_455
O2 O3 La 78.3(4) 4_554 4_455
La O3 La 75.58(19) 1_554 4_455
Ga3 O3 La 69.36(17) 2_565 4_455
O2 O3 La 61.9(3) 3_454 4_455
La O3 La 152.0(3) 2 4_455
O2 O3 La 65.7(3) 4 4_455
O2 O3 La 47.9(2) 3_455 4_455
La O3 La 42.73(11) 2_565 4_455
Ga2 O3 La 146.6(3) 2 4_455
O2 O3 La 125.0(3) 5 4_455
O1 O3 La 51.29(19) 1_554 4_455
Ga3 O3 La 40.49(10) . 4_455
Ga2 O3 La 69.68(15) . 4_455
La O3 La 93.4(2) 4 4_455
O1 O3 La 130.5(3) 1_545 4_455
O3 O3 La 101.51(13) 1_554 4_455
O3 O3 La 78.49(13) 1_556 4_455
O2 O3 La 148.6(3) 3_554 4_455
Ga3 O3 La 108.9(2) 1_656 4_455
O2 O3 La 89.5(3) 4_444 4_455
O2 O3 La 23.51(18) 2_565 4_455
La O3 La 114.2(2) 4_444 4_455
O2 O3 La 129.0(3) 3 4_455
O1 O3 La 69.75(18) 2_565 4_455
Ga2 O3 La 35.48(8) 2_566 4_455
O2 O3 La 78.5(3) 4_445 4_455
O1 O3 La 141.5(2) 1_544 4_455
O3 O3 La 101.9(2) 4_445 4_455
O3 O3 La 43.4(2) 3_455 4_455
Ga2 O3 La 74.28(18) 1_664 4_455
O2 O3 La 55.0(2) 6_556 4_455
O2 O3 La 130.7(3) 5_445 4_455
La O3 La 62.43(12) 2_455 4_455
O2 O3 La 159.7(3) 6_545 4_455
O2 O3 La 103.5(3) 2_556 4_455
O1 O3 La 90.02(19) 2_454 4_455
La O3 La 148.2(3) 2_554 4_455
O3 O3 La 126.7(3) 3_554 4_455
O3 O3 La 104.22(19) 3_556 4_455
O3 O3 La 102.9(4) 4_554 4_455
O3 O3 La 82.6(3) 4_556 4_455
La O3 La 66.08(16) 2_564 4_455
O2 O3 La 79.4(2) 6_554 4_455
O1 O3 La 156.9(3) 2 4_455
Ga3 O3 O2 16.9(4) 4_445 2_554
Nb O3 O2 122.4(5) . 2_554
Ga1 O3 O2 122.4(5) . 2_554
La O3 O2 131.6(4) . 2_554
Ga3 O3 O2 82.1(3) 2_564 2_554
O2 O3 O2 110.5(5) 6 2_554
O3 O3 O2 170.4(4) 6 2_554
O3 O3 O2 46.6(5) 6_554 2_554
O3 O3 O2 76.3(4) 3 2_554
O3 O3 O2 102.7(3) 4 2_554
O2 O3 O2 56.2(3) 2 2_554
O2 O3 O2 27.8(3) 1_554 2_554
O1 O3 O2 88.2(4) 2_455 2_554
O2 O3 O2 125.2(5) . 2_554
O3 O3 O2 116.4(5) 2 2_554
Ga2 O3 O2 60.7(2) 1_554 2_554
O3 O3 O2 24.2(3) 2_554 2_554
Ga3 O3 O2 66.1(3) 1_655 2_554
La O3 O2 85.4(2) 4_445 2_554
Ga2 O3 O2 97.2(3) 2_565 2_554
O2 O3 O2 103.6(4) 5_455 2_554
O3 O3 O2 128.2(4) 5 2_554
O3 O3 O2 58.9(3) 5_554 2_554
Ga3 O3 O2 134.1(4) 4_446 2_554
Nb O3 O2 34.2(2) 1_554 2_554
Ga1 O3 O2 34.2(2) 1_554 2_554
O1 O3 O2 142.8(4) . 2_554
O2 O3 O2 81.3(4) 4_554 2_554
La O3 O2 48.05(18) 1_554 2_554
Ga3 O3 O2 163.7(3) 2_565 2_554
O2 O3 O2 65.4(3) 3_454 2_554
La O3 O2 83.2(3) 2 2_554
O2 O3 O2 146.7(4) 4 2_554
O2 O3 O2 126.9(3) 3_455 2_554
La O3 O2 131.9(3) 2_565 2_554
Ga2 O3 O2 47.17(19) 2 2_554
O2 O3 O2 86.5(3) 5 2_554
O1 O3 O2 77.0(3) 1_554 2_554
Ga3 O3 O2 86.8(2) . 2_554
Ga2 O3 O2 126.1(3) . 2_554
La O3 O2 115.4(3) 4 2_554
O1 O3 O2 87.8(3) 1_545 2_554
O3 O3 O2 27.3(2) 1_554 2_554
O3 O3 O2 152.7(2) 1_556 2_554
O2 O3 O2 53.9(4) 3_554 2_554
Ga3 O3 O2 126.9(3) 1_656 2_554
O2 O3 O2 53.40(18) 4_444 2_554
O2 O3 O2 112.6(4) 2_565 2_554
La O3 O2 23.37(18) 4_444 2_554
O2 O3 O2 106.7(4) 3 2_554
O1 O3 O2 115.6(3) 2_565 2_554
Ga2 O3 O2 158.4(3) 2_566 2_554
O2 O3 O2 105.7(3) 4_445 2_554
O1 O3 O2 28.5(2) 1_544 2_554
O3 O3 O2 70.5(2) 4_445 2_554
O3 O3 O2 96.0(2) 3_455 2_554
Ga2 O3 O2 97.6(3) 1_664 2_554
O2 O3 O2 177.7(4) 6_556 2_554
O2 O3 O2 60.3(2) 5_445 2_554
La O3 O2 97.2(2) 2_455 2_554
O2 O3 O2 60.5(2) 6_545 2_554
O2 O3 O2 122.4(4) 2_556 2_554
O1 O3 O2 35.46(18) 2_454 2_554
La O3 O2 27.17(19) 2_554 2_554
O3 O3 O2 26.4(3) 3_554 2_554
O3 O3 O2 132.2(4) 3_556 2_554
O3 O3 O2 47.1(2) 4_554 2_554
O3 O3 O2 152.6(4) 4_556 2_554
La O3 O2 76.3(2) 2_564 2_554
O2 O3 O2 53.8(3) 6_554 2_554
O1 O3 O2 77.0(3) 2 2_554
La O3 O2 123.1(3) 4_455 2_554
Ga3 O3 La 75.0(4) 4_445 4_554
Nb O3 La 81.3(4) . 4_554
Ga1 O3 La 81.3(4) . 4_554
La O3 La 130.2(5) . 4_554
Ga3 O3 La 24.04(18) 2_564 4_554
O2 O3 La 64.5(4) 6 4_554
O3 O3 La 111.9(6) 6 4_554
O3 O3 La 38.1(3) 6_554 4_554
O3 O3 La 66.7(3) 3 4_554
O3 O3 La 39.03(11) 4 4_554
O2 O3 La 107.0(4) 2 4_554
O2 O3 La 88.2(5) 1_554 4_554
O1 O3 La 145.9(4) 2_455 4_554
O2 O3 La 160.7(4) . 4_554
O3 O3 La 111.4(3) 2 4_554
Ga2 O3 La 115.6(3) 1_554 4_554
O3 O3 La 53.13(16) 2_554 4_554
Ga3 O3 La 37.79(15) 1_655 4_554
La O3 La 147.2(3) 4_445 4_554
Ga2 O3 La 74.8(2) 2_565 4_554
O2 O3 La 101.9(4) 5_455 4_554
O3 O3 La 79.0(4) 5 4_554
O3 O3 La 13.37(13) 5_554 4_554
Ga3 O3 La 133.5(3) 4_446 4_554
Nb O3 La 33.08(11) 1_554 4_554
Ga1 O3 La 33.08(11) 1_554 4_554
O1 O3 La 103.9(3) . 4_554
O2 O3 La 24.0(3) 4_554 4_554
La O3 La 67.78(19) 1_554 4_554
Ga3 O3 La 101.5(2) 2_565 4_554
O2 O3 La 99.8(3) 3_454 4_554
La O3 La 96.8(2) 2 4_554
O2 O3 La 80.0(3) 4 4_554
O2 O3 La 150.1(4) 3_455 4_554
La O3 La 73.1(2) 2_565 4_554
Ga2 O3 La 100.2(2) 2 4_554
O2 O3 La 43.6(2) 5 4_554
O1 O3 La 63.4(2) 1_554 4_554
Ga3 O3 La 106.1(3) . 4_554
Ga2 O3 La 166.8(3) . 4_554
La O3 La 53.28(14) 4 4_554
O1 O3 La 126.3(2) 1_545 4_554
O3 O3 La 50.97(11) 1_554 4_554
O3 O3 La 129.03(11) 1_556 4_554
O2 O3 La 46.41(18) 3_554 4_554
Ga3 O3 La 93.54(19) 1_656 4_554
O2 O3 La 114.0(3) 4_444 4_554
O2 O3 La 78.8(2) 2_565 4_554
La O3 La 89.47(18) 4_444 4_554
O2 O3 La 86.7(2) 3 4_554
O1 O3 La 49.3(2) 2_565 4_554
Ga2 O3 La 113.6(3) 2_566 4_554
O2 O3 La 171.9(3) 4_445 4_554
O1 O3 La 86.7(2) 1_544 4_554
O3 O3 La 137.37(19) 4_445 4_554
O3 O3 La 125.7(3) 3_455 4_554
Ga2 O3 La 33.47(9) 1_664 4_554
O2 O3 La 111.8(3) 6_556 4_554
O2 O3 La 119.2(3) 5_445 4_554
La O3 La 148.4(3) 2_455 4_554
O2 O3 La 97.3(2) 6_545 4_554
O2 O3 La 136.8(3) 2_556 4_554
O1 O3 La 84.01(19) 2_454 4_554
La O3 La 61.55(12) 2_554 4_554
O3 O3 La 42.09(18) 3_554 4_554
O3 O3 La 111.6(3) 3_556 4_554
O3 O3 La 22.86(15) 4_554 4_554
O3 O3 La 100.9(3) 4_556 4_554
La O3 La 39.91(10) 2_564 4_554
O2 O3 La 43.65(17) 6_554 4_554
O1 O3 La 73.74(18) 2 4_554
La O3 La 102.3(2) 4_455 4_554
O2 O3 La 66.9(2) 2_554 4_554
Ga3 O3 O3 135.1(6) 4_445 5_455
Nb O3 O3 111.1(5) . 5_455
Ga1 O3 O3 111.1(5) . 5_455
La O3 O3 7.4(2) . 5_455
Ga3 O3 O3 101.0(3) 2_564 5_455
O2 O3 O3 61.0(3) 6 5_455
O3 O3 O3 62.5(2) 6 5_455
O3 O3 O3 106.7(3) 6_554 5_455
O3 O3 O3 156.3(2) 3 5_455
O3 O3 O3 113.9(6) 4 5_455
O2 O3 O3 124.7(5) 2 5_455
O2 O3 O3 100.0(4) 1_554 5_455
O1 O3 O3 52.6(3) 2_455 5_455
O2 O3 O3 62.9(4) . 5_455
O3 O3 O3 106.4(6) 2 5_455
Ga2 O3 O3 69.4(3) 1_554 5_455
O3 O3 O3 149.7(6) 2_554 5_455
Ga3 O3 O3 157.7(3) 1_655 5_455
La O3 O3 85.3(3) 4_445 5_455
Ga2 O3 O3 51.95(8) 2_565 5_455
O2 O3 O3 29.0(2) 5_455 5_455
O3 O3 O3 104.8(4) 5 5_455
O3 O3 O3 137.98(19) 5_554 5_455
Ga3 O3 O3 79.6(3) 4_446 5_455
Nb O3 O3 130.9(3) 1_554 5_455
Ga1 O3 O3 130.9(3) 1_554 5_455
O1 O3 O3 29.20(7) . 5_455
O2 O3 O3 100.9(3) 4_554 5_455
La O3 O3 85.4(2) 1_554 5_455
Ga3 O3 O3 69.3(2) 2_565 5_455
O2 O3 O3 61.1(3) 3_454 5_455
La O3 O3 134.6(4) 2 5_455
O2 O3 O3 75.1(3) 4 5_455
O2 O3 O3 25.5(3) 3_455 5_455
La O3 O3 60.60(8) 2_565 5_455
Ga2 O3 O3 128.4(3) 2 5_455
O2 O3 O3 141.1(4) 5 5_455
O1 O3 O3 68.87(19) 1_554 5_455
Ga3 O3 O3 40.37(14) . 5_455
Ga2 O3 O3 47.9(2) . 5_455
La O3 O3 107.7(2) 4 5_455
O1 O3 O3 108.4(3) 1_545 5_455
O3 O3 O3 113.4(2) 1_554 5_455
O3 O3 O3 66.6(2) 1_556 5_455
O2 O3 O3 171.3(3) 3_554 5_455
Ga3 O3 O3 105.6(3) 1_656 5_455
O2 O3 O3 79.1(3) 4_444 5_455
O2 O3 O3 46.11(17) 2_565 5_455
La O3 O3 109.0(3) 4_444 5_455
O2 O3 O3 124.7(4) 3 5_455
O1 O3 O3 88.79(17) 2_565 5_455
Ga2 O3 O3 34.09(12) 2_566 5_455
O2 O3 O3 56.0(3) 4_445 5_455
O1 O3 O3 131.7(3) 1_544 5_455
O3 O3 O3 82.5(3) 4_445 5_455
O3 O3 O3 31.6(3) 3_455 5_455
Ga2 O3 O3 96.18(15) 1_664 5_455
O2 O3 O3 52.5(2) 6_556 5_455
O2 O3 O3 110.3(4) 5_445 5_455
La O3 O3 42.81(19) 2_455 5_455
O2 O3 O3 137.3(3) 6_545 5_455
O2 O3 O3 85.6(3) 2_556 5_455
O1 O3 O3 91.0(3) 2_454 5_455
La O3 O3 153.0(3) 2_554 5_455
O3 O3 O3 141.4(3) 3_554 5_455
O3 O3 O3 94.7(2) 3_556 5_455
O3 O3 O3 122.7(4) 4_554 5_455
O3 O3 O3 80.8(3) 4_556 5_455
La O3 O3 87.41(15) 2_564 5_455
O2 O3 O3 96.7(3) 6_554 5_455
O1 O3 O3 153.0(4) 2 5_455
La O3 O3 22.63(7) 4_455 5_455
O2 O3 O3 126.5(4) 2_554 5_455
La O3 O3 124.9(2) 4_554 5_455
Ga3 O3 O3 78.5(4) 4_445 5_445
Nb O3 O3 98.2(5) . 5_445
Ga1 O3 O3 98.2(5) . 5_445
La O3 O3 77.9(5) . 5_445
Ga3 O3 O3 172.0(5) 2_564 5_445
O2 O3 O3 143.4(5) 6 5_445
O3 O3 O3 87.7(8) 6 5_445
O3 O3 O3 132.6(6) 6_554 5_445
O3 O3 O3 91.9(5) 3 5_445
O3 O3 O3 144.2(4) 4 5_445
O2 O3 O3 44.2(3) 2 5_445
O2 O3 O3 76.8(5) 1_554 5_445
O1 O3 O3 41.9(3) 2_455 5_445
O2 O3 O3 35.1(4) . 5_445
O3 O3 O3 62.3(2) 2 5_445
Ga2 O3 O3 61.5(3) 1_554 5_445
O3 O3 O3 98.97(18) 2_554 5_445
Ga3 O3 O3 117.9(2) 1_655 5_445
La O3 O3 4.70(10) 4_445 5_445
Ga2 O3 O3 127.5(4) 2_565 5_445
O2 O3 O3 100.3(4) 5_455 5_445
O3 O3 O3 104.8(4) 5 5_445
O3 O3 O3 137.98(19) 5_554 5_445
Ga3 O3 O3 53.0(2) 4_446 5_445
Nb O3 O3 123.4(3) 1_554 5_445
Ga1 O3 O3 123.4(3) 1_554 5_445
O1 O3 O3 104.9(4) . 5_445
O2 O3 O3 171.2(4) 4_554 5_445
La O3 O3 110.3(3) 1_554 5_445
Ga3 O3 O3 96.8(4) 2_565 5_445
O2 O3 O3 84.9(4) 3_454 5_445
La O3 O3 61.94(10) 2 5_445
O2 O3 O3 120.1(4) 4 5_445
O2 O3 O3 58.1(3) 3_455 5_445
La O3 O3 134.8(3) 2_565 5_445
Ga2 O3 O3 51.12(6) 2 5_445
O2 O3 O3 121.8(3) 5 5_445
O1 O3 O3 130.3(3) 1_554 5_445
Ga3 O3 O3 88.9(3) . 5_445
Ga2 O3 O3 40.6(3) . 5_445
La O3 O3 133.1(3) 4 5_445
O1 O3 O3 30.82(7) 1_545 5_445
O3 O3 O3 113.4(2) 1_554 5_445
O3 O3 O3 66.6(2) 1_556 5_445
O2 O3 O3 106.2(2) 3_554 5_445
Ga3 O3 O3 86.5(3) 1_656 5_445
O2 O3 O3 57.4(3) 4_444 5_445
O2 O3 O3 128.0(3) 2_565 5_445
La O3 O3 70.89(19) 4_444 5_445
O2 O3 O3 83.5(3) 3 5_445
O1 O3 O3 152.7(4) 2_565 5_445
Ga2 O3 O3 94.3(3) 2_566 5_445
O2 O3 O3 26.4(3) 4_445 5_445
O1 O3 O3 66.03(18) 1_544 5_445
O3 O3 O3 25.3(2) 4_445 5_445
O3 O3 O3 71.6(3) 3_455 5_445
Ga2 O3 O3 171.3(4) 1_664 5_445
O2 O3 O3 91.7(4) 6_556 5_445
O2 O3 O3 32.5(2) 5_445 5_445
La O3 O3 46.7(2) 2_455 5_445
O2 O3 O3 54.9(2) 6_545 5_445
O2 O3 O3 43.1(3) 2_556 5_445
O1 O3 O3 86.7(3) 2_454 5_445
La O3 O3 89.99(13) 2_554 5_445
O3 O3 O3 111.5(3) 3_554 5_445
O3 O3 O3 70.5(3) 3_556 5_445
O3 O3 O3 137.1(3) 4_554 5_445
O3 O3 O3 91.8(3) 4_556 5_445
La O3 O3 153.3(3) 2_564 5_445
O2 O3 O3 134.1(4) 6_554 5_445
O1 O3 O3 84.64(14) 2 5_445
La O3 O3 104.9(3) 4_455 5_445
O2 O3 O3 90.1(2) 2_554 5_445
La O3 O3 151.2(2) 4_554 5_445
O3 O3 O3 82.4(3) 5_455 5_445
Ga3 O3 O3 96.0(5) 4_445 5_454
Nb O3 O3 148.9(5) . 5_454
Ga1 O3 O3 148.9(5) . 5_454
La O3 O3 55.9(2) . 5_454
Ga3 O3 O3 76.2(3) 2_564 5_454
O2 O3 O3 55.0(3) 6 5_454
O3 O3 O3 107.9(3) 6 5_454
O3 O3 O3 60.8(3) 6_554 5_454
O3 O3 O3 154.4(3) 3 5_454
O3 O3 O3 113.5(6) 4 5_454
O2 O3 O3 117.8(6) 2 5_454
O2 O3 O3 61.6(5) 1_554 5_454
O1 O3 O3 59.6(3) 2_455 5_454
O2 O3 O3 103.5(4) . 5_454
O3 O3 O3 153.8(6) 2 5_454
Ga2 O3 O3 46.7(3) 1_554 5_454
O3 O3 O3 101.9(6) 2_554 5_454
Ga3 O3 O3 127.8(4) 1_655 5_454
La O3 O3 100.6(3) 4_445 5_454
Ga2 O3 O3 30.59(7) 2_565 5_454
O2 O3 O3 21.9(3) 5_455 5_454
O3 O3 O3 139.40(15) 5 5_454
O3 O3 O3 101.2(4) 5_554 5_454
Ga3 O3 O3 126.8(4) 4_446 5_454
Nb O3 O3 83.4(3) 1_554 5_454
Ga1 O3 O3 83.4(3) 1_554 5_454
O1 O3 O3 62.2(2) . 5_454
O2 O3 O3 75.5(3) 4_554 5_454
La O3 O3 36.6(2) 1_554 5_454
Ga3 O3 O3 111.2(2) 2_565 5_454
O2 O3 O3 23.0(3) 3_454 5_454
La O3 O3 157.4(3) 2 5_454
O2 O3 O3 103.5(3) 4 5_454
O2 O3 O3 66.8(3) 3_455 5_454
La O3 O3 74.34(8) 2_565 5_454
Ga2 O3 O3 113.0(3) 2 5_454
O2 O3 O3 135.3(4) 5 5_454
O1 O3 O3 30.03(10) 1_554 5_454
Ga3 O3 O3 13.37(11) . 5_454
Ga2 O3 O3 87.9(3) . 5_454
La O3 O3 120.0(2) 4 5_454
O1 O3 O3 131.1(3) 1_545 5_454
O3 O3 O3 64.6(2) 1_554 5_454
O3 O3 O3 115.4(2) 1_556 5_454
O2 O3 O3 126.6(4) 3_554 5_454
Ga3 O3 O3 150.7(3) 1_656 5_454
O2 O3 O3 56.1(3) 4_444 5_454
O2 O3 O3 43.0(2) 2_565 5_454
La O3 O3 73.6(3) 4_444 5_454
O2 O3 O3 170.4(3) 3 5_454
O1 O3 O3 91.94(17) 2_565 5_454
Ga2 O3 O3 76.67(14) 2_566 5_454
O2 O3 O3 82.5(3) 4_445 5_454
O1 O3 O3 101.1(3) 1_544 5_454
O3 O3 O3 82.7(3) 4_445 5_454
O3 O3 O3 33.0(3) 3_455 5_454
Ga2 O3 O3 83.95(19) 1_664 5_454
O2 O3 O3 96.5(2) 6_556 5_454
O2 O3 O3 107.0(3) 5_445 5_454
La O3 O3 57.0(2) 2_455 5_454
O2 O3 O3 132.5(3) 6_545 5_454
O2 O3 O3 129.2(4) 2_556 5_454
O1 O3 O3 48.3(2) 2_454 5_454
La O3 O3 108.4(3) 2_554 5_454
O3 O3 O3 92.7(2) 3_554 5_454
O3 O3 O3 143.4(3) 3_556 5_454
O3 O3 O3 79.0(4) 4_554 5_454
O3 O3 O3 124.5(3) 4_556 5_454
La O3 O3 54.62(16) 2_564 5_454
O2 O3 O3 51.8(3) 6_554 5_454
O1 O3 O3 158.0(4) 2 5_454
La O3 O3 41.83(9) 4_455 5_454
O2 O3 O3 81.8(3) 2_554 5_454
La O3 O3 92.7(3) 4_554 5_454
O3 O3 O3 48.76(13) 5_455 5_454
O3 O3 O3 101.3(4) 5_445 5_454
Ga3 O3 O3 37.9(2) 4_445 5_444
Nb O3 O3 129.9(4) . 5_444
Ga1 O3 O3 129.9(4) . 5_444
La O3 O3 102.1(5) . 5_444
Ga3 O3 O3 123.3(4) 2_564 5_444
O2 O3 O3 133.9(5) 6 5_444
O3 O3 O3 136.3(8) 6 5_444
O3 O3 O3 84.1(6) 6_554 5_444
O3 O3 O3 91.9(5) 3 5_444
O3 O3 O3 143.0(4) 4 5_444
O2 O3 O3 36.9(4) 2 5_444
O2 O3 O3 29.3(4) 1_554 5_444
O1 O3 O3 50.2(4) 2_455 5_444
O2 O3 O3 82.9(4) . 5_444
O3 O3 O3 99.33(19) 2 5_444
Ga2 O3 O3 36.0(3) 1_554 5_444
O3 O3 O3 60.7(3) 2_554 5_444
Ga3 O3 O3 99.4(2) 1_655 5_444
La O3 O3 44.26(14) 4_445 5_444
Ga2 O3 O3 110.2(3) 2_565 5_444
O2 O3 O3 96.2(4) 5_455 5_444
O3 O3 O3 139.40(15) 5 5_444
O3 O3 O3 101.2(4) 5_554 5_444
Ga3 O3 O3 100.6(3) 4_446 5_444
Nb O3 O3 77.5(2) 1_554 5_444
Ga1 O3 O3 77.5(2) 1_554 5_444
O1 O3 O3 130.3(3) . 5_444
O2 O3 O3 122.4(4) 4_554 5_444
La O3 O3 67.5(3) 1_554 5_444
Ga3 O3 O3 145.5(4) 2_565 5_444
O2 O3 O3 57.9(3) 3_454 5_444
La O3 O3 76.60(9) 2 5_444
O2 O3 O3 168.9(5) 4 5_444
O2 O3 O3 88.6(4) 3_455 5_444
La O3 O3 155.1(3) 2_565 5_444
Ga2 O3 O3 33.07(6) 2 5_444
O2 O3 O3 117.6(3) 5 5_444
O1 O3 O3 97.2(3) 1_554 5_444
Ga3 O3 O3 76.1(3) . 5_444
Ga2 O3 O3 82.8(3) . 5_444
La O3 O3 151.0(3) 4 5_444
O1 O3 O3 60.11(18) 1_545 5_444
O3 O3 O3 64.6(2) 1_554 5_444
O3 O3 O3 115.4(2) 1_556 5_444
O2 O3 O3 84.2(3) 3_554 5_444
Ga3 O3 O3 123.2(2) 1_656 5_444
O2 O3 O3 25.6(3) 4_444 5_444
O2 O3 O3 123.8(3) 2_565 5_444
La O3 O3 22.14(13) 4_444 5_444
O2 O3 O3 108.3(2) 3 5_444
O1 O3 O3 158.4(4) 2_565 5_444
Ga2 O3 O3 131.1(4) 2_566 5_444
O2 O3 O3 62.5(3) 4_445 5_444
O1 O3 O3 30.52(10) 1_544 5_444
O3 O3 O3 27.1(3) 4_445 5_444
O3 O3 O3 71.9(3) 3_455 5_444
Ga2 O3 O3 139.6(3) 1_664 5_444
O2 O3 O3 137.9(4) 6_556 5_444
O2 O3 O3 28.53(16) 5_445 5_444
La O3 O3 60.2(3) 2_455 5_444
O2 O3 O3 52.06(15) 6_545 5_444
O2 O3 O3 89.4(3) 2_556 5_444
O1 O3 O3 42.3(2) 2_454 5_444
La O3 O3 55.85(14) 2_554 5_444
O3 O3 O3 68.7(3) 3_554 5_444
O3 O3 O3 113.2(3) 3_556 5_444
O3 O3 O3 89.9(2) 4_554 5_444
O3 O3 O3 138.9(3) 4_556 5_444
La O3 O3 110.2(3) 2_564 5_444
O2 O3 O3 87.2(3) 6_554 5_444
O1 O3 O3 87.61(14) 2 5_444
La O3 O3 114.7(3) 4_455 5_444
O2 O3 O3 43.4(2) 2_554 5_444
La O3 O3 110.3(3) 4_554 5_444
O3 O3 O3 101.3(4) 5_455 5_444
O3 O3 O3 48.76(13) 5_445 5_444
O3 O3 O3 80.9(3) 5_454 5_444
Ga3 O3 O2 152.9(6) 4_445 5_456
Nb O3 O2 84.4(4) . 5_456
Ga1 O3 O2 84.4(4) . 5_456
La O3 O2 21.6(2) . 5_456
Ga3 O3 O2 108.8(4) 2_564 5_456
O2 O3 O2 70.3(4) 6 5_456
O3 O3 O2 35.7(2) 6 5_456
O3 O3 O2 130.0(5) 6_554 5_456
O3 O3 O2 128.3(2) 3 5_456
O3 O3 O2 101.7(5) 4 5_456
O2 O3 O2 120.8(5) 2 5_456
O2 O3 O2 124.4(4) 1_554 5_456
O1 O3 O2 65.9(4) 2_455 5_456
O2 O3 O2 46.6(2) . 5_456
O3 O3 O2 80.0(5) 2 5_456
Ga2 O3 O2 91.6(3) 1_554 5_456
O3 O3 O2 175.7(2) 2_554 5_456
Ga3 O3 O2 141.6(3) 1_655 5_456
La O3 O2 81.9(3) 4_445 5_456
Ga2 O3 O2 72.2(2) 2_565 5_456
O2 O3 O2 55.5(3) 5_455 5_456
O3 O3 O2 79.4(4) 5 5_456
O3 O3 O2 142.5(3) 5_554 5_456
Ga3 O3 O2 54.5(2) 4_446 5_456
Nb O3 O2 153.7(4) 1_554 5_456
Ga1 O3 O2 153.7(4) 1_554 5_456
O1 O3 O2 28.8(2) . 5_456
O2 O3 O2 109.2(4) 4_554 5_456
La O3 O2 113.0(3) 1_554 5_456
Ga3 O3 O2 44.15(18) 2_565 5_456
O2 O3 O2 88.4(4) 3_454 5_456
La O3 O2 111.6(3) 2 5_456
O2 O3 O2 57.3(3) 4 5_456
O2 O3 O2 26.7(3) 3_455 5_456
La O3 O2 57.48(17) 2_565 5_456
Ga2 O3 O2 128.6(3) 2 5_456
O2 O3 O2 121.3(4) 5 5_456
O1 O3 O2 91.9(3) 1_554 5_456
Ga3 O3 O2 68.3(2) . 5_456
Ga2 O3 O2 37.02(17) . 5_456
La O3 O2 90.7(2) 4 5_456
O1 O3 O2 93.6(3) 1_545 5_456
O3 O3 O2 140.77(19) 1_554 5_456
O3 O3 O2 39.23(19) 1_556 5_456
O2 O3 O2 153.6(4) 3_554 5_456
Ga3 O3 O2 77.8(2) 1_656 5_456
O2 O3 O2 99.5(4) 4_444 5_456
O2 O3 O2 60.37(16) 2_565 5_456
La O3 O2 130.5(3) 4_444 5_456
O2 O3 O2 96.7(2) 3 5_456
O1 O3 O2 82.6(3) 2_565 5_456
Ga2 O3 O2 17.16(13) 2_566 5_456
O2 O3 O2 54.7(3) 4_445 5_456
O1 O3 O2 142.5(4) 1_544 5_456
O3 O3 O2 89.6(2) 4_445 5_456
O3 O3 O2 56.5(2) 3_455 5_456
Ga2 O3 O2 97.1(2) 1_664 5_456
O2 O3 O2 27.5(3) 6_556 5_456
O2 O3 O2 110.0(4) 5_445 5_456
La O3 O2 56.3(2) 2_455 5_456
O2 O3 O2 125.7(3) 6_545 5_456
O2 O3 O2 63.0(3) 2_556 5_456
O1 O3 O2 117.9(3) 2_454 5_456
La O3 O2 167.4(3) 2_554 5_456
O3 O3 O2 167.3(3) 3_554 5_456
O3 O3 O2 67.0(2) 3_556 5_456
O3 O3 O2 141.2(4) 4_554 5_456
O3 O3 O2 54.0(3) 4_556 5_456
La O3 O2 104.0(2) 2_564 5_456
O2 O3 O2 120.0(3) 6_554 5_456
O1 O3 O2 125.6(3) 2 5_456
La O3 O2 40.64(15) 4_455 5_456
O2 O3 O2 152.1(3) 2_554 5_456
La O3 O2 130.6(3) 4_554 5_456
O3 O3 O2 27.98(19) 5_455 5_456
O3 O3 O2 77.6(3) 5_445 5_456
O3 O3 O2 76.4(2) 5_454 5_456
O3 O3 O2 115.0(4) 5_444 5_456
Ga3 O3 La 84.1(4) 4_445 1_655
Nb O3 La 29.0(2) . 1_655
Ga1 O3 La 29.0(2) . 1_655
La O3 La 134.7(4) . 1_655
Ga3 O3 La 80.0(3) 2_564 1_655
O2 O3 La 106.2(4) 6 1_655
O3 O3 La 77.82(11) 6 1_655
O3 O3 La 99.06(17) 6_554 1_655
O3 O3 La 20.0(4) 3 1_655
O3 O3 La 44.5(4) 4 1_655
O2 O3 La 77.1(5) 2 1_655
O2 O3 La 119.9(4) 1_554 1_655
O1 O3 La 144.0(4) 2_455 1_655
O2 O3 La 98.4(4) . 1_655
O3 O3 La 47.4(3) 2 1_655
Ga2 O3 La 147.4(3) 1_554 1_655
O3 O3 La 69.7(4) 2_554 1_655
Ga3 O3 La 32.82(12) 1_655 1_655
La O3 La 102.3(3) 4_445 1_655
Ga2 O3 La 128.9(3) 2_565 1_655
O2 O3 La 151.6(4) 5_455 1_655
O3 O3 La 35.3(2) 5 1_655
O3 O3 La 57.3(3) 5_554 1_655
Ga3 O3 La 72.58(18) 4_446 1_655
Nb O3 La 79.84(18) 1_554 1_655
Ga1 O3 La 79.84(18) 1_554 1_655
O1 O3 La 115.4(3) . 1_655
O2 O3 La 80.6(3) 4_554 1_655
La O3 La 127.7(3) 1_554 1_655
Ga3 O3 La 70.62(16) 2_565 1_655
O2 O3 La 158.0(3) 3_454 1_655
La O3 La 41.70(11) 2 1_655
O2 O3 La 68.2(3) 4 1_655
O2 O3 La 131.3(4) 3_455 1_655
La O3 La 92.3(2) 2_565 1_655
Ga2 O3 La 78.81(18) 2 1_655
O2 O3 La 20.87(17) 5 1_655
O1 O3 La 126.1(3) 1_554 1_655
Ga3 O3 La 168.9(3) . 1_655
Ga2 O3 La 113.3(2) . 1_655
La O3 La 41.72(9) 4 1_655
O1 O3 La 71.63(17) 1_545 1_655
O3 O3 La 101.31(12) 1_554 1_655
O3 O3 La 78.69(12) 1_556 1_655
O2 O3 La 40.4(2) 3_554 1_655
Ga3 O3 La 36.61(8) 1_656 1_655
O2 O3 La 136.9(4) 4_444 1_655
O2 O3 La 121.1(3) 2_565 1_655
La O3 La 110.0(2) 4_444 1_655
O2 O3 La 22.81(16) 3 1_655
O1 O3 La 68.89(14) 2_565 1_655
Ga2 O3 La 106.15(19) 2_566 1_655
O2 O3 La 121.2(3) 4_445 1_655
O1 O3 La 84.19(18) 1_544 1_655
O3 O3 La 118.0(4) 4_445 1_655
O3 O3 La 168.60(13) 3_455 1_655
Ga2 O3 La 73.40(15) 1_664 1_655
O2 O3 La 87.5(2) 6_556 1_655
O2 O3 La 90.5(3) 5_445 1_655
La O3 La 146.8(3) 2_455 1_655
O2 O3 La 60.97(19) 6_545 1_655
O2 O3 La 72.9(3) 2_556 1_655
O1 O3 La 128.7(2) 2_454 1_655
La O3 La 67.00(13) 2_554 1_655
O3 O3 La 74.3(2) 3_554 1_655
O3 O3 La 52.00(19) 3_556 1_655
O3 O3 La 80.6(2) 4_554 1_655
O3 O3 La 59.4(2) 4_556 1_655
La O3 La 101.5(2) 2_564 1_655
O2 O3 La 106.9(2) 6_554 1_655
O1 O3 La 24.10(8) 2 1_655
La O3 La 133.6(2) 4_455 1_655
O2 O3 La 93.5(3) 2_554 1_655
La O3 La 64.14(12) 4_554 1_655
O3 O3 La 139.9(3) 5_455 1_655
O3 O3 La 102.2(2) 5_445 1_655
O3 O3 La 156.1(3) 5_454 1_655
O3 O3 La 111.59(16) 5_444 1_655
O2 O3 La 113.3(3) 5_456 1_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.362(12) .
La O3 2.362(12) 6
La O2 2.405(15) 3_455
La O2 2.405(15) 5_455
La O1 2.502(6) .
La O1 2.502(6) 2_455
La O2 2.75(2) .
La O2 2.75(2) 6
La Ga2 3.374(2) .
La Ga2 3.374(2) 2_565
La Nb 3.4528(12) .
La Ga1 3.4528(12) .
Ga1 O3 1.958(12) 3
Ga1 O3 1.959(12) 6
Ga1 O3 1.959(12) .
Ga1 O3 1.959(12) 2
Ga1 O3 1.959(12) 5
Ga1 O3 1.959(12) 4
Ga1 O2 3.476(18) 2
Ga1 O2 3.476(18) 3
Ga1 O2 3.476(18) 5
Ga1 O2 3.476(18) .
Ga1 O2 3.476(18) 4
Ga1 O2 3.476(18) 6
Ga2 O1 1.761(19) 2_456
Ga2 O2 1.854(15) 4_445
Ga2 O2 1.854(15) .
Ga2 O2 1.854(15) 3_455
Ga2 O1 3.262(19) 2_455
Ga2 La 3.374(2) 4_445
Ga2 La 3.374(2) 2_455
Ga2 O3 3.399(12) 4_446
Ga2 O3 3.399(12) 1_556
Ga2 O3 3.399(12) 3_456
Ga2 La 3.513(2) 4_446
Ga3 O2 1.810(15) 3_454
Ga3 O2 1.810(15) 5_455
Ga3 O3 1.817(12) 5_454
Ga3 O3 1.817(12) 3_455
Ga3 O3 2.524(15) 2_454
Ga3 O3 2.524(15) 4_455
Ga3 Nb 3.1231(13) 1_454
Ga3 Nb 3.1231(13) 1_455
Ga3 O1 3.541(9) 2_455
Ga3 O1 3.541(9) 1_554
Ga3 O3 3.612(12) 6_454
Ga3 O3 3.612(12) 1_455
Nb O3 1.958(12) 3
Nb O3 1.959(12) 6
Nb O3 1.959(12) .
Nb O3 1.959(12) 2
Nb O3 1.959(12) 5
Nb O3 1.959(12) 4
Nb Ga3 3.1231(13) 4_445
Nb Ga3 3.1231(13) 4_446
Nb Ga3 3.1231(13) 1_656
Nb Ga3 3.1231(13) 1_655
Nb Ga3 3.1231(13) 2_565
Nb Ga3 3.1231(13) 2_564
O1 Ga2 1.761(19) 2_566
O1 La 2.502(6) 2_565
O1 La 2.502(6) 4_455
O1 O2 2.86(2) 6
O1 O2 2.86(2) 5_455
O1 O2 2.86(2) 2_565
O1 O3 3.113(13) 6
O1 O3 3.113(13) 2_565
O1 O3 3.113(13) 5_455
O1 O2 3.12(2) 6_556
O1 O2 3.12(2) 5_456
O1 O2 3.12(2) 2_566
O1 Ga2 3.262(19) 2_565
O1 Ga3 3.541(9) 2_565
O1 Ga3 3.541(9) 1_556
O1 Ga3 3.541(9) 4_456
O1 O2 3.556(16) 4
O1 O2 3.556(16) 3_455
O1 O2 3.556(16) 1_565
O1 O3 4.258(15) .
O1 O3 4.258(15) 3_565
O1 O3 4.258(15) 4_455
O1 Ga3 4.586(13) 2_564
O1 Ga3 4.586(13) 4_455
O1 O2 4.66(2) .
O1 O2 4.66(2) 3_565
O1 O2 4.66(2) 4_455
O1 Ga1 4.669(3) 1_455
O1 Nb 4.669(3) 1_455
O1 Ga1 4.669(3) 1_565
O1 Nb 4.669(3) 1_565
O1 O3 4.78(2) 1_556
O1 O3 4.78(2) 3_566
O1 O3 4.78(2) 4_456
O1 La 4.796(16) 1_556
O1 La 4.796(16) 2_566
O1 La 4.796(16) 4_456
O1 Ga2 4.853(6) 1_665
O1 Ga2 4.853(6) 1_565
O1 O1 4.893(12) 2_455
O1 O1 4.893(12) 2_565
O1 O1 4.893(12) 2_465
O1 O3 4.824(18) 4
O1 O3 4.824(18) 3_455
O1 O3 4.824(18) 1_565
O1 O1 5.0232 1_556
O1 O1 5.0232 1_554
O1 Ga3 5.225(6) 4_446
O1 Ga3 5.225(6) 1_666
O1 Ga3 5.225(6) 2_465
O1 O3 5.291(15) 5
O1 O3 5.291(15) 2_455
O1 O3 5.291(15) 6_565
O1 O3 5.289(16) 4_556
O1 O3 5.289(16) 3_456
O1 O3 5.289(16) 1_566
O1 O3 5.602(19) 6_554
O1 O3 5.602(19) 2_564
O1 O3 5.602(19) 5_454
O1 O2 5.58(2) 4_554
O1 O2 5.58(2) 3_454
O1 O2 5.58(2) 1_564
O1 O1 5.67(2) 2_456
O1 O1 5.67(2) 2_566
O1 O1 5.67(2) 2_466
O1 Ga2 5.745(11) 1_554
O1 Ga2 5.745(11) 1_664
O1 Ga2 5.745(11) 1_564
O1 La 5.807(3) 4
O1 La 5.807(3) 2_455
O1 La 5.807(3) 1_565
O1 O3 5.756(12) 2
O1 O3 5.756(12) 5_565
O1 O3 5.756(12) 6_455
O1 O2 6.170(16) 1_665
O2 Ga3 1.810(15) 4_446
O2 La 2.405(15) 4_445
O2 O3 2.69(3) 6
O2 O3 2.77(2) 2
O2 O1 2.86(2) 2_455
O2 O2 2.81(3) 4_445
O2 O2 2.81(3) 3_455
O2 O3 2.928(17) 1_556
O2 O2 2.89(3) 2_556
O2 O1 3.12(2) 2_456
O2 O3 3.26(2) .
O2 O1 3.556(16) 1_545
O2 O2 3.68(3) 2
O2 Ga2 3.659(18) 2_556
O2 O3 3.86(2) 5_445
O2 Ga3 4.044(18) 2_565
O2 La 3.975(18) 4_446
O2 La 4.195(13) 1_556
O2 Ga3 4.301(15) 4_445
O2 La 4.245(15) 2_455
O2 O3 4.33(2) 3_556
O2 O3 4.26(2) 4_446
O2 Ga3 4.232(19) 2_455
O2 Ga3 4.354(15) 1_556
O2 Ga2 4.428(15) 1_554
O2 O2 4.53(3) 6_556
O2 La 4.478(14) 2
O2 O3 4.56(2) 3
O2 O3 4.49(2) 4_445
O2 O2 4.508(15) 5_446
O2 O2 4.508(15) 5_456
O2 O3 4.69(2) 5
O2 Ga2 4.742(18) 2_566
O2 Nb 4.701(15) 1_556
O2 Ga1 4.701(15) 1_556
O2 Ga3 4.802(16) 1_656
O2 O2 5.07(4) 6
O2 O2 5.053(18) 5_445
O2 O2 5.053(18) 5_455
O2 O2 5.0232 1_554
O2 O2 5.0232 1_556
O2 O3 5.02(2) 4_556
O2 Ga3 4.96(2) 1_546
O2 O3 5.089(19) 3_456
O2 O3 5.29(2) 2_455
O2 O3 5.22(2) 4
O2 Ga2 5.258(13) 2
O2 O3 5.28(2) 3_455
O2 O2 5.42(3) 3
O2 O2 5.42(3) 4
O2 La 5.295(15) 2_456
O2 Ga1 5.330(18) 1_445
O2 Nb 5.330(18) 1_445
O2 O2 5.27(3) 6_446
O2 O2 5.27(3) 6_546
O2 O3 5.410(19) 6_556
O2 O3 5.39(2) 5_455
O2 O3 5.36(3) 6_445
O2 La 5.484(16) 2_556
O2 Ga3 5.619(19) 2_564
O2 O3 5.45(2) 2_556
O2 O1 5.58(2) 1_546
O2 O2 5.74(2) 6_445
O2 O2 5.74(2) 6_545
O2 O2 5.753(13) 4_444
O2 O2 5.753(13) 3_454
O2 O2 5.753(13) 4_446
O2 O2 5.753(13) 3_456
O2 O3 5.97(2) 6_554
O2 La 5.854(17) 1_545
O2 O3 6.007(19) 2_554
O2 La 6.12(2) 2_565
O2 O2 6.05(3) 3_445
O2 O2 6.05(3) 4_545
O2 O3 6.08(2) 5_446
O3 Ga3 1.817(12) 4_445
O3 Ga3 2.524(15) 2_564
O3 O2 2.69(3) 6
O3 O3 2.58(2) 6
O3 O3 2.80(3) 6_554
O3 O3 2.68(2) 3
O3 O3 2.68(2) 4
O3 O2 2.77(2) 2
O3 O2 2.928(17) 1_554
O3 O1 3.113(13) 2_455
O3 O3 3.17(3) 2
O3 Ga2 3.399(12) 1_554
O3 O3 3.35(2) 2_554
O3 Ga3 3.612(12) 1_655
O3 La 3.705(15) 4_445
O3 Ga2 3.929(15) 2_565
O3 O2 3.86(2) 5_455
O3 O3 3.86(2) 5
O3 O3 4.01(3) 5_554
O3 Ga3 3.916(14) 4_446
O3 Nb 4.127(13) 1_554
O3 Ga1 4.127(13) 1_554
O3 O2 4.33(2) 4_554
O3 La 4.333(13) 1_554
O3 Ga3 4.290(12) 2_565
O3 O2 4.26(2) 3_454
O3 La 4.242(14) 2
O3 O2 4.56(2) 4
O3 O2 4.49(2) 3_455
O3 La 4.601(14) 2_565
O3 Ga2 4.537(14) 2
O3 O2 4.69(2) 5
O3 O1 4.78(2) 1_554
O3 La 4.868(13) 4
O3 O1 4.824(18) 1_545
O3 O3 5.0232 1_554
O3 O3 5.0232 1_556
O3 O2 5.02(2) 3_554
O3 Ga3 5.008(12) 1_656
O3 O2 5.089(19) 4_444
O3 O2 5.29(2) 2_565
O3 La 5.189(12) 4_444
O3 O2 5.22(2) 3
O3 O1 5.291(15) 2_565
O3 Ga2 5.332(12) 2_566
O3 O2 5.28(2) 4_445
O3 O1 5.289(16) 1_544
O3 O3 5.36(2) 4_445
O3 O3 5.36(2) 3_455
O3 Ga2 5.464(15) 1_664
O3 O2 5.410(19) 6_556
O3 O2 5.39(2) 5_445
O3 La 5.507(12) 2_455
O3 O2 5.36(3) 6_545
O3 O2 5.45(2) 2_556
O3 O1 5.602(19) 2_454
O3 La 5.585(12) 2_554
O3 O3 5.695(10) 3_554
O3 O3 5.695(10) 3_556
O3 O3 5.695(10) 4_554
O3 O3 5.695(10) 4_556
O3 La 5.862(16) 2_564
O3 O2 5.97(2) 6_554
O3 O1 5.756(12) 2
O3 La 6.004(13) 4_455
O3 O2 6.007(19) 2_554
O3 La 6.074(14) 4_554
O3 O3 6.035(19) 5_455
O3 O3 6.035(19) 5_445
O3 O3 6.131(18) 5_454
O3 O3 6.131(18) 5_444
O3 O2 6.08(2) 5_456
O3 La 6.111(12) 1_655
